Survey

* Your assessment is very important for improving the workof artificial intelligence, which forms the content of this project

Survey

Document related concepts

no text concepts found

Transcript

Superconductivity This page intentionally left blank Superconductivity Charles P. Poole, Jr. Horacio A. Farach Richard J. Creswick Department of Physics and Astronomy University of South Carolina Columbia, South Carolina Ruslan Prozorov Ames Laboratory Department of Physics and Astronomy Iowa State University Ames Iowa Amsterdam – Boston – Heidelberg – London – New York – Oxford Paris – San Diego – San Francisco – Singapore – Sydney – Tokyo Academic Press is an imprint of Elsevier Academic Press is an imprint of Elsevier 84 Theobald’s Road, London WC1X 8RR, UK Radarweg 29, PO Box 211, 1000 AE Amsterdam, The Netherlands Linacre House, Jordan Hill, Oxford OX2 8DP, UK 30 Corporate Drive, Suite 400, Burlington, MA 01803, USA 525 B Street, Suite 1900, San Diego, CA 92101-4495, USA First edition 1995 Second edition 2007 Copyright © 1995–2007 Elsevier Ltd. All rights reserved No part of this publication may be reproduced, stored in a retrieval system or transmitted in any form or by any means electronic, mechanical, photocopying, recording or otherwise without the prior written permission of the publisher Permissions may be sought directly from Elsevier’s Science & Technology Rights Department in Oxford, UK: phone (+44) (0) 1865 843830; fax (+44) (0) 1865 853333; email: [email protected]. Alternatively you can submit your request online by visiting the Elsevier web site at http://elsevier.com/locate/permissions, and selecting Obtaining permission to use Elsevier material Notice No responsibility is assumed by the publisher for any injury and/or damage to persons or property as a matter of products liability, negligence or otherwise, or from any use or operation of any methods, products, instructions or ideas contained in the material herein. Because of rapid advances in the medical sciences, in particular, independent verification of diagnoses and drug dosages should be made ISBN: 0-12-561456-X ISBN: 978-0-12-088761-3 first edition (1995) second edition (revised version) For information on all Academic Press publications visit our website at books.elsevier.com Printed and bound in The Netherlands 07 08 09 10 11 10 9 8 7 6 5 4 3 2 1 Working together to grow libraries in developing countries www.elsevier.com | www.bookaid.org | www.sabre.org One of us wishes to dedicate this book to the memory of his wife of 51 years Kathleen Theresa Walsh Poole (November 12, 1932–November10, 2004) This page intentionally left blank Contents Preface to the First Edition . . . xvii Preface to the Second Edition . xxi XIII. XIV. XV. XVI. � Electromagnetic Fields 14 Boundary Conditions 15 Magnetic Susceptibility 16 Hall Effect 18 Further Reading 20 Problems 20 1 Properties of the Normal State I. II. III. IV. V. VI. VII. VIII. IX. X. XI. XII. Introduction 1 Conduction Electron Transport 1 Chemical Potential and Screening 4 Electrical Conductivity 5 Frequency Dependent Electrical Conductivity 6 Electron–Phonon Interaction 7 Resistivity 7 Thermal Conductivity 8 Fermi Surface 8 Energy Gap and Effective Mass 10 Electronic Specific Heat 11 Phonon Specific Heat 12 � 2 Phenomenon of Superconductivity I. II. III. IV. Introduction 23 Brief History 24 Resistivity 27 A. Resistivity above Tc 27 B. Resistivity Anisotropy 28 C. Anisotropy Determination 31 D. Sheet Resistance of Films: Resistance Quantum 32 Zero Resistance 34 A. Resistivity Drop at Tc 34 B. Persistent Currents below Tc 35 vii viii CONTENTS V. VI. VII. Transition Temperature 36 Perfect Diamagnetism 40 Magnetic Fields Inside a Superconductor 43 VIII. Shielding Current 44 IX. Hole in Superconductor 45 X. Perfect Conductivity 48 XI. Transport Current 49 XII. Critical Field and Current 52 XIII. Temperature Dependences 52 XIV. Two Fluid Model 54 XV. Critical Magnetic Field Slope 55 XVI. Critical Surface. 55 Further Reading 58 Problems 58 � 3 Classical Superconductors I. II. III. IV. V. VI. VII. VIII. IX. X. XI. Introduction 61 Elements 61 Physical Properties of Superconducting Elements 64 Compounds 67 Alloys 71 Miedema’s Empirical Rules 72 Compounds with the NaCl Structure 75 Type A15 Compounds 76 Laves Phases 78 Chevrel Phases 80 Chalcogenides and Oxides 82 Problems 82 Discontinuity at TC 89 Specific Heat below TC 90 Density of States and Debye Temperature 90 VI. Thermodynamic Variables 91 VII. Thermodynamics of a Normal Conductor 92 VIII. Thermodynamics of a Superconductor 95 IX. Superconductor in Zero Field 97 X. Superconductor in a Magnetic Field 98 XI. Normalized Thermodynamic Equations 103 XII. Specific Heat in a Magnetic Field 105 XIII. Further Discussion of the Specific Heat 107 XIV. Order of the Transition 109 XV. Thermodynamic Conventions 109 XVI. Concluding Remarks 110 Problems 110 III. IV. V. � 5 Magnetic Properties I. II. III. IV. V. VI. � 4 Thermodynamic Properties I. II. Introduction 83 Specific Heat above TC 84 VII. VIII. IX. X. XI. XII. Introduction 113 Susceptibility 114 Magnetization and Magnetic Moment 114 Magnetization Hysteresis 116 Zero Field Cooling and Field Cooling 117 Granular Samples and Porosity 120 Magnetization Anisotropy 121 Measurement Techniques 122 Comparison of Susceptibility and Resistivity Results 124 Ellipsoids in Magnetic Fields 124 Demagnetization Factors 125 Measured Susceptibilities 127 ix CONTENTS XIII. XIV. XV. XVI. XVII. XVIII. XIX. Sphere in a Magnetic Field 128 Cylinder in a Magnetic Field 129 ac Susceptibility 131 Temperature-Dependent Magnetization 134 A. Pauli Paramagnetism 134 B. Paramagnetism 134 C. Antiferromagnetism 136 Pauli Limit and Upper Critical Field 137 Ideal Type II Superconductor 139 Magnets 141 Problems 142 Further Reading 168 Problems 169 � 7 BCS Theory I. II. III. IV. V. VI. � 6 Ginzburg–Landau Theory I. II. III. Introduction 143 Order Parameter 144 Ginzburg–Landau Equations 145 IV. Zero-Field Case Deep Inside Superconductor 146 V. Zero-Field Case near Superconductor Boundary 148 VI. Fluxoid Quantization 149 VII. Penetration Depth 150 VIII. Critical Current Density 154 IX. London Equations 155 X. Exponential Penetration 155 XI. Normalized Ginzburg– Landau Equations 160 XII. Type I and Type II Superconductivity 161 XIII. Upper Critical Field BC2 162 XIV. Structure of a Vortex 164 A. Differential Equations 164 B. Solutions for Short Distances 165 C. Solution for Large Distances 166 VII. Introduction 171 Cooper Pairs 172 The BCS Order Parameter 174 The BCS Hamiltonian 176 The Bogoliubov Transformation 177 The Self-Consistent Gap Equation 178 A. Solution of the Gap Equation Near Tc 179 B. Solution at T = 0 179 C. Nodes of the Order Parameter 179 D. Single Band Singlet Pairing 180 E. S-Wave Pairing 180 F. Zero-Temperature Gap 182 G. D-Wave Order Parameter 184 H. Multi-Band Singlet Pairing 185 Response of a Superconductor to a Magnetic Field 188 Appendix A. Derivation of the Gap Equation Near Tc 190 Further Reading 192 � 8 Cuprate Crystallographic Structures I. II. Introduction 195 Perovskites 196 x III. IV. V. VI. VII. VIII. IX. X. XI. XII. CONTENTS A. Cubic Form 196 B. Tetragonal Form 198 C. Orthorhombic Form 198 D. Planar Representation 199 Perovskite-Type Superconducting Structures 200 Aligned YBa2 Cu3 O7 202 A. Copper Oxide Planes 204 B. Copper Coordination 204 C. Stacking Rules 205 D. Crystallographic Phases 205 E. Charge Distribution 206 F. YBaCuO Formula 207 G. YBa2 Cu4 O8 and Y2 Ba4 Cu7 O15 207 Aligned HgBaCaCuO 208 Body Centering 210 Body-Centered La2 CuO4 , Nd2 CuO4 and Sr2 RuO4 211 A. Unit Cell of La2 CuO4 Compound (T Phase) 211 B. Layering Scheme 212 C. Charge Distribution 212 D. Superconducting Structures 213 E. Nd2 CuO4 Compound (T Phase) 213 F. La2−x−y Rx Sry CuO4 Compounds (T* Phase) 216 G. Sr2 RuO4 Compound (T Phase) 217 Body-Centered BiSrCaCuO and TlBaCaCuO 218 A. Layering Scheme 218 B. Nomenclature 219 C. Bi-Sr Compounds 220 D. Tl-Ba Compounds 220 E. Modulated Structures 221 F. Aligned Tl-Ba Compounds 222 G. Lead Doping 222 Symmetries 222 Layered Structure of the Cuprates 223 Infinite-Layer Phases 225 Conclusions 227 Further Reading 227 Problems 228 � 9 Unconventional Superconductors I. II. III. IV. V. VI. VII. VIII. Introduction 231 Heavy Electron Systems 231 Magnesium Diboride 236 A. Structure 236 B. Physical Properties 237 C. Anisotropies 237 D. Fermi Surfaces 239 E. Energy Gaps 241 Borocarbides and Boronitrides 243 A. Crystal Structure 243 B. Correlations of Superconducting Properties with Structure Parameters 244 C. Density of States 245 D. Thermodynamic and Electronic Properties 247 E. Magnetic Interactions 249 F. Magnetism of HoNi2 B2 C 254 Perovskites 256 A. Barium-PotassiumBismuth Cubic Perovskite 256 B. Magnesium-CarbonNickel Cubic Perovskite 257 C. Barium-Lead-Bismuth Lower Symmetry Perovskite 258 Charge-Transfer Organics 259 Buckminsterfullerenes 260 Symmetry of the Order Parameter in Unconventional Superconductors 262 A. Symmetry of the Order Parameter in Cuprates 262 xi CONTENTS IX. a. Hole-doped high-Tc cuprates 262 b. Electron-doped cuprates 263 B. Organic Superconductors 264 C. Influence of Bandstructure on Superconductivity 266 a. MgB2 266 b. NbSe2 267 c. CaAlSi 268 D. Some Other Superconductors 268 a. Heavy-fermion superconductors 268 b. Borocarbides 269 c. Sr2 RuO4 269 d. MgCNi3 270 Magnetic Superconductors 270 A. Coexistence of superconductivity and magnetism 270 B. Antiferromagnetic Superconductors 272 C. Magnetic Cuprate Superconductor – SmCeCuO 272 � 10 Hubbard Models and Band Structure I. II. III. Introduction 275 Electron Configurations 276 A. Configurations and Orbitals 276 B. Tight-Binding Approximation 277 Hubbard Model 281 A. Wannier Functions and Electron Operators 281 B. One-State Hubbard Model 282 C. Electron-Hole Symmetry 283 IV. V. VI. VII. VIII. IX. X. XI. D. Half-Filling and Antiferromagnetic Correlations 284 E. t-J Model 285 F. Resonant-Valence Bonds 286 G. Spinons, Holons, Slave Bosons, Anyons, and Semions 287 H. Three-State Hubbard Model 287 I. Energy Bands 288 J. Metal-Insulator Transition 289 Band Structure of YBa2 Cu3 O7 290 A. Energy Bands and Density of States 291 B. Fermi Surface: Plane and Chain Bands 292 Band Structure of Mercury Cuprates 293 Band Structures of Lanthanum, Bismuth, and Thallium Cuprates 299 A. Orbital States 299 B. Energy Bands and Density of States 299 Fermi Liquids 302 Fermi Surface Nesting 303 Charge-Density Waves, Spin-Density Waves, and Spin Bags 303 Mott-Insulator Transition 304 Discussion 305 Further Reading 305 Problems 305 � 11 Type I Superconductivity and the Intermediate State I. II. Introduction 307 Intermediate State 308 xii III. IV. V. VI. VII. VIII. IX. X. XI. XII. CONTENTS Surface Fields and Intermediate-State Configurations 308 Type I Ellipsoid 310 Susceptibility 311 Gibbs Free Energy for the Intermediate State 313 Boundary-Wall Energy and Domains 315 Thin Film in Applied Field 317 Domains in Thin Films 318 Current-Induced Intermediate State 322 Recent Developments in Type I Superconductivity 326 A. History and General Remarks 326 B. The Intermediate State 329 C. Magneto-Optics with In-Plane Magnetization – a Tool to Study Flux Patterns 330 D. AC Response in the Intermediate State of Type I Superconductors 332 Mixed State in Type II Superconductors 333 Problems 334 IV. V. VI. � 12 Type II Superconductivity I. II. III. Introduction 337 Internal and Critical Fields 338 A. Magnetic Field Penetration 338 B. Gimzburg-Landau Parameter 340 C. Critical Fields 342 Vortices 345 A. Magnetic Fields 346 B. High-Kappa Approximation 347 VII. C. Average Internal Field and Vortex Separation 349 D. Vortices near Lower Critical Field 350 E. Vortices near Upper Critical Field 352 F. Contour Plots of Field and Current Density 352 G. Closed Vortices 354 Vortex Anisotropies 355 A. Critical Fields and Characteristic Lengths 356 B. Core Region and Current Flow 357 C. Critical Fields 357 D. High-Kappa Approximation 361 E. Pancake Vortices 363 F. Oblique Alignment 363 Individual Vortex Motion 364 A. Vortex Repulsion 364 B. Pinning 367 C. Equation of Motion 368 D. Onset of Motion 369 E. Magnus Force 369 F. Steady-State Motion 370 G. Intrinsic Pinning 371 H. Vortex Entanglement 371 Flux Motion 371 A. Flux Continuum 371 B. Entry and Exit 372 C. Two-Dimensional Fluid 372 D. Dimensionality 373 E. Solid and Glass Phases 374 F. Flux in Motion 374 G. Transport Current in a Magnetic Field 375 H. Dissipation 376 I. Magnetic Phase Diagram 377 Fluctuations 378 A. Thermal Fluctuations 378 B. Characteristic Length 378 C. Entanglement of Flux Lines 379 D. Irreversibility Line 379 xiii CONTENTS E. Kosterlitz–Thouless Transition 381 Problems 381 � VII. VIII. 13 Irreversible Properties � I. II. III. I. IV. V. VI. Introduction 385 Critical States 385 Current–Field Relationships 386 A. Transport and Shielding Current 386 B. Maxwell Curl Equation and Pinning Force 387 C. Determination of Current–Field Relationships 388 Critical-State Models 388 A. Requirements of a Critical-State Model 388 B. Model Characteristics 388 Bean Model 389 A. Low-Field Case 389 B. High-Field Case 390 C. Transport Current 392 D. Combining Screening and Transport Current 393 E. Pinning Strength 395 F. Current-Magnetic Moment Conversion Formulae 396 a. Elliptical cross-section 396 b. Rectangular cross-section 396 c. Triangular cross-section 396 d. General remarks 397 Reversed Critical States and Hysteresis 397 A. Reversing Field 398 B. Magnetization 401 C. Hysteresis Loops 401 D. Magnetization Current 403 Perfect Type-I Superconductor 405 Concluding Remarks 406 Problems 406 14 Magnetic Penetration Depth II. III. IV. V. VI. VII. VIII. IX. X. Isotropic London Electrodynamics 409 Penetration Depth in Anisotropic Samples 411 Experimental Methods 413 Absolute Value of the Penetration Depth 414 Penetration Depth and the Superconducting Gap 416 A. Semiclassical Model for Superfluid Density 416 a. Isotropic Fermi Surface 417 b. Anisotroic Fermi Surface, Isotropic gap function 418 B. Superconducting Gap 418 C. Mixed Gaps 419 D. Low-Temperatures 420 a. s-wave pairing 420 b. d-wave pairing 420 c. p-wave pairing 420 Effect of Disorder and Impurities on the Penetration Depth 421 A. Non-Magnetic Impurities 421 B. Magnetic Impurities 422 Surface Andreev Bound States 423 Nonlocal Electrodynamics of Nodal Superconductors 425 Nonlinear Meissner Effect 426 AC Penetration Depth in the Mixed State (Small Amplitude Linear Response) 428 xiv XI. CONTENTS The Proximity Effect and its Identification by Using AC Penetration Depth Measurements 430 VI. � 15 Energy Gap and Tunneling I. II. III. IV. V. Introduction 433 Phenomenon of Tunneling 433 A. Conduction-Electron Energies 434 B. Types of Tunneling 435 Energy Level Schemes 435 A. Semiconductor Representation 435 B. Boson Condensation Representation 436 Tunneling Processes 436 A. Conditions for Tunneling 436 B. Normal Metal Tunneling 438 C. Normal Metal – Superconductor Tunneling 438 D. Superconductor – Superconductor Tunneling 439 Quantitative Treatment of Tunneling 440 A. Distribution Function 440 B. Density of States 442 C. Tunneling Current 442 D. N–I–N Tunneling Current 444 E. N–I–S Tunneling Current 444 F. S–I–S Tunneling Current 445 G. Nonequilibrium Quasiparticle Tunneling 447 VII. VIII. H. Tunneling in unconventional superconductors 449 a. Introduction 449 b. Zero-Bias Conductance Peak 450 c. c-Axis Tunneling 451 Tunneling Measurements 451 A. Weak Links 452 B. Experimental Arrangements for Measuring Tunneling 452 C. N–I–S Tunneling Measurements 454 D. S–I–S Tunneling Measurements 454 E. Energy Gap 455 F. Proximity Effect 457 G. Even–Odd Electron Effect 459 Josephson Effect 459 A. Cooper Pair Tunneling 460 B. dc Josephson Effect 460 C. ac Josephson Effect 462 D. Driven Junctions 463 E. Inverse ac Josephson Effect 466 F. Analogues of Josephson Junctions 469 Magnetic Field and Size Effects 472 A. Short Josephson Junction 472 B. Long Josephson Junction 476 C. Josephson Penetration Depth 478 D. Two-Junction Loop 479 E. Self-Induced Flux 480 F. Junction Loop of Finite Size 482 G. Ultrasmall Josephson Junction 482 H. Arrays and Models for Granular Superconductors 485 I. Superconducting Quantum Interference Device 485 Problems 486 xv CONTENTS � 16 Transport Properties � I. II. I. II. III. IV. V. VI. VII. VIII. IX. X. Introduction 489 Inductive Superconducting Circuits 489 A. Parallel Inductances 490 B. Inductors 490 C. Alternating Current Impedance 491 Current Density Equilibration 492 Critical Current 495 A. Anisotropy 495 B. Magnetic Field Dependence 496 Magnetoresistance 497 A. Fields Applied above Tc 498 B. Fields Applied below Tc 500 C. Fluctuation Conductivity 501 D. Flux-Flow Effects 502 Hall Effect 504 A. Hall Effect above Tc 505 B. Hall Effect below Tc 507 Thermal Conductivity 508 A. Heat and Entropy Transport 508 B. Thermal Conductivity in the Normal State 509 C. Thermal Conductivity below Tc 511 D. Magnetic Field Effects 513 E. Anisotropy 513 Thermoelectric and Thermomagnetic Effects 513 A. Thermal Flux of Vortices 515 B. Seebeck Effect 516 C. Nernst Effect 518 D. Peltier Effect 522 E. Ettingshausen Effect 522 F. Righi–Leduc Effect 524 Photoconductivity 524 Transport Entropy 527 Problems 528 17 Spectroscopic Properties III. IV. V. VI. VII. VIII. Introduction 531 Vibrational Spectroscopy 532 A. Vibrational Transitions 532 B. Normal Modes 533 C. Soft Modes 533 D. Infrared and Raman Active Modes 533 E. Kramers-Kronig Analysis 535 F. Infrared Spectra 536 G. Light-Beam Polarization 538 H. Raman Spectra 539 I. Energy Gap 541 Optical Spectroscopy 543 Photoemission 545 A. Measurement Technique 545 B. Energy Levels 546 C. Core-Level Spectra 551 D. Valence Band Spectra 552 E. Energy Bands and Density of States 554 X-Ray Absorption Edges 555 A. X-Ray Absorption 555 B. Electron-Energy Loss 558 Inelastic Neutron Scattering 559 Positron Annihilation 561 Magnetic Resonance 565 A. Nuclear Magnetic Resonance 566 B. Quadrupole Resonance 571 C. Electron-Spin Resonance 574 D. Nonresonant Microwave Absorption 575 E. Microwave Energy Gap 577 F. Muon-Spin Relaxation 578 G. Mössbauer Resonance 579 Problems 581 References . . . . . . . . . . . . . . . . . . . .583 Index . . . . . . . . . . . . . . . . . . . . . . . . .633 This page intentionally left blank Preface to the First Edition When we wrote our 1988 book, Cooper Oxide Superconductors, our aim was to present an early survey of the experimen tal aspects of the field of high temperature superconductivity as an aid to researchers who were then involved in the worldwide effort to (a) understand the phenomenon of cuprate superconductivity and (b) search for ways to raise the critical temperature and produce materials suitable for the fabrication of magnets and other devices. A great deal of experimental data are now available on the cuprates, and their superconducting proper ties have been well characterized using high quality untwinned monocrystals and epitax ial thin films. Despite this enormous research effort, the underlying mechanisms respon sible for the superconducting properties of the cuprates are still open to question. Nev ertheless, we believe that the overall pic ture is now clear enough to warrant the writing of a text-book that presents our present-day understanding of the nature of the phenomenon of superconductivity, sur veys the properties of various known super conductors, and shows how these properties fit into various theoretical frameworks. The aim is to present this material in a format suitable for use in a graduate-level course. An introduction to superconductivity must be based on a background of funda mental principles found in standard solid state physics texts, and a brief introductory chapter provides this background. This initial chapter on the properties of normal conduc tors is limited to topics that are often referred to throughout the remainder of the text: elec trical conductivity, magnetism, specific heat, etc. Other background material specific to particular topics is provided in the appro priate chapters. The presence of the initial normal state chapter makes the remainder of the book more coherent. The second chapter presents the essen tial features of the superconducting state— the phenomena of zero resistance and xvii xviii perfect diamagnetism. Super current flow, the accompanying magnetic fields, and the transition to this ordered state that occurs at the transition temperature Tc are described. The third chapter surveys the properties of the various classes of superconductors, including the organics, the buckminister fullerenes, and the precursors to the cuprates, but not the high temperature superconduc tors themselves. Numerous tables and figures summarize the properties of these materials. Having acquired a qualitative under standing of the nature of superconductivity, we now proceed, in five subsequent chapters, to describe various theoretical frameworks which aid in understanding the facts about superconductors. Chapter 4 discusses super conductivity from the view-point of ther modynamics and provides expressions for the free energy—the thermodynamic func tion that constitutes the starting point for the formulations of both the Ginzburg–Landau (GL) and the BCS theories. The GL the ory is developed in Chapter 5 and the BCS theory in Chapter 6. GL is a readily under standable phenomenological theory that pro vides results that are widely used in the interpretation of experimental data, and BCS in a more fundamental, and mathematically challenging, theory that makes predictions that are often checked against experimen tal results. Most of Chapter 5 is essential reading, whereas much of the formalism of Chapter 6 can be skimmed during a first reading. The theoretical treatment is interrupted by Chapter 7, which presents the details of the structures of the high temperature super conductors. This constitutes important back ground material for the band theory sections of Chapter 8, which also presents the Hub bard and related models, such as RVB and t–J. In addition, Chapter 8 covers other theoretical approaches involving, for exam ple, spinons, holons, slave bosons, anyons, semions, Fermi liquids, charge and spin den sity waves, spin bags, and the Anderson PREFACE TO THE FIRST EDITION interlayer tunneling scheme. This completes the theoretical aspects of the field, except for the additional description of critical state models such as the Bean model in Chapter 12. The Bean model is widely used for the interpretation of experimental results. The remainder of the text covers the magnetic, transport, and other properties of superconductors. Most of the examples in these chapters are from the literature on the cuprates. Chapter 9 introduces Type II superconductivity and describes magnetic properties, Chapter 10 continues the dis cussion of magnetic properties, Chapter 11 covers the intermediate and mixed states, and Chapter 12, on critical state models, completes the treatment of magnetic proper ties. The next two chapters are devoted to transport properties. Chapter 13 covers var ious types of tunneling and the Josephson effect, and Chapter 14 presents the remain ing transport properties involving the Peltier, Seebeck, Hall, and other effects. When the literature was surveyed in preparation for writing this text, it became apparent that a very significant percentage of current research on superconductivity is being carried out by spectroscopists, and to accommodate this, Chapter 15 on spec troscopy was added. This chapter lets the reader know what the individual branches of spectroscopy can reveal about the properties of superconductors, and in addition, it pro vides an entrée to the vast literature on the subject. This book contains extensive tabulations of experimental data on various supercon ductors, classical as well as high Tc types. Figures from research articles were gener ally chosen because they exemplify princi ples described in the text. Some other figures, particularly those in Chapter 3, provide cor relations of extensive data on many samples. There are many cross-references between the chapters to show how the different topics fit together as on unified subject. Most chapters end with sets of problems that exemplify the material presented and PREFACE TO THE FIRST EDITION sets of references for additional reading on the subject. Other literature citations are scat tered throughout the body of each chapter. Occasional reference is made to our earlier work, Copper Oxide Superconductors, for supplementary material. One of us (C.P.P.) taught a graduate-level superconductivity course three times using lecture notes which eventually evolved into the present text. It was exciting to learn with the students while teaching the course and simultaneously doing research on the subject. We thank the following individuals for their helpful discussions and comments on the manuscript: C. Almasan, S. Aktas, D. Castellanos, T. Datta, N. Fazyleev, J. B. Goodenough, K. E. Gray, D. U. Gubser, D. R. Harshman, A. M. Herman, Z. Iqbal, E. R. Jones, A. B. Kaiser, D. Kirvin, xix O. Lopez, M. B. Maple, A. P. Mills, Jr., S. Misra, F. J. Owens, M. Pencarinha, A. Petrile, W. E. Pickett, S. J. Poon, A. W. Sleight, O. F. Schuette, C. Sisson, David B. Tanner, H. Testardi, C. Uher, T. Usher, and S. A. Wolf. We also thank the graduate students of the superconductiv ity classes for their input, which improved the book’s presentation. We appreciate the assistance given by the University of South Carolina (USC) Physics Department; our chairman, F. T. Avignone; the secretaries, Lynn Waters and Cheryl Stocker; and espe cially by Gloria Phillips, who is thanked for her typing and multiple emendations of the BCS chapter and the long list of refer ences. Eddie Josie of the USC Instructional Services Department ably prepared many of the figures. This page intentionally left blank Preface to the Second Edition It has been an exciting two decades spending most of my time playing a rela tively minor role in the exciting world-wide Superconductivity Endeavor. My involve ment began on March 18th , 1987, when I attended what became known later as the “Woodstock of Physics”, the “Special Panel Discussion on Novel High Temperature Superconductivity” held at the New York meeting of the American Physical Society. I came a half hour early and found the main meeting room already full, so several hun dred physicists and I watched the proceed ings at one of the many TV monitors set up in the corridors of the hotel. That evening in the hotel room my colleague Timir Datta said to me “Why don’t we try to write the first book on high temperature superconductivity?” When we arrived back in Columbia I enlisted the aid of Horacio, my main collaborator for two prior decades, and the work began. Timir and I spent many nights working until two or three in the morning gathering together material, collating, and writing. We had help from two of our USC students M. M. Rigney and C. R. Sanders. In this work Copper Oxide Superconductors we managed to comment on, summarize, and collate the data by July of 1988, and the book appeared in print toward the end of that year. By the mid 1990’s the properties of the cuprates had become well delineated by measurements carried out with high quality untwinned single crystals and epitaxial thin films. There seemed to be a need to assem ble and characterize the enormous amount of accumulated experimental data on a multi tude of superconducting types. To undertake this task and acquire an understanding of the then current status of the field, during 1993 and 1994 I mailed postcards to researchers all over the world requesting copies of their work on the subject. This was supplemented by xerox copies of additional articles made in our library, and provided a collection of over 2000 articles on superconductivity. xxi xxii These reprints and xeroxes were sorted into categories which became chapters and sec tions of the first edition of this present book. For several months the floor of my study at home remained covered with piles of reprints as I proceeded to sort, peruse, and transpose data and information from them. This was a tedious, but nonetheless very exciting task. There were some surprises, such as the relatively large number of articles on spec troscopy, most of which were very informa tive, and they became Chap. 15. This chapter contained material that most closely matched my pre-superconductivity era research endeavors, and I was pleased to learn how much spectroscopy had contributed to an understanding of the nature of superconduc tors. There were also many articles on mag netic properties, critical states, tunneling, and transport properties, which became Chapters 10, 12, 13, and 14, respectively. Most of the relatively large number of articles on the Hubbard Model did not, in my opinion, add very much to our understanding of super conductivity. Some of them were combined with more informative articles on band struc ture to form Chap. 8. There was a plethora of articles on the crystallographic structures of various cuprates, with a great deal of redundancy, and the information culled from them constituted Chap. 7. Chapter 9, Type II Superconductivity, summarized information from a large number of reprints. The Intermediate and Mixed States Chapter 11 depended much less on informa tion garnered from the reprints, and much more on classical sources. The same was true of Chap. 3 Classical Superconductors, Chap. 4 Thermodynamic Properties, Chap. 5 Ginzburg-Landau Theory, and Chap. 6 BCS Theory written by Rick. Finally the begin ning of the First Edition text, namely Chap. 1 Properties of the Normal State, and Chap. 2 The Phenomenon of Superconductivity, were introductory in nature, and relied very little on material garnered from the reprint col lection. Thus our first edition provided an PREFACE TO SECOND EDITION overall coverage of the field as it existed at the end of 1994. In 1996 and 1999, respectively, the books The New Superconductors and Elec tromagnetic Absorption in Superconductors were written in collaboration with Frank J. Owens as the principal author. The next project was the Handbook of Superconductivity, published during the mil lennial year 2000. It assembled the experi mental data that had accumulated up to that time. Chapters in this volume were written by various researchers in the field. Of partic ular importance in this work were Chapters 6 and 8 by Roman Gladyshevski and his two coworkers which tabulated and explicated extensive data on, respectively, the Classical and the Cuprate Superconductors. His classi fication of the cuprate materials is especially incisive. Seven years have now passed since the appearance of the Handbook, and our under standing of the phenomenon of Supercon ductivity is now more complete. Much of the research advances during this period have been in the area of magnetism so I enlisted Ruslan Prozorov, who was then a member of our Physics Department at USC, and an expert on the magnetic properties of super conductors, to join Horacio, Rick, and myself in preparing a second edition of our 1995 book. In the preparation of this edition some of the chapters have remained close to the original, some have been shortened, some have been extensively updated, and some are entirely new. The former Chap. 10, Mag netic Properties, has been moved earlier and becomes Chap. 5. Aside from this change, the first six chapters are close to what they were in the original edition. Chapter 7, BCS Theory, has been rewritten to take into account advances in some topics of recent interest such as d-wave and multiband super conductivity. Chapter 8, on the Structures of the Cuprates, has material added to it on the superconductor Sr2 RuO4 , layerng schemes, and infinite layer phases. xxiii PREFACE TO SECOND EDITION Chapter 9 on Nonclassical Supercon ductors describes superconducting materi als which do not fit the categories of Chap. 3. It discusses the properties of the relatively recently discovered superconduc tor magnesium diboride, MgB2 , as well as borocarbides, boronitrides, perovskites such as MgCNi3 , charge transfer organics, heavy electron systems, and Buckminsterfullerenes. The chapter ends with a discussion of the symmetry of the order parameter, and a section that treats magnetic superconductors and the coexistence of superconductivity and magnetism. The coverage of the Hubbard Model and Band Structure in Chap. 10 is sig nificantly shorter than it was in the first edi tion. Chapter 11, Type I Superconductors and the Intermediate State, includes some recent developments in addition to what was cov ered in the first edition. Chapter 12 describes the nature and properties of Type II Super conductors, and is similar to its counterpart in the first edition. Chapter 13, Irreversible Properties, discusses critical states and the Bean model, the treatment of the latter being much shorter than it was in the first edition. In addition there are sections on current-magnetic moment conversion formu lae, and susceptibility measurements of a perfect superconductor. Chapter 14, Magnetic Penetration Depth, written by Ruslau is entirely new. It covers the topics of isotropic London electrodynamics, the superconductivity gap and Fermi surfaces, the semiclassical model for superfluid density, mixed gaps, s- and d-wave pairing, the effect of disorder on the penetration depth, surface Andreev bound states, nonlocal electrodynamics of nodal superconductors, the nonlinear Meiss ner Effect, the Campbell penetration depth, and proximity effect identification. Chapter 15, Energy Gap and Tunneling, includes a new section on tunneling in unconventional superconductors. Finally Chapters 16 and 17 discuss, respectively, transport properties and spectroscopic properties of superconduc tors, and are similar in content to their coun terparts in the first edition. Recent data on superconducting materials have been added to the tables that appeared in various chapters of the first edition, and there are some new tables of data. References to the literature have been somewhat updated. Two of us (Horacio and I) are now octo genarians, but we continue to work. Over the decades Horacio has been a great friend and collaborator. It is no longer “publish or per ish” but “stay active or perish.” We intend to remain active, deo volente. Professor Prozorov would like to acknowledge partial support of NSF grants numbered DMR-06-03841 and DMR 05-53285, and also the Alfred P. Sloan Foundation. He wishes to thank his wife Tanya for her support, and for pushing him to finish his chapters. He also affirms that: “In my short time with the USC Department of Physics, one of the best things that happened was to get to know Charles Poole Jr., Horacio Farach, Rick Creswick, and Frank Avignone III whose enthusiasm was contagious, and I will always cherish the memory of our discussions.” Charles P. Poole, Jr. June 2007 This page intentionally left blank 1 Properties of the Normal State I. INTRODUCTION This text is concerned with the phenomenon of superconductivity, a phe nomenon characterized by certain electri cal, magnetic, and other properties, many of which will be introduced in the follow ing chapter. A material becomes supercon ducting below a characteristic temperature, called the superconducting transition tem perature Tc , which varies from very small values (millidegrees or microdegrees) to val ues above 100 K. The material is called nor mal above Tc , which merely means that it is not superconducting. Elements and com pounds that become superconductors are conductors—but not good conductors—in their normal state. The good conductors, such as copper, silver, and gold, do not superconduct. It will be helpful to survey some proper ties of normal conductors before discussing the superconductors. This will permit us to review some background material and to define some of the terms that will be used throughout the text. Many of the normal state properties that will be discussed here are modified in the superconducting state. Much of the material in this introductory chapter will be referred to later in the text. II. CONDUCTING ELECTRON TRANSPORT The electrical conductivity of a metal may be described most simply in terms of the constituent atoms of the metal. The atoms, in this representation, lose their valence electrons, causing a background lattice of 1 2 1 PROPERTIES OF THE NORMAL STATE Table 1.1 Characteristics of Selected Metallic Elementsa � 77 K � 273 K � 77 K � 273 K Å �� cm �� cm fs rs Å fs Radius Xtal Å type aÅ Å Z Element Valence Å ne 11 Na 19 K 29 Cu 47 Ag 41 Nb 20 Ca 38 Sr 56 Ba 13 Al 81 Tl 50 Sn(W) 1 1 1 1 1 2 2 2 3 3 4 0.97 1.33 0.96 1.26 1.0 0.99 1.12 1.34 0.51 0.95 0.71 2.65 1.40 8.47 5.86 5.56 4.61 3.55 3.51 18.1 10.5 14.8 2.08 2.57 1.41 1.60 1.63 1.73 1.89 1.96 1.10 1.31 1.17 7 17 0.3 3.7 2.1 82 Pb 51 Sb 83 Bi 4 5 5 0.84 0.62 0.74 13.2 16.5 14.1 1.22 1.19 1.13 4.7 8 35 a bcc bcc fcc fcc bcc fcc fcc bcc fcc bcc tetrg 4.23 5.23 3.61 4.09 3.30 5.58 6.08 5.02 4.05 3.88 a = 582 c = 317 fcc 4.95 rhomb 4.51 rhomb 4.75 1022 cm3 0.8 1.38 0.2 0.3 3.0 4.2 6.1 1.56 1.51 15.2 3.43 23 60 2.45 15 10.6 19.0 39 107 170 180 210 200 21 14 6.6 65 9.1 11 5.7 2.7 0.72 32 41 27 40 4.2 22 4.4 1.9 8.0 2.2 2.3 1.4 0.55 0.23 KWth cm K 1.38 1.0 4.01 4.28 0.52 2.06 ≈ 0.36 ≈ 0.19 2.36 0.5 0.64 0.38 0.18 0.09 Notation: a, lattice constant; ne , conduction electron density; rs = 3/4ne 1/3 ; , resistivity; , Drude relaxation time; Kth , thermal conductivity; L = Kth /T is the Lorentz number; , electronic specific heat parameter; m∗ , effective mass; RH , Hall constant; D , Debye temperature; p , plasma frequency in radians per femtosecond 10−15 s; IP, first ionization potential; WF, work function; EF , Fermi energy; TF , Fermi temperature in kilokelvins; kF , Fermi wavenumber in mega reciprocal centimeters; and F , Fermi velocity in centimeters per microsecond. positive ions, called cations, to form, and the now delocalized conduction electrons move between these ions. The number density n (electrons/cm3 ) of conduction electrons in a metallic element of density m g/cm3 , atomic mass number A (g/mole), and valence Z is given by n= NA Zm A (1.1) where NA is Avogadro’s number. The typi cal values listed in Table 1.1 are a thousand times greater than those of a gas at room temperature and atmospheric pressure. The simplest approximation that we can adopt as a way of explaining conductivity is the Drude model. In this model it is assumed that the conduction electrons 1. do not interact with the cations (“free electron approximation”) except when one of them collides elastically with a cation which happens, on average, 1/ times per second, with the result that the velocity of the electron abruptly and randomly changes its direc tion (“relaxation-time approximation”); 2. maintain thermal equilibrium through col lisions, in accordance with Maxwell– Boltzmann statistics (“classical-statistics approximation”); 3. do not interact with each other (“independent-electron approximation”). This model predicts many of the general fea tures of electrical conduction phenomena, as we shall see later in the chapter, but it fails to account for many others, such as tunnel ing, band gaps, and the Bloch T 5 law. More satisfactory explanations of electron trans port relax or discard one or more of these approximations. Ordinarily, one abandons the freeelectron approximation by having the elec trons move in a periodic potential arising from the background lattice of positive ions. Figure 1.1 gives an example of a simple potential that is negative near the positive 3 II CONDUCTING ELECTRON TRANSPORT L � ∗ �� W mJ m K2 me mole K2 0.021 0.022 0.023 0.023 0.029 0.026 0.030 0.042 0.021 0.028 0.025 0.026 0.026 0.035 1.5 2.0 0.67 0.67 8.4 2.7 3.6 2.7 1.26 1.5 1.8 2.9 0.63 0.084 1.3 1.2 1.3 1.1 12 1.8 2.0 1.4 1.4 1.1 1.3 1.9 0.38 0.047 1 RH ne −1.1 −1.1 −1.4 −1.2 −0.76 +1.0 �D K 150 100 310 220 265 230 150 110 394 96 170 88 200 120 � p IP rad eV fs 8.98 5.98 3.85 14.5 5.14 4.34 7.72 7.57 6.87 6.11 5.69 5.21 5.99 6.11 7.34 7.41 8.64 7.29 WF eV EF eV TF kK kF M cm−1 �F cm �s 2.75 2.3 4.6 4.3 4.3 2.9 2.6 2.7 4.3 3.8 4.4 4.3 4.6 4.2 3.24 2.12 7.0 5.49 5.32 4.69 3.93 3.64 11.7 8.15 10.2 9.47 10.9 9.90 37.7 24.6 81.6 63.8 61.8 54.4 45.7 42.3 136 94.6 118 110 127 115 92 75 136 120 118 111 102 98 175 146 164 158 170 161 107 86 157 139 137 128 118 113 203 169 190 183 196 187 the distribution function f0 v = Figure 1.1 Muffin tin potential has a constant nega tive value −V0 near each positive ion and is zero in the region between the ions. ions and zero between them. An electron moving through the lattice interacts with the surrounding positive ions, which are oscillat ing about their equilibrium positions, and the charge distortions resulting from this inter action propagate along the lattice, causing distortions in the periodic potential. These distortions can influence the motion of yet another electron some distance away that is also interacting with the oscillating lat tice. Propagating lattice vibrations are called phonons, so that this interaction is called the electron-phonon interaction. We will see later that two electrons interacting with each other through the intermediary phonon can form bound states and that the result ing bound electrons, called Cooper pairs, become the carriers of the super current. The classical statistics assumption is generally replaced by the Sommerfeld approach. In this approach the electrons are assumed to obey Fermi-Dirac statistics with 1 (1.2) exp m 2 /2 − /kB T + 1 (see the discussion in Section IX), where kB is Boltzmann’s constant, and the constant is called the chemical potential. In Fermi– Dirac statistics, noninteracting conduction electrons are said to constitute a Fermi gas. The chemical potential is the energy required to remove one electron from this gas under conditions of constant volume and constant entropy. The relaxation time approximation assumes that the distribution function fv t is time dependent and that when fv t is disturbed to a nonequilibration configuration f col , collisions return it back to its equilib rium state f 0 with time constant in accor dance with the expression df f col − f 0 =− dt (1.3) Ordinarily, the relaxation time is assumed to be independent of the velocity, resulting in a simple exponential return to equilibrium: fv t = f 0 v + f col v − f 0 ve−t/ (1.4) 4 In systems of interest fv t always remains close to its equilibrium configuration (1.2). A more sophisticated approach to collision dynamics makes use of the Boltzmann equa tion, and this is discussed in texts in solid state physics (e.g., Ashcroft and Mermin, 1976; Burns, 1985; Kittel, 1976) and statis tical mechanics (e.g., Reif, 1965). It is more realistic to waive the independent-electron approximation by rec ognizing that there is Coulomb repulsion between the electrons. In the following section, we will show that electron screen ing makes electron–electron interaction neg ligibly small in good conductors. The use of the Hartree–Fock method to calculate the effects of this interaction is too complex to describe here; it will be briefly discussed in Chapter 10, Section VII. When a method developed by Landau (1957a, b) is employed to take into account electron–electron interactions so as to ensure a one-to-one correspondence between the states of the free electron gas and those of the interacting electron system, the conduction electrons are said to form a Fermi liquid. Due to the Pauli exclusion principle, momentumchanging collisions occur only in the case of electrons at the Fermi surface. In what are called marginal Fermi liquids the one-to-one correspondence condition breaks down at the Fermi surface. Chapter 10, Section VII pro vides a brief discussion of the Fermi liquid and the marginal Fermi liquid approaches to superconductivity. 1 PROPERTIES OF THE NORMAL STATE perhaps one-tenth as great in the case of hightemperature superconductors and A15 com pounds in their normal state. If we take as the time between collisions, the mean free path l, or average distance traveled between collisions, is l= F For aluminum the mean free path is 15 × 10−8 m at 300 K, 13 × 10−7 m at 77 K, and 67 × 10−4 m at 4.2 K. To see that the interactions between con duction electrons can be negligible in a good conductor, consider the situation of a point charge Q embedded in a free electron gas with unperturbed density n0 . This negative charge is compensated for by a rigid back ground of positive charge, and the delocal ized electrons rearrange themselves until a static situation is reached in which the total force density vanishes everywhere. In the presence of this weak electrostatic interac tion the electrons constitute a Fermi liquid. The free energy F in the presence of an external potential is a function of the local density nr of the form F n = F0 n − e nrrd3 r (1.6) where r is the electric potential due to both the charge Q and the induced screening charge and F0 n is the free energy of a noninteracting electron gas with local density n. Taking the functional derivative of F n we have F n = 0 r − er nr III. CHEMICAL POTENTIAL AND SCREENING Ordinarily, the chemical potential is close to the Fermi energy EF and the con duction electrons move at speeds F corre sponding to kinetic energies 21 m F2 close to EF = kB TF . Typically, F ≈ 106 m/s for good conductors, which is 1/300 the speed of light; (1.5) = (1.7) (1.8) where 0 r is the local chemical potential of the free electron gas in the absence of charge Q and is a constant. At zero temperature, which is a good approximation because T TF , the local chemical potential is 0 = �2 3 2 n2/3 2m (1.9) 5 IV ELECTRICAL CONDUCTIVITY Solving this for the density of the electron gas, we have 1 nr = 3 2 2m + er �2 3/2 (1.10) Typically the Fermi energy is much greater than the electrostatic energy so Eq. (1.10) can be expanded about = 0 to give 3 e nr = n0 1 + · 2 (1.11) where n0 = 2m /� 2 3/2 /3 2 . The total induced charge density is then i r = e n0 − nr 3 n e2 r =− · 0 2 (1.12) Poisson’s equation for the electric potential can be written as 2 r − −2 sc r = −4Qr (1.13) where the characteristic distance sc , called the screening length, is given by 2sc = 1 · 6 n0 e2 (1.14) Equation (1.13) has the well-known Yukawa solution Q i r = − e−r/sc r (1.15) Note that at large distances the poten tial of the charge falls off exponentially, and that the characteristic distance sc over which the potential is appreciable decreases with the electron density. In good conductors the screening length can be quite short, and this helps to explain why electron–electron interaction is negligible. Screening causes the Fermi liquid of conduction electrons to act like a Fermi gas. IV. ELECTRICAL CONDUCTIVITY When a potential difference exists between two points along a conducting wire, a uniform electric field E is established along the axis of the wire. This field exerts a force F = −eE that accelerates the electrons: d (1.16) −eE = m dt and during a time t that is on the order of the collision time the electrons attain a velocity eE (1.17) =− m The electron motion consists of successive periods of acceleration interrupted by colli sions, and, on average, each collision reduces the electron velocity to zero before the start of the next acceleration. To obtain an expression for the current density J, J = nevav (1.18) we assume that the average velocity vav of the electrons is given by Eq. (1.17), so we obtain 2 ne E (1.19) J= m The dc electrical conductivity 0 is defined by Ohm’s law, J = 0 E (1.20) E 0 (1.21) = where 0 = 1/0 is the resistivity, so from Eq. (1.19) we have 0 = ne2 m (1.22) We infer from the data in Table 1.1 that metals typically have room temperature 6 1 PROPERTIES OF THE NORMAL STATE Figure 1.2 Typical temperature dependence of the conduction electron relaxation time . resistivities between 1 and 100 cm. Semiconductor resistivities have values from 104 to 1015 cm, and for insulators the resistivities are in the range from 1020 to 1028 cm. Collisions can arise in a number of ways, for example, from the motion of atoms away from their regular lattice positions due to thermal vibrational motion—the dominant process in pure metals at high temperatures (e.g., 300 K), or from the presence of impu rities or lattice imperfections, which is the dominant scattering process at low tempera tures (e.g., 4 K). We see from a comparison of the data in columns 11 and 12 of Table1.1 that for metallic elements the collision time decreases with temperature so that the elec trical conductivity also decreases with tem perature, the latter in an approximately linear fashion. The relaxation time has the limit ing temperature dependences ≈ T −3 T −1 T T D (1.23) D as shown in Figure 1.2; here D is the Debye temperature. We will see in Section VI that, for T D , an additional phonon scattering correction factor must be taken into account in the temperature dependence of 0 . V. FREQUENCY DEPENDENT ELECTRICAL CONDUCTIVITY When a harmonically varying electric field E = E0 e−i t acts on the conduction electrons, they are periodically accelerated in the forward and backward directions as E reverses sign every cycle. The conduc tion electrons also undergo random collisions with an average time between the col lisions. The collisions, which interrupt the regular oscillations of the electrons, may be taken into account by adding a frictional damping term p/ to Eq. (1.16), dp p + = −eE dt (1.24) where p = mv is the momentum. The momentum has the same harmonic time vari ation, p = mv0 e−i t . If we substitute this into Eq. (1.24) and solve for the velocity v0 , we obtain v0 = −eE0 · m 1−i (1.25) Comparing this with Eqs. (1.18) and (1.22) with v0 playing the role of vav gives us the ac frequency dependent conductivity: = 0 1−i (1.26) This reduces to the dc case of Eq. (1.22) when the frequency is zero. When 1, many collisions occur during each cycle of the E field, and the aver age electron motion follows the oscillations. When 1, E oscillates more rapidly than the collision frequency, Eq. (1.24) no longer applies, and the electrical conductiv ity becomes predominately imaginary, corre sponding to a reactive impedance. For very high frequencies, the collision rate becomes unimportant and the electron gas behaves like a plasma, an electrically neutral ionized gas in which the negative charges are mobile electrons and the positive charges are fixed in position. Electromagnetic wave phenomena can be described in terms of the frequencydependent dielectric constant , = 0 1 − 2 p 2 (1.27) 7 VII RESISTIVITY where p is the plasma frequency, p = ne2 0 m the more scattering in the forward direc tion tends to dominate, and this introduces another T 2 factor, giving the Bloch T 5 law, 1/2 (1.28) Thus p is the characteristic frequency of the conduction electron plasma below which the dielectric constant is negative—so elec tromagnetic waves cannot propagate—and above which is positive and propagation is possible. As a result metals are opaque when < p and transparent when > p . Some typical plasma frequencies p /2 are listed in Table1.1. The plasma wavelength can also be defined by setting p = 2c/ p . VI. ELECTRON–PHONON INTERACTION We will see later in the text that for most superconductors the mechanism responsible for the formation of Cooper pairs of electrons, which carry the supercurrent, is electron–phonon interaction. In the case of normal metals, thermal vibrations dis turb the periodicity of the lattice and pro duce phonons, and the interactions of these phonons with the conduction electrons cause the latter to scatter. In the high-temperature region T D , the number of phonons in the normal mode is proportional to the temperature (cf. Problem 6). Because of the disturbance of the conduction electron flow caused by the phonons being scattered, the electrical conductivity is inversely propor tional to the temperature, as was mentioned in Section IV. At absolute zero the electrical conduc tivity of metals is due to the presence of impurities, defects, and deviations of the background lattice of positive ions from the condition of perfect periodicity. At finite but low temperatures, T D , we know from Eq. (1.23) that the scattering rate 1/ is pro portional to T 3 . The lower the temperature, ≈ T −5 T D (1.29) which has been observed experimentally for many metals. Standard solid-state physics texts dis cuss Umklapp processes, phonon drag, and other factors that cause deviations from the Bloch T 5 law, but these will not concern us here. The texts mentioned at the end of the chapter should be consulted for further details. VII. RESISTIVITY Electrons moving through a metallic conductor are scattered not only by phonons but also by lattice defects, impurity atoms, and other imperfections in an otherwise perfect lattice. These impurities produce a temperature-independent contribution that places an upper limit on the overall electrical conductivity of the metal. According to Matthiessen’s rule, the conductivities arising from the impurity and phonon contributions add as reciprocals; that is, their respective individual resistivities, 0 and ph , add to give the total resistivity T = 0 + ph T (1.30) We noted earlier that the phonon term ph T is proportional to the temperature T at high temperatures and to T 5 via the Bloch law (1.29) at low temperatures. This means that, above room temperature, the impurity con tribution is negligible, so that the resistivity of metallic elements is roughly proportional to the temperature: T T ≈ 300 K 300 K < T 300 (1.31) 8 1 PROPERTIES OF THE NORMAL STATE Figure 1.3 Temperature dependence of the resistiv ity of a pure 0 and a less pure conductor. Impurities limit the zero temperature resistivity 0 in the latter case. At low temperatures far below the Debye temperature, the Bloch T 5 law applies to give T = 0 + AT 5 T D (1.32) Figure 1.3 shows the temperature depen dence of the resistivity of a high-purity (low 0 ) and a lower-purity (larger 0 ) good con ductor. Typical resistivities at room temperature are 1.5 to 2 cm for very good conductors (e.g., Cu), 10 to 100 for poor conductors, 300 to 10,000 for high-temperature super conducting materials, 104 to 1015 for semi conductors, and 1020 to 1028 for insulators. We see from Eqs. (1.31) and (1.32) that met als have a positive temperature coefficient of resistivity, which is why metals become better conductors at low temperature. In con trast, the resistivity of a semiconductor has a negative temperature coefficient, so that it increases with decreasing temperature. This occurs because of the decrease in the number of mobile charge carriers that results from the return of thermally excited conduction elec trons to their ground states on donor atoms or in the valence band. VIII. THERMAL CONDUCTIVITY When a temperature gradient exists in a metal, the motion of the conduction electrons provides the transport of heat (in the form of kinetic energy) from hotter to cooler regions. In good conductors such as copper and silver this transport involves the same phonon collision processes that are responsi ble for the transport of electric charge. Hence these metals tend to have the same thermal and electrical relaxation times at room tem perature. The ratio Kth /T , in which both thermal Kth J cm−1 s−1 K −1 and electri cal −1 cm−1 ) conductivities occur (see Table1.1 for various metallic elements), has a value which is about twice that predicted by the law of Wiedermann and Franz, Kth 3 = 2 T kB e 2 (1.33) = 111 × 10−8 W/K 2 where the universal constant called the Lorenz number. (1.34) 3 kB /e2 2 is IX. FERMI SURFACE Conduction electrons obey Fermi–Dirac statistics. The corresponding F–D distribu tion function (1.2), written in terms of the energy E, fE = 1 exp E − /kB T + 1 (1.35) is plotted in Fig 1.4a for T = 0 and in Fig 1.4b for T > 0. The chemical potential corresponds, by virtue of the expression ≈ EF = kB TF (1.36) to the Fermi temperature TF , which is typ ically in the neighborhood of 105 K. This means that the distribution function fE is 1 for energies below EF and zero above EF , and assumes intermediate values only in a region kB T wide near EF , as shown in Fig. 1.4b. 9 IX FERMI SURFACE for electrons (a) at T = 0 K, and (b) above 0 K. Figure 1.5 One-dimensional free electron energy band shown occupied out to the first Brillouin zone boundaries at k = ±/a. The electron kinetic energy can be writ ten in several ways, for example, Lx = Ly = Lz = L. Hence the total number of electrons N is given as Figure 1.4 Fermi-Dirac distribution function fE 1 p2 � 2 k2 = Ek = m 2 = 2 2m 2m 2 � = k2 + ky2 + kz2 2m x N =2 (1.37) where p = �k, and the quantization in kspace, sometimes called reciprocal space, means that each Cartesian component of k can assume discrete values, namely 2nx /Lx in the x direction of length Lx , and likewise for the y and z directions of length Ly and Lz , respectively. Here nx is an integer between 1 and Lx /a, where a is the lattice constant; ny and nz are defined analogously. The onedimensional case is sketched in Fig. 1.5. At absolute zero these k-space levels are doubly occupied by electrons of opposite spin up to the Fermi energy EF , EF = � 2 kF2 2m (1.38) as indicated in the figure. Partial occupancy occurs in a narrow region of width kB T at EF , as shown in Fig. 1.4b. For simplic ity we will assume a cubic shape, so that =2 occupied k-space volume k-space volume per electron 4kF3 /3 2/L3 (1.39) The electron density n = N/V = N/L3 at the energy E = EF is n= kF3 1 = 3 2 3 2 2mEF �2 3/2 (1.40) and the density of states DE per unit vol ume, which is obtained from evaluating the derivative dn/dE of this expression (with EF replaced by E), is d 1 nE = DE = dE 2 2 = DEF E/EF 1/2 2m �2 3/2 E 1/2 (1.41) and this is shown sketched in Fig. 1.6. Using Eqs. (1.36) and (1.38), respectively, the den sity of states at the Fermi level can be written in two equivalent ways, 10 1 PROPERTIES OF THE NORMAL STATE states above Tc , this is not the case, and DE has a more complicated expression. It is convenient to express the electron density n and the total electron energy ET in terms of integrals over the density of states: n = DEfEdE ET = DEfEEdE Figure 1.6 Density of states DE of a free electron energy band E = h/ 2 k2 /2m. (1.43) (1.44) The product DEfE that appears in these integrands is shown plotted versus energy in Fig. 1.7a for T = 0 and in Fig. 1.7b for T > 0. X. ENERGY GAP AND EFFECTIVE MASS The free electron kinetic energy of Equation (1.37) is obtained from the plane wave solution = e−i k·r of the Schrödinger equation, �2 − 2 r + Vrr = Er 2m (1.45) Figure 1.7 Energy dependence of occupation of a free electron energy band by electrons (a) at 0 K and (b) for T > 0 K. The products DEfE are calculated from Figs. 1.4 and 1.6. ⎧ 3n ⎪ ⎪ ⎨ 2kB TF DEF = ⎪ ⎪ ⎩ mkF �22 (1.42) for this isotropic case in which energy is independent of direction in k-space (so that the Fermi surface is spherical). In many actual conductors, including the hightemperature superconductors in their normal with the potential Vr set equal to zero. When a potential, such as that shown in Fig. 1.1, is included in the Schrödinger equa tion, the free-electron energy parabola of Fig. 1.5 develops energy gaps, as shown in Fig 1.8. These gaps appear at boundaries k = ±n/a of the unit cell in k-space, called the first Brillouin zone, and of successively higher Brillouin zones, as shown. The ener gies levels are closer near the gap, which means that the density of states DE is larger there (see Figs. 1.9 and 1.10). For weak potentials, V EF , the density of states is close to its free-electron form away from the gap, as indicated in the figures. The number of points in k-space remains the same, that is, it is conserved, when the gap forms; it is the density D(E) that changes. 11 XI ELECTRONIC SPECIFIC HEAT Figure 1.10 Energy dependence of the density of states DE corresponding to the case of Fig. 1.9 in the presence of a gap. Figure 1.8 A one-dimensional free electron energy band shown perturbed by the presence of a weak peri odic potential Vx h/ 2 2 /2ma2 . The gaps open up at the zone boundaries k = ±n/a, where n = 1 2 3 . function of k, which takes into account bend ing of the free-electron parabola near the gap. It can be evaluated from the second deriva tive of Ek with respect to k: 1 1 = 2 m∗ � d 2 Ek dk2 (1.47) EF This differentiation can be carried out if the shapes of the energy bands near the Fermi level are known. The density of states DEF also deviates from the free-electron value near the gap, being proportional to the effec tive mass m∗ , DEF = Figure 1.9 Spacing of free electron energy levels in the absence of a gap (left) and in the presence of a small gap (right) of the type shown in Fig. 1.8. The increase of D(E) near the gap is indicated. m ∗ kF �22 (1.48) as may be inferred from Eq. (1.42). There is a class of materials called heavy fermion compounds whose effective conduc tion electron mass can exceed 100 free elec tron masses. Superconductors of this type are discussed in Sect. 9.II. XI. ELECTRONIC SPECIFIC HEAT If the kinetic energy near an energy gap is written in the form, Ek = � 2 k2 2m∗ (1.46) the effective mass m∗ k, which is different from the free-electron value m, becomes a The specific heat C of a material is defined as the change in internal energy U brought about by a change in temperature dU C= (1.49) dT v 12 1 PROPERTIES OF THE NORMAL STATE We will not make a distinction between the specific heat at constant volume and the spe cific heat at constant pressure because for solids these two properties are virtually indis tinguishable. Ordinarily, the specific heat is measured by determining the heat input dQ needed to raise the temperature of the mate rial by an amount dT , dQ = CdT (1.50) In this section, we will deduce the contribu tion of the conduction electrons to the spe cific heat, and in the next section we will provide the lattice vibration or phonon par ticipation. The former is only appreciable at low temperatures while the latter dominates at room temperature. The conduction electron contribution Ce to the specific heat is given by the deriva tive dE /dT . The integrand of Eq. (1.44) is somewhat complicated, so differentiation is not easily done. Solid-state physics texts carry out an approximate evaluation of this integral, to give Ce = T (1.51) where the normal-state electron specific heat constant , sometimes called the Sommerfeld constant, is given as 2 = (1.52) DEF kB2 3 This provides a way to experimentally evalu ate the density of states at the Fermi level. To estimate the electronic specific heat per mole we set n = NA and make use of Eq. (1.42) to obtain the free-electron expression ˙0 = 2R 2TF (1.53) where R = NA kB is the gas constant. This result agrees (within a factor of 2) with experiment for many metallic elements. A more general expression for is obtained by applying DEF from Eq. (1.48) instead of the free-electron value of (1.42). This gives ∗ m (1.54) = 0 m where 0 is the Sommerfeld factor (1.53) for a free electron mass. This expression will be discussed further in Chapter 9, Section II, which treats heavy fermion compounds that have very large effective masses. XII. PHONON SPECIFIC HEAT The atoms in a solid are in a state of con tinuous vibration. These vibrations, called phonon modes, constitute the main contri bution to the specific heat. In models of a vibrating solid nearby atoms are depicted as being bonded together by springs. For the one-dimensional diatomic case of alternating small and large atoms, of masses ms and m1 , respectively, there are low-frequency modes called acoustic (A) modes, in which the two types of atoms vibrate in phase, and highfrequency modes, called optical (O) modes, in which they vibrate out of phase. The vibra tions can also be longitudinal, i.e., along the line of atoms, or transverse, i.e., perpendicu lar to this line, as explained in typical solidstate physics texts. In practice, crystals are three-dimensional and the situation is more complicated, but these four types of modes are observed. Figure 1.11 presents a typical wave vector dependence of their frequencies. It is convenient to describe these vibra tions in k-space, with each vibrational mode having energy E = � . The Planck distribu tion function applies, fE = 1 expE/kB T − 1 (1.55) where the minus one in the denominator indi cates that only the ground vibrational level is occupied at absolute zero. There is no chem ical potential because the number of phonons 13 XII PHONON SPECIFIC HEAT The vibration density of states per unit volume Dph = dn/d is Dph = 2 2 2 3 (1.59) and the total vibrational energy Eph is obtained by integrating the phonon mode energy � times the density of states (1.59) over the distribution function (1.55) (cf. de Wette et al., 1990) D 2 � d Eph = (1.60) 2 3 � 2 e /kB T − 1 0 Figure 1.11 Typical dependence of energy E on the wave vector k for transverse (T), longitudinal (L), opti cal (O), and acoustic (A) vibrational modes of a crystal. The vibrational or phonon specific heat Cph = dEph /dT is found by differentiating Eq. (1.60) with respect to the temperature, is not conserved. The total number of acous tic vibrational modes per unit volume N is calculated as in Eq. (1.39) with the factor 2 omitted since there is no spin, N= = occupied k-space volume k-space volume per atom 4kD3 /3 2/L3 Cph = 9R 3 where L is the volume of the crystal and kD is the maximum permissible value of k. In the Debye model, the sound velocity is assumed to be isotropic x = y = z and independent of frequency, (1.61) and Fig. 1.12 compares this temperature dependence with experimental data for Cu and Pb. The molar specific heat has the respective low- and high-temperature limits Cph = 12 4 T 3 R 5 D Cph = 3R T T D k (1.57) Writing D = kD and substituting this expression in Eq. (1.56) gives, for the density of modes n = N/L3 , 3 D 2 6 3 (1.58) where the maximum permissible frequency D is called the Debye frequency. D (1.62b) far below and far above the Debye tempera ture D n= x4 ex dx ex − 12 (1.62a) 3 = D 0 D (1.56) T = h/ D kB (1.63) and the former limiting behavior is shown by the dashed curve in Fig. 1.12. We also see from the figure that at their superconduct ing transition temperatures Tc the element Pb and the compound LaSrCuO are in the T 3 region, while the compound YBaCuO is significantly above it. Since at low temperatures a metal has an electronic specific heat term (1.51) that is lin ear in temperature and a phonon term (1.62a) 14 1 PROPERTIES OF THE NORMAL STATE Figure 1.12 Temperature dependence of the phonon-specific heat in the Debye model compared with experimental data for Cu and Pb. The low-temperature T 3 approximation is indicated by a dashed curve. The locations of the three superconductors Pb, La0925 Sr 0075 2 CuO4 , and YBa2 Cu3 O7− at their transition temperature Tc on the Debye curve are indicated (it is assumed that they satisfy Eq. (1.61)). that is cubic in T , the two can be experimen tally distinguished by plotting Cexp /T versus T 2 , where Cexp = + AT 2 T (1.64) as shown in Fig. 1.13. The slope gives the phonon part A and the intercept at T = 0 gives the electronic coefficient Materials with a two-level system in which both the ground state and the excited state are degenerate can exhibit an extra contribution to the specific heat, called the Schottky term. This contribution depends on the energy spacing ESch between the ground and excited states. When ESch kB T , the Schottky term has the form aT −2 (Crow and Ong, 1990). The resulting upturn in the observed specific heat at low temperatures, sometimes called the Schottky anomaly, has been observed in some superconductors. XIII. ELECTROMAGNETIC FIELDS Figure 1.13 Typical plot of Cexp /T versus T 2 for a conductor. The phonon contribution is given by the slope of the line, and the free electron contribution is given by the intercept obtained by the extrapolation T → 0. Before discussing the magnetic proper ties of conductors it will be helpful to say a few words about electromagnetic fields, and to write down for later reference several of the basic equations of electromagnetism. These equations include the two homo geneous Maxwell’s equations · B = 0 (1.65) 15 XIV BOUNDARY CONDITIONS ×E+ B = 0 t (1.66) and the two inhomogeneous equations · D = ×H = J+ (1.67) D t (1.68) where and J are referred to as the free charge density and the free current density, respectively. The two densities are said to be ‘free’ because neither of them arises from the reaction of the medium to the presence of externally applied fields, charges, or cur rents. The B and H fields and the E and D fields, respectively, are related through the expressions B = H = 0 H + M (1.69) D = E = 0 E + P (1.70) where the medium is characterized by its per meability and its permittivity , and 0 and 0 are the corresponding free space values. These, of course, are SI formulae. When cgs units are used, 0 = 0 = 1 and the factor 4 must be inserted in front of M and P. The fundamental electric (E) and mag netic (B) fields are the fields that enter into the Lorentz force law F = qE + v × B (1.71) for the force F acting on a charge q moving at velocity v in a region containing the fields E and B. Thus B and E are the macroscopi cally measured magnetic and electric fields, respectively. Sometimes B is called the mag netic induction or the magnetic flux density. It is convenient to write Eq. (1.68) in terms of the fundamental field B using Eq. (1.69) × B = 0 J + × M + 0 D (1.72) t where the displacement current term D/t is ordinarily negligible for conductors and superconductors and so is often omitted. The reaction of the medium to an applied mag netic field produces the magnetization cur rent density � × M which can be quite large in superconductors. XIV. BOUNDARY CONDITIONS We have been discussing the relation ship between the B and H fields within a medium or sample of permeability . If the medium is homogeneous, both and M can be constant throughout, and Eq. (1.69), with B = H, applies. But what happens to the fields when two media of respective perme abilities and are in contact? At the interface between the media the B and H fields in one medium will be related to the B and H fields in the other medium through the two boundary conditions illustrated in Fig. 1.14, namely: 1. The components of B normal to the inter face are continuous across the boundary: B⊥ = B⊥ (1.73) 2. The components of H tangential to the interface are continuous across the boundary: H = H (1.74) Figure 1.14 Boundary conditions for the compo nents of the B and H magnetic field vectors perpendicu lar to and parallel to the interface between regions with different permeabilities. The figure is drawn for the case = 2 . 16 1 PROPERTIES OF THE NORMAL STATE If there is a surface current density Jsurf present at the interface, the second condition must be modified to take this into account, n̂ × H − H = Jsurf (1.75) where n is a unit vector pointing from the double primed ( ) to the primed region, as indicated in Fig. 1.14, and the surface current density Jsurf , which has the units ampere per meter, is perpendicular to the field direction. When H and H are measured along the surface parallel to each other, Eq. (1.75) can be written in scalar form: H − H = Jsurf (1.76) In like manner, for the electric field case the normal components of D and the tangential components of E are continuous across an interface, and the condition on D must be modified when surface charges are present. XV. MAGNETIC SUSCEPTIBILITY It is convenient to express Eq. (1.69) in terms of the dimensionless magnetic suscep tibility , = M H (1.77) to give B = 0 H1 + SI SI units (1.78a) B = H1 + 4cgs cgs units (1.78b) The susceptibility is slightly nega tive for diamagnets, slightly positive for paramagnets, and strongly positive for ferromagnets. Elements that are good conductors have small susceptibilities, some times slightly negative (e.g., Cu) and some times slightly positive (e.g., Na), as may be seen from Table 1.2. Nonmagnetic inorganic compounds are weakly diamagnetic (e.g., NaCl), while magnetic compounds con taining transition ions can be much more strongly paramagnetic (e.g., CuCl2 ). The magnetization in Eq. (1.77) is the magnetic moment per unit volume, and the susceptibility defined by this expres sion is dimensionless. The susceptibility of a material doped with magnetic ions is propor tional to the concentration of the ions in the material. In general, researchers who study the properties of these materials are more interested in the properties of the ions them selves than in the properties of the material containing the ions. To take this into account it is customary to use molar susceptibilities M , which in the SI system have the units m3 per mole. Table 1.2 cgs Molar Susceptibility cgs and Dimensionless SI Volume Susceptibility of Several Materials Material MW g/mole Density g/cm3 �cgs cm3 /mole � — Free space Na NaCl Cu CuCl2 Fe alloy Perfect SC — 22.99 58.52 63.54 134.6 ≈ 60 — 0.0 0.97 2.165 8.92 3.386 7–8 — 0 16 × 10−5 −303 × 10−5 −546 × 10−6 108 × 10−3 103 –104 — 0 848 × 10−6 −141 × 10−5 −963 × 10−6 341 × 10−4 103 –104 −1 17 XV MAGNETIC SUSCEPTIBILITY It is shown in solid-state physics texts (e.g., Ashcroft and Mermin, 1976; Burns, 1985; Kittel, 1976) that a material containing paramagnetic ions with magnetic moments that become magnetically ordered at low temperatures has a high-temperature mag netic susceptibility that obeys the Curie– Weiss Law: M = n2 3kB T − C = T − (1.79a) (1.79b) where n is the concentration of paramag netic ions and C is the Curie constant. has a pos The Curie–Weiss temperature itive sign when the low-temperature align ment is ferromagnetic and a negative sign when it is antiferromagnetic. Figure 1.15 shows the temperature dependence of M for the latter case, in which the denom inator becomes T + . The temperature TN at which antiferromagnetic alignment occurs is referred to as the Néel tempera ture, and typically TN = . When = 0, Eq. (1.79) is called the Curie law. For a rare earth ion with angular momen tum J � we can write 2 = g 2 2B JJ + 1 (1.80) where J = L + S is the sum of the orbital L and spin S contributions, B = e�/2m is the Bohr magneton, and the dimensionless Landé g factor is g= 3 SS + 1 − LL + 1 + 2 2JJ + 1 (1.81) For a first transition series ion, the orbital angular momentum L� is quenched, which means that it is uncoupled from the spin angular momentum and becomes quantized along the crystalline electric field direction. Only the spin part of the angular momentum contributes appreciably to the susceptibility, to give the so-called spin-only result 2 = g 2 2B SS + 1 (1.82) where for most of these ions g ≈ 2. For conduction electrons the only con tribution to the susceptibility comes from the electrons at the Fermi surface. Using an argument similar to that which we employed for the electronic specific heat in Section XI we can obtain the temperature-independent expression for the susceptibility in terms of the electronic density of states, = 2B DEF (1.83) which is known as the Pauli susceptibility. For a free electron gas of density n we sub stitute the first expression for DEF from Eq. (1.42) in Eq. (1.83) to obtain, for a mole, M = Figure 1.15 Magnetic susceptibility of a material that is paramagnetic above the Néel transition temper ature TN and antiferromagnetic with axial symmetry below the transition. The extrapolation of the param agnetic curve below T = 0 provides the Curie-Weiss temperature . 3n2B 2kB TF (1.84) For alkali metals the measured Pauli sus ceptibility decreases with increasing atomic number from Li to Cs with a typical value ≈ 1 × 10−6 . The corresponding free-electron 18 1 PROPERTIES OF THE NORMAL STATE values from Eq. (1.84) are about twice as high as their experimental counterparts, and come much closer to experiment when electron–electron interactions are taken into account. For very low temperatures, high magnetic fields, and very pure materials there is an additional dia-magnetic correction term Landau , called Landau diamagnetism, which arise from the orbital electronic inter action with the magnetic field. For the freeelectron this correction has the value Landau = − 13 Pauli (1.85) In preparing Table 1.2 the dimensionless SI values of listed in column 5 were cal culated from known values of the molar cgs M susceptibility cgs , which has the units cm3 per mole, using the expression m = 4 M (1.86) MW cgs where m is the density in g per cm3 and MW is the molecular mass in g per mole. Some authors report per unit mass susceptibility g data in emu/g, which we are calling cgs . The latter is related to the dimension-less through the expression g = 4m cgs (1.87) The ratio of Eq. (1.52) to Eq. (1.83) gives the free-electron expression M = 1 3 kB B 2 (1.88) where M is the susceptibility arising from the conduction electrons. An experimen tal determination of this ratio provides a test of the applicability of the free-electron approximation. This section has been concerned with dc susceptibility. Important information can also be obtained by using an ac applied field B0 cos t to determine ac = + i , which has real part , called dispersion, in phase with the applied field, and an imaginary lossy part , called absorption, which is out of phase with the field (Khode and Couach, 1992). D. C. Johnston (1991) reviewed nor mal state magnetization of the cuprates. XVI. HALL EFFECT The Hall effect employs crossed electric and magnetic fields to obtain information on the sign and mobility of the charge carriers. The experimental arrangement illustrated in Fig. 1.16 shows a magnetic field B0 applied in the z direction perpendicular to a slab and a battery that establishes an electric field Ey in the y direction that causes a current I = JA to flow, where J = ne is the current density. The Lorentz force F = qv × B0 (1.89) of the magnetic field on each moving charge q is in the positive x direction for both posi tive and negative charge carriers, as shown in Figs. 1.17a and 1.17b, respectively. This causes a charge separation to build up on the sides of the plate, which produces an elec tric field Ex perpendicular to the directions of the current y and magnetic z fields. The induced electric field is in the negative x direction for positive q, and in the posi tive x direction for negative q, as shown in Figs. 1.17c and 1.17d, respectively. After the charge separation has built up, the elec tric force qEx balances the magnetic force qv × B0 , qEx = qv × B0 (1.90) and the charge carriers q proceed along the wire undeflected. The Hall coefficient RH is defined as a ratio, RH = Ex J y Bz (1.91) XVI HALL EFFECT Figure 1.16 Experimental arrangement for Hall effect measurements showing an electrical current I passing through a flat plate of width d and thickness a in a uniform transverse magnetic field Bz . The voltage drop V2 − V1 along the plate, the voltage difference Vx across the plate, and the electric field Ex across the plate are indicated. The figure is drawn for negative charge carriers (electrons). Figure 1.17 Charge carrier motion and transverse electric field direction for the Hall effect experimental arrangement of Fig. 1.16. Positive charge carriers deflect as indicated in (a) and produce the transverse electric field Ex shown in (c). The corresponding deflection and resulting electric field for negative charge carriers are sketched in (b) and (d), respectively. 19 20 1 PROPERTIES OF THE NORMAL STATE Substituting the expressions for J and Ex from Eqs. (1.18) and (1.90) in Eq. (1.91) we obtain for holes q = e and electrons q = −e, respectively, RH = 1 ne RH = − holes 1 ne (1.92a) electrons = H Ex Ey (1.93) Sometimes the dimensionless Hall number is reported, Hall # = V0 RH e (1.94) where V0 is the volume per chemical formula unit. Thus the Hall effect distinguishes elec trons from holes, and when all of the charge carriers are the same this experiment pro vides the charge density n. When both posi tive and negative charge carriers are present, partial (or total) cancellation of their Hall effects occurs. The mobility is the charge carrier drift velocity per unit electric field, = av E RH Ey J (1.97) In the presence of a magnetic field, this expression is written m = Ey J (1.98) where m is called the transverse magnetoresistivity. There is also a longitudinal mag netoresistivity defined when E and B0 are parallel. For the present case the resistiv ity does not depend on the applied field, so m = . For very high magnetic fields m and can be different. In the supercon ducting state m arises from the movement of quantized magnetic flux lines, called vor tices, so that it can be called the flux flow resistivity ff . Finally, the Hall effect resis tivity xy (Ong, 1991) is defined by xy = Ex J (1.99) FURTHER READING Most of the material in this chapter may be found in standard textbooks on solid state physics (e.g., Ashcroft and Mermin, 1976; Burns, 1985; Kittel, 1996). (1.95) and with the aid of Eqs. (1.18), (1.21), and (1.92) we can write H = = (1.92b) where the sign of RH is determined by the sign of the charges. The Hall angle H is defined by tan the direction of current flow to the current density, (1.96) where the Hall mobility H is the mobility determined by a Hall effect measurement. It is a valid measure of the mobility (1.95) if only one type of charge carrier is present. By Ohm’s law (1.21) the resistivity is the ratio of the applied electric field in PROBLEMS 1. Show that Eq. (1.61) for the phonon specific heat has the low- and hightemperature limits (1.62a) and (1.62b), respectively. 2. Aluminum has a magnetic susceptibil ity +165 × 10−6 cgs, and niobium, 195 × 10−6 cgs. Express these in dimensionless SI units. From these values estimate the density of states and the electronic spe cific heat constant for each element. PROBLEMS 3. Copper at room temperature has 847 × 1022 conduction electrons/cm3 , a Fermi energy of 7.0 eV, and = 27 × 10−14 s. Calculate its Hall coefficient, average conduction electron velocity in an electric field of 200 V/cm, electrical resistivity, and mean free path. 4. Calculate the London penetration depth, resistivity, plasma frequency, and density of states of copper at room temperature. 5. It was mentioned in Section 1. II that the chemical potential is the energy required to remove one electron from a Fermi gas under the conditions of con stant volume and constant entropy. Use a thermodynamic argument to prove this assertion, and also show that equals the change in the Gibbs free energy when one 21 electron is removed from the Fermi gas under the conditions of constant tempera ture and constant pressure. 6. Show that well above the Debye temper ature the number of phonons in a normal mode of vibration is proportional to the temperature. 7. For the two-dimensional square lattice draw the third Brillouin zone in (a) the extended zone scheme and (b) the reduced zone scheme in which the third zone is mapped into the first zone. Show where each segment in the extended scheme goes in the first zone. Draw constant energy lines for = 20 , 30 , 40 , 50 . Sketch the Fermi surface for F = 450 . Indicate the electron-like and hole-like regions. This page intentionally left blank 2 Phenomenon of Superconductivity I. INTRODUCTION A perfect superconductor is a material that exhibits two characteristic properties, namely zero electrical resistance and perfect diamagnetism, when it is cooled below a particular temperature Tc , called the critical temperature. At higher temperatures it is a normal metal, and ordinarily is not a very good conductor. For example, lead, tantalum, and tin become superconductors, while cop per, silver, and gold, which are much better conductors, do not super-conduct. In the nor mal state some super-conducting metals are weakly diamagnetic and some are paramag netic. Below Tc they exhibit perfect electrical conductivity and also perfect or quite pro nounced diamagnetism. Perfect diamagnetism, the second charac teristic property, means that a superconduct ing material does not permit an externally applied magnetic field to penetrate into its interior. Those superconductors that totally exclude an applied magnetic flux are known as Type I superconductors, and they constitute the subject matter of this chapter. Other super conductors, called Type II superconductors, are also perfect conductors of electricity, but their magnetic properties are more complex. They totally exclude magnetic flux when the applied magnetic field is low, but only partially exclude it when the applied field is higher. In the region of higher magnetic fields their diamagnetism is not perfect, but rather of a mixed type. The basic properties of these mixed magnetism superconductors are described in Chapters 5 and 12. 23 24 II. BRIEF HISTORY In 1908, H. Kamerlingh Onnes initi ated the field of low-temperature physics by liquifying helium in his laboratory at Leiden. Three years later he found that below 4.15 K of the dc resistance of mercury dropped to zero (Onnes, 1911). With that finding the field of superconductivity was born. The next year Onnes discovered that the application of a sufficiently strong axial magnetic field restored the resistance to its normal value. One year later, in 1913, the element lead was found to be superconducting at 7.2 K (Onnes, 1913). Another 17 years were to pass before this record was surpassed, by the ele ment niobium Tc = 92 K (vide Ginzburg and Kitzhnits, 1977, p. 2). A considerable amount of time went by before physicists became aware of the second distinguishing characteristic of a superconductor—namely, its perfect diamag netism. In 1933, Meissner and Ochsen feld found that when a sphere is cooled below its transition temperature in a magnetic field, it excludes the magnetic flux. The report of the Meissner effect led the London brothers, Fritz and Heinz, to propose equations that explain this effect and predict how far a static external magnetic field can penetrate into a super conductor. The next theoretical advance came in 1950 with the theory of Ginzburg and Landau, which described superconduc tity in terms of an order parameter and provided a derivation for the London equa tions. Both of these theories are macro scopic in character and will be described in Chapter 6. In the same year it was predicted theoretically by H. Fröhlich (1950) that the transition temperature would decrease as the average isotopic mass increased. This effect, called the isotope effect, was observed experimentally the same year (Maxwell, 1950; Reynolds et al., 1950). 2 PHENOMENON OF SUPERCONDUCTIVITY The isotope effect provided support for the electron–phonon interaction mechanism of superconductivity. Our present theoretical understanding of the nature of superconductivity is based on the BCS microscopic theory proposed by J. Bardeen, L. Cooper, and J. R. Schrieffer in 1957 (we will describe it in Chapter 7). In this theory it is assumed that bound elec tron pairs that carry the super current are formed and that an energy gap between the normal and superconductive states is cre ated. The Ginzburg–Landau (1950) and Lon don (1950) results fit well into the BCS formalism. Much of the present theoretical debate centers around how well the BCS the ory explains the properties of the new hightemperature superconductors. Alloys and compounds have been exten sively studied, especially the so-called A15 compounds, such as Nb3 Sn, Nb3 Ga, and Nb3 Ge, which held the record for the highest transition temperatures from 1954 to 1986, as shown in Table 2.1. Table 2.1 Superconducting Transition Temperature Records through the Yearsa Material Tc K Year Hg Pb Nb NbN096 Nb3 Sn Nb3 Al 3 Ge 1 41 72 92 152 181 20–21 1911 1913 1930 1950 1954 1966 203 232 30–35 52 95 110 125 131 133 155 133 164 1971 1973 1986 1986 1987 1988 1988 1993 1993 1993 1994 1994 4 4 Nb3 Ga Nb3 Ge Bax La5−x Cu5 Oy La09 Ba01 2 CuO4− at 1 GPa YBa2 Cu3 O7− Bi2 Sr 2 Ca2 Cu3 O10 Tl2 Ba2 Ca2 Cu3 O10 Tl2 Ba2 Ca2 Cu3 O10 at 7 GPa HgBa2 Ca2 Cu3 O8+ HgBa2 Ca2 Cu3 O8+ at 25 GPa Hg08 Pb02 Ba2 Ca2 Cu3 Ox HgBa2 Ca2 Cu3 O8+ at 30 GPa a cf. Ginzburg and Kirzhnits, 1977. 25 II BRIEF HISTORY Many other types of compounds have been studied in recent years, particularly the socalled heavy fermion systems in which the superconducting electrons have high effec tive masses of 100me or more. Organic superconductors have shown a dramatic rise in transition temperatures during the past decade. On April 17, 1986, a brief article, enti tled “Possible High Tc Superconductivity in the Ba–La–Cu–O System,” written by J. G. Bednorz and K. A. Müller was received by the Zeitschrift für Physik, initiating the era of high-temperature superconductivity. When the article appeared in print later that year, it met with initial skepticism. Sharp drops in resistance attributed to “high-Tc ” superconductivity had appeared from time to time over the years, but when exam ined they had always failed to show the required diamagnetic response or were oth erwise unsubstantiated. It was only when a Japanese group (Uchida et al., 1987) and Chu’s group in the United States (Chu et al., 1987b) reproduced the original results that the results found by Bednorz and Müller began to be taken seriously. Soon many other researchers became active, and the recorded transition temperature began a rapid rise. By the beginning of 1987, scientists had fabricated the lanthanum compound, which went superconducting at close to 40 K at atmospheric pressure (Cava et al., 1987; Tarascon et al., 1987c) and at up to 52 K under high pressure (Chu et al., 1987a). Soon thereafter, the yttrium–barium system, which went superconducting in the low 90s (Chu et al., 1988a; Zhao et al., 1987), was dis covered. Early in 1988, superconductivity reached 110 K with the discovery of BiSrCaCuO (Chu et al., 1988b; Maeda et al., 1988; Michel et al., 1987), and then the 120–125 K range with TIBaCaCuO (Hazen et al., 1988; Sheng and Herman, 1988; Sheng et al., 1988). More recently, Berkley et al. (1993) reported Tc = 1318 K for Tl2 Ba2 Ca2 Cu3 O10−x at a pressure of 7 GPa. Several researchers have reported Tc above 130 K for the Hg series of compounds HgBa2 Can Cun+1 O2n+4 with n = 1 2, sometimes with Pb doping for Hg (Chu et al., 1993a; Iqbal et al., 1994; Schilling et al., 1993, 1994a). The transition temperature of the Hg compounds increases with pressure (Chu, 1994; Klehe et al., 1992, 1994; Rabinowitz and McMullen, 1994) in the manner shown in Fig. 2.1a (Gao et al., 1994) and onset Tc values in the 150 K range are found for pressures above 10 GPa (Chu et al., 1993b, Ihara et al., 1993). We see from Fig. 2.1b that the transitions are broad, with midpoint Tc located 7 or 8 K below the onset, and the zero resistivity point comes much lower still (Gao et al., 1994). This rapid pace of change and improve ment in superconductors exceeds that of ear lier decades, as the data listed in Table 2.1 and plotted in Fig. 2.2 demonstrate. For 56 years the element niobium and its com pounds had dominated the field of supercon ductivity. In addition to providing the highest Tc values, niobium compounds such as NbTi and Nb3 Sn are also optimal magnet mate rials: for NbTi, Bc2 = 10 T and for Nb3 Sn, Bc2 = 22 T at 4.2 K, where Bc2 is the uppercritical field of a Type II superconductor, in the sense that it sets a limit on the magnetic field attainable by a magnet; thus applica tion of an applied magnetic field in excess of Bc2 drives a superconductor normal. The period from 1930 to 1986 can be called the Niobium Era of superconductivity. The new period that began in 1986 might become the Copper Oxide Era because, thus far, the pres ence of copper and oxygen has, with rare exceptions, been found essential for Tc above 40 K. It is also interesting to observe that Hg was the first known superconductor, and now a century later mercury compounds have become the best! 26 2 PHENOMENON OF SUPERCONDUCTIVITY Figure 2.1 Effect of pressure on the transition temperature of the superconductor HgBa2 Ca2 Cu3 O8+ showing (a) pressure dependence of the onset (upper curve), midpoint (middle curve), and final off-set (lower curve) values of Tc , and (b) temperature dependence of the resistivity derivative dp/dT at 1.5 (1), 4 (2), 7 (3), and 18.5 GPa (6). Definitions of Tco onset, Tcm midpoint, and Tcf final offset that are plotted in (a) are given in (b) (Gao et al., 1993). 27 III RESISTIVITY A. Resistivity above Tc Figure 2.2 Increase in the superconducting transition temperature with time. A linear extrapolation of the data before 1986 predicts that room temperature would be reached in about 1000 years. From left to right X = Sn Al075 Ge025 , Ga, and Ge for the data points of the A15 compound Nb3 X (Adapted from Fig. I-1, Poole et al., 1988). III. RESISTIVITY Before beginning the discussion of super currents, we will examine the resistivity of superconducting materials in their normal state above the transition temperature Tc ; we will then make some comments on the drop to zero resistance at Tc ; finally, we will describe the measurements that have set upper limits on resistivity below Tc . In Chapter 1, Section VII, we explained, and now we illustrate in Figs. 2.3–2.6, how the resistivity of a typical conductor depends linearly on temperature at high temperatures and obeys the T 5 Bloch law at low temper atures. Classical or low-temperature super conductors are in the Bloch law region if the transition temperature is low enough, as illustrated in Fig. 2.3a. High-temperature superconductors have transition temperatures that are in the linear region, corresponding to the resistivity plot of Fig. 2.3b. However, the situation is actually more complicated because the resistivity of single crystals of high-temperature superconductors is strongly anisotropic, as we will show later. Several theoretical treatments of the resistivity of cuprates have appeared (e.g., Griessen, 1990; Micnas et al., 1987; Song and Gaines, 1991; Wu et al., 1989; Zeyhe, 1991). Good conductors such as copper and silver have room temperature resistivities of about 15 cm, whereas at liquid nitrogen temperatures the resistivity typ ically decreases by a factor in the range 3–8, as shown by the data in Table 1.1. The elemental superconductors, such as Nd, Pb, and Sn, have room temperature resistivities a factor of 10 greater than good conductors. The metallic elements Ba, Bi, Figure 2.3 Abrupt drop of the resistivity to zero at the superconducting transition temperature Tc (a) for a low-temperature superconductor in the Bloch T 5 region and (b) for a high-temperature superconductor in the linear region. 28 2 PHENOMENON OF SUPERCONDUCTIVITY La, Sr, Tl, and Y, which are also present in oxide superconductors, have room temper ature resistivities 10 to 70 times that of Cu. The copper-oxide superconductors have even higher room temperature resistivities, more than three orders of magnitude greater than that of metallic copper, which puts them within a factor of 3 or 4 of the semiconduc tor range, as shown by the data in Table 2.2. The resistivity of these materials above Tc decreases more or less linearly with decreas ing temperature down to the neighborhood of Tc , with a drop by a factor of 2 or 3 from room temperature to this point, as shown in Fig. B. and by the data in Table 2.2. Figure 2.5 shows that the linearity extends far above room temperature, especially for the lanthanum compound (Gurvitch and Fiory, 1987a, b, c; Gurvitch et al., 1988). It has been linked to the two-dimensional character of electron transport (Micnas et al., 1990). We see from the figure that YBa2 Cu3 O7− begins to deviate from linearity at about 600– 700 K, near the orthorhombic-to-tetragonal phase transformation (cf. Chapter 8, Section IV.D) where it changes from a metal lic material below the transition to a semi conductor above. Heating causes a loss of oxygen, as shown in Fig. 2.6 which presents the dependence of resistivity on the oxy gen partial pressure (Grader et al., 1987). The temperature dependence of resistivity has been related to the loss of oxygen [cf. Eq. (X-1) from Poole et al., 1988; cf. Chaki and Rubinstein, 1987; Fiory et al., 1987]. The resistivity of poor metals at high temperatures tends to saturate to a temperature-independent value when the mean free path l approaches the wavelength F = 2 /kF associated with the Fermi level, where kF is the Fermi wave vector. The Ioffe–Regel criterion for the onset of this saturation is kF l ≈ 1. The quantity kF l for YBa2 Cu3 O7− has been estimated to have a value of 30 for T = 100 K (Hagen et al., 1988) and 3 for T = 1000 K (Crow and Ong, 1990). These considerations, together with the curves in Fig. 2.5, indicate that, in practice, the Ioffe–Regel criterion does not cause the resistivity to saturate in hightemperature superconductors. The A15 com pound V3 Si, whose crystal structure is stable up to 1950 C, does exhibit saturation in its resistivity-versus-temperature plot. B. Resistivity Anisotropy The resistivity of YBa2 Cu3 O7− is around two orders of magnitude greater along the c-axis than parallel to the a, b-plane; thus c / ab ≈ 100 and for Bi2+x Sr 2−y CuO6+ ≈ 105 (Fiory et al., 1989). The tem perature dependence of these resistivities, measured by the method described in the fol lowing section, exhibits a peak near Tc in the case of c , and this is shown in Fig. 2.7. When the data are fitted to the expressions (Anderson and Zou, 1988) c / ab Aab + Bab T T Ac + Bc T c = T ab = (2.1) (2.2) by plotting ab T and c T from the data of Fig. 2.7 versus T 2 , a good fit is obtained, as shown in Fig. 2.8. The angular dependence of the resistivity is found to obey the expression (Wu et al., 1991b) = ab sin2 + c cos2 (2.3) where is the angle of the current direction relative to the c axis. Typical measured resistivities of poly crystalline samples are much closer to the inplane values. The anisotropy ratio c / ab ≈ 100 is so large that the current encounters less resistance when it follows a longer path Table 2.2 Resistivity Data on Superconducting Single Crystals Slightly above Tc and near Room Temperature. The Slopes /T Are Averages for the Typical Range from 150 K to 290 K. (Earlier data on mostly polycrystalline samples are given in Table X-1 of Poole et al. 1988a ) Material T K �ab �� cm �c m� cm �c /�ab Re 50 08 00005 06 Re 275 175 0013 07 TaS2 2H–TaSe2 ��ab /�T �� cm/K ��c /�T m� cm/K 0075 0055 Volkenshteyn et al. (1978) Volkenshteyn et al. (1978) 450 4 Reference Wattamaniuk et al. (1975) 1200 Martin et al. (1990) Pfalzgraf and Spreckels (1987) K3 C60 thin filme 290 25 m cm Palstra et al. (1992) 19 La0925 Sr0075 2 CuO4 50 2500 La0925 Sr0075 2 CuO4 290 5000 Nd0925 Ce0075 2 CuO4 30 1700 500 300 Nd0925 Ce0075 2 CuO4 273 4800 1300 270 YBa2 Cu3 O7− 290 ∼ 380 ∼ 15 ∼ 45 YBa2 Cu3 O7− 100 ∼ 180 ∼ 15 ∼ 90 Bi2 Sr2 CuO6± 25 90 14000 16 × 105 Bi2 Sr2 CuO6± 290 275 6000 22 × 104 Bi2 Sr22 CaCu2 O8 100 55b 5200 95 × 104 Bi2 Sr22 CaCu2 O8 300 c 8880 59 × 104 T12 Ba2 CuO6 110 900 Mukaida et al. (1990) T12 Ba2 CaCu2 O8 110 3500 Mukaida et al. (1990) a b 150 13 Preyer et al. (1991) Preyer et al. (1991) Typical semiconductors range from 104 to 1015 cm and insulators from 1020 to 1028 cm. Averages of a = 60 b = 50 cm at 100 K, and a = 180 b = 120 cm at 300 K. 19 37 20 Crusellas et al. (1991) Crusellas et al. (1991) averages ∼ 08 09 ∼ 02 −6 averages Martin et al. (1990) Martin et al. (1990) 046 15 Martin et al. (1998) Martin et al. (1998) 29 30 2 PHENOMENON OF SUPERCONDUCTIVITY Figure 2.4 Temperature dependence of resistivity for various rare earth substituted RBa2 Cu3 O7 compounds. For these compounds Tc is in the linear region (Tarascon et al., 1987b). Figure 2.5 Comparison of the resistivities of La09125 Sr 00825 2 CuO4 and YBa2 Cu3 O7− with those of the A15 compound V3 SiTc = 171 K, and with nonsuperconducting copper (Gurvitch and Fiory, 1987a, b, c). in the planes than when it takes the shorter path perpendicular to the planes, so it tends to flow mainly along the crystallite planes. Each individual current zigzags from one Figure 2.6 Temperature dependence of the resistiv ity of YBa2 Cu3 O7− for various oxygen partial pres sures (Grader et al., 1987). crystallite to the next, so that its total path is longer than it would be if all of the crystal lites were aligned with their planes parallel to the direction of the current. The increase in the resistivity of a polycrystalline sample beyond ab can be a measure of how much the average path length increases. 31 III RESISTIVITY Figure 2.7 Resistivity for current flow parallel ab and perpendicular c to the CuO planes of YBa2 Cu3 O7 . Data are given for three samples A, B, and C. Note from the change in scale that ab c (Hagen et al., 1988). Such compacted samples require appropri ate heat treatments to maintain the proper oxygen content. Uniaxial compression tends to align the grains with their c-axes parallel so that the resulting compressed pellets have different resistivities when measured paral lel to the compression direction compared to when they are measured perpendicular to this direction. Hysteresis effects have been seen in the resistance-versus-temperature curves, as illustrated in Fig. X-1 of the monograph by Poole et al. (1988), for Y0875 Ba0125 2 CuO4− (Tarascon et al., 1987a). These hysteresis effects occur in the presence of both mag netic fields and transport currents, with the latter illustrated in Figure X-1. C. Anisotropy Determination Figure 2.8 Plot of 2 c T versus T to test the validity of Eq. (2.2) for five single crystals of YBa2 Cu3 O7− (Hagen et al., 1988). Polycrystalline samples should be com pacted or pressed into pellets before resis tivity measurements are made, in order to reduce the number of voids in the sample and minimize intergrain contact problems. The most common way of measuring the resistivity of a sample is the four-probe method sketched in Fig. 2.9. Two leads or probes carry a known current into and out of the ends of the sample, and two other leads separated by a distance L measure the volt age drop at points nearer the center where the current approximates uniform, steady-state flow. The resistance R between measurement points 3 and 4 is given by the ratio V/I of the measured voltage to the input current, Figure 2.9 Experimental arrangement for the four-probe resistivity determination. 32 2 PHENOMENON OF SUPERCONDUCTIVITY and the resistivity expression R= is calculated from the L A (2.4) where A is the cross-sectional area. This four-probe technique is superior to a twoprobe method in which uniform, steady-state current flow is not assured, and errors from lead and contact resistance are greater. The four-probe method is satisfactory for use with an anisotropic sample if the sample is cut with one of its principal direc tions along the direction √ of current flow and if the condition L A is satisfied. For a high-temperature superconductor, this requires two samples for the resistivity deter mination, one with the c-axis along the cur rent flow direction and one with the c-axis perpendicular to this direction. Transverse and longitudinal resistance determinations, Rt and R1 respectively, can both be made on a sample cut in the shape of a rectangular solid with a = b, with the shorter c-axis along the current direction, as shown in Fig. 2.10 (Hagen et al., 1988). These resistances Rt and R1 are used to cal culate the resistivity ab in the a, b-plane and the resistivity and c perpendicular to this plane, i.e., along c. The expressions that relate the resistances depend on the parameter x, x= c a �1/2 � c (2.5) ab where c / ab ≈ 100 for YBa2 Cu3 O7− . For the limiting case x 1, the measured resis tances are given by (Montgomery, 1971): � � a 4 ln 2 Rt = 1 − x 1 (2.6) bc ab � � c 16 exp− /x R1 = x 1 ab c x (2.7) and for the opposite limit x 1 we have � � a 16x exp− x Rt = x 1 bc ab (2.8) � � 4 ln 2 c R1 = 1− x 1 (2.9) ab c x Both the resistance with the exponential fac tor and the correction term containing the factor 4 ln 2/ are small. Contributions to the electrical conduc tivity in the normal state near Tc arising from fluctuations of regions of the sample into the superconducting state, sometimes called paraconductivity, have been observed and discussed theoretically (X. F. Chem et al., 1993; Friedman et al., 1989; Lawrence and Doniach, 1971; Shier and Ginsberg, 1966). Several more theoretical articles treat ing resistivity have appeared (e.g., Gijs et al., 1990a; Hopfengärtner et al., 1991; Kumar and Jayannavar, 1992; Sanborn et al., 1989; Yel et al., 1991). D. Sheet Resistance of Films: Resistance Quantum Figure 2.10 Experimental arrangement for measur ing anisotropic resistivities (see explanation in text) (Hagen et al., 1988). When a current flows along a film of thickness d through a region of surface with dimensions a × a, as shown in Fig. 2.11, 33 III RESISTIVITY Figure 2.11 Geometrical arrangement and current flow direction for sheet resistance determination. it encounters the resistance Rs which, from Eq. (2.4), is given by Rs = a = ad d (2.10) The resistance /d is called the sheet resis tance, or the resistance per square, because it applies to a square section of film, as shown in Fig. 2.11, and is independent of the length of the side a. It is analogous to the sur face resistance Rs = / of a metallic surface interacting with an incident high-frequency electromagnetic wave, where is the skin depth of the material at the frequency of the wave. There is a quantum of resistance h/4e2 with the value h = 645 k 4e2 (2.11) where the charge is 2e per pair. When the films are thin enough so that their sheet resistance in the normal state just above Tc exceeds this value, they no longer become superconducting (Hebard and Paalanen, 1990; Jaeger et al., 1989; Lee and Ketterson, 1990; Li et al., 1990; Pyun and Lemberger, 1991; Seidler et al., 1992; Tanda et al., 1991; Valles et al., 1989; T. Wang et al., 1991). It has been found experimentally (Haviland et al., 1989) that bismuth and lead films deposited on ger manium substrates become superconducting only when they have thicknesses greater than 0.673 nm and 0.328 nm, respectively. The variation in Tc with the sheet resistance for these two thin films is shown in Fig. 2.12. Figure 2.13 shows the sharp drop in resis tivity at Tc for bismuth films with a range Figure 2.12 Dependence of the transition temper ature Tc of Bi and Pb films on the sheet resistance (Haviland et al., 1989). of thickness greater than 0.673 nm. Thinner films exhibit resistivity increases down to the lowest measured temperatures, as shown in the figure. The ordinary transition tem peratures, which occur for the limit /d h/4e2 , are 6.1 K for Bi films and 7.2 K for Pb. Copper-oxide planes in hightemperature superconductors can be considered thin conducting layers, with thickness c for YBa2 Cu3 O7− corresponding to a sheet resistance ab / 21 c. Using this layer approximation, the Ioffe–Regel parameter kF l mentioned in Section A can be estimated from the expression kF l = = conductance per square conductance quantum (2.12) h/4e2 2 ab / 21 c (2.13) where the conductances are the reciprocals of the resistances. Note that the two reported kF l values for YBa2 Cu3 O7− calculated by this method and referred to earlier assumed kF = 46 × 107 cm−1 . It is of interest that metallic con tacts of atomic size exhibit conduction jumps at integral multiples of 2e2 /h (Agraït 34 2 PHENOMENON OF SUPERCONDUCTIVITY Figure 2.14 Resistivity-versus-temperature plot obtained by Kamerlingh Onnes when he discovered superconductivity in Leiden in 1911. Figure 2.13 Temperature dependence of the sheet resistance of films of Bi deposited on Ge as a function of film thickness in the range from 4.36 Å to 74.27 Å (Haviland et al., 1989). et al., 1993), and that the Hall effect resis tance in one-dimensional objects, so-called quantum wires, is quantized to h/2Ne2 , where N = 1 2 3 (Akera and Andu, 1989). IV. ZERO RESISTANCE In 1911, when Onnes was measuring the electrical resistance of mercury, he expected to find a temperature dependence of the type given by Eq. (1.30). Instead, to his sur prise, he found that below 4.2 K the electri cal resistance dropped to zero, as shown in Fig. 2.14. He had discovered superconductiv ity! At this temperature mercury transforms from the normal metallic state to that of a superconductor. Figure 2.3a shows the abrupt change to zero resistance for the case of an old superconductor, where Tc is in the lowtemperature Bloch T 5 region, while Fig. 2.3b shows what happens in the case of a hightemperature superconductor where Tc is in the linear region. A. Resistivity Drop at Tc Figures 2.3a, 2.3b, 2.7, and 2.8 show the sharp drop in resistance that occurs at Tc . We will see later in the chapter that there is an analogous drop in susceptibility at Tc . 35 IV ZERO RESISTANCE A susceptibility measurement is a more typical thermodynamic indicator of the superconducting state because magnetization is a thermodynamic state variable. Resistiv ity, on the other hand, is easier to mea sure, and can be a better guide for appli cations. Generally, the Tc value determined from the resisitivity drop to zero occurs at a somewhat higher temperature than its susceptibility counterpart. This is because any tiny part of the material going super conductive loses its resistance, and R = 0 when one or more continuous superconduct ing paths are in place between the mea suring electrodes. In contrast, diamagnetism measurements depend on macroscopic cur rent loops to shield the B field from an appreciable fraction of the sample material, and this happens when full superconduct ing current paths become available. There fore, filamentary paths can produce sharp drops in resistivity at temperatures higher than the temperatures at which there are pronounced drops in diamagnetism, which also require extensive regions of supercon ductivity. Such filamentary behavior can be described in terms of percolation thresholds (Gingold and Lobb 1990; Lin, 1991; Phillips, 1989b; Tolédano et al., 1990; Zeng et al., 1991). B. Persistent Currents below Tc To establish a transport current in a loop of superconducting wire, the ends of the wire may be connected to a battery in series with a resistor, thus limiting the current, as shown in Fig. 2.15. When switch S2 is closed, current commences to flow in the loop. When switch S1 is closed in order to bypass the battery and S2 opened in order to disconnect the battery, the loop resistance drops to zero and the current flow enters the persistent mode. The zero resistance property implies that the current will continue flowing indefinitely. Many investigators have established cur rents in loops of superconducting wire and have monitored the strength of the associated magnetic field through the loop over pro longed periods of time using, for example, a magnetometer with a pickup coil, as shown in Fig. 2.15. In experiments it was found that there is no detectable decay of the current for periods of time on the order of several years. The experiments established lower limits on the life-time of the current and upper limits on the possible resistivity of superconducting materials. Currents in copper oxide super conductors persist for many months or in excess of a year, and resistivity limits have been reported as low as 10−18 (Yeh et al., Figure 2.15 Experimental arrangement for establishing and measuring a persistent current. Switch S2 is closed to send current through the loop and S1 is closed to confine the current flow to the loop. The magnetometer measures the magnetic field through the loop and thereby determines the current. 36 2 PHENOMENON OF SUPERCONDUCTIVITY 1987) and 10−22 cm (Kedve et al., 1987). Super current lifetimes of low-temperature superconductors are also greater than a < 10−23 cm (Chandrasekhar, year for 1969). Persistent current flow has also been treated theoretically (e.g., Ambegaokar and Eckern, 1991; Cheun et al., 1988; Kopietz, 1993; Riedel et al., 1989; von Oppen and Riedel, 1991). It will be instructive to estimate the min imum resistivity of a simple loop of super conducting wire of loop radius r and wire radius a. The inductance L of the loop is given by L ≈ 0 r ln8r/a − 2 (2.14) The loop has ‘length’ 2 r and crosssectional area a2 , so that its resistance R is R= 2r a2 (2.15) This gives it a time constant = L/R. Com bining Eqs. (2.14) and (2.15) gives the prod uct ≈ 21 0 a2 00794 + lnr/a (2.16) Using 0 = 4 × 10−7 H/m and typical loop dimensions of a = 15 mm and r = 15 cm gives ≈ 66 × 10−10 cm s (2.17) for the product . A super current Is can be made to flow in the loop by subjecting it to a changing magnetic field below Tc , in accordance with Faraday’s and Lenz’ laws. The magnitude of the current that is flowing can be determined by measuring the induced magnetic field. At a point P along the axis a distance z above the loop, as shown in Fig. 2.16, this magnetic field has the following value, as given in standard general physics texts: 0 Is r 2 Bz = 2r 2 + z2 3/2 (2.18) Figure 2.16 Magnetic field Bz along the axis of a circular loop of wire of radius r carrying the current I. The wire itself has radius a. and once Bz is measured, Is can be calculated. If the super current persists unchanged for over a year > 316×107 s without any appreciable decrease (we are assuming that a 1% decrease is easily detectable), Eq. (2.17) can be used to place an upper limit on the resistivity: < 21 × 10−17 cm (2.19) which is in the range mentioned earlier, and is 11 orders of magnitude less than the resis tivity of copper = 156 cm. A similar loop of copper wire at room temperature has ≈ 042 ms, so that the current will be gone after several milli-seconds. We will see in Section XIV that the drop to zero resistance can be explained in terms of a two–fluid model in which some of the normal electrons turn into super electrons which move through the material without resistance. The current carried by the flow of super electrons is then assumed to short circuit the current arising from the flow of normal electrons, causing the measured resis tance to vanish. V. TRANSITION TEMPERATURE Before proceeding to the discussion of magnetic and transport properties of super conductors, it will be helpful to say a few 37 V TRANSITION TEMPERATURE words about the transition temperature. We will discuss it from the viewpoint of the resis tivity change even though the onset of the energy gap and pronounced diamagnetism are more fundamental indices of Tc . Pechan and Horvath (1990) described a fast and inexpensive method for accurate determina tion of transition temperatures above 77 K. Although the theoretical transition from the normal to the superconducting state is very sharp, experimentally it sometimes occurs gradually and sometimes abruptly. Figure 2.17 shows the gradual decrease in resistivity near Tc that was reported by Bednorz and Müller (1986) in the first pub lished article on the new superconductors. We see from this figure that the range of temperatures over which the resistivity changes from its normal-state value to zero is comparable with the transition tempera ture itself. An example of a narrow transition centered at 90 K with width of ≈ 03 K is shown in Fig. 2.18. These two cases corre spond to T/Tc ≈ 1/2 and T/Tc ≈ 0003, respectively. The sharpness of the drop to zero resis tance is a measure of the goodness or purity of the sample. Figure 2.19 shows how the drop to zero in pure tin becomes broader and shifts to a higher temperature in an impure specimen. In a sense impure tin is a better superconductor because it has a higher Tc but worse because it has a broader transition. When high-temperature superconductors are Figure 2.17 First reported drop to zero resistance for a high-temperature superconductor (Bednorz and Müller, 1986). 38 2 PHENOMENON OF SUPERCONDUCTIVITY Figure 2.18 Sharp drop to zero resistance of a YBa2 Cu3 O7 epi taxial film (Hopfengärtner et al., 1991). Figure 2.19 Narrow and broad superconducting resistivity drop in pure and impure tin, respectively. Reprinted from Rose Innes and Rhoderick (1978), p. 7, with kind permission of Pergamon Press, Headington Hill Hall, Oxford OX3 0BW, UK. doped with paramagnetic ions at copper sites, the transition temperature both shifts to lower values and broadens, whereas doping at the yttrium sites of YBaCuO has very little effect on Tc , as may be seen by comparing the data plotted in Figs. 2.20 and 2.4, respectively. This can be explained in terms of delocal ization of the super electrons on the copper oxide planes. There are various ways of defining the position and sharpness, or width, of the superconducting transition temperature, and the literature is far from consistent on this point. Authors talk in terms of the onset, 5%, 10%, midpoint, 90%, 95%, and zero resis tance points, and Fig. 2.21 shows some of these on an experimental resistivity curve. The onset, or 0% point, is where the exper imental curve begins to drop below the extrapolated high-temperature linear behav ior of Eq. (1.30), indicated by the dashed line in the figure. The Tc values that we cite or list in the tables are ordinarily midpoint values at which T has decreased by 50% below the onset. Many of the published reports of unusually high transition temperatures actu ally cited onset values, which can make them suspect. The current density can influence the resistive transition (Goldschmidt, 1989). The point at which the first derivative of the resistivity curve, shown in Fig. 2.22b, reaches its maximum value could be selected as defining Tc , since it is the inflection point on the original curve (Azoulay, 1991; Datta et al., 1988; Nkum and Datars, 1992; Poole and Farach, 1988). The width T between the half-amplitude points of the first deriva tive curve, or the peak-to-peak width Tpp 39 V TRANSITION TEMPERATURE Figure 2.20 Influence of doping YBa2 Cu09 M01 3 O6+y with the first transition series ions M = Ti, Cr, Fe, Co, Ni, and Zn on the resistivity transition near Tc (Xiao et al., 1987a). Figure 2.21 Temperature dependence of the resistivity and zero-field-cooled magnetization of HoBa2 Cu3 O7 . The 10%-drop, midpoint, and 90%-drop points are indicated on the resistivity curve (Ku et al., 1987). of the second derivative curve sketched in Fig. 2.22c, are both good quantitative mea sures of the width of the transition. An asym metry parameter, equal to A−B/A+B, may also be evaluated from Fig. 2.22c. There appear to be enough data points near the midpoint of Fig. 2.22a to accurately define the transition, but the first and second derivative curves of Figs. 2.22b and 2.22c, respectively, show that this is not the case. This need for additional data points demon strates the greater precision of the derivative method. Phase transitions in general have finite widths, and a typical approach is to define Tc in terms of the point of most rapid change from the old to the new phase. Critical expo nents are evaluated in this region near Tc . Ordinarily, less account is taken of the more gradual changes that take place at the onset or during the final approach to the new equilibrium state. The onset of supercon ductivity is important from a physics view point because it suggests that superconduct ing regions are being formed, whereas the zero point is important from an engineering viewpoint because it is where the material can finally carry a super current. 40 2 PHENOMENON OF SUPERCONDUCTIVITY Figure 2.22 Zero-field-susceptibility of YBa2 Cu3 O7 as a function of temperature in a magnetic field of 0.1 mT: (a) usual susceptibility plot ; (b) first derivative plot d /dT ; and (c) second derivative plot d2 /d2 T (Almasan et al., 1988). VI. PERFECT DIAMAGNETISM The property of perfect diamagnetism, which means that the susceptibility = −1 in Eq. (1.78a), B =0 H1 + (2.20) =0 H + M (2.21) is equivalent to the assertion that there can be no B field inside a perfect diamagnet because 41 VI PERFECT DIAMAGNETISM the magnetization M is directed opposite to the H field and thereby cancels it: M = −H (2.22) When a superconductor is placed between the pole pieces of a magnet, the B field lines from the magnet go around it instead of entering, and its own internal field remains zero, as shown in Fig. 2.23. This field dis tribution is the result of the super-position of the uniform applied field and a dipole field from the reversely magnetized super conducting sphere, as illustrated in Fig. 2.24 (Jackson, 1975; cf. Section 5–10). There are two aspects to perfect diamag netism in superconductors. The first is flux exclusion: If a material in the normal state is zero field cooled (ZFC), that is, cooled below Tc to the superconducting state with out any magnetic field present, and is then placed in an external magnetic field, the field will be excluded from the superconductor. The second aspect is flux expulsion: If the same material in its normal state is placed in a magnetic field, the field will penetrate and have almost the same value inside and out side because the permeability is so close to the free-space value 0 . If this material is then field cooled (FC), that is, cooled below Tc in the presence of this field, the field will be expelled from the material, a phe nomenon called the Meissner effect. These two processes are sketched on the left side of Fig. 2.25. Although ZFC and FC lead to the same result (absence of magnetic flux inside the sample below Tc ), nevertheless the two Figure 2.23 Curvature of magnetic field lines around a superconducting sphere in a constant applied field. Figure 2.24 Sketch of constant applied magnetic field (a) and dipole field (b) that superimpose to provide the magnetic field lines shown in Fig. 2.23 (Jackson, 1975). 42 2 PHENOMENON OF SUPERCONDUCTIVITY Figure 2.25 Effect of zero field cooling (ZFC) and field cooling (FC) of a solid superconducting cylinder (left), a superconducting cylinder with an axial hole (center), and a perfect conductor (right). processes are not equivalent, as we will see in Section IX. Thompson et al. (1991) found that for a “defect-free” high-purity niobium sphere the ZFC and FC susceptibilities are almost identical. A second high-purity sphere of similar composition that exhibited strong pinning was also examined and the same ZFC results were obtained, except that no Meissner flux expulsion following field cool ing was observed. The pinning was so strong that the vortices could not move out of the sample. Figure 2.25 is drawn for the case of very weak pinning, in which virtually all of the flux is expelled from the superconducting material following field cooling. 43 VII MAGNETIC FIELDS INSIDE A SUPERCONDUCTOR VII. MAGNETIC FIELDS INSIDE A SUPERCONDUCTOR To further clarify the magnetic field configurations inside a superconductor, con sider a long cylindrical sample placed in a uniform applied magnetic field with its axis in the field direction, as indicated in Fig. 2.26. Since there are no applied currents, the boundary condition at the surface given in Chapter 1, Section XIV, H = H (2.23) shows that the H field is uniform inside with the same value as the applied field: Happ = Hin (2.24) The B field has only a z component with value Bapp = 0 Happ outside and zero inside, Bin = 0. There is, however, a transition layer of thickness , called the penetration depth, Figure 2.26 Boundary region and internal fields for a superconducting cylinder in an axial external magnetic field Bapp . at the surface of the superconductor where the B field drops exponentially from its value Bapp on the outside to zero inside, in accor dance with the expression Br ≈ Bapp exp −R − r/ (2.25) as shown in Fig. 2.27. Thus the B field exists only in the surface layer, and not in the bulk. Since Bin r = Hin + Mr (2.26) with Hin = Happ , we have for Mr � Mr = −Happ � �� R − r 1 − exp − (2.27) again subject to the assumption that R, and this is also sketched in Fig. 2.27. We will show later in Chapter 6, Sections VII and VIII, that this expo nential decay process arises naturally in the Ginzburg–Landau and London theories, and that these theories provide an explicit Figure 2.27 Plot of the fields B and 0 H and of the magnetization 0 M outside r > R and inside r < R a superconducting cylinder of radius R in an axial applied field Bapp . At the center of the sphere r = 0. 44 2 PHENOMENON OF SUPERCONDUCTIVITY formula for what is called the London pene tration depth L , namely � L = m 0 ns e 2 �1/2 (2.28) where ns is the density of superconducting electrons. VIII. SHIELDING CURRENT In the absence of any applied transport current we set J = 0 (also D/t = 0) in Maxwell’s equation, Eq. (1.72), to obtain � × Bin =0 � × M =0 Jsh (2.29a) (2.29b) where Jsh is called the shielding or demag netization current density: Jsh = � × M (2.30) Since Bin has only a z or axial component, the curl, expressed in terms of cylindrical coor dinates, gives the following shielding current density flowing around the cylinder in the negative direction: 1 dB · (2.31) 0 dr � � � � Bapp R − r ≈− exp − (2.32) 0 � � R − r ≈ − J0 exp − (2.33) Jsh r = − where Bapp = 0 J0 (2.34) again with R, and this circular current flow is sketched in Fig. 2.28 and graphed in Fig. 2.29. In other words, the vectors B and Jsh do not exist in the bulk of the supercon ductor but only in the surface layer where Figure 2.28 Shielding current flow Jsh in a surface layer of thickness around a superconducting cylinder in an axial applied magnetic field Bapp . they are perpendicular to each other, with B oriented vertically and Jsh flowing around the cylinder in horizontal circles. It may be looked upon as a circulating demagnetizing current that shields or screens the interior of the superconductor by producing a nega tive B field that cancels Bapp so that Bin = 0 inside. Thus we see that the superconducting medium reacts to the presence of the applied field by generating shielding currents that cancel the interior B field. The reaction of the 45 IX HOLE IN SUPERCONDUCTOR Figure 2.29 Dependence of the shielding current density Jsh on the position inside a superconducting cylinder of radius R in an applied axial field Bapp . Note that Jsh has the value Happ / at the surface. medium may also be looked upon as generat ing a magnetization M that cancels the inte rior B field, as was explained above. These are two views of the same phenomenon, since the shielding current density Jsh and the compensating magnetization M are directly related through Eq. (2.30). The negative B field that cancels Bapp is really a magnetiza tion in the negative z direction. It is instructive to see how Eq. (2.34) is equivalent to the well-known formula B0 = 0 NI L (2.35) for the magnetic field B0 of an N -turn solenoid of length L. Since each turn carries the current I, the total current is NI. This total current also equals the current density J0 times the area L, corresponding to NI = LJ0 (2.36) Substituting NI from this expression in Eq. (2.35) gives Eq. (2.34). Thus the circu lating shielding current is equivalent to the effect of a solenoid that cancels the applied B field inside the superconductor. The dipole field of the superconducting sphere sketched in Fig. 2.24 may be consid ered as arising from demagnetizing currents circulating in its surface layers, as shown in Fig. 2.30. These demagnetizing currents pro vide the reverse magnetization that cancels Figure 2.30 Shielding current flow around the sur face of a superconducting sphere in an applied magnetic field Bapp . the applied field to make B = 0 inside, just as in the case of a cylinder. IX. HOLE IN SUPERCONDUCTOR As an example of how ZFC and FC can lead to two different final states of mag netism let us examine the case of a hole inside a superconductor. Consider a cylindrical superconducting sample of length L and radius R with a con centric axial hole through it of radius r, as shown in Fig. 2.31. This will be referred to as an “open hole” because it is open to the out side at both ends. If this sample is zero-field cooled in the manner described in Section VI, an axial magnetic field applied after cooling below Tc will be excluded from the super conductor and also from the open axial hole. 46 2 PHENOMENON OF SUPERCONDUCTIVITY Figure 2.31 Superconducting tube of radius R with an axial hole of radius r. Surface currents shield the superconducting regions from the external field and bring about the flux exclusion shown in Fig. 2.25. These same surface currents also shield the hole from the applied field. This means that the superconductor plus the hole act like a perfect diamagnet under zero-field cooling. The entire volume R2 L, including the open hole volume r 2 L, has an effective suscep tibility of −1, eff = −1 (2.37) If this same sample, still with an open hole, is field cooled, once it attains the super conducting state the magnetic flux will be expelled from the superconducting material, but will remain in the hole. The same outer surface currents flow to shield the supercon ductor from the applied field, but the sur face currents flowing in the reverse direction around the inside surface of the cylinder, i.e., around the hole periphery as indicated in Fig. 2.32, cancel the effect of the out side surface currents and sustain the original magnetic flux in the hole. The volume of the superconducting material, R2 − r 2 L, has a susceptibility of −1, but the space in Figure 2.32 Magnetic field lines, shielding current flow Jsh on the outside surface, and reverse-direction shielding current flow JR on the inside surface of a superconducting tube in an applied axial magnetic field. The magnetic field lines pass through the hole because the cylinder has been field cooled. the open hole, r 2 L, does not exhibit dia magnetism, so that for the hole = 0. The effective susceptibility of the cylinder with the hole is the average of −1 for the super conducting material and 0 for the hole, cor responding to � � r �2 � eff = − 1 − (2.38) R which reduces to −1 for no hole r = 0 and to 0 for r = R. This experimentally measur able result is different from the ZFC open hole case (2.37). Experimentally, it is found that the magnetic susceptibility is less nega tive for field-cooled samples than for zerofield-cooled samples, as shown by the data in Fig. 2.33. Mohamed et al. (1990) give plots of the ZFC and FC magnetic field dis tributions of a 16-mm diameter, 2-mm thick superconducting disk with a 3-mm diameter axial hole. 47 IX HOLE IN SUPERCONDUCTOR Figure 2.33 Zero-field-cooled (closed symbols) and field-cooled (open symbols) mag netic susceptibility of YBa2 Cu3 O7 nonaligned powder (circles) and grain-aligned samples with the applied field parallel to the c-axis (triangles) and perpendicular to the c-axis (squares). Results are shown in an applied field of (a) 5 mT and (b) 0.3 T. Note the change in abscissa and ordinate scales between the two figures (Lee and Johnston, 1990). Another important case to consider is that of a totally enclosed hole of the type shown in Fig. 2.34, which we call a closed hole or cavity. It is clear that for ZFC the closed hole behaves the same as the open hole, that is, flux is excluded from it, with eff = −1, as shown in the fifth column of Fig. 2.25. Flux is also excluded for field cooling. To see this, we recall that the B field lines must be continuous and can only 48 Figure 2.34 Superconducting cylinder with a totally enclosed hole. begin or end at the poles of a magnet. In the open hole case, the B field lines in the hole either join to the externally applied field lines or form loops that close outside the sample, as shown at the bottom of column 4 of Fig. 2.25. The B field lines have no way of leaving a closed hole to connect with the external field or to form closed loops out side, so such lines cannot exist inside a cavity completely surrounded by a superconducting material. Therefore, flux is expelled during field cooling, so again eff = −1. Thus a superconductor with a cavity behaves like a solid superconductor with the difference that magnetization can exist only in the super conductor, not in the cavity. In this section we have discussed the cases of open and closed holes in superconductors. We showed in Table 1.2 that the susceptibility of typical diamagnetic and paramagnetic samples is quite close to zero, so that the empty hole results also apply to holes filled with typical nonsuper con ducting materials. Experimentally, we deal with samples with a known overall or exter nal volume, but with an unknown fraction of this volume taken up by holes, intergranular 2 PHENOMENON OF SUPERCONDUCTIVITY spaces, and nonsuperconducting material that could respond to ZFC and FC precondition ing the same way as a hole. If a sample is a mixture of a supercon ducting material and a non-superconducting material with the nonsuperconducting part on the outside so that the applied magnetic field can penetrate it under both ZFC and FC conditions, the average sample suscepti bility will be the average of = 0 for the normal material and = −1 for the super conducting part. Thus both the ZFC and the FC measurement will give values of eff that are less negative than −1. A granular superconducting sample can have an admix ture of normal material on the outside or inside and space between the grains that pro duce ZFC and FC susceptibilities of the type shown in Fig. 2.33, where, typically, the measured susceptibilities are zfc ≈ −07 and fc ≈ −03. X. PERFECT CONDUCTIVITY We started this chapter by describ ing the perfect conductivity property of a superconductor—namely, the fact that it has zero resistance. Then we proceeded to explain the property of perfect diamagnetism exhibited by a superconductor. In this section we will treat the case of a perfect conduc tor, i.e., a conductor that has zero resistivity but the susceptibility of a normal conduc tor, i.e., ≈ 0. We will examine its response to an applied magnetic field and see that it excludes magnetic flux, but does not expel flux, as does a superconductor. We will start with a good conductor and then take the limit, i.e., letting its resistance fall to zero so that it becomes a hypothetical perfect conductor. A static magnetic field penetrates a good conductor undisturbed because its magnetic permeability is quite close to the magnetic permeability of free space 0 , as the suscep tibility data of Table 1.2 indicate. Therefore, 49 XI TRANSPORT CURRENT a good conductor placed in a magnetic field leaves the field unchanged, except perhaps for current transients that arise while the field is turned on and die out rapidly. In Section IV we estimated the decay time constant for a loop of copper wire 15 cm in diameter to be 0.42 ms. Consider a closed current path within the conductor. When the magnetic field Bapp is applied, the magnetic flux through this circuit = A · Bapp changes, so that by Lenz’ law a voltage −A · dBapp /dt is induced in the circuit and a current I flows, as indicated in Fig. 2.35, in accordance with the expression −A · dBapp dI = RI + L dt dt (2.39) The current rapidly dies out with time con stant L/R. For a perfect conductor the resis tance term in Eq. (2.39) vanishes. Solving the resultant equation, −A · dBapp dI =L dt dt (2.40) gives LI + A · Bapp = Total (2.41) which means that the total flux LI + A · Bapp remains constant when the field is applied. If no fields or currents are present and the field Bapp is applied, the flux LI will be induced to cancel that from the applied field and main tain the B = 0 state inside the perfect conduc tor. In real conductors the induced currents Figure 2.35 Magnetic field B rapidly established through a loop of wire and induced current I. which, by Lenz’ law, flows in a direction to oppose the establish ment of this field. die out so rapidly that the internal B field builds up immediately to the applied field value. Hence a perfect conductor exhibits flux exclusion since a magnetic field turned on in its presence does not penetrate it. It will, however, not expel flux already present because flux that is already there will remain forever. In other words, an FC-perfect con ductor retains magnetic flux. Thus we find that a ZFC-perfect conduc tor excludes magnetic flux just like a ZFC superconductor. The two, however, differ in their field-cooled properties, the perfect con ductor retaining flux and a superconductor excluding flux after FC. A perfect conductor acts like an open hole in a superconductor! We do not know of any examples of per fect conductors in nature. The phenomenon has been discussed because it provides some insight into the nature of superconductivity. XI. TRANSPORT CURRENT In the previous section we discussed the shielding currents induced by the presence of applied magnetic fields. We saw how a field applied along the cylinder axis gives rise to currents circulating around this axis. When a current is applied from the outside and made to flow through a superconduc tor, it induces magnetic fields near it. An applied current is called transport current, and the applied current density constitutes the so-called “free” current density term on the right side of Maxwell’s inhomogeneous equation (1.68). Suppose that an external current source causes current I to flow in the direction of the axis of a superconducting cylinder of radius R, in the manner sketched in Fig. 2.36. We know from general physics that the wire has a circular B field around it, as indicated in the figure, and that this field decreases with distance r from the wire in accordance with the expression B= 0 I 2 r r ≥ R (2.42) 50 2 PHENOMENON OF SUPERCONDUCTIVITY Figure 2.38 Transport current flow in a surface layer of thickness radius R. of a Type I superconducting wire of Figure 2.36 Magnetic field lines B around a wire carrying a current I. as shown sketched in Fig. 2.37, with the fol lowing value on the surface: Bsurf = 0 I 2 R (2.43) We also know that if the current density were uniform across the cross section of the wire, the B field inside would be proportional to the distance from the axis, B = Bsurf r/R, as shown in Fig. 2.37. Since magnetic flux is excluded from inside a superconducting wire, the current density cannot be uniform, and instead the transport current must flow in a surface layer of thickness , as shown in Fig. 2.38, to maintain the B field equal to zero inside. This current density Jr must have the same exponential dependence on distance as given by Eq. (2.31) for the case of the shielding current: � � R − r B (2.44) Jr = surf exp − 0 � � I R − r = exp − (2.45) 2 R Figure 2.39 shows how the current distribu tion changes at the junction between a nor mal wire and a superconducting wire from uniform density flow in the normal conduc tor to surface flow in the superconductor. The total current I is the integral of the cur rent density Jr from Eq. (2.45) over the cross section of the superconducting wire, with value I = 2 R J (2.46) where J = JR is the maximum value of Jr, which is attained at the surface, and the quantity 2 R is the effective crosssectional area of the surface layer. Substitut ing the expression for I from Eq. (2.46) in Eq. (2.43) gives Bsurf = 0 J Figure 2.37 Dependence of the internal r < R and external r > R magnetic field on distance from the center of a normal conductor wire carrying a current of uniform density. (2.47) which is the same form as Eq. (2.34) for the shielding current. Comparing Eqs. (2.32) and (2.44) we obtain for the magnetic field inside the wire � � R − r r ≤ R Br = Bsurf exp − (2.48) 51 XI TRANSPORT CURRENT Figure 2.39 Current flow through a wire that is normal on the left and Type I superconducting on the right. Note that the penetration depth determines the thickness of both the transition region at the interface and that of the surface layer. as shown sketched in Fig 2.40. In Chapter 5, Sections VII and IX, we show how to derive these various exponential decay expressions from the Ginzburg–Landau and London the ories. Outside the wire the magnetic field exhibits the same decline with distance in both the normal and superconducting cases, as can be seen by comparing Figs. 2.37 and 2.40. There is really no fundamental differ ence between the demagnetizing current and the transport current, except that in the present case of a wire their directions are orthogonal to each other. When a current is impressed into a superconductor it is called a transport current, and it induces a magnetic field. When a superconductor is placed in an external magnetic field, the current induced by this field is called demagnetization cur rent or shielding current. The current–field relationship is the same in both cases. This is why Eqs. (2.25) and (2.48) are the same. Figure 2.40 Dependence of the internal r < R and external r > R magnetic field on distance from the center of a superconducting wire carrying a current that is confined to the surface layer. This figure should be compared with Fig. 2.37. 52 2 PHENOMENON OF SUPERCONDUCTIVITY XII. CRITICAL FIELD AND CURRENT We noted in Section II that application of a sufficiently strong magnetic field to a superconductor causes its resistance to return to the normal state value, and each supercon ductor has a critical magnetic field Bc above which it returns to normal. There is also a critical transport current density J c that will induce this critical field at the surface and drive the superconductor normal. Compar ing Eqs. (2.34) and (2.47), respectively, we have for both the demagnetizing and trans port cases Bc T = 0 TJc T (2.49) where all three quantities are temperature dependent in a way that will be described in the following section. Either an applied field or an applied current can destroy the super conductivity if either exceeds its respective critical value. At absolute zero, we have Bc 0 = 0 0Jc 0 (2.50) and this is often written B c = 0 Jc (2.51) where T = 0 is understood. A particular superconducting wire of radius R has a maximum current, called the critical current Ic , which, by Eq. (2.46), has the value Ic = 2 R Jc (2.52) Using Eq. (2.51), the value of the critical current may be written as Ic = 2 RBc 0 = 5 × 106 RHc (2.53a) (2.53b) The transformation of a superconducting wire to the normal state when the current passing through it exceeds the critical value is called the Silsbee effect. In Type I superconductors with thick nesses much greater than the penetration depth , internal magnetic fields, shielding currents, and transport currents are able to exist only in a surface layer of thickness . The average current carried by a supercon ducting wire is not very high when most of the wire carries zero current. To achieve high average super current densities, the wire must have a diameter less than the penetra tion depth, which is typically about 50 nm for Type I superconductors. The fabrication of such filamentary wires is not practical, and Type II superconductors are used for this application. XIII. TEMPERATURE DEPENDENCES In the normal region above the tran sition temperature there is no critical field Bc = 0 and there is total magnetic field penetration = . As a superconductor is cooled down through the transition tempera ture Tc , the critical field gradually increases to its maximum value Bc 0 at absolute zero T = 0, while the penetration depth decreases from infinity to its minimum value 0 at absolute zero. The explicit temper ature dependences of Bc T and T are given by the Ginzburg–Landau theory that will be presented in Chapter 6, where 0 = L as given by Eq. (2.28), � 0 = m 0 ns e 2 �1/2 (2.54) which assumes that all of the conduction electrons are super electrons at T = 0. The critical current density may be written as the ratio Jc T = Bc T 0 T (2.55) 53 XIII TEMPERATURE DEPENDENCES given in Eq. (2.49) in order to obtain the temperature dependence of Jc T. These tem perature dependences have the form � �� T 2 Bc = Bc 0 1 − (2.56) Tc � � �4 �−1/2 T = 0 1 − (2.57) Tc � � �4 �1/2 � �2 � � T T Jc = Jc 0 1 − 1− Tc Tc (2.58) � and are sketched in Figs. 2.41, 2.42, and 2.43. Also shown by dashed lines in the figures are the asymptotic behaviors near the transition temperature T ≈ Tc (Nicol and Carbotte, 1991): Figure 2.42 Temperature dependence of the pen etration depth T corresponding to Eq. (2.57). The asymptotic behaviors near T = 0 and T = Tc are indi cated by dashed lines. Figure 2.43 Temperature dependence of the critical current density Jc T in accordance with Eq. (2.58). The asymptotic behavior near T = 0 and T = Tc is indicated by dashed lines. Figure 2.41 Temperature dependence of the critical field Bc T corresponding to the behavior expressed by Eq. (2.56). The asymptotic behaviors near T = 0 and T = Tc are indicated by dashed lines. � � T Bc ≈ 2Bc 0 1 − Tc � � T −1/2 1 ≈ 2 0 1 − Tc (2.59) (2.60) 54 2 PHENOMENON OF SUPERCONDUCTIVITY � � T 3/2 Jc ≈ 4Jc 0 1 − Tc (2.61) Jiang and Carbotte (1992) give plots of 0/ T for various theoretical models and anisotropies. The asymptotic behav iors near absolute zero, T → 0, are as follows: � � �2 � T Bc = Bc 0 1 − (2.62) Tc � � �� 1 T 4 ≈ 0 1 + (2.63) 2 Tc � � �2 � T Jc ≈ Jc 0 1 − (2.64) Tc which are proven in Problems 5 and 6, respectively. Note that Eq. (2.62) is iden tical to Eq. (2.56). Some authors report other values of the exponents or expressions related to Eqs. (2.56)–(2.64) for Bc (Miu, 1992; Miu et al., 1990), (Däumling and Chandrashekhar, 1992; Hebard et al., 1989; Kanoda et al., 1990; Kogan et al., 1988), and Jc (Askew et al., 1991; Freltoft et al., 1991). For later reference we give here the tem perature dependence of the superconducting energy gap Eg in the neighborhood of Tc : � � T 1/2 Eg ≈ 352 kB Tc 1 − Tc (2.65) (cf. Section VI, Chapter 7 for an explana tion of the energy gap and a plot (Fig. 7.7) of this expression). Another length param eter that is characteristic of the supercon ducting state is the coherence length ; this parameter will be introduced in Chapter 6 and referred to frequently throughout the remainder of the text. It is reported to have a 1 − T/Tc −n dependence, with n = 1/2 expected; the penetration depth also depends on 1 − T/Tc −n near Tc (Chakravarty et al., 1990; Duran et al., 1991; Schneider, 1992). XIV. TWO FLUID MODEL Many properties of superconductors can be described in terms of a two-fluid model that postulates a fluid of normal electrons mixed with a fluid of superconducting elec trons. The two fluids interpenetrate but do not interact. A similar model of interpene trating fluids consisting of normal and super fluid atoms is used to explain the properties of He4 below its lambda point. When a superconductor is cooled below Tc , normal electrons begin to transform to the super electron state. The densities of the normal and the super electrons, nn and ns , respec tively, are temperature dependent, and sum to the total density n of the conduction electrons, nn T + ns T = n (2.66) where at T = 0 we have nn 0 = 0 and ns 0 = n. If we assume that Eq. (2.54) is valid for any temperature below Tc , � T = m 0 ns T e2 �1/2 (2.67) then 0 = m/0 ne2 1/2 , and we can write ns = n � 0 T �2 (2.68) which becomes, with the aid of Eq. (2.57), � � �4 � T ns ≈ n 1 − (2.69) Tc Figure 2.44 shows a sketch of ns versus tem perature. Substituting the latter in Eq. (2.66) gives for the normal electron density � nn ≈ n T Tc �4 (2.70) Equation (2.68) is useful for estimating super electron densities. 55 XVI CRITICAL SURFACE 2B 0 dBc2 = − c2 ≈ −183 T/K dT Tc (2.73) For high-temperature superconductors the slopes of Eqs. (2.72) and (2.73) near Tc can be quite anisotropic. XVI. CRITICAL SURFACE Figure 2.44 Temperature dependence of the density of superconducting electrons ns as given by Eq. (2.69). The dashed lines show the slope dns /dT = 0 at T = 0 and −4 at Tc . XV. CRITICAL MAGNETIC FIELD SLOPE We showed in the previous section that the critical magnetic field has the parabolic dependence on temperature given by Eq. (2.56), and this is plotted in Fig. 2.41. The slope of the curve near Tc is given by Eq. (2.59) and may also be written dBc T 2B 0 =− c Tc dT (2.71) For most Type I superconductors this ratio varies between −15 and −50 mT/K; for example, it has a value of −223 mT/K for lead. A Type II superconductor has two crit ical fields, a lower-critical field Bc1 and an upper-critical field Bc2 , where Bc1 < Bc2 , as we will see in Chapter 12. These critical fields have temperature dependences similar to that of Eq. (2.71). Typical values of these two slopes for a high-temperature supercon ductor are (see Fig. 12.8, Table 12.5) 2B 0 dBc1 = − c1 ≈ −1 mT/K dT Tc The critical behavior of a superconduc tor may be described in terms of a critical surface in three-dimensional space formed by the applied magnetic field Bapp , applied transport current Jtr , and temperature T , and this is shown in Fig. 2.45. The surface is bounded on the left by the Bc T versus T curve (d–c–b–a) drawn for Jtr = 0; this curve also appears in Figs. 2.41 and 2.46. The surface is bounded on the right by the Jc T versus T curve (g–h–i–a) drawn for Bapp = 0, which also appears in Figs. 2.43 and 2.47. Figure 2.46 shows three Bc T versus T curves projected onto the Jtr = 0 plane, while Fig. 2.47 presents three Jc T versus T curves projected onto the Bapp = 0 plane. Finally, Fig. 2.48 gives projections of (2.72) Figure 2.45 Critical surface of a superconductor. Values of applied field Bapp , transport current Jtr , and temperature T corresponding to points below the critical surface, which are in the superconducting region, and points above the critical surface, which are in the normal region. The points on the surface labeled A, B , , L also appear in Figs. 2.46–2.49. 56 Figure 2.46 Projection of constant current curves of the critical surface of Fig. 2.45 on the Bapp , T -plane. Projections are shown for Jtr = 0 Jtr Jc , and Jtr ≈ Jc . The Jtr = 0 curve is calculated from Eq. (2.56). The other two curves are drawn so as to have the same shape as the curve for Jtr = 0. Figure 2.47 Projection of constant applied field curves of the critical surface of Fig. 2.45 onto the Jtr , T plane. Projections are shown for Bapp = 0, Bapp Bc , and Bapp ≈ Bc . The Bapp = 0 curve is calculated from Eq. (2.58). The other two curves are drawn to have the same shape as the curve for Bapp = 0. three Jc T versus Bc T curves onto the T = 0 plane. The points a, b , , 1 in the various figures are meant to clarify how the projec tions are made. The notation Bc 0 = Bc and Jc 0 = Jc is used in these figures. 2 PHENOMENON OF SUPERCONDUCTIVITY Figure 2.48 Projection of constant-temperature curves of the critical surface of Fig. 2.45 onto the Jtr Bapp plane. Projection isotherms are shown for T = 0 T Tc , and T ≈ Tc . The shapes given for these curves are guesses. The x- and y-coordinates of this surface are, respectively, the applied magnetic field Bapp and the applied transport current Jtr . The former does not include the magnetic fields that are induced by the presence of transport currents, while the latter does not include shielding currents arising from the applied fields. What the critical surface means is that at a particular temperature T there is a characteristic critical field Bc T that will drive the superconductor normal if applied in the absence of a transport current. Simi larly there is a critical current density Jc T that will drive the superconductor normal if it is applied in zero field. In the presence of an applied field a smaller transport current will drive the superconductor normal, and if a transport current is already passing through a superconductor, a smaller applied magnetic field will drive it normal. This is evident from the three constant temperature Bc T versus Jc T curves shown in Fig. 2.48. One of these (h–l–k–c) is redrawn in Fig. 2.49. It will be instructive to illustrate the significance of Figs. 2.48 and 2.49 by an example. Consider the case of a long, cylin drical superconductor of radius R L with 57 XVI CRITICAL SURFACE Figure 2.49 Projection of the h-l-k-c curve of Fig. 2.45 onto the Jc T versus Bapp plane showing the critical fields and current densities at the points k and l. Figure 2.51 Net magnetic field Bnet on the surface of a superconducting cylinder resulting from vector addi tion of the applied field Bapp and the field Btr produced by the transport current. field Btr , Btr = 0 Itr 2 R (2.74) at the surface of the cylinder. This magnetic field is at right angles to Bapp at the surface, as shown in Fig. 2.51, so that the net field Bnet at the surface is the square root of the sum of the squares of Bapp and Btr : 2 Bnet = Bapp + Btr2 1/2 Figure 2.50 Type I superconducting cylinder (a) car rying a transport current Itr of density Jtr in an applied magnetic field Bapp , and (b) flow of this transport current in a surface layer of thickness . an applied transport current Itr flowing along its axis and located in a magnetic field Bapp along its axis, as indicated in Fig. 2.50. This situation is analyzed by taking into account the magnetic field produced at the surface by the transport current, assum ing that Jc T/Jc 0 = Bc T/Bc 0 and that the normalized Jc T-versus-Bc T curve of Fig. 2.49 is an arc of a circle. We can see from Eq. (2.43) that the transport current produces the magnetic (2.75) Using Eq. (2.74) this equation can be written explicitly in terms of the transport current: � Bnet = � 2 Bapp + 0 Itr 2 R �2 �1/2 (2.76) The superconductor will go normal when the combination of Bapp and Itr is high enough to make Bnet equal Bc T, the critical field for this temperature in the absence of transport currents: � � � �1/2 0 Itr 2 2 (2.77) Bc T = Bapp + 2 R If we consider the case of the superconductor going normal at the point k of Fig. 2.49 then, 58 2 PHENOMENON OF SUPERCONDUCTIVITY FURTHER READING Figure 2.52 Net current density Jnet flowing on the surface of a superconducting cylinder resulting from vector addition of the transport current density Jtr and the shielding current density Jsh . in the notation of that figure, we have at this point, Bapp = Bk (2.78) Itr = 2 R Jk (2.79) where in a typical experimental situation the applied quantities Bapp and Itr are often known. This analysis was carried out by equat ing the vector sum of the applied field and the field arising from the transport current to the critical field Bc T . An alternate way of analyzing this situation is to equate the vector sum of the transport current density and the shielding current density to the critical cur rent density Jc T at the same temperature. This can be done with the aid of Fig. 2.52 to give the expression �� Jc T = Bapp 0 �2 � Itr + 2 R �2 �1/2 (2.80) which is the counterpart of Eq. (2.77). In this section we assumed axially applied fields and currents and neglected demagnetizing effects that depend on the shape of the sample. More general cases are far more difficult to analyze. Several superconductivity texts cover the material found in this chapter. Five of them may be cited: Kresin and Wolf, 1990; Orlando and Delin, 1991; Rose-Innes and Rhoderick, 1994; Tilley and Tilley, 1986; Tinkham, 1985. Ott (1993) surveyed the progress in superconduc tivity from 1980 to 1990 and provided a collection of reprinted articles. Other sources of introductory material are Hettinger and Steel (1994), Sheahan (1994), and Shi (1994). There are Landolt–Börnstein data tabulations on the classic superconductors by Flükiger and Klose (1993) and on the cuprates and related compounds by Kazei and Krynetskii (1993). The book by Hermann and Yakhmi (1993) is devoted to the thallium com pounds. The Handbook of superconductivity edited by Poole (2000) contains much pertinent information. PROBLEMS 1. A wire with a radius of 1 cm is produced from a superconductor with a transition temperature of 120 K. It is in a longitudi nal magnetic field of 40 T at 60 K, and it is found that increasing the applied cur rent to 103 A drives it normal. What are the values of the upper critical field, the critical current, and the critical current density for the wire at 60 K and in the limit T → 0 K? Assume that Bc and Bc2 exhibit the same temperature behavior. 2. A cylindrical superconductor of radius 200 cm with an axial hole in the cen ter of radius 100 cm is located in a par allel magnetic field of 2 T at 300 K. It has a penetration depth of 2000 Å. What amount of flux is stored in the super conducting material and in the hole if the sample is cooled to 40 K, well below Tc = 90 K. If the applied field is reduced to 0.5 T, how will these stored fluxes change? What is the value of the current density on the outside surface and on the inside surface for these two cases? 3. What is the resistance of a 50-cm length of niobium wire of diameter 3 mm at 300 K? How much longer would a wire made of copper have to be in order to have the same resistance? 59 PROBLEMS 4. A superconducting wire 4 mm in diame ter is formed into a loop of radius 7 cm. If a super current persists unchanged in this wire for 12 years, what is the approxi mate upper limit on the resistivity? 5. Show that Eqs. (2.59)–(2.61) provide the limiting behaviors of Eqs. (2.56)–(2.58), respectively, in the limit T → Tc . 6. Show that Eqs. (2.62)–(2.64) provide the limiting behaviors of Eqs. (2.56)– (2.58), respectively, as the temperature approaches absolute zero. 7. Explain how the analysis of Fig. 2.49 that is given in Section XVI is based on the assumptions that were made con cerning Jc T Bc T, and the shape of the curve in the figure. 8. Derive Eq. (2.80). 9. Give the location of point in Fig. 2.46, of point k in Fig. 2.47, and of point j in Fig. 2.48. 10. What is the concentration of super elec trons at T = 0 K T = 41 Tc , T = 21 Tc , and T = 11Tc in a superconductor with a penetration depth of 150 nm? What is the concentration of normal conduction electrons at these temperatures? 11. A Type I superconductor has a critical field Bc = 03 T and a critical current 12. 13. 14. 15. 16. density Jc = 2 × 104 A/cm2 at 0 K. Find Bc Jc , and ns at T = 21 Tc . If a transport current density of 9000 A/cm2 is flowing through the super-conductor of Problem 11 at 0 K, what magnetic field will drive it normal? A Type I superconducting wire 3 mm in diameter has a critical field Bc = 04 T and a critical current density Jc = 3 × 104 A/cm2 at 0 K. What is the max imum transport current that can flow through it at 0 K in an applied field of 0.35 T? A Type I superconductor with Tc = 7 K has slope dBc /dT = 25 mT/K at Tc . Estimate its critical field at T = 6 K. Show that for a particular temperature T a plot of the critical surface Bapp versus 0 Jtr is an arc of a circle a distance Bc T from the origin. If it is assumed that the a direction electrical conductivity arises from the planes and that the b direction con ductivity is the sum of the contribu tions from the planes and chains (as explained in Section 7.VI), find plane and chain for YBa2 Cu3 O7 at 100 K and 275 K. This page intentionally left blank 3 Classical Superconductors I. INTRODUCTION In this chapter we will survey the prop erties of various classes of elements and compounds that are superconductors below about 25 K. We will begin with the sim plest group, namely the elements, and will proceed to discuss the binary, ternary, and larger compounds. Then we will treat the A15 compounds such as Nb3 Sn that, until the discovery of the high Tc types, produced the highest transition temperatures of all. Following this discussion we will review the Laves phases, the Chevrel phases, the chalco genides, and the oxides. II. ELEMENTS Superconductivity was first observed in 1911 in the element mercury with Tc = 41 K, as shown in Fig. 2.2. Two years later lead surpassed mercury with Tc = 72 K. Niobium with Tc = 925 K held the record for high est Tc for the longest period of time, from 1930 to 1954 when the A15 compounds came to prominence. Other relatively high-Tc ele ments are Tl (2.4 K), In (3.4 K), Sn (3.7 K), Ta (4.5 K), V (5.4 K), La (6.3 K), and Tc (7.8 K), as shown in Table 3.1. Figure 3.1 shows how the super-conducting elements are clustered in two regions of the peri odic table, with the transition metals on the left and the nontransition metals on the right. Some elements become superconduct ing only as thin films, only under pressure, or only after irradiation, as indicated in the figure. We see from Table 3.1 that the great majority of the superconducting elements 61 62 3 CLASSICAL SUPERCONDUCTORS Table 3.1 Properties of the Superconducting Elementsa Z 4 13 21 22 23 30 31 40 41 42 43 44 48 49 50 57 57 71 72 73 74 75 76 77 80 80 81 82 90 91 95 a b Elementb Ne Be Al Sc Ti V Zn Ga Zr Nb Mo Tc Ru Cd In Sn(w) La La Lu Hf Ta W Re Os Ir Hg Hg Tl Pb Th Pa Am 2 3 3 4 5 12 3 4 5 6 7 8 12 3 4 3 3 3 4 5 6 7 8 9 12 12 3 4 4 5 9 Crystal Tc Structurec (K) �D (K) hcp fcc hcp hcp bcc hcp orthr hcp bcc bcc hcp hcp hcp tetrg tetrg hcp fcc hcp hcp bcc bcc hcp hcp fcc trig tetrg hcp fcc fcc 940 420 470 415 383 316 325 290 276 460 411 580 210 108 195 152 140 fcc 0026 118 001 040 540 085 108 061 925 092 78 049 0517 341 372 488 63 01 013 447 0015 170 066 011 415 39 238 720 138 14 10 252 258 383 415 500 425 88 93 79 96 165 Bc (mT) 2Bc /Tc (mT/K) � � � � × 106 mJ cm3 /mole mole K2 105 18 56 1410 54 583 47 2060 96 1410 69 28 282 305 800 1100 <350 127 829 012 200 70 16 411 339 178 803 160 28 52 12 11 15 45 21 36 28 11 17 16 33 37 021 14 109 33 982 066 060 277 780 183 628 28 069 167 178 98 113 20 37 16 24 21 29 20 17 15 22 23 22 615 090 235 235 32 181 137 147 31 432 � �∗c 155 300 038 060 017 017 129 212 89 270 39 041 082 041 015 015 010 038 014 70 162 53 68 13 24 014 075 025 037 044 035 010 012 080 155 Nc is as defined in Fig. 3.1; D , Debye temperature; Bc , critical field; , electronic specific heat parameter; , susceptibility; , electron–phonon coupling constant; ∗c , Coulomb pseudopotential; P, pressure; WF, work function Eq , energy gap; and DEF , density of states at the Fermi level. Most of the data in the table come from Roberts (1976), Vonsovsky et al. (1982), and Handbook of Chemistry as Physics, 70th edition (1989–1990). Sn is the gray diamond structure form below 132 C, and the white tetragonal form above; La is the fcc form above 310 C, and the hcp form at lower temperatures. have crystallographic structures of very high symmetry, either face-centered cubic (10, fcc), hexagonal close-packed (15, hcp), or body-centered cubic (11, bcc), with the unit cells sketched in Fig. 3.2. The fcc and hcp structures provide the densest possible crystallographic packing, with each atom sur- rounded by 12 equidistant nearest neighbors. Other cases include trigonal Hg, tetragonal In, tetragonal (white) Sn, and orthorhom bic Ga. Slightly more than half of the ele ments that are superconducting are mem bers of different transition series, for exam 63 II ELEMENTS dT c /dP (K/GPa) 06 63 P (GPa) � 0–1.4 0–2.5 045 150 −20 −14 −125 −23 0–2.0 0–2.5 0–2.5 0–1.5 0–1.8 190 110 0–2.3 −26 −26 0–1.0 −23 −18 0–1.8 0 037 0 05 047 WF (eV) Eg = 2� (meV) Eg /kT c 035 34 16 023 033 34 32 35 30 026 24 015 014 105 14 15 38 34 36 35 32 36 44 35 50 43 59 433 43 43 405 43 46 50 47 42 38 438 45 023 020 050 452 050 048 37 43 0028 0044 ≈17 ≈0006 078 029 0048 17 ple, the first transition series from scandium to zinc (5), which has an incomplete 3dn electron shell; the second transition series from yttrium to cadmium (8), with 4dn electrons; the third such series from lute cium to mercury (8), with 5dn electrons; the rare earths from lanthanum to ytterbium (3), which have an incomplete 4f n electron shell; and the actinides from actinium to lawren cium (4), with 5f n electrons (the number of superconductors in each class is given in parenthesis). Among the elements niobium has the highest transition temperature, and perhaps not coincidentally it is also a constituent of 079 27 041 33 39 ≈35 ≈45 34 48 56 46 38 43 34 DEF (states, atom eV) ≈14 ≈21 ≈08 ≈21 065 091 083 ≈17 ≈05 076 070 Z 4 13 21 22 23 30 31 40 41 42 43 44 48 49 50 57 57 71 72 73 74 75 76 77 80 80 81 82 90 91 95 higher Tc compounds such as Nb3 Ge. Nio bium has not appeared prominently in the newer copper oxide superconductors. Of the transition elements most com monly found in the newer ceramic-type superconductors, lanthanum is superconduct ing with a moderately high Tc (4.88 K for the or hcp form and 6.3 K for the or fcc form), yttrium becomes superconducting only under pressure (Tc ≈ 2 K for pressure P in the range 110 ≤ P ≤ 160 kbar), and copper is not known to super conduct. Studies of the transition temperature of copper alloys as a function of copper content have provided an extrapolated value of Tc = 6 × 10−10 K for 64 3 CLASSICAL SUPERCONDUCTORS Figure 3.1 Periodic table showing the superconducting elements together with their transition temperatures Tc and some of their properties (Poole et al., 1988). Figure 3.2 Body-centered cubic, face-centered cubic, and hexagonal close-packed unit cells. Cu which, while nonzero, cannot be achieved experimentally. The nontransition elements oxygen and strontium present in these com pounds do not superconduct, barium does so only under pressure (Tc = 1 K to 5.4 K under pressures from 55 to 190 kbar), bis muth likewise superconducts under pressure, and thallium is a superconductor with Tc = 24 K. Lead, added in low concentrations to stabilize the bismuth and thallium high-Tc compounds, is also a well-known elemen tal superconductor. Thus the superconduct ing properties of the elements are not always indicative of the properties of their com pounds, although niobium seems to be an exception. III. PHYSICAL PROPERTIES OF SUPERCONDUCTING ELEMENTS Figure 3.1 gives the transition tempera ture Tc , Debye temperature D , Sommerfeld constant, or normal-state electronic spe cific heat constant from Eq. (1.51), Ce = T , dimensionless electron–phonon coupling constant (cf. Chapter 6), and den sity of states DEF at the Fermi level (1.42) III PHYSICAL PROPERTIES OF SUPERCONDUCTING ELEMENTS for different elemental superconductors. The columns of the periodic table are labeled with the number of (valence) elec trons Ne outside the closed shells. Table 3.1 lists various properties of some of these elements. When an element has more than one isotope, the transition temperature often decreases with increasing isotopic mass M in accordance with the relation M Tc = constant 65 corresponding to the configuration of the next lower noble gas. Figure 3.3 shows that Tc is a maximum for transition metals with five and seven valence electrons; Figs. 3.4, 3.5, 3.6, and 3.7 show that the Sommer feld factor of the conduction-electron heat capacity Ce = T , the magnetic sus ceptibility = M/ 0 H, the square of the (3.1) where = 1/2 for the simplified BCS model described in Chapter 7. This is to be expected for a simple metal because the phonon fre quency is proportional to the square root of the atom’s mass. However electron– phonon coupling can also be mass depen dent, and deviations from Eq. (3.1) are not unusual. Some elemental superconductors have isotope effect coefficients close to 1/2, such as Hg (0.50), Pb (0.48), Sn (0.47), and Zn (0.45). Most values of listed in Table 3.1 for the transition metal supercon ductors are less than this BCS-theory esti mate. For the two metals zirconium and ruthenium, both with Tc < 01 K is zero to within experimental error. The BCS theory predicts that twice the energy gap 2 of a superconductor is 3.52 times kB Tc (cf. Chapter 7, Section VI) and from the data in Table 3.1 it is clear that this prediction is fairly well satisfied for the elements. In rhenium the energy gap is anisotropic, varying between 2.9 and 39 kB Tc , depending upon the direction. The anisotropies found for molybdenum and vanadium are half as large and almost within the experimental accuracy. It has been found that some of the properties of an element correlate with the number Ne of its valence electrons in the same manner as the transition temperature (Vonsovsky et al., 1982). Here Ne is the number of electrons outside the filled shells Figure 3.3 Dependence of transition temperature on the number of valence electrons Ne in the super conducting transition elements (Vonsovsky et al., 1982, p. 184). Figure 3.4 Dependence of electronic specific heat on Ne , as in Fig. 3.3 (Vonsovsky et al., 1982, p. 184). 66 3 CLASSICAL SUPERCONDUCTORS Figure 3.7 Dependence of electron–phonon coupling constant p. 211). Figure 3.5 Dependence of magnetic susceptibility on Ne , as in Fig. 3.3 (Vonsovsky et al., 1982, p. 185). inverse of the Debye temperature D , and the electron–phonon coupling constant defined by Eq. (7.96) all exhibit similar behavior. These quantities, together with the dimensionless screened Coulomb interaction Figure 3.6 Dependence of inverse Debye tempera ture squared 1/D2 on Ne , as in Fig. 3.3 (Vonsovsky et al., 1982, p. 185). on Ne , as in Fig. 3.3 (Vonsovsky et al., 1982, parameter ∗C (cf. Chapter 6), are tabulated in Table 3.1 for the superconducting elements. The correlation of the melting points of the transition metals, as plotted in Fig. 3.8, with the number of valence electrons Ne tends to be opposite to the correlation of Tc with Ne — thus the highest melting points occur for six valence electrons for which Tc is the lowest in each series. The chemical bonding of the transition metals is mainly ionic, but there can also be contributions of a covalent type. The Figure 3.8 Dependence of melting temperature on Ne , as in Fig. 3.3 (Vonsovsky et al., 1982, p. 186). 67 IV COMPOUNDS amount of covalency is particularly strong in the two metals molybdenum and tung sten, each of which has five valence elec trons. This fact has been used to account for the low- transition temperatures of these tw elements. Another important electronic parameter of a metal is its density of states DEF at the Fermi level, and Table 3.1 lists values of DEF for different elements. In several cases the value in the table is an average of several determinations with a large amount of scatter. For example, four reported values for niobium of 1.6, 1.8, 2.1, and 2.7 are given by Vonsovsky et al. (1982, p. 202) along with a rounded-off average of 2.1 states/atom eV. These large scatters lead one to sus pect the accuracy of cases in which only one determination is available. The d electrons dominate this density of states, with small contributions from the remaining valence electrons. For example, in vanadium the per centage contributions to DEF from the s, p, d, and f electrons are 1%, 14%, 84%, and 1%, respectively, while for niobium the cor responding percentages are 3%, 14%, 81%, and 2%. When a metal is subjected to high pres sure, the density of states at the Fermi level changes. This change may be detected by the change in the conduction-electron heat capacity factor , since from Eq. (1.52) is proportional to DEF . Sometimes the derivative dTc /dP is positive, as in the case of vanadium (see curve for vanadium plot ted in Fig. 3.9), so that here Tc increases with increasing pressure, and sometimes it is negative, as with tantalum (cf. Fig. 3.9), where high pressures lead to lower val ues of Tc . With some elements the situa tion is more complicated. For example, when niobium is subjected to high pressure Tc decreases until about 40 kbar is reached, then it begins to increase with increasing pressure and, eventually, above 150 kbar, surpasses its atmospheric value, as indicated in Fig. 3.9. Finally some elements, such as P, As, Se, Y, Figure 3.9 Dependence of transition temperature Tc on pressure for the elements Nb, Ta, and V (Vonsovsky et al., 1982, p. 188). Sb, Te, Ba, Ce, and U, become superconduct ing only when subjected to high pressure. Tc of some transition metals rises dra matically when the metal is in the form of thin films made by ion sputtering on var ious substrates. For example, the transition temperature of tungsten (bulk value 0.015 K) rises to 5.5 K in a film, that for molybde num (bulk value 0.915 K) rises to 7.2 K, and that for titanium (bulk value 0.40 K) rises to 2.52 K. Chromium and lithium only super conduct in the thin-film state, while other nonsuperconductors such as Bi, Cs, Ge, and Si can be made to superconduct either by applying pressure or by preparing them as thin films. Figure 3.1 summarizes this infor mation. IV. COMPOUNDS Superconductivity workers sometimes use the old Strukturbericht notation which uses the letter A to denote elements, B for AB compounds, C for AB2 com pounds, and D for Am Bn binary compounds, with additional letters assigned to com pounds containing three or more dissimilar atoms. Superconductors of the class Nb3 Sn were originally assigned to the -W struc ture (Wyckoff, 1963, p. 42), which has 68 3 CLASSICAL SUPERCONDUCTORS two types of tungsten atoms, one type in the center and the other six on the faces of the cubic unit cell; these A3 B compounds came to be called the A15 compounds. The nota tion has endured despite the fact that other compounds such as UH3 and Cr3 Si had been assigned to this structure (Wyckoff, 1964, p. 119) before Pearson described the nota tion in the 1958 Handbook. This notation is no longer widely used outside the supercon ducting community. Several structures contain a large num ber of superconductors. Table 3.2 presents data on the principal superconductors, together with the transition temperature of a representative compound from each group. The table provides the Strukturbericht sym bol, Tc of a prototype compound, and the number of superconducting compounds that are found in the listings of Phillips (1989a) and Vonsovsky et al. (1982) for each group. All of the known nonradioactive elements are constituents of at least one superconduct ing compound, as Table 3.3 shows. The table catalogs the structure types with binary super conducting compounds, and gives the value of Table 3.2 Structure Types and Transition Temperatures of Representative Compounds of each Typea Type Referencec 26 10 10 15 18 a b c d e Ph, Ph, Ph, Ph, Ph, 26 120 12 27 f g Ph, 359 Ph, 347, Vo, 388 HfV2 ZrRe2 RhZr 2 Nb3 Sn La3 Tl UBe13 94 68 113 18 89 09 40 19 16 60 24 9 h i j k l m Ph, 370; Vo, 375 Ph, 357; Vo, 375 Ph, 350 Ph, 336, 363; Vo, 259 Ph, 362 Table 3.10 MoN HfPRu 148 99 170 11 n o Ph, Appendix C Ph, 357 SrTiO3 03 LiTi2 O4 137 3 q Ph, 339; Vo, 431 YRh4 B4 LaMo6 Se8 Ge10 As4 Y5 C60 Rb2 Cs 119 114 91 31 10 88 11 12 r s t u Ph, 347; Vo, 415 Ph, 361; Vo, 418 Ph, 348 Structure and Type Example Tc (K) B1, NaCl, fc cubic B2, CsCl, bc cubic B13, MnP, ortho A12 -Mn, bc cubic B81 , NiAs, hex D102 Fe3 Th7 , hex, 3–7 compound D8b , CrFe, tetrag, -phase C15 MgCu2 , fc cubic, Laves C14 MgZn2 , hex, Laves C16 Al2 Cu, bc tetrag A15 UH3 b , cubic LI2 AuCu3 , cubic Binary heavy fermions Miscellaneous binary compounds C22 Fe2 P, Trig E21 CaTiO3 , cubic, perovskite HI1 MgAl2 O4 , cubic, spinel B4 CeCo4 , tetrag, ternary boride PbMo6 S8 , trig, Chevrel Co4 Sc5 Si10 , tetrag fcc, buckminsterfullerene MoC VRu GeIr Nb018 Re082 Pd11 Te 143 50 47 10 41 B3 Ru7 Mo03 Tc07 a b c Nbr 336, 369; Vo, 393 362; Vo, 385 341 368; Vo, 388 354 p The at one time important but now antiquated Pearson (1958) symbols (e.g., A15) are given for most of the structures. The numbers of compounds listed in column 4 were deduced from data given in the references of column 6. A15 is sometimes called the -Mn or the Cr3 Si structure. Ph and Vo followed by page numbers denote the references Phillips (1989a) and Vonsovsky et al. (1982), respectively. Additional data may be found in Roberts (1976). 69 IV COMPOUNDS Table 3.3 Number of Superconducting Binary Compounds Am Bn of the Elements Discussed in the Literature, and Tc of a Representative Compound of each Element among the Classical Superconductors (see column 5 of Table 3.2 for key to the compound types) Element Binary Compounds Symbol Tc Ka 1 2 11 19 37 55 H Li Na K Rb Cs — — — — — 15P 4 12 20 38 56 Be Mg Ca Sr Ba 5 13 31 49 81 Representative Compound Types Compound Tc K Type 1 2 3 2 2 2 n n n h h h HNb2 LiTi2 O4 Na2 Mo6 S8 Bi2 K C60 Rb2 K Bi2 Cs 73 137 86 358 24 48 n q s h u h 86F — 0.52 — 50P 1 7 6 2 3 n bn hln h n BeTc HgMg Au5 Ca Rh2 Sr BaBi02 O3 Pb08 52 14 038 62 45 n b n h p B Al Ga In Tl — 1.18 1.08 3.41 2.38 12 17 13 9 6 afjrn dghjklmn cjkln ackln ln B4 LuRh4 Nb3 Al Nb3 Ga V3 In TlMo6 Se8 117 19 21 139 122 r k k k s 6 14 32 50 82 C Si Ge Sn Pb — 6.7 5.3 3.7 7.20 14 14 18 16 13 anu chkn ackmn acklmn hjkln C60 Rb2 Cs Nb3 Si Nb3 Ge Nb3 Sn Ta3 Pb 32 19 232 18 17 u k k k k 7 5 33 51 83 N P As Sb Bi — 58P 05P 27P 61F 11 6 9 8 25 an n ckn kn cehln NbN PbP Ge10 As4 Y5 Ti3 Sb BaBi02 O3 Pb08 173 78 91 58 45 a n t k p 8 16 34 52 O S Se Te — — 69P 39P 4 7 7 12 a a a a LiTi2 O4 Sn06 Mo6 S4 TlMo6 Se8 Mo6 S48 Te32 137 142 122 25 q s s s 9 17 35 53 F Cl Br I — — — — 0 0 0 0 — — — — F012 K01 Li002 O288 W Cl3 Mo6 Se8 Br2 Mo6 S6 I2 Mo6 S6 11 91 138 140 n s s s 21 22 23 24 25 26 27 28 29 30 Sc Ti V Cr Mn Fe Co Ni Cu Zn 0.01 0.40 5.40 — — — — — — 0.85 10 10 21 7 9 5 12 5 8 5 bdhin abdkn abghk ghk bcjkmn fgn dfgjn fjkn bjmn n ScMo6 S8 LiTi2 O4 V3 Si Cr3 Os Mn3 Si Fe3 Re2 CoZr 2 Ni3 Th7 Cu18 Mo6 S8 Mo66 S8 Zn11 36 137 172 468 125 66 63 198 108 36 s q k k k g j f s s 39 Y 25P 20 abfhiln B4 YRh4 113 r Z Number u u u u n n n ein (Continued) 70 3 CLASSICAL SUPERCONDUCTORS Table 3.3 (Continued) Element Binary Compounds Representative Compound Symbol Tc Ka Number Types Compound Tc K Type 40 41 42 43 44 45 46 47 48 Zr Nb Mo Tc Ru Rh Pd Ag Cd 0.61 9.25 0.92 7.8 0.49 — — — 0.517 25 41 24 6 18 32 28 6 1 adghijkln acdghjkn adghkmn dgkn bfghikn cfghjkn cdegjkn n n ZrN Nb3 Ge Tc3 Mo Tc3 Mo HfPRu B4 LuRh4 Bi2 Pd3 Ag16 Mo64 S8 CdHg 107 232 158 158 99 117 40 91 177 a k g g o r e s n 71 72 73 74 75 76 77 78 79 80 Lu Hf Ta W Re Os Ir Pt Au Hg 1.0 0.13 4.47 0.015 1.7 0.66 0.11 — — 4.15 6 10 18 12 24 20 30 23 17 10 bhiln adhin acdgjkn adgkn adfghikn bdfghijk dfghikmn bcefghkmn bchjkn n B4 LuRh4 HfV2 Ta3 Pb W3 Re Mo3 Re LaOs2 Ir 04 Nb06 Nb3 Au Ta3 Au Hg2 Mg 117 94 17 114 15 65 10 115 16 40 r h k k k i d k k n 57 58 59 60 61 62 63 64 65 66 67 68 69 70 La Ce Pr Nd Pm Sm Eu Gd Tb Dy Ho Er Tm Yb 4.9 1.7P — — — — — — — — — — — — 21 4 0 0 0 0 1 0 0 0 0 0 0 0 ahn hmn LaMo6 S8 B4 LuRh4 PrMo6 S8 NdMo6 Se8 71 117 40 82 s r s s B4 SmRh4 Eu0012 La0988 GdMo6 Se8 TbMo6 Se8 Dy12 Mo6 Se8 Ho12 Mo6 Se8 B4 ErRh4 B4 TmRh4 Yb12 Mo6 Se8 27 02 56 57 82 61 87 98 62 r n s s s s r r s 90 91 92 Th Pa U 1.38 1.4 1.0 27 0 9 afhijln Pb3 Th 555 l lmn UPt 3 043 m Z a n P denotes Tc measured under pressure, and F indicates measurement on thin film. Tc for a representative superconductor of each element. It is clear that transition temperatures above 10 K are widely distributed among the elements and compounds. On the whole, there is a tendency for the superconducting materials to be stoichiometric, i.e., with ratios of the constituent elements generally integral. Even some of the solid solutions, such as Nb075 Zr 025 and Nb075 Ti025 , have atom ratios that are easily expressed in terms of integers (Nb3 Zr and Nb3 Ti), though others, such as Mo038 Re062 , do not fit this format. Indeed, Tc is often sensitive to stoichiometry, and experiments in which Nb3 Ge gradually approached stoi chiometry raised its measured Tc from 6 K V ALLOYS to 17 K and, finally, to the previous record value of 23.2 K. Other materials have under gone the same evolution with the approach to ideal stoichiometry, such as Nb3 Ga (Tc going from 14.9 to 20.3 K), V3 Sn (Tc from 3.8 to 17.9 K), and V3 Ge (Tc increasing from 6.0 to 11.2 K). In contrast, there are compounds, such as Cr3 Os Mo3 Ir Mo3 Pt, and V3 Ir, in which the highest Tc does not occur at the ideal stoichiometric composition and in which Tc is generally less dependent on composition. For example Tc = 016 K in stoichiometric Cr3 Ir but Tc = 075 K in Cr082 Ir 018 . Although less prevalent among the older superconducting types, this phe nomenon is not unusual among the newer superconductors (cf. Vonsovsky et al., 1982, for more details). V. ALLOYS An alloy is a solid solution or mixture in which the constituent atoms are randomly distributed on the lattice sites. An intermetal lic compound, on the other hand, contains definite ratios of atoms that are crystallo graphically ordered in the sense that there is a unit cell that replicates itself through out space to generate the lattice. Some alloys become ordered for particular ratios of atoms. Both random and ordered materials can become superconducting. First we will consider the random binary alloys. In these types of alloys two transi tion elements are mixed in all proportions. There are several possibilities for the transi tion temperature of such an alloy: it can be higher than that of both elements, between the Tc values of the constituents, or lower than either constituent taken by itself. The curve of Tc versus binary alloy concentration can be close to a straight line, concave down wards with a minimum, or concave upwards with an intermediate maximum value. These three alternatives are illustrated in Fig. 3.10. The figure shows how Tc varies with Nb con tent when niobium is alloyed with any one of 71 the transition elements V, Zr, Mo, Ta, or W, with the plots arranged in the order in which the five transition elements are distributed around niobium in the periodic table. We see from Fig. 3.10 that the transition temperature reaches a maximum with an alloy containing 25 at-% zirconium. The figure also shows that it can be very small for alloys with Zr, Mo, or W. To gain some understanding of the shapes of these curves systematic studies involving sequences of transition metals that are adjacent to each other in the periodic table have been carried out. (See Vonsovsky et al., 1982.) The results indicate that Tc varies with the number of valence electrons Ne in the manner illustrated in Fig. 3.11. The curves have two maxima of Tc , one near Ne = 47 and one near Ne = 65. The peak in the Nb versus Zr plot of Fig. 3.10 occurs close to Ne = 47. Amorphous alloys exhibit only one maximum for each series, as indi cated in Fig. 3.12. Other properties, such as the electronic specific-heat factor that was defined in Eq. (1.51), magnetic susceptibility , and pressure derivative dTc /dP have the dependences on electron concentration that are illustrated in Figs. 3.13, 3.14, and 3.15, respectively. The specific heat and suscep tibility plots are similar to the Tc versus Ne graph of Fig. 3.11. In addition to the correlation of the tran sition temperature with the valence elec tron concentration, there is also a correlation with the lattice properties. The body-centered cubic structure is the stable one for Ne in the range from 4.5–6.5, with hcp the stable struc ture outside this range, as shown in Fig. 3.16. The peaks in the plot of Tc versus Ne occur at the boundaries of instability—i.e., where a lattice rearrangement transition can occur between the two structure types. The lowest Tc occurs (Fig. 3.11) for Ne ≈ 55–6, which is also where the bcc structure is most stable. The alloy types listed in Table 3.2 are binary; most of them having their compo nent elements in an atom ratio of 1 : 1, 1 : 2, 72 3 CLASSICAL SUPERCONDUCTORS Figure 3.10 Dependence of transition temperature Tc on concentration for binary alloys of Nb with adjacent transition elements in the periodic table. The abscissae are expressed in percentages (adapted from Vonsovsky et al., 1982, pp. 234, 235). or 1 : 3. In most cases at least one con stituent is an elemental superconductor, and sometimes (e.g., NbTc3 , VRu) both elements superconduct. Occasionally, more than one intermetallic stoichiometry (e.g., RhZr 2 and RhZr 3 Nb3 Ge and NbGe2 ) is superconduct ing. The binary superconductors in Table 3.2 have Tc values higher than the highest Tc of their constituents, although even here VRu is an exception. The high-Tc semiconduct ing and layered compounds tend to be binary also. Some of the compounds in Table 3.2 are ternary types and even Lu075 Th025 Rh4 B4 is really the ternary compound MRh4 B4 with Lu occupying three-quarters and Th onequarter of the M sites. VI. MIEDEMA’S EMPIRICAL RULES Matthias (1953, 1955) interpreted the shape of the curve of Tc versus Ne as indi cating the presence of favorable and unfa vorable regions of Ne and suggested rules 73 VI MIEDEMA’S EMPIRICAL RULES Figure 3.11 Dependence of transition temperature Tc on the number of valence electrons Ne in solid solutions of adjacent 3d 4d , and 5d� elements in the periodic table. Dark symbols are for pure elements (Vonsovsky et al., 1982, p. 239). for explaining the Tc -versus-concentration curves. One rule, for example, explains the increase of Tc in terms of the shift of Ne toward more favorable values; thus Ne = 5V Tc = 54 K Nb Tc = 93 K Ta Tc = 45 K and Ne = 7 Tc Tc = 78 K Re Tc = 17 K. Miedema (1973, 1974) proposed an empirical method of correlating the con centration dependence of the transition temperature and other physical characteris- Figure 3.12 Dependence of transition temperature Tc on the number of valence electrons Ne in amorphous alloys of 3d 4d, and 5d elements, using the notation of Fig. 3.11 (Vonsovsky et al., 1982, p. 241). tics of alloys. The method assumes that the density of states DEF AB = DAB at the Fermi level of an alloy AB is an additive function of its constituents, DAB = fA DA NA + fB DB NB (3.2) where fA and fB are the mole fractions of the components A and B, and the densities of states DA and DB depend on the num ber of valence electrons NA and NB of atoms A and B, respectively (cf. Vonsovsky et al. (1982, Section 5.4) for evaluation of the Figure 3.13 Dependence of electronic specific heat on Ne , as in Fig. 3.11 (Vonsovsky et al., 1982, p. 237). 74 3 CLASSICAL SUPERCONDUCTORS AB = fA A NA + fB B NB (3.3) The density of states and depend upon the number of valence electrons per atom Ni in a similar manner for the 3d 4d, and 5d tran sition ion series. Some electron concentra tion is transferred between the atoms during alloying, so that the number of valence elec trons of the ith component Ni differs from its free atom value Nei by the factor Ni = Nei + K 1 − fi Figure 3.14 Dependence of magnetic susceptibility on Ne , as in Fig. 3.11. Points are plotted for Mo– Ru instead of Tc–Ru, and for Ta–Re instead of Ta–W for the same Ne , since data were not available for the preferred adjacent elements (Vonsovsky et al., 1982, p. 242). Ni dependences of the functions Di and i in Eq. (3.2)). Equation (1.52) permits us to write a similar expression for the electronic heat capacity factor : (3.4) where is the difference between the work functions (cf. Chapter 15, Section II, A) of the two pure metals involved in the alloy. Table 3.1 lists the work functions of the superconducting elements. Empirical expres sions similar to Eqs. (3.2) and (3.3) have been written for the electron–phonon cou pling constant AB , AB = fA A NA + fB B NB (3.5) and for the quantity lnTc /D −1 for the binary alloys, fA 1 = lnTc /D AB lnTc /D A + fB lnTc /D B Figure 3.15 Dependence of pressure derivative dTc /dP on Ne in alloys of adjacent 4d and 5d elements, following Fig. 3.11 (Vonsovsky et al., 1982, p. 238). (3.6) 75 VII COMPOUNDS WITH THE NaCl STRUCTURE VII. COMPOUNDS WITH THE NaCl STRUCTURE Figure 3.16 Sketch of the structure dependence of the transition temperature for alloys of adjacent transi tion elements, showing how Tc peaks at the boundaries between structure types (Vonsovsky et al., 1982, p. 245). Figure 3.17 shows that the agreement of Eqs. (3.3) and (3.6) with experiment is good for four isoelectronic alloy systems over the entire solid solution range. We see from this figure that the linear approximation obtained by setting K = 0 in Eq. (3.4), hence replacing Ni by Nei in Eqs. (3.2)–(3.6), does not agree with experiment. The B1 class of AB superconductors has the metallic atoms A and nonmetallic atoms B arranged on a sodium chloride-type lat tice that consists of two interpenetrating fcc lattices with each atom of one type in the center of an octahedron whose vertices are occupied by atoms of the other type, as indi cated in Fig. 3.18. As of 1981, 26 B1 com pounds (out of the 40 B1 compounds that had been tested) had been found to be super conducting. The carbides AC and nitrides AN, such as NbN with Tc = 17 K (Kim and Riseborough, 1990), had the 12 high est transition temperatures, while the metallic A atoms with Tc values above 10 K were Nb, Mo, Ta, W, and Zr. Niobium always seems to be the best! Three examples of supercon ducting NaCl-type compounds are given in Tables 3.2 and 3.3. The NaCl-type superconductors are compositionally stoichiometric but not struc turally so. In other words, these compounds have a small to moderate concentration of vacancies in the lattice, as indicated in Table 3.4. We see from the table that YS has Figure 3.17 Comparison of calculated (—) and experimental (symbols) values of the specific heat coefficient and the transition temperature Tc for four isoelectronic binary alloys. The linear approximation (- - - -), which is obtained by setting Ni = Nei in Eqs. (3.3) and (3.6), does not fit the data very well (Vonsovsky et al., 1982, p. 250). 76 3 CLASSICAL SUPERCONDUCTORS Table 3.5 Nonstoichiometric Compounds Ax By with NaCl Structure with Vacancy Ordering on One Sublattice and Stoichiometric Compounds Ax Bx with this Structure (shown in square brackets) with Vacancy Ordering on Two Sublatticesa � Ax Bx C N Ti Figure 3.18 Structure of NaCl in which each atom ) is in the center of an octahedron of one type ( or whose vertices are occupied by atoms of the other type ( or ). • • 10% vacancies, which means that its chem ical formulae should properly be written Y09 S09 . Nonstoichiometric NaCl-type com pounds, such as Ta10 C076 , also exist. Ordinarily the vacancies are random, but sometimes they are ordered on the met alloid (e.g., Nb10 C075 ) or on the metal lic (e.g., V0763 O10 ) sublattice, and can also produce a larger unit cell in, for example, Ti10 O07 . The vacancies can also be ordered on both sublattices in stoichiometric com pounds, such as Nb075 O075 . Table 3.5 lists several NaCl-type compounds with ordering Table 3.4 Percentage of Vacancy Concentration 1001 − x in Stoichiometric Compounds Ax Bx with NaCl Structurea � Ax Bx C N O Ti V Y Zr Nb Hf Ta 2 8.5 40 10 15 11–15 3.5 0.5–3.0 4 0.5 35 13 a 20 After Vonsovsky et al., 1982. 25 S Se 10 20 16 V Nb Ta a V10 C084 Nb10 C075 Ta10 C076 V10 N075 O Ti10 O07 Ti085 O085 V0763 O10 Nb075 O075 After Vonsovsky et al., 1982, p. 394. of the vacancies. It has been found that the metallic and nonmetallic atoms can be absent over broad composition ranges. VIII. TYPE A15 COMPOUNDS The highest transition temperatures for the older superconductors were obtained with the A15 intermetallic compounds A3 B, and extensive data are available on these com pounds. Nb3 Sn can be considered the proto type of this class. These compounds have the (simple) cubic structure (Pm3n, O3h ) sketched in Fig. 3.19 with the two B atoms in the unit cell at the body center 21 21 21 and apical (0, 0, 0) positions, and the six A atoms paired on each face at the sites 0 21 41 0 21 43 21 41 0 21 3 0 41 0 21 43 0 21 , a configura 4 tion that amounts to the presence of chains of A atoms with spacing of one-half the lat tice constant a. The A atom is any one of the transition elements (but not Hf) shown in the center of Fig. 3.10. The B element is either a transition element or is in row III (Al, Ga, In, Tl), row IV (Si, Ge, Sn, Pb), row V (P, As, Sb, Bi), or row VI (Te) of the periodic table. High transition temperatures occur when B is either a metal (Al, Ga, Sn) 77 VIII TYPE A15 COMPOUNDS Table 3.6 Superconducting transition temperatures Tc of some A15 compounds A3 B. The number of valence electrons is given for each element. Data are from Phillips (1989a) and Vonsovsky et al. (1982). B Figure 3.19 The unit cell of the A15 compound A3 B showing B atoms at the apical and body center positions and A atoms in pairs on the faces of the cube (Vonsovsky et al., 1982, p. 260; see also Wyckoff, 1964, p. 119). or a nonmetal (Si, Ge), but not a transition element. Table 3.6 shows seven A elements and 20 B elements for a total of 140 possibil ities, 60 of which superconduct. Two addi tional A15 superconductors are V3 Ni with Tc = 03 K and W3 Os with Tc = 114 K. Stoichiometry is important, and paying attention to it has produced higher transition temperatures, as was explained in Section IV. Typical A15 compounds A3 + x B1 − x have nar row ranges of homogeneity. They are homo geneous toward A, with deviations from stoichiometry, x > 0, that tend to main tain the chains intact. Some atypical com pounds, such as A3 − x B1 + x , are homoge neous toward B so that the chains are affected, and can have their highest Tc val ues when they deviate from ideal stoichiom etry. Figure 3.20 shows that there is a close correlation between the transition tempera ture and the valence electron concentration Ne . We see that high values of Tc occur for Ne = 45 Nb3 Ga Tc = 203 K Ne = Tc = 232 K Ne = 475 Nb3 Ge 625 Nb3 Pt Tc = 109 K, and Ne = 65 (TaAu, Tc = 13 K). The specific-heat fac tor plotted in Fig. 3.21 and the magnetic (Vonsovsky et al., 1982) susceptibility show the same correlation (cf. Hellman and Geballe, 1987). The Villars–Phillips approach (1988, Phillips 1989a, p. 324) adds A3 Ti 4 Zr V 4 5 Nb 5 Al 3 Ga 3 In 3 Tl 3 118 168 139 188 203 92 9 Si 4 Ge 4 Sn 4 Pb 4 171 112 09 70 08 19 232 180 80 As 5 Sb 5 Bi 5 58 02 08 58 34 22 45 Ta 5 Cr 6 06 08 80 84 17 12 150 150 Ru 8 Os 8 Pd 10 Pt 10 Au 11 17 18 07 Tc 7 Re 7 Rh 9 Ir 9 Mo 6 34 106 47 127 57 11 54 10 17 26 32 100 66 05 008 37 109 04 09 32 115 03 08 96 88 160 two additional parameters for high-Tc values. For further details see Sect. XIII of Chap. 7 of the first edition of this work. The superconducting energy gap data vary over a wide range, with 2 /kB Tc in the range 0.2–4.8, low values probably rep resenting poor junctions. The A15 group has some weak-coupled, BCS-like com pounds, such as V3 Si with 2 /kB Tc ≈ 35, and some strong coupled compounds, such as Nb3 Sn with 2 /kB Tc ≈ 43 and Nb3 Ge with 2 /kB Tc ≈ 43. The electron–phonon coupling constant has been reported to vary between the weak coupling value of 0.1 and the strong coupling value of 2.0 (see Table 7.3). 78 3 CLASSICAL SUPERCONDUCTORS Figure 3.20 Dependence of transition temperature Tc on the number of valence electrons Ne in A075 B025 compounds with the A15 structure. The A element is specified by the symbol at the top right, and the B element (see Fig. 3.19) is indicated at the experimental points (Vonsovsky et al., 1982, p. 269). Some A15 compounds undergo a reversible structural phase transformation above Tc from a high-temperature cubic phase to a low-temperature tetragonal phase that deviates very little from cubic c − a/a ≈ 3 × 10−3 . At the transformation each atom remains close to its original site and the volume of the unit cell remains the same. Table 3.7 lists some transformation temper atures and c − a/a ratios. There is no isotope effect in this class of compounds, meaning that = 0 in Eq. (3.1). In addition there is a large scatter in the data on the change of Tc with pressure, dTc /dP, as Fig. 3.22 indicates (cf. Ota, 1987). IX. LAVES PHASES There are several dozen metallic AB2 compounds called Laves phases which are superconducting; the transition temperatures of some of these compounds are listed in Table 3.8. The C15 Laves phases have the cubic Fd3m O7h structure sketched in Fig. 3.23, and the C14 phases are hexagonal, 79 IX LAVES PHASES Figure 3.21 Dependence of electronic specific heat on Ne in A15 compounds, using the notation of Fig. 3.20 (Vonsovsky et al., 1982, p. 271). The dependence of the magnetic susceptibility on Ne produces a similar plot (Vonsovsky et al., 1982, p. 271). Table 3.7 Structural Transformation Temperature Tstr and Anisotropy c − a/a in the Low-Temperature Tetragonal Phase of Several A15 type Superconductorsa Compound Tstr (K) Tc (K) V3 Si Nb3 Sn V3 Ga Nb3 Al Nb3 Al075 Ge025 Nb31 Al07 Ge03 21 43 >50 80 105 130 17 18 145 179 185 174 a cf. Vonsovsky et al., 1982, p. 278. Anisotropy c − a/a 00024 −00061 — — −0003 — Reference Batterman and Barrett (1964) Mailfert et al. (1967) Nembach et al. (1970) Kodess (1973, 1982) Kodess (1973, 1982) Kodess (1973, 1982) 80 3 CLASSICAL SUPERCONDUCTORS Figure 3.22 Dependence of pressure derivative dTc /dP on Ne in A15 compounds, following Fig. 3.20 (Vonsovsky et al., 1982, p. 288). Table 3.8 Superconducting transition temperatures Tc of selected Laves phase AB2 compounds. Those labeled with an asterisk ∗ are hexagonal, and the remaining ones are cubic. The data are from Phillips (1989a) and Vonsovsky et al. (1982). A B2 V 6 Mo 6 Te 6 Re 7 Ru 8 Os 8 Ca 2 Sr 2 Sc 3 Y3 La 3 Zl 4 Hf 4 Th 4 96 94 013 007∗ 76∗ 56∗ 42∗ 18∗ 23∗ 24∗ 44 46∗ 47∗ 89 68∗ 56∗ 50∗ 18∗ 30∗ 27∗ Lu as noted in Table 3.2. One additional Laves superconductor HfMo2 has the C36 hexagonal structure with a larger unit cell. Some have critical temperatures above 10 K and high critical fields. For example, Zr 21 Hf 21 V2 has Tc = 101 K Bc2 = 24 T, and a compound with a different Zr/Hf ratio has similar Tc and Bc2 values with Jc ≈ 4 × 105 A/cm2 . These materials also have the advantage of not being as hard and brittle as some other intermetallics and alloys with comparable transition temperatures. Rh 9 Ir 9 64 62 62 57 62 25 21 05 07 05 41 35 09∗ Pt 16 65 35∗ 13 29 X. CHEVREL PHASES The Chevrel phases Ax Mo6 X8 are mostly ternary transition metal chalco genides, where X is S, Se, or Te and A can be almost any element (Fischer, 1978). These compounds have relatively high transition temperatures and critical fields Bc2 of several teslas. However, the critical currents, typi cally 2 to 500 A/cm2 , are rather low. Sub stituting oxygen for sulphur in Cu18 Mo6 S8 raises Tc (Wright et al., 1987). Table 3.9 81 X CHEVREL PHASES Figure Figure 3.23 Crystal structure of the Laves phase (Vonsovsky et al., 1982, p. 376). lists several dozens of these superconductors and their transition temperatures. Figure 3.24 compares the critical currents (see Fig. 5.26 for a comparison of the critical fields for several superconductors). The trigonal structure sketched in Fig. 3.25, with space group R3, C23i , is a simple cubic arrangement slightly dis torted along the (111) axis of the Mo6 X8 group building blocks, each consisting of a deformed cube with large X atoms at the vertices and small Mo atoms at the cen ters of the faces. The Mo6 X8 group may be looked on as an Mo6 octahedron inscribed in an X8 cube. Mo6 X12 -group building blocks 3.24 Comparison of the critical current densities on the applied field for a, SnGa025 Mo6 S8 b V3 Ga, and c, Nb3 Sn (Alekseevskii et al., 1977). Figure 3.25 Structure of the Chevrel phase Ax Mo6 X8 (Vonsovsky et al., 1982, p. 431). Table 3.9 Superconducting Transition Temperatures of some Chevrel compoundsa Ax Mo6 S8 Tc K Ax Mo6 Se8 Tc K Misc. Compounds Tc K Mo6 S8 Cu2 Mo6 S8 LaMo6 S8 PrMo6 S8 NdMo6 S8 Sm12 Mo6 S8 Tb12 Mo6 S8 Dy12 Mo6 S8 Ho12 Mo6 S8 Er12 Mo6 S8 Tm12 Mo6 S8 Yb12 Mo6 S8 Lu12 Mo6 S8 185 107 70 26 35 24 14 17 20 20 20 ≈ 87 20 Mo6 Se8 Cu2 Mo6 Se8 La2 Mo6 Se8 PrMo6 Se8 NdMo6 Se8 Sm12 Mo6 Se8 Tb12 Mo6 Se8 Dy12 Mo6 Se8 Ho12 Mo6 Se8 Er12 Mo6 Se8 Tm12 Mo6 Se8 Yb12 Mo6 Se8 Lu12 Mo6 Se8 65 59 117 92 84 68 57 58 61 62 63 58 62 Pb09 Mo6 S75 PbGd02 Mo6 S8 PbMo6 S8 Sn12 Mo6 S8 SnMo6 S8 LiMo6 S8 NaMo6 S8 KMo6 S8 Br2 Mo6 S6 I2 Mo6 Se7 BrMo6 Se7 IMo6 Se7 I2 Mo6 Te6 152 143 126 142 118 40 86 29 138 140 71 76 26 a See Phillips (1989a, pp. 339, 361) and Vonsovsky et al. (1982, p. 419) for more complete listings. 82 are also found. The distortions are not shown in the figure. The parameter x in the for mula Ax Mo6 X8 assumes various values such as x = 1 (e.g., YMo6 S8 LaMo6 S8 ), x = 12 (e.g., V12 Mo6 Se8 ), x = 16 (e.g., Pb16 Mo6 S8 ), and x = 2 (e.g., Cu2 Mo6 Se8 ). This parameter can vary because of the large num ber of available sites between the cubes for the A cations. Most of the space is occu pied by the large chalcogenide anions, which have radii of 0.184 nm (S), 0.191 nm (Se), and 0.211 nm (Te). The electronic and superconducting properties depend mainly on the Mo6 X8 group. No correlations are evident between the type of A ion and the superconducting properties. Magnetic order and superconduc tivity are known to coexist in Chevrel phase compounds. When A is a rare earth its mag netic state does not influence the supercon ducting properties, but when A is a transition metal ion the magnetic properties suppress the superconductivity. This may be explained on structural grounds by pointing out that the large rare earths occupy sites between the Mo6 X8 groups, as shown in Fig. 3.25, where they are remote from the molybdenums with only X as nearest neighbors. The smaller transition ions, on the other hand, can fit into octahedral sites with six Mo as their nearest neighbors (Ø. Fischer, 1990). 3 CLASSICAL SUPERCONDUCTORS a commonality that links the older and the newer superconductors. The two oxide compounds listed in Table 3.2 are cubic and ternary. One is the well-known ferroelectric perovskite SrTiO3 , which has a very low transition temperature (0.03–0.35 K). Nb-doped SrTiO3 , with its small carrier concentration Ne ≈ 2 × 1020 and high electron–phonon coupling, has Tc = 07 K (Baratoff and Binnig, 1981; Binnig et al., 1980). The other cubic ternary oxide is the spinel LiTi2 O4 with moderately high Tc = 137 K (Johnston et al., 1973). The system Lix Ti3−x O4 is superconducting in the range 08 ≤ x ≤ 133 with Tc in the range 7–13 K. It is interesting to note that the stoichiomet ric compound with x = 1 is near the com position where the metal-to-insulator transi tion occurs. A band structure calculation of this Li–Ti spinel (Satpathy and Martin, 1987) is consistent with resonance valence bond superconductivity (Chapter 10, Section III, F) and a large electron–phonon coupling constant ≈ 18. Only three more of the 200 known spinels superconduct—namely, CuRh2 Se4 with Tc = 35 K, CuV2 S4 with Tc = 45, and CuRh2 S4 with Tc = 48—so LiTi2 O4 turns out to be the only spinel oxide superconductor. PROBLEMS XI. CHALCOGENIDES AND OXIDES Many of the classical superconductors (for example, the Chevrel phases discussed in Section X) contain an element of row VI in the periodic table, namely O, S, Se, or Te, with oxygen by far the least represented among the group. The newer superconduc tors in contrast, are oxides. Since the pres ence of lighter atoms tends to raise the Debye temperature, oxides are expected to have higher Debye temperatures than the other chalcogenides (Gallo et al., 1987, 1988). Thus the presence of group VI elements is 1 Show why the alloys of Fig. 3.17 contain isoelectronic elements. 2 Consider the following expression as an alternate to Eq. (3.3) for describing the electronic specific heat of alloys: AB = fA A NeA + fB B NeB + fA fB Evaluate the constant for the three cases of Fig. 3.17, and compare the goodness of fit to the data with the results obtained from Eq. (3.3), as plotted in Fig. 3.17. 4 Thermodynamic Properties I. INTRODUCTION The first three chapters surveyed normal state conductivity, properties characteristic of superconductivity, and the principal types of superconducting materials. But none of the theoretical ideas that have been proposed to account for these phenomena were devel oped. In the present chapter we will refer to certain principles of thermodynamics as a way of providing some coherence to our understanding of the material that has been covered so far. In Chapters 6, 7 and 10 we will deepen our understanding by examin ing in succession the London approach, the Ginzburg–Landau phenomenological theory, the microscopic theory of Bardeen, Cooper, and Schrieffer (BCS), the Hubbard model, and the band structure. Then, after having acquired some understanding of the theory, we will proceed to examine other aspects of superconductivity from the perspective of the theoretical background, with an emphasis on the high-transition temperature cuprates. The overall behavior of the heat absorp tion process that will be examined in this chapter can be understood by deriving the thermodynamic functions of the nor mal state from the known specific heat– temperature dependence. The corresponding superconducting-state thermodynamic func tions can then be deduced from the critical field dependence of the Gibbs free energy. We will begin by presenting experimental results on specific heat, following that with a derivation of the different thermodynamic functions associated with specific heat in the normal and superconducting states. 83 84 4 THERMODYNAMIC PROPERTIES A specific heat determination is of inter est because it provides a good measure of the range of applicability of the phonon-mediated BCS theory (cf. Chapter 7, Section VI, E). This theory predicts characteristics of the discontinuity in specific heat at Tc . �D is the sum of a linear term Ce = �T arising from the conduction electrons, a lat tice vibration or phonon term Cph = AT 3 , and sometimes an additional Schottky con tribution aT −2 (Crow and Ong, 1990) (cf. Chapter 1, Section XII). Cn = aT −2 + �T + AT 3 � II. SPECIFIC HEAT ABOVE TC One of the most extensively studied properties of superconductors is the specific heat. It represents a “bulk” measurement that sees the entire sample since all of the sample responds. Many other measurements are sen sitive to only part of the sample, for exam ple, microscopy in which only the surface is observed. Above the transition temperature Tc the specific heat Cn of high-temperature super conductors tends to follow the Debye theory described in Chapter 1, Section XII (cf. Fig. 1.12, which shows the positions of the lanthanum and yttrium compounds on the Debye plot at their transition temperatures). We know from Eq. (1.64) that Cn of a nor mal metal far below the Debye temperature (4.1) For the present we will ignore the Schottky term aT −2 . The Cexp /T versus T 2 plot of Fig. 4.1 shows how the yttrium compound obeys Eq. (4.1) at low temperatures and then deviates from it at higher temperatures, as expected for the Debye approximation. The normalized specific heat plots of Fig. 4.2 compare for the case of several metals the electronic and photon contributions to the specific heat at low temperatures. In the free-electron approximation the electronic contribution to the specific heat per mole of conduction electrons is given by Eqs. (1.51) and (1.53), which we combine as follows: T 1 2 Ce = �T = 2 � R TF T = 4�93R � (4.2) TF Figure 4.1 Plot of Cexp /T versus T 2 for YBa2 Cu3 O7−� showing how the devi ation from linearity begins far below the transition temperature Tc = 90 K (Zhaojia et al., 1987). 85 II SPECIFIC HEAT ABOVE TC for in terms of effective masses, as will be explained subsequently. The vibrational and electronic contribu tions to the specific heat at T = Tc may be compared with the aid of Eqs. (4.2) and (4.3), Cph ATc2 = Ce �� 47�5 TF = · Tc2 � � �D3 Figure 4.2 Comparison of the electronic specific heat Ce = �T of several conductors and superconduc tors at low temperature. The low-temperature Debye approximation Cph ≈ AT 3 , multiplied by 10, is shown for comparison. The specific heats are normalized rel ative to the gas constant R and are expressed in terms of gram atoms. The heavy fermions are off scale on the upper left. In the Debye approximation the phonon con tribution to the specific heat per gram atom is given by Eq. (1.62a), 12� 4 T 3 R Cph = AT = 5 �D 3 T = 234R � (4.3) �D 3 where R = kB NA is the gas constant and TF the Fermi temperature. For a typical hightemperature superconductor we see from Table 4.1 that � ≈ 10 mJ/mole Cu K2 , and Eq. (4.2) gives TF ≈ 4�0 × 103 K. This is much smaller than typical good conductor values, such as 8�2×104 K for Cu, as listed in Table 1.1. This discrepancy can be accounted (4.4) (4.5) where the factor �, which is the ratio of the number of conduction electrons to the number of atoms in the compound, is needed when Ce is expressed in terms of moles of conduction electrons and Cph in terms of moles of atoms. When both spe cific heats are in the same units, � is set equal to 1. Typical values of the Fermi and Debye temperatures are 105 K and 350 K, respectively. For most low-temperature superconduc tors the transition temperature Tc is suffi ciently below �D so that the electronic term in the specific heat is appreciable in magni tude, and sometimes dominates. This is not the case for high-temperature superconduc tors, however. Using measured values of � and A we have shown in our earlier work (Poole et al., 1988), that ATc2 � � for �La0�9 Sr0�1 �2 CuO4−� and YBa2 Cu3 O7−� � so for oxide superconductors the vibrational term dominates at Tc , in agreement with the data plotted in Figs. 4.1 and 4.3. If the conduction electrons have effec tive masses m∗ that differ from the freeelectron mass m, the conduction-electron specific heat coefficient � is given by Eq. (1.54), �= m∗ �0 � m (4.6) 86 Table 4.1 Debye temperature �D , Density of States D�EF �, and Speciﬁc Heat Dataa Material Cd Al Sn, white Pb Nb Zr0�7 Ni0�3 V3 Ge�A15� V3 Si�A15� Nb3 Sn�A15� HfV2 (laves) �Hf0�5 Zr0�5 �V2 (laves) ZrV2 (laves) PbMo6 S8 (chevrel) PbMo6 Se8 (chevrel) SnMo6 S8 (chevrel) YMo6 S7 (chevrel) UPt3 (heavy fermion) UCd11 (heavy fermion) URu2 Si2 (heavy fermion) CeRu2 Si2 (heavy fermion) �TMTSF�2 ClO4 (organic) K-�ET�2 Cu�NCS�2 (organic) Tc �K� �D �K� 0�55 1�2 3�72 7�19 9�26 2�3 11�2 17�1 18�0 9�2 252 423 196 102 277 203 10�1 8�5 12�6 3�8 11�8 6�3 0�46 187 197 219 5 1�1 ≈ 0�8 200 1�2 213 9�3 �n mJ mole K2 0�67 1�36 1�78 3�14 7�66 4�04 7 17 13 21�7 28�3 16�5 79 28 105 34 460 290 31 340 10�5 34 �Cs −Cn �/�Tc 1�36 1�45 1�60 2�71 1�93 ≈1�65 A �mJ/mole K4 � D�EF � �states/eV� 1�55 2�0 0�23 2�30 2�97 1�86 ≈ 0�9 1525 115 0�42 3�5 1�67 Reference 11�4 Sürgers el al. (1989) Vonsovsky et al. (1982, Vonsovsky et al. (1982, Vonsovsky et al. (1982, Vonsovsky et al. (1982, pp. 269ff.) pp. 269ff.) pp. 269ff.) p. 379) Vonsovsky et al. (1982, p. 379) Vonsovsky et al. (1982, p. 379) Vonsovsky et al. (1982, p. 420) Vonsovsky et al. (1982, p. 420) Vonsovsky et al. (1982, p. 420) Vonsovsky et al. (1982, p. 420) Ellman et al. (1990); Fisher et al. (1989); Schuberth et al. (1992) deAndrade et al. (1991) Ramirez et al. (1991) van de Meulen et al. (1991) Garohce et al. (1982) Graebner et al. (1990) K3 C60 (buckyball) 19 Rb3 C60 (buckyball) Cs3 C60 (buckyball) BaPb1−x Bix O3 (perovskite) �La0�925 Sr0�075 �2 CuO4 30�5 47�4 10 37 360 �La0�925 Ba0�075 �2 CuO4 YBa2 Cu3 O7 (orthorhombic) 27 370 92 410 YBa2 Cu4 O8�5 80 350 Bi2 Sr2 CaCu2 O8 95 250 Bi2 Sr2 Ca2 Cu3 O10 Tl2 Ba2 CaCu2 O8 Tl2 Ba2 Ca2 Cu3 O10 110 110 125 260 260 280 HgBa2 Ca2 Cu3 O8 133 a 70 9�3 10�9 12�7 0�6 4�5 8 2�0 0�24 1�9 Junod (1990) Junod (1990); Sun et al. (1991) Junod (1990) 0�035 2�0 2�1 2�1 Collocott et al. (1990a); Junod (1990); Stupp et al. (1991) Junod (1990); Junod et al. (1991) Junod (1990); Fisher and Huse (1988); Urbach et al. (1989) Junod (1990) Junod (1990) Junod (1990); Urbach et al. (1989) Schilling et al. (1994a, b) 1�1 4−10 3�6 4�9 Ramir et al. (1992b); Novikov et al. (1992) Novikov et al. (1992) Novikov et al. (1992) ≈8 >2�8 2�0 Some of the high-temperature superconductor values are averages from Junod (1990), in many cases with a wide scatter of the data. The density of states is expressed per atom for the elements and per copper atom for the high-temperature superconductors. For the latter �n is the electronic specific heat factor determined from normal state measurements, and �n∗ is the value obtained from the limit T → 0, as explained by Junod. The BCS theory predicts �Cs − Cn �/�n Tc = 1�43. 87 88 4 THERMODYNAMIC PROPERTIES Figure 4.3 Discontinuity in the specific heat of �La0�9 Sr0�1 �2 CuO4 near 40 K. The inset shows the magnitude of the jump. The AT 3 behavior indicated by the dashed curve shows that the transition occurs beyond the region where the T 3 approximation is valid (Nieva et al., 1987). where �0 is the ordinary electron counterpart of � from Eq. (1.51). In the free-electron approximation we have from Eq. (4.2) �0 = 1 2 � R 2 TF � (4.7) which gives for the effective mass ratio �T m∗ = 1 2F � m � R 2 (4.8) Table 1.1 lists effective mass ratios for the elemental superconductors calculated from this expression. The unusually low estimate of TF given following Eq. (4.3) for a hightemperature superconductor can be explained in terms of a large effective mass. We see from Table 9.1 and Fig. 4.2 that large effec tive masses make the electronic term � very large for the heavy fermions. The plot of Tc versus � in Fig. 4.4 shows that the points for Figure 4.4 Comparison of the electronic specific-heat factor � for a selection of superconductors and superconducting types over a wide range of Tc values. The dashed lines delimit the region of phonon-mediated superconductivity (Crow and Ong, 1990, p. 239). 89 III DISCONTINUITY AT TC BCS phonon-mediated superconductors clus ter in a region delimited by the dashed lines. The heavy fermions lie far to the right, as expected, while the oxide and cuprate com pounds lie somewhat above those in the main group. A diagram similar to Fig. 4.4 may be found in Batlogg et al. (1987). We have seen that the specific heat is a measure of how effectively the introduc tion of heat into a material, and it raises its temperature. A related quantity is the ther mal conductivity which is a measure of how easily heat flows through a material from a region at a high temperature to a region at a low temperature. Thermal conduction and the flow of heat through materials will be discussed in Sect. VII of Chap. 16. III. DISCONTINUITY AT TC The transition from the normal to the superconducting state in the absence of an applied magnetic field is a secondorder phase transition, as we will show in Section XIV. This means that there is no latent heat, but nevertheless a discontinuity in the specific heat. The BCS theory, which will be explained in Chapter 7, predicts that the electronic specific heat jumps abruptly at Tc from the normal state value �Tc to the superconducting state value Cs with ratio Cs − �Tc = 1�43� �Tc (4.9) Figure 4.5, as well as Fig. IX-12 of our ear lier work (Poole et al., 1988) show details of this jump for an element and for a hightemperature superconductor, respectively. For the latter case the magnitude of the jump is small compared to the magnitude of the total specific heat because it is superim posed on the much larger AT 3 vibrational term, as indicated in Fig. 4.3. This is seen Figure 4.5 Specific heat jump in superconducting Al compared with the normal-state specific heat (Phillips, 1959; see Crow and Ong, 1990, p. 225). if Eq. (4.9) is used to express Eq. (4.5) in the form ATc3 67�9 TF = · 3 Tc2 � (4.10) Ce − �Tc � �D Figure 4.6 illustrates how the small change at Tc is resolved by superimposing curves of C/T versus T 2 obtained in zero field and in a magnetic field large enough �Bapp > Bc2 � to destroy the superconductivity. It is clear from the figure that the data in the supercon ducting state extrapolate to zero, and that the normal state data extrapolate to � at 0 K. Many researchers have observed the jump in the specific heat at Tc (cf. Table 4.1 for results from a number of studies). Table 4.1 also lists experimental values of Tc , �D , and �, together with the ratios �Cs − Cn �/Tc and �Cs − Cn �/�Tc , for sev eral elements and a number of copper oxide superconductors. Some of the elements are close to the BCS value of 1.43, but the strongly coupled ones, Pb and Nb, which have large electron–phonon coupling con stants �, are higher. Several experimental results for YBaCuO are close to 1.43, as indicated in the table. Some researchers have failed to observe a specific heat discontinu ity, however. 90 4 THERMODYNAMIC PROPERTIES Figure 4.6 Plot of Cexp /T versus T 2 for monocrystals of the organic superconductor K–�ET�2 Cu�NCS�2 in the superconducting state with no applied magnetic field, and also in the presence of applied fields that destroy the superconductivity. The superconducting state data extrapo late to a value � = 0, while the normal-state extrapolation indicates � ≈ 25 mJ/mole K 2 (Andraka et al., 1989). V. DENSITY OF STATES AND DEBYE TEMPERATURE IV. SPECIFIC HEAT BELOW TC For T � Tc BCS theory predicts that the electronic contribution to the specific heat Ce will depend exponentially on temperature, � Cs ≈ a exp − � kB T (4.11) where 2� is the energy gap in the super conducting density of states. We see from Fig. 4.5 that the fit of this equation to the data for aluminum is good, with the spe cific heat falling rapidly to zero far below Tc , as predicted. The vibrational term AT 3 also becomes negligible as 0 K is approached, and other mechanisms become important, for example, antiferromagnetic ordering and nuclear hyperfine effects, two mechanisms that are utilized in cryogenic experiments to obtain temperatures down to the microdegree region. The density of states at the Fermi level D�EF � can be estimated from Eq. (1.52): D�EF � = 3 � 1 · · � � 2 R kB (4.12) For a typical high-temperature superconduc tor with � ≈ 0�01 J/mole Cu K we obtain D�EF � ≈ 4�5 states � eV Cu atom (4.13) The Debye temperature may be esti mated from the slope of the normal state Cn /T -versus-T 2 curve sketched in Fig. 1.13, since with the aid of Eq. (1.62a) we can write �D3 = 12� 4 R � �5�slope�� (4.14) Typical values for �D are from 200 to 350 K. 91 VI THERMODYNAMIC VARIABLES We have been using formulae that involve the free-electron approximation. To estimate the validity of this approximation we can make use of Eq. (1.88), which gives the ratio of � to the magnetic susceptibility � arising from the conduction electrons, � 1 = � 3 �kB �B 2 � (4.15) in terms of well-known physical constants. VI. THERMODYNAMIC VARIABLES We have been discussing the specific heat of a superconductor in its normal and superconducting states in the absence of an applied magnetic field. When a magnetic field is present the situation is more com plicated, and we must be more careful in describing the specific heat as the result of a thermodynamic process. In this section we will develop some of the necessary back ground material required for such a descrip tion, and in the following sections we will apply the description to several cases. Later on, in Chapter 5, Section X, we will learn why the magnetic energy of a superconducting sample in a magnetic field depends on its shape and orientation. In the present chapter we will not be concerned with these demagnetization effects and will instead assume that the sample is in the shape of a cylinder and that the internal magnetiza tion M is directed along the axis of the cylin der, as illustrated in Fig. 2.26. If an external field Bapp is applied, it will also be directed along this axis. This means that the applied B field is related to the internal H field by means of the expression Bapp = �0 Hin � (4.16) This geometry simplifies the mathematical expressions for the free energy, enthalpy, and other properties of a superconductor in the presence of a magnetic field. In the next few sections we will simplify the notation by using the symbol B instead of Bapp for the applied magnetic field, but throughout the remainder of the text the symbol Bapp will be used. In treating the superconducting state it is convenient to make use of the free energy because (1) the superconductivity state is always the state of lowest free energy at a particular temperature, and (2) the free energies of the normal and super conducting states are equal at the transi tion temperature. We will use the Gibbs free energy G�T� P� B� = G�T� B� rather than the Helmholtz free energy F�T� V� M� = F�T� M�� where the variables P and V are omit ted because pressure–volume effects are negligible for superconductors. The Gibbs free energy G�T� B� is selected because the experimenter has control over the applied magnetic field B, whereas the magnetization M�T� B� is produced by the presence of the field. The remaining thermodynamic func tions will be expressed in terms of the two independent variables T and B. In the treatment that follows we will be dealing with thermodynamic quantities on a per-unit-volume basis, so that G will denote the Gibbs free energy density and S the entropy density. For simplicity, we will gen erally omit the term density by, for example, calling G the Gibbs free energy. The first law of thermodynamics for a reversible process expresses the conservation of energy. For a magnetic material the dif ferential of the internal energy dU may be written in terms of the temperature T , the entropy S, the applied magnetic field B, and the magnetization M of the material as dU = TdS + B · dM� (4.17) where the usual –PdV term for the mechan ical work is negligible and hence omitted, 92 4 THERMODYNAMIC PROPERTIES while the +B · dM term for the magnetic work is included. (Work is done when an applied pressure P decreases the volume of a sample or an applied magnetic field B increases its magnetization.) So these two work terms are opposite in sign. The work term �0 H · dM that appears in Eq. (4.17) is positive. This equation does not include the 1 term d�B2 /2�0 � = �− 0 B · dB for the work involved in building up the energy density of the applied field itself since we are only interested in the work associated with the superconductor. We will be concerned with a constant applied field rather than a constant magne tization, so it is convenient to work with the enthalpy H � rather than the internal energy U , H � = U − B · M� (4.18) with differential form dH � = TdS − M · dB� (4.19) The second law of thermodynamics permits us to replace TdS by CdT for a reversible process, where C is specific heat, CdT = TdS� (4.20) which gives for the differential enthalpy dH � = CdT − M · dB� (4.21) Finally we will be making use of the Gibbs free energy G = H � − TS� (4.22) VII. THERMODYNAMICS OF A NORMAL CONDUCTOR and its differential form dG = −SdT − M · dB� H, and M are parallel and write, for example, MdB instead of M · dB. The fundamental thermodynamic expressions (4.17)–(4.23) provide a starting point for discussing the thermodynamics of the superconducting state. Two procedures will be followed in applying these expres sions to superconductors. For the normal state we will assume a known specific heat (4.1) and then determine the enthalpy by integrating Eq. (4.21), determine the entropy by integrating Eq. (4.20), and finally find the Gibbs free energy from Eq. (4.22). For the superconducting case we will assume a known magnetization and critical field, and determine the Gibbs free energy by integrating Eq. (4.23), the entropy by differentiating Eq. (4.23), the enthalpy from Eq. (4.22), and finally the specific heat by differentiating Eq. (4.21). The first procedure, called the specific heat-to-free energy procedure, goes in the direction C → H� → S → G and the second, called the free energy-to-specific heat procedure, goes in the opposite direction G → S → H� → C. The former procedure will be presented in the following section and the latter in the succeeding three sections. We will assume specific expressions for C and M, respectively, to obtain closed-form expressions for the temperature dependences of the difference thermodynamic variables. This will give us considerable physical insight into the thermodynamics of the superconducting state. These assumptions also happen to approximate the behavior of many real superconductors. (4.23) Note the prime in the symbol H � for enthalpy to distinguish it from the symbol H for the magnetic field. For the balance of the chapter we will also be assuming that the vectors B, In this section we will use the specific heat-to-free energy procedure. We deduce in succession the enthalpy, entropy, and Gibbs free energy of a normal conductor by assum ing that its low-temperature specific heat Cn 93 VII THERMODYNAMICS OF A NORMAL CONDUCTOR is given by Eq. (4.1) with the Schottky term omitted: Cn = �T + AT 3 � (4.24) The enthalpy at zero magnetic field is obtained by setting MdB = 0, MdB = �−1 0 �n BdB ≈ 0� (4.25) where �n = �0 M/B. Integrating Eq. (4.21), we find that dHn� = T 0 ��T + AT �dT� 3 Hn� �T� = 21 �T 2 + 41 AT 4 � (4.26) (4.27) where it is assumed that � and A are inde pendent of temperature, and that Hn� �0� = 0. Figure 4.7 A similar calculation for the entropy involves integrating Eq. (4.20), dSn = T 0 ��T + AT 3 � dT � T Sn �T � = �T + 13 AT 3 � (4.28) (4.29) where Sn �0� = 0. The normal-state Gibbs free energy at zero field may be determined either from Eq. (4.22) or by integrating Eq. (4.23) with MdB set equal to zero. It has the following temperature dependence: Gn �T � = − 21 �T 2 − 121 AT 4 � (4.30) The normal-state specific heat, entropy, enthalpy, and Gibbs free energy from Eqs. (4.24), (4.29), (4.27), and (4.30) are plotted in Figs. 4.7, 4.8, 4.9, and 4.10, respec tively, for the very-low-temperature region. Temperature dependence of the normal-state Cn (- - -) and superconducting-state Cs (—) specific heats. The figure shows the specific heat jump √ 1�43�Tc of Eq. (4.9) that is predicted by the BCS theory, the crossover point at T = Tc / 3, and the maximum negative jump 0�44��Tc at T = Tc /3. In this and the following 12 figures it is assumed that only the linear electronic term �T exists in the normal state (i.e, AT 3 = 0). 94 4 THERMODYNAMIC PROPERTIES Figure 4.8 Temperature dependence of the normal-state Sn (---) and superconducting-state Ss (—) entropies. The transition is second order so there is no discontinuity in entropy at Tc . Figure 4.9 Temperature dependence of the normal state Hn (---) and super conducting state Hs (—) enthalpies. The transition is second order so there is no discontinuity in enthalpy, and hence no latent heat at Tc . Here the AT 3 term is negligible, and only the �T term is appreciable in magnitude. In this section we have derived sev eral thermodynamic expressions for a normal conductor in the absence of a magnetic field. The permeability � of such a conductor is so close to that of free space �0 (cf. Chapter 1, Section XV, and Table 1.2), that the mag netic susceptibility �n is negligibly small and M ≈ 0. Therefore, the thermodynamic quan tities (4.24), (4.27), (4.29), and (4.30) are not appreciably influenced by a magnetic field, and we will assume that they are valid even when there is a magnetic field present. For example, we assume that Gn �T� B� ≈ Gn �T� 0� (4.31) 95 VIII THERMODYNAMICS OF A SUPERCONDUCTOR Figure 4.10 Temperature dependence of the normal-state Gn (---) and superconducting-state Gs (—) Gibbs free energies. Since the transition is second order, both G and its first derivative are continuous at Tc . and it is convenient to simplify the notation by writing Gn �T� B� ≈ Gn �T�� (4.32) Thus all of the equations derived in this section are applicable when a magnetic field is also present. VIII. THERMODYNAMICS OF A SUPERCONDUCTOR If we had a well-established expression for the specific heat Cs of a superconduc tor below Tc it would be easy to follow the same C → H� → S → G procedure to obtain the quantities Hs� � Ss , and Gs , as in the case of a normal conductor. Unfortu nately, there is no such expression, although many experimental data far below Tc have been found to follow the BCS expression (4.11). Equation (4.11) does not cover the entire temperature range of the superconduct ing region, however, and, in addition it does not integrate in closed form. Another compli cation is that the thermodynamic properties of the superconducting state are intimately related to its magnetic properties, as we will demonstrate below, and the specific heat relation (4.11) does not take magnetism into account. Because of the close relationship between superconductivity and magnetism we will adopt the free energy-to-specific heat procedure and examine the Gibbs free energy of a superconductor in the presence of an applied magnetic field B. We will not resort to any model for the temperature dependence of the specific heat or that of the critical field, so the results that will be obtained will be general. Then in the following two sec tions we will return to the specific model based on Eq. (4.24) to obtain more practical results. We begin by seeking an expression for the free-energy difference Gs �T� B� − Gn �T� B� between the superconducting and normal states to allow us to deduce Ss and Hs� by differentiation. To accomplish this we 96 4 THERMODYNAMIC PROPERTIES write down the differential of the Gibbs free energy from Eq. (4.23) assuming isothermal conditions �dT = 0�, dG = −MdB� (4.33) and examine its magnetic field dependence in the superconducting and normal states. We treat the case of a Type I supercon ductor that has the magnetization given by Eq. (2.22), M = −H = −B/�0 , and assume that surface effects involving the penetra tion depth are negligible. Demagnetization effects are also inconsequential, as explained in Section VI, so Eq. (4.33) becomes 1 dGs = �− 0 BdB� (4.34) If this expression is integrated from B = 0 to a field B we obtain 2 Gs �T� B� = Gs �T� 0� + 21 �−1 0 B � (4.35) where, of course, the magnetic energy den sity B2 /2�0 is independent of temperature. When the applied field B equals the criti cal field Bc �T� for a particular temperature T < Tc , the free energy becomes 2 Gs �T� Bc �T�� = Gs �T� 0� + 21 �−1 0 Bc �T� T = Tc �B�� (4.36) and recalling that this is a phase transition for which Gs = Gn , we have where, of course, B < Bc �T�. In the absence of an applied field Eq. (4.38) becomes 2 Gs �T� 0� = Gn �T� − 21 �−1 0 Bc �T� �B = 0�� (4.39) so the Gibbs free energy in the super conducting state depends on the value of the critical field at that temperature. This confirms that there is indeed a close relation ship between superconductivity and mag netism. Figure 4.11 shows that the curves for Gs �T� 0� and Gn �T� intersect at the tem perature Tc , while those for Gs �T� B� and Gn �T� intersect at the temperature Tc �B�. 2 The figure also shows that 21 �−1 0 Bc is the spacing between the curves of Gs �T� 0� 1 2 and Gn �T�, and that 21 �− 0 B is the spac ing between the curves of Gs �T� B� and Gs �T� 0�. The figure is drawn for a particu lar value of the applied field corresponding to Tc �B� = 21 Tc . Since we know that the Gibbs free energy of the superconducting state depends only on the applied magnetic field and the temperature, we can proceed to write down general expressions for the other thermody namic functions that can be obtained through differentiation of Gs �T� with respect to the temperature when the applied field B is kept constant. The value of B, of course, does not depend on T . For the entropy we have, using Eq. (4.23), 1 2 Gn �T� = Gs �T� 0� + 21 �− 0 Bc �T� T = Tc �B�� (4.37) 1 2 where 21 �− 0 Bc �T� is the magnetic-energy density associated with the critical field, and, from Eq. (4.32), Gn �T� does not depend on the field. Subtracting Eq. (4.35) from Eq. (4.37) gives 1 2 2 Gs �T� B� = Gn �T� − 21 �− 0 �Bc �T� − B �� (4.38) S s − Sn = − d �G − Gn �� dT s (4.40) and for the free energy, from Eq. (4.38), Ss �T� = Sn �T� + Bc �T� d B �T�� �0 dT c (4.41) The entropy Ss �T� B� does not depend explic itly on the applied field, so it is denoted Ss �T�. From this expression, together with 97 IX SUPERCONDUCTOR IN ZERO FIELD Figure 4.11 Effect of an applied magnetic field Bapp = 0�75Bc on the Gibbs free energy Gs �T� B� in the superconducting state. In this and the succeeding figures dashed curves are used to indicate both the normal-state extrapolation below Tc� and the zero-field superconducting state behavior, where Tc� denotes the transition temperature when there is a field present. Eqs. (4.22) and (4.39), we can write down the enthalpy at constant field, 1 2 2 Hs� �T� B� = Hn� �T� − 21 �− 0 �Bc �T � − B � + TBc �T � d B �T �� �0 dT c (4.42) which shows that the enthalpy does depend on the magnetic energy B2 /2�0 . We see from Eq. (4.21) that the enthalpy can be differen tiated to provide the specific heat at constant field: Cs �T � = Cn �T� + �−1 0 TBc �T � T + �0 2 d dT Bc �T� � d2 B �T � dT 2 c (4.43) The specific heat does not depend explic itly on the applied field, so we write Cs �T � instead of Cs �T� B�. We will see below that the terms in this expression that depend on Bc �T � become negative at the lowest tem peratures, making Cs �T � less than Cn �T�. At zero field �B = 0� the transition temper ature is Tc itself, and we know (e.g., from Eq. (4.45) in Section IX) that Bc �Tc � = 0, so that only the second term on the right exists under this condition: 2 T d Cs �T � = Cn �T �+ Bc �T � �0 dT T = Tc � (4.44) This is known as Rutger’s formula. It pro vides the jump in the specific heat at Tc that is observed experimentally, as shown in Figs. 4.3, 4.5, and 4.6. We will show in Section XIII how this expression can be used to evaluate the electronic specific-heat factor �. IX. SUPERCONDUCTOR IN ZERO FIELD We will develop the thermodynamics of a Type I superconductor in the absence of 98 4 THERMODYNAMIC PROPERTIES a magnetic field using the free energy-to specific heat procedure G → S → H� → C. We apply the general expression (4.39) to the particular case in which the free energy of the normal state is given by Eq. (4.30) and the critical magnetic field Bc �T� has a parabolic dependence on temperature, 2 T � (4.45) Bc �T � = Bc �0� 1 − Tc given by Eq. (2.56). Substituting these expressions in Eq. (4.39) gives 2 Gs �T� 0� = − 21 �T 2 − 121 AT 4 − 21 �−1 0 Bc �0� 2 2 T × 1− � (4.46) Tc which is plotted in Fig. 4.10 with A set equal to zero. The difference between the entropies in the normal and superconducting states is obtained by substituting the expressions from Eqs. (4.29) and (4.45) in Eq. (4.41) and car rying out the differentiation: 1 2 Ss �T � = �T + 13 AT 3 − 2�− 0 Bc �0� T T2 × 1 − � (4.47) Tc2 Tc2 The last term on the right is zero for both T = 0 and T = Tc , so Ss = Sn for both lim its. The former result is expected from the third law of thermodynamics. Differentiation shows that the last term√on the right is a maximum when T = Tc / 3, so that the dif ference Ss − Sn is a maximum for this tem perature. The entropy Ss with A = 0 is plotted in Fig. 4.8. The enthalpy Hs� �T� 0� of the super conducting state in zero field is obtained from Eq. (4.22), 2 Hs� �T� 0� = 21 �T 2 + 41 AT 4 − 21 �−1 0 Bc �0� T2 T2 × 1 − 2 1 + 3 2 � (4.48) Tc Tc and the specific heat of the superconducting state from Eq. (4.20), dSs � (4.49) Cs = T dT H by differentiating Eq. (4.47) at constant field, to give 2 Cs �T� = �T + AT 3 + 2�−1 0 Bc �0� 2 T T × 3 2 −1 � (4.50) Tc2 Tc The last √term on the right changes sign at T = Tc / 3. Expressions (4.48) and (4.50) are plotted in Figs. 4.9 and 4.7, respectively, with the AT 3 term set equal to zero. The results given in this section are for a Type I superconductor in zero field with electronic specific heat given by Eq. (4.24) and a critical field with the temperature dependence of Eq. (4.45). Figures 4.7, 4.8, 4.9, and 4.10 show plots of the tempera ture dependence of the thermodynamic func tions Cs , Ss , Hs� , and Gs under the additional assumption A = 0. X. SUPERCONDUCTOR IN A MAGNETIC FIELD In the previous section we derived Eq. (4.38) for the Gibbs free energy Gs �T� B� of the superconducting state in the absence of an applied magnetic field B. With the aid of Eqs. (4.30), (4.38), and (4.45) this can be written in the following form for the case of an applied field: Gs �T� B� = − 21 �T 2 − 121 AT 4 − 21 �0−1 2 T2 2 2 × Bc �0� 1 − 2 − B � Tc (4.51) Since the applied field B does not depend on the temperature, the entropy obtained from 99 X SUPERCONDUCTOR IN A MAGNETIC FIELD Eq. (4.40) by differentiating the Gibbs free energy (4.51) assuming the presence of a field is the same as in the case where there is no magnetic field present, 1 2 Ss �T� = �T + 13 AT 3 − 2�− 0 Bc �0� T2 T (4.52) × 2 1− 2 � Tc Tc The enthalpy obtained from Eq. (4.22) does depend explicitly on this field, Hs� �T� B� = 21 �T 2 + 41 AT 4 − 1 −1 � Bc �0�2 2 0 T2 1− 2 Tc T2 2 × 1 + 4 2 + 21 �−1 0 B � Tc (4.53) but the specific heat from Eq. (4.20) does not, 1 2 + 2�− 0 Bc �0� Cs �T� = �T + AT 2 T T × 2 3 2 −1 � Tc Tc 3 (4.54) where Eqs. (4.52) and (4.54) are the same as their zero-field counterparts (4.47) and (4.50), respectively. The field-dependent Gs and Hs� terms of Eqs. (4.51) and (4.53), on the other hand, differ from their zero-field counterparts (4.46) and (4.48) by the addition of the magnetic-energy density B2 /2�0 . In a magnetic field the sample goes nor mal at a lower temperature than in zero field. We denote this magnetic-field transi tion temperature by Tc �B� = Tc� , where, of course, Tc �0� = Tc and Tc� < Tc . This transi tion from the superconducting to the normal state occurs when the applied field H equals the critical field Bc �T� given by Eq. (4.45) at that temperature. Equation (4.45) may be rewritten in the form B 1/2 � (4.55) Tc = T c 1 − Bc �0� to provide an explicit expression for the tran sition temperature Tc� in an applied field B. We show in Problem 7 that this same expres sion is obtained by equating the Gibbs free energies Gs �T� B� and Gn �T� for the super conducting and normal states at the transition point, Gs �T� B� = Gn �T� T = Tc� � (4.56) At the transition temperature Tc� = Tc �B� the superconducting and normal state entropies (4.52) and (4.29), respectively, dif fer. Their difference gives the latent heat L of the transition by means of the standard thermodynamic expression L = �Sn − Ss �Tc �B� −1 2 Tc �B� = 2�0 Bc Tc T �B� × 1− c Tc (4.57) 2 2 � (4.58) We show in Problem 9 that this same result can be obtained from the enthalpy differ ence L = Hn� − Hs� . The latent heat is a maxi mum at the √ particular transition temperature Tc �B� = Tc / 2, as may be shown by setting the derivative of Eq. (4.58) with respect to temperature equal to zero. We see from this equation that there is no latent heat when the transition occurs in zero field, i.e., when T = Tc , or at absolute zero, T = 0. In addi tion to the latent heat, there is also a jump in the specific heat at Tc �B� which will be discussed in the following section. Figures 4.12, 4.13, 4.14, and 4.15 show the temperature dependences of the thermo dynamic functions C, S, H � , and G, respec tively, for high applied fields in which Tc �B� is far below Tc . Figures 4.16, 4.17, 4.18, and 4.19 show these same plots for low applied fields in which Tc �B� is slightly below Tc . All of these plots are for the case A = 0. We see from Figs. 4.12, 4.16, 4.13, and 4.17, respec tively, that the specific heat Cs and entropy Ss 100 4 THERMODYNAMIC PROPERTIES Figure 4.12 Temoerature dependence of the specific heat in the normal and superconducting states in the presence of a strong applied magnetic field. The downward jump in specific heat �C at Tc� is indicated. Figure 4.13 Temperature dependence of the entropy in the normal and super conducting states in the presence of a strong applied magnetic field. The latent heat factor L/Tc� of the jump in entropy at Tc� is indicated. curves (assuming the presence of a magnetic field) coincide with their zero-field counter parts below Tc �B� and with their normal-state counterparts above Tc �B�. In contrast, from Figs. 4.14, 4.18, 4.15, and 4.19 it is clear that the enthalpy Hs� and Gibbs free energy Gs curves in a magnetic field lie between their normal-state and zero-field superconducting state counterparts below the transition point Tc �B�, and coincide with the normal-state curves above the transition. These plots also show the jumps associated with the specific heat and the latent heat as well as the continu ity of the Gibbs free energy at the transition. 101 X SUPERCONDUCTOR IN A MAGNETIC FIELD Figure 4.14 Temperature dependence of the enthalpy in the normal and super conducting states in the presence of a strong applied magnetic field. The jump in entropy at the transition temperature Tc� is equal to the latent heat L, as indicated. Figure 4.15 Temperature dependence of Gibbs free energy in the normal and superconducting states in the presence of a strong applied magnetic field. The transition is first order so that there is no discontinuity in free energy at the transition temperature Tc� , but there is a discontinuity in the derivative. The normal �Gn � and superconducting �Gs � branches of the upper curve are indicated. The lower dashed (- - -) curve shows the Gibbs free energy in the superconducting state at zero field �Bapp = 0� for comparison. Figure 4.20 shows the experimentally determined Gibbs free-energy surface of YBa2 Cu3 O7 obtained by plotting G�T� B� − G�T� 0� versus temperature and the applied field close to the superconducting transi tion temperature (Athreya et al., 1988). The free-energy differences are obtained by integrating Eq. (4.33) using measured magnetization data for M�T� B�: G�T� 0� − G�T� B� = MdB� � (4.59) This procedure is possible because close to the transition temperature magnetic flux 102 4 THERMODYNAMIC PROPERTIES Figure 4.16 Temperature dependence of specific heat in the normal and super conducting states in the presence of a weak applied magnetic field. The jump in specific heat �C at Tc� is upward, in contrast to the downward jump shown in Fig. 4.12 for the high-field case. Figure 4.17 Temperature dependence of entropy in the normal and supercon ducting states in the presence of a weak applied magnetic field showing the jump in entropy L/Tc� at Tc� , as expected for a first-order transition. moves easily and reversibly into and out of the material, which makes the magnetization a thermodynamic variable. Magnetization is linear in �Tc − T�2 near Tc . The free-energy surface varies with the magnetic field all the way up to 92 K. Fang et al. (1989) determined free-energy surfaces for thallium-based superconductors. 103 XI NORMALIZED THERMODYNAMIC EQUATIONS Figure 4.18 Temperature dependence of enthalpy in the normal and super conducting states in the presence of a weak applied magnetic field, showing the presence of a latent heat jump L at the transition temperature Tc� , indicating a first-order transition. Figure 4.19 Temperature dependence of Gibbs free energy in the normal and superconducting states in the presence of a weak applied magnetic field using the notation of Fig. 4.15. The transition is first order so that the change in G at Tc� is continuous, but the change in its derivative is discontinuous (cf. Athreya et al., 1988). XI. NORMALIZED THERMODYNAMIC EQUATIONS The equations for Gs �T� B�, Ss �T�, and Cs �T� given in the previous section, together with Hs� �T� B� of Problem 9, can be written in normalized form by defining two dimensionless independent variables, t= T Tc b= B Bc (4.60) and two dimensionless parameters, a= ATc2 � �= Bc2 � �0 �Tc2 (4.61) 104 4 THERMODYNAMIC PROPERTIES in the table are the normalized specific heat jump �C/�Tc and the normalized latent heat L/�Tc2 . These expressions are valid under the condition t2 + b < 1� (4.62) The sample becomes normal when either t or b are increased to the point where t2 + b = 1, and the value of t that satisfies this expression is called t� : t�2 + b = 1� Figure 4.20 Free-energy surface for YBa2 Cu3 O7 close to the transition temperature (Athreya et al., 1988). The resulting normalized expressions for gs , ss , and h�s are given in Table 4.2. Also given (4.63) This is the normalized equivalent of Eq. (4.55), where t� = Tc� /Tc is the normalized transition temperature in a magnetic field. The normalized specific heat jump has the following special values: �C = 2�t� �3t�2 − 1� �Tc Table 4.2 Normalized Equations for the Thermodynamic Functions of a Superconductor in an Applied Magnetic Field Ba Gibbs Free Energy gs = Gs 1 = − 21 t2 − 12 at4 − 21 ���1 − t2 �2 − b2 � �Tc2 Entropy ss = Ss = t + 13 at3 − 2�t�1 − t2 � �Tc Specific Heat cs = Cs = t + at3 + 2�t�3t2 − 1� �Tc Enthalpy h�s = Hs� = 21 t2 + 41 at4 − 21 ���1 − t2 ��1 + 3t3 − b2 �� �Tc2 Specific Heat Jump �C = 2�t� �3t�2 − 1� �Tc Latent Heat L = 2�t�2 �1 − t�2 � �Tc2 Definitions of normalized variables �t� b� and parameters: a t= T Tc b= B Bc �0� t� = T� Tc b� = Bc �T � � Bc �0� a= �= ATc2 � �Bc �0��2 �0 �Tc2 The first four expressions are valid under the condition t2 + b < 1 of Eq. (4.62), and the last two are valid at the transition point given by t�2 + b = 1 from Eq. (4.63). 105 XII SPECIFIC HEAT IN A MAGNETIC FIELD ⎧ ⎪0 ⎪ ⎪ ⎪ ⎨ 4� − = 9 ⎪ ⎪ 0 ⎪ ⎪ ⎩ 4� t� = 0 t� = 1 3 √1 3 �max�� (4.64) t� = t� = 1 where 4�/9 is its maximum magnitude of �C/�Tc for√ reduced temperatures in the range 0 < t� < 1/ 3, as indicated in Fig. 4.12. The normalized latent heat has the special values L = 2�t�2 �1 − t�2 � �Tc2 ⎧ � ⎪ ⎨0 t = 0 1 1 = 2 � t� = √2 ⎪ ⎩ 0 t� = 1 �max�� (4.65) √ where its maximum 21 � is at t� = 1/ 2. XII. SPECIFIC HEAT IN A MAGNETIC FIELD A number of authors have measured or calculated the specific heat of hightemperature superconductors in a magnetic field (Hikami and Fujita, 1990a,b; Riecke et al., 1989; Quade and Abrahams, 1988; Watson et al., 1989). Reeves et al., (1989) found that the quantity C/ T of YBa2 Cu3 O7−� in an applied magnetic field is linear in T 2 in the range 4 K < T < 6 K in accordance with the expression C = �� + � � �B��T + �A − A� �B��T 3 � (4.66) which is compared in Fig. 4.21 with exper imental data for applied fields up to 3 T. It was also found that � = 4�38 mJ/mole K2 and A = 0�478 mJ/mole K 4 , with the coef ficients � � �B� and A� �B� increasing as the applied magnetic field was increased. At the highest measured field of 3 T, it turned out that � = 0�54� �� (4.67) A = 0�11� A� Figure 4.21 Low-temperature specific heat of YBa2 Cu3 O7−� in a magnetic field. The straight lines are fits of Eq. (4.66) to the data for each field value (Reeves et al., 1989). Reeves et al., also mention that other workers have obtained results that differ from those described by Eq. (4.66). Bonjour et al. (1991), Inderhees et al. (1991), and Ota et al. (1991) mea sured the magnetic-field dependence of the anisotropies in the specific heat near Tc . The results obtained by Inderhees et al. for untwinned YBa2 Cu3 O7−� , which are pre sented in Fig. 4.22, turned out to be similar to those obtained by the other two groups. We see that increasing the magnetic field shifts the specific-heat jump to lower tem peratures and broadens it, especially for an applied field parallel to the c-axis. Ebner and Stroud (1989) obtained a good approxima tion to the specific heat curves of Fig. 4.22 with B � c by including fluctuations in the Ginzburg–Landau free energy (cf. Chapter 6, Section III) and carrying out Monte–Carlo simulations. Figure 4.23 shows how the dif ference between the specific heat measured 106 4 THERMODYNAMIC PROPERTIES Figure 4.22 Specific heat jump of untwinned YBa2 Cu3 O7−� near Tc for different applied magnetic fields aligned parallel (top) and perpendicular (bottom) to the c-axis (Inderhees et al., 1991). at zero field C0 and that measured in the field CH depends on the value of the applied field at a temperature of 88 K, which is close to Tc . The difference is about five times larger in the parallel field orientation than in the perpendicular field orientation. Bonjour et al. (1991) used their own specific heat data to determine the depen dence of the entropy difference S0 − SH on the applied field, where S0 �T� is the entropy in the absence of the field and SH �T� B� the entropy assuming the presence of a field; their results are given in Fig. 4.24. They were aided by recent magnetic data of Welp et al. (1989; cf. Hake, 1968) in deducing the experimental entropy. Bonjour et al. com pared their measured entropies with the fol lowing generalization of Eq. (4.41) to the mixed state of a Type II superconductor: SH �T� B� = Sn �T� + � � �T� × Bc2 �T� − B d · B �T�� �0 dT c2 (4.68) where � � = �0 dM/dB is called the ‘differ ential susceptibility.’ This gives S0 �Ti � − SH �Ti � B� = � � �Ti � × B d · B �T �� �0 dT c2 i (4.69) where Ti = 80 K is the temperature at which all the specific heat curves are still superimposed. The values for B = 5 T calcu lated from Eq. (4.68) using the data of Welp et al. are reasonably close to the measured values, as indicated in the figure. 107 XIII FURTHER DISCUSSION OF THE SPECIFIC HEAT XIII. FURTHER DISCUSSION OF THE SPECIFIC HEAT Earlier in the chapter we mentioned the jump in the specific heat in zero field (4.44), in a magnetic field (4.43), and as predicted by the BCS theory (4.9). We also gave expres sions for the temperature dependence of the specific heat in the superconducting state, one of which (Eq. (4.11)) appeared to be incompatible with the other two expressions (Eqs. (4.50) and (4.54)). In this section we compare these results and use them to evalu ate the electronic specific-heat coefficient � for zero field, after which we will write down an expression for the jump in the specific heat in a magnetic field. At the transition temperature T = Tc in zero field, Eq. (4.50), with A = 0, simpli fies to Figure 4.23 Magnetic field dependence of the spe cific heat difference for parallel and perpendicular fields (Athreya et al., 1988). Cs �Tc � − Cn �Tc � = 4�Bc �0��2 � � 0 Tc (4.70) where Cn �Tc � = �Tc . If the BCS prediction (4.9) is substituted in Eq. (4.70), we obtain for the normalized specific heat factor � of Eq. (4.61) � = 0�357� (4.71) The curves of Figs. 4.7–4.9 were drawn for this value. Since Bc2 /2�0 is an energy den sity expressed in units J/m3 and � is given in units mJ/mole K, it is necessary to multi ply � by the density � and divide it by the molecular weight (MW) in Eq. (4.71), giving us the BCS dimensionless ratio RBCS = Figure 4.24 Magnetic field dependence of the entropy difference of parallel and perpendicular fields showing measured (�) and calculated (•) values for YBa2 Cu3 O7 (Bonjour et al., 1991). �Bc �0��2 �MW� = 449� �0 Tc2 �� (4.72) where Bc is expressed in units mT, � in mJ/mole K 2 , � in g/cm3 , and Tc in degrees Kelvin. It is reasonable to assume that this expression will be a good approximation for Type I superconductors, and we see from the last column of Table 4.3 that this is indeed 108 4 THERMODYNAMIC PROPERTIES Table 4.3 Variation of the Dimensionless Ratio R = Bc2 �MW�/�0 Tc2 �� of Several a Elemental Superconductors Element Tc K B2c �MW� �0 Tc2 �� mT2 cm3 mJ W Ir Ru Zr Os Re Sn V Pb Tc Nb BCS theory 0.015 0.11 0.49 0.61 0.66 1.7 3.72 5.4 7.20 7.80 9.25 — 676 569 577 300 403 522 615 571 733 443 697 449 a R/RBCS 1.51 1.27 1.29 0.67 0.90 1.16 1.37 1.27 1.63 0.99 1.55 1.00 where � has the BCS value 0.357 and the coefficient 1.76 in the exponential expression is chosen because the BCS theory predicts � = 1�76 kTc in Eq. (4.11). The coefficient 14 is selected to normalize Eq. (4.75) to the BCS value (4.11); i.e., Cs �Tc � = 2�43�Tc at the transition point. Figure 4.25 compares the temperature dependence of (4.74) and (4.75), and shows that they are close at all but the lowest temperatures. Equation (4.74) is slightly lower for T near Tc and Eq. (4.75) is significantly lower for T � Tc . The first of these expressions for Cs �T�, i.e., Eq. (4.74), is based on Eq. (4.45), which is a good approximation to the tempera- Bc = Bc �0�, MW is molecular weight, � density, and � electronic specific heat. the case for the elemental superconductors. Equation (4.72) was derived for materials in which the number density of the conduction electrons is the same as the number density of the atoms. For materials in which this is not the case, the effective electron density �� can be used, where � is the factor introduced in Eq. (4.4), to give �Bc �0��2 �MW� = 449� �0 Tc2 ��� (4.73) Equations (4.54) and (4.11) constitute entirely different dependences of Cs �T� on temperature, and it is of interest to compare them. In normalized form, with A set equal to zero, they are 2 T T Cs �T� = 0�285 + 2�145 � �Tc Tc Tc (4.74) Cs �T� T = 14 exp −1�76 c � (4.75) �Tc T Figure 4.25 Comparison of the thermodynamic and BCS expressions (4.74) and (4.75), respectively, for the specific heat ratio Cs /�Tc normalized to the same value at T = Tc . 109 XV THERMODYNAMIC CONVENTIONS ture dependence of the critical field Bc �T� near the critical temperature. However, the temperature derivatives of Eq. (4.45) that enter into the Cs �T� expression (4.43) are not expected to be valid quantitatively far below Tc . The second expression, Eq. (4.75), on the other hand, is based on excitation of quasi particles to energies above the superconduct ing ground state, and is valid at temperatures far below Tc where most of the electrons that contribute to the superconductivity are con densed as Cooper pairs in the ground-energy state. Therefore, we might expect an experi mental Cs �T�-versus-T curve to approximate Eq. (4.75) far below Tc , as in the case of the superconducting Al data shown in Fig. 4.5. Now that we have found explicit expres sions for the specific heat in the supercon ducting state in the absence of a magnetic field, let us examine the case when there is a field present. We will continue to assume that �T = Cn �T� and A = 0, and that the BCS expression (4.10) is valid in zero field at Tc . Thus, in a magnetic field Eq. (4.74) can be written T 2 Cs �T� − Cn �T� = 0�715�T 3 −1 � Tc (4.76) and the jump in specific heat at the transition temperature Tc� in a magnetic field is given by Tc� 2 � � Cs �Tc � − Cn �Tc � = 0�175�T 3 −1 � Tc √ where Tc� = Tc / 3. In addition to the jump in specific heat, there is also latent heat present, Eq. (4.57), in the presence of a magnetic field. XIV. ORDER OF THE TRANSITION We mentioned in Section III that the transition from the normal to the super conducting state in the absence of a mag netic field is a second-order phase transition, which means that the Gibbs free energy and its temperature derivative are continuous at the transition: Gs �Tc � = Gn �Tc �� (4.78) dGs dGn = � dT dT (4.79) This can be seen from Eq. (4.39), using the condition Bc �Tc � = 0 from Eq. (4.45). There fore, there is no latent heat, but there is a discontinuity in the specific heat given, for example, by Eqs. (4.44) and (4.70). We showed in Section X that the transi tion from the superconducting to the normal state in the presence of a magnetic field does have a latent heat given by Eq. (4.58) and, therefore, is a first-order phase transition. XV. THERMODYNAMIC CONVENTIONS (4.77) This change in specific heat Cs − Cn is neg √ � < T / 3 and positive for Tc� > ative for T c c √ Tc / 3. This means that with increasing tem perature there is an upward √ jump in the spe T / cific heat for Tc� < √ c 3 and a downward jump for Tc� > Tc / 3, as shown in Figs. 4.12, and 4.16, respectively. We also see that no jump at all occurs at the crossover point of the normal-state and superconducting curves, There are several conventions in vogue for formulating the thermodynamic approach to superconductivity. Some of these conven tions make use of the total internal energy Utot , which includes the energy of the mag netic field B2 /2�0 = 21 �0 H 2 that would be present in the absence of the superconductor, whereas others, including the one adopted in the present work, use the internal energy U , which excludes this field energy. The 110 4 THERMODYNAMIC PROPERTIES total internal energy and internal energy are related through the expressions Utot = U + B2 � 2�0 (4.80) dUtot = TdS + H · dB� 2 B = dU + d � 2�0 (4.81) (4.82) Some authors, including ourselves, deduce the properties of superconductors with the aid of the Gibbs free energy G defined in Eq. (4.22), while others resort to Gtot , where � Gtot = Htot − TS� (4.83) Still other authors instead employ the Helmholtz free energy F or Ftot , where F = U − TS� (4.84) Ftot = Utot − TS (4.85) B2 � 2�0 (4.86) =F+ that the BCS expression Cs �Tc � = 2�43�Tc of Eq. (4.9) is also valid. It is believed that these models provide a good physical picture of the thermodynamics of the superconduct ing state. A more appropriate description for the high-temperature superconductors would include the AT 3 term in the specific heat. It is, of course, also true that real superconduc tors have more complex temperature depen dences than is implied by these simple mod els. The theoretical approaches presented in the following two chapters are needed to achieve a more basic understanding of the nature of superconductivity. An added complication in making compar ison between results arrived at by different authors arises because some authors use the cgs system instead of SI units. XVI. CONCLUDING REMARKS In the beginning of this chapter we discussed the experimental results of spe cific heat measurements, and then proceeded to develop the thermodynamic approach to superconductivity, an approach in which the specific heat plays a major role. Some of the expressions that were derived are fairly general. Others, however, are for the partic ular model in which the specific heat (4.24) in the normal state obeys the linear lowtemperature relation �T and the critical field (4.45) has a simple parabolic dependence �1 − �T/Tc �2 � on temperature. Some expres sions make use of the additional assumption PROBLEMS 1. Consider a metallic element such as cop per that contributes one electron per atom to the conduction band. Show that in the free-electron approximation the electronic and phonon contributions to the specific heat will be equal at the temperature T = �D �5/24� 2 �1/2 �D TF 1/2 2. Show that the factor � in Eq. (4.5) has the value 1 for an element, 1/7 for the LaSrCuO compound, and 3/13 for the YBaCuO compound. 3. A superconductor has a Fermi energy of 3 eV. What is the density of states at the Fermi level and the electronic specificheat factor �. If this superconductor has an effective mass m∗ of 81, what will be the value of these quantities? What other measurable quantities depend on the effective mass? 4. Consider a BCS-type superconductor with transition temperature Tc = 20 K and a critical field Bc �0� = 0�2 T. What is its electronic specific-heat factor �? What are the values of its specific heat, entropy, Gibbs free energy, and enthalpy 111 PROBLEMS in the superconducting state at 10 K, both in zero field and in an applied magnetic field of 0.1 T? (Ignore the vibrational contribution to the specific heat.) 5. With the initial conditions of the pre vious problem, what applied magnetic field will drive the superconductor nor mal at 10 K? What will be the latent heat? What will be the change in the spe cific heat at the transition? (Ignore the vibrational contribution to the specific heat.) 6. Show that the following expressions for the enthalpy are valid: 9. 10. 11. � Htot = Utot − H · B = H � − 21 �0 H 2 � dHtot = TdS − B · dH = dH � − d 21 �0 H 2 � 7. Show that equating the superconductingand normal-state Gibbs free energies Gs �T� H� = Gn �T� at the critical temper ature leads to Eq. (4.55): � Tc = T c 1 − B Bc �0� 1/2 � 8. Calculate the transition temperature Tc� , jump in specific heat, jump in entropy, jump in enthalpy, and the values of the Gibbs and Helmholtz free energies at the temperature T = Tc� of a Type I super conductor in an applied magnetic field Bapp = 21 Bc . Express your answers in 12. terms of � and Tc , assuming that � = 4�0 and A = �/3Tc2 . We know from thermodynamics that at the transition temperature T = Tc �B� in an applied magnetic field B, the latent heat equals the difference in enthalpy, L = Hn� − Hs� . Show that this difference gives Eq. (4.57). Derive the expression for the enthalpy of a superconductor in a magnetic field, and show that in its normalized form it agrees with the expression Hs� /�Tc2 in Table 4.2. Show that the specific heat jump in a magnetic field has the maximum √ 4��Tc /9 in the range 0 < Tc < 1/ 3, and that the latent heat has the maximum 1 ��Tc2 . 2 Show that the following normalized ther modynamic expressions are valid, du = tds + b · dm� cdt = tds� h� = u − b · m� g = h� − ts� and write down expressions for the nor malized internal energy u and magneti zation m. 13. Derive Eq. (4.70) from Rutger’s for mula. 14. Sketch a three-dimensional Gibbs free energy surface analogous to the surface presented in Fig. 4.20 using the equa tions in Section X. This page intentionally left blank 5 Magnetic Properties I. INTRODUCTION Superconductivity can be defined as the state of perfect diamagnetism, and con sequently researchers have always been interested in the magnetic properties of superconductors. In the second chapter we explained how magnetic fields are excluded from and expelled from superconductors. Then in the previous chapter we examined the thermodynamics of the interactions of a superconductor with a magnetic field. The present chapter will extend the discourse to a number of additional magnetic properties. We begin with a discussion of magne tization, zero field cooling, and field cool ing, with comments on the granularity and porosity of high-temperature superconduc tors. Next we will explain how magnetiza tion depends on the shape of the material and how this shape dependence affects the measured susceptibility. Both ac and dc sus ceptibilities will be treated. Finally, we will show how samples can be categorized in terms of traditional magnetic behavior, such as diamagnetism, paramagnetism, and anti ferromagnetism. The chapter will conclude with remarks on ideal Type II superconduc tors and on magnets. In the present chapter we do not always distinguish between Type I and Type II superconductors since many of the results that will be obtained here apply to both types of superconductors. In later chapters we will discuss addi tional magnetic properties of superconduc tors, such as, in Chapter 11, the intermediate and mixed states of Type I and Type II 113 114 5 MAGNETIC PROPERTIES superconductors, respectively. In Chapter 13 we will present the Bean model which pro vides a good description of some magnetic properties, especially hysteresis loops. II. SUSCEPTIBILITY A material in the mixed state of a Type II superconductor contains magnetic flux in vortices that are embedded in a super conducting matrix with = −1. From a macroscopic perspective we average over this structure and consider the material to be homogeneous with a uniform susceptibil ity having a value that is constant through out the volume. The internal fields Bin Hin , and M are also averages that are uniform at this level of observation. In this chapter we will be working with these average quantities and ignore the underlying mesoscopic vortex structure. We saw in Chapter 1 how the B and H fields within a homogeneous medium are related to the magnetization M and the sus ceptibility through Eqs. (1.69), (1.77), and (1.78a), Bin = 0 Hin + M (5.1) = 0 Hin 1 + (5.2) = M Hin (5.3) where 0 is the permeability of free space and is an intrinsic property of the medium. In the general case the susceptibility is a symmetric tensor with components ij because of the off-diagonal components i = j the vector fields Bin Hin , and M are in different directions. In the principal coordinate system the susceptibility tensor is diagonal with components x y , and z along the three orthogonal principle direc tions. High-temperature superconductors are planar with values a ≈ b in the plane of the CuO2 layers different from c , which is measured along the c direction perpendicular to the layers. This axial anisotropy manifests itself in the large difference in the critical fields of single crystals when measured par allel to and perpendicular to the CuO2 layers, as shown in Table 12.5. Several figures in the present chapter will illustrate this anisotropy. However, for the present we will restrict our attention to the isotropic case, for which = x = y = z . III. MAGNETIZATION AND MAGNETIC MOMENT The magnetization M is the magnetic moment per unit volume. This means that the overall magnetic moment of a sample is the volume integral of M throughout it, � = M dV (5.4) Many magnetic studies of superconductors are carried out using samples with shapes that can be approximated by ellipsoids. When the magnetic field Bapp = 0 Happ is applied along or perpendicular to the symme try axis of such a sample, the internal fields Bin and Hin , and the magnetization M as well, are uniform and parallel to the applied field, with M given by M= V (5.5) where V is the sample volume. Long thin cylinders and thin films are limiting cases of this general ellipsoidal geometry. We begin by analyzing the parallel geometry case of a superconductor in the shape of a long cylinder located in an applied field directed along its axis, as shown in Fig. 12.1. For this case the fields can be written as scalars. We wish to express the internal fields in terms of the known applied field Bapp : Bapp = 0 Happ (5.6) 115 III MAGNETIZATION AND MAGNETIC MOMENT For this particular geometry the boundary condition (1.74) shows that the internal field Hin equals Happ . From Eqs. (5.2) and (5.3) the internal fields are given by Bin = Bapp 1 + Bapp 0 Bapp M= 0 Hin = (5.7) (5.8) VBapp 0 Bin = 0 Bapp 0 Bapp M =− 0 VBapp =− 0 Hin = (5.9) Experimentally, it is the magnetic moment , given by = the applied field Bapp , and that M is propor tional to Bapp through Eq. (5.9). For an ideal superconductor the property of perfect diamagnetism means that = −1, so that Eqs. (5.7)–(5.10) become, respec tively, (5.10) which is measured, for example, by a Super conducting Quantum Interference Device (SQUID) magnetometer. Since V and Bapp are known, Eqs. (5.10) and (5.9) can be used to determine the susceptibility and magneti zation, respectively. In these expressions is the volume susceptibility corresponding to the magnetic moment per unit field per unit volume. We assume that is independent of (5.11) (5.12) (5.13) (5.14) and we see that the internal field Bin vanishes. This is the case illustrated in Fig. 12.1. The fact that Bin vanishes can also be explained in terms of the shielding currents (see Fig. 6.19) which flow on the surface and act like a solenoid to produce a field Bin which can cels Bapp . This was discussed at length in Chapter 2, Section VIII. Figure 5.1 shows the experimentally measured magnetization curve for La09 Sr01 2 CuO4 Figure 5.1 Zero-field magnetization of annealed La09 Sr01 2 CuO4 in applied magnetic fields up to 100 mT at a temperature of 5 K. The maximum of the curve occurs near the lower-critical field Bcl ≈ 30 mT. The dashed line is the low-field asymptote for perfect diamagnetic shielding (Maletta et al., 1987). The inset shows the magnetization in applied fields up to 4.5 T. 116 5 MAGNETIC PROPERTIES Figure 5.2 Typical magnetization curve for T = 01Tc (cf. Fig. 5.3, which is drawn to the same scale). Figure 5.3 Typical magnetization curve for T = 07 Tc drawn to the same scale as Fig. 5.2. plotted against the applied field. The applied field reaches a maximum at 30 mT, which is approximately the lower critical field Bc1 (Maletta et al., 1987; see Müller et al., 1987). The upper critical field is well beyond the highest field used, 4.5 T, as shown in the inset to the figure. Note that the abscissa scale is in terms of milliteslas for the main figure, and in terms of teslas for the inset. We see in Fig. 12.36 that the critical fields Bc1 and Bc2 are highest at 0 K and that they decrease continuously with increas ing temperature until they become zero at the transition temperature Tc . Thus, a mag netization curve, such as that presented in Fig. 10.1, contracts as temperature increases. This situation is illustrated graphically by Figs. 10.2 and 10.3, which show sketches of magnetization curves at two temperatures T = 01Tc and T = 07Tc . IV. MAGNETIZATION HYSTERESIS Many authors have reported hystere sis in the magnetization of superconduc tors, meaning that the magnetization depends on the previous history of how magnetic fields were applied. Hysteresis is observed when the magnetic field is increased from zero to a particular field, then scanned back through zero to the negative of this field, and finally brought back to zero again. Figure 5.4 sketches a low-field hysteresis loop show ing the coercive field Bcoer , or value of the applied field that reduces the magnetiza tion to zero, and the remanent magnetiza tion Mrem , or magnitude of the magnetization when the applied field passes through zero. Figures 5.5 and 5.6, respectively, show how low-field hysteresis loops vary with changes in the scanning-field range and tem perature. It is clear from these figures that the hysteresis loop is thin and close to linear when the scan range is much less than the lower-critical field and when the temperature is close to Tc . Decreasing the temperature broadens the loop. The larger the magnetic field excursion, the more the loop becomes elongated horizontally, which increases the ratio Bcoer /0 Mrem between the coercive field and the remanent magnetization. Figure 5.7 shows how hysteresis loops traversed over a broad field range vary with 117 V ZERO FIELD COOLING AND FIELD COOLING Figure 5.4 Typical low-field hysteresis loop showing the coercive field Bcoer , where magnetization is zero, and the remanent magnetization Mrem which remains when the applied field is reduced to zero. Chapter 13 will present a model, called the critical-state model, which provides an explanation for the shapes of many hysteresis loops. V. ZERO FIELD COOLING AND FIELD COOLING Figure 5.5 Low-field hysteresis loops of La09 Sr01 2 CuO4 at 4.5 K cycled over different ranges of field up to 2 mT (Marcus et al., 1987). the temperature. Each loop has a peak near the lower-critical field Bc1 . Beyond this point flux penetrates and the magnetization begins to decrease gradually. Ideally, no flux pene trates below Bc1 , but in practice some of it does, as Fig. 5.1 suggests. The large hystere sis is indicative of flux pinning. It is observed that as the temperatures is lowered, the loop increases in area, as shown in the figures. Paranthaman et al. (1993) obtained similar results with the superconductor HgBaCuO4+ In Chapter 2 we discussed the magnetic properties of a perfectly diamagnetic material with a hole that is either open or closed to the outside. We examined these two cases for the conditions of (a) zero field cooling (ZFC), a condition characterized by flux exclusion from both the open hole and the enclosed cavity, a phenomenon called diamagnetic shielding, and (b) field cooling (FC), a condi tion characterized by flux expulsion from the cavity but not from the hole, a phenomenon called the Meissner effect. For both cases, the flux is absent from the superconduct ing portion. Hence, the overall sample can exclude more flux when it is zero field cooled than it expels when it is is field cooled. The difference between the amount of excluded 118 5 MAGNETIC PROPERTIES Figure 5.6 Low-field hysteresis loops of YBa2 Cu3 O7 cycled over the same field scan, −3 mT ≤ Bapp ≤ 3 mT, over a range of tempera tures. The loops gradually collapse as the temperature increases. The virgin curve for the initial rise in magnetization is given for each loop (Senoussi et al., 1988). flux and the amount of expelled flux is the trapped flux. To clarify some of the principles involved in ZFC and FC experiments, we will examine the rather idealized case of a cylindrical sample of total volume VT that contains a volume Vs of perfectly supercon ducting material = −1, a cylindrical hole of volume Vh open at the top and bottom, and a totally enclosed cylindrical cavity of volume Vc , material; since the effect in the two cases is the same, we will consider them empty. The magnetic field Bapp is applied parallel to the cylinder axis, as indicated in Fig. 5.9; demagnetizing effects arising from the lack of cylindrical symmetry will not be taken into account. For this composite sample the mea sured or effective magnetic moment eff can receive contributions from three individual components, V T = V s + Vh + Vc eff = s + h + c (5.15) as shown in Fig. 5.8. The hole and cav ity could either be empty or contain normal (5.16) with s due to the superconducting mate rial itself, h resulting from the presence of 119 V ZERO FIELD COOLING AND FIELD COOLING Figure 5.9 The superconducting cylinder sketched in Fig. 5.10 after field cooling in an axial applied field, showing the shielding currents flowing around the out side, the reverse-direction current flow around the walls of the open hole, and the absence of currents in the enclosed cavity. Figure 5.7 High-field hysteresis loops of YBa2 Cu3 O7 cycled over the same field scan, −3 T ≤ Bapp ≤ 3 T, over a range of temperatures. The loops gradually collapse as the temperature increases. The deviation of the virgin curve from linearity occurs near the lower-critical field Bc1 , which increases as the temperature is lowered (Senoussi et al., 1988). the open hole, and c due to the enclosed cavity. In the case of zero field cooling, the circulating surface currents shield the super conductor, hole, and cavity, so Eq. (5.10), with = −1, becomes zfc = −Vs + Vh + Vc Bapp 0 (5.17) For field cooling, the magnetic field is trapped in the open hole, while surface cur rents shield the superconductor itself and the enclosed cavity from this field, which gives for the magnetic moment fc = −Vs + Vc Bapp 0 (5.18) Associated with the effective magnetic moment (5.16) there is an effective magneti zation Meff defined by Eq. (5.5) in terms of the total volume (5.15) Meff = Figure 5.8 Cylindrical superconducting sample with hole of volume Vh open at the top and bottom, and a totally enclosed cavity of volume Vc . Bapp eff = eff VT 0 (5.19) which can be employed to write down the ZFC and FC magnetization, respectively. 120 5 MAGNETIC PROPERTIES The corresponding susceptibilities zfc and fc are determined in Problem 1. We know from Eqs. (5.9) and (5.10) and the above expressions that the ratios between the FC and ZFC moments, magnetizations, and sus ceptibilities all have the same value, fc M = fc = fc zfc Mzfc zfc V s + Vc = Vs + Vh + Vc (5.20) and that this value is independent of the units used. If field cooling is carried out in an applied field Bfc = 0 Hfc that differs from the field Bapp which is applied to measure the magnetic moment, we obtain, neglecting hysteresis (see Problem 3), 0 fc = −Vs + Vc Bapp + Bfc − Bapp Vh (5.21) which reduces to Eq. (5.18) when Bapp = Bfc . Thus, the field trapped in the hole acts like a magnetization with the same magnitude and direction as the quantity (Bfc − Bapp ). Ordi narily, field cooling is carried out in the same field as the susceptibility measurements, so that Bapp = Bfc and Eq. (5.18) applies. As long as the sample is kept below Tc the field Bfc remains in the open hole irre spective of whether the outside field is turned off or another applied field is turned on. Bfc is maintained in the hole by surface currents circulating in opposite directions around the inside of the superconducting tube, as shown in Fig. 5.9 and explained in Chapter 2, Sec tions VIII and IX. This trapped flux sub tracts from the diamagnetic response to make the measured susceptibility and magnetiza tion less negative for the Meissner effect (FC) than for diamagnetic shielding (ZFC). This is shown in Fig. 5.10 for the rubidium fullerene compound (C.-C. Chen et al., 1991; Politis et al., 1992), where the ZFC data points are far below the corresponding FC data, as expected from Eq. (5.20). The ear liest HgBaCaCuO compound samples pro duced FC susceptibilities that were far above Figure 5.10 Rb3 C60 powder sample showing that the zero-field-cooled magnetic susceptibility is more nega tive than its field-cooled counterpart (C.-C. Chen et al., 1991). ZFC ones (Adachi et al., 1993; Gao et al., 1993; Meng et al., 1993b, Schilling et al., 1993). Clem and Hao (1993) examined the four cases of ZFC, FC with data collected on cool ing (FCC), FC with data collected on warm ing (FCW), and remanence. In the fourth case the applied field is turned off after the specimen has been FC, and the remanent magnetization is measured as a function of increasing temperature. VI. GRANULAR SAMPLES AND POROSITY The analysis of the previous section can help us understand experimental suscepti bility data on granular samples. The grains sometimes consist of a mixture of super conducting and normal material of about the same density, with empty space between and perhaps within the material. The two densities can be comparable when the sam ple preparation procedure does not com pletely transform the starting materials into the superconducting phase. A well-made granular superconductor does not contain any 121 VII MAGNETIZATION ANISOTROPY normal material, but it does have intergran ular and perhaps intragranular spaces, either of which can trap flux. The field-cooled moment can be significantly less than the zero-field-cooled moment, as shown by the data in Table VIII.1 of previous work (Poole et al., 1988). A quantitative measure of the degree of granularity of a sample is its porosity P, which is defined by P = 1 − / x-ray where the density (5.22) of the sample is = m VT (5.23) and the x-ray density is calculated from the expression x-ray = MW V0 N A (5.24) where NA is Avogadro’s number and V0 is the volume of the sample per formula unit, with the value V0 = abc V0 = YBa2 Cu3 O7− (5.25) 1 abc 2 LaSrCuO BiSrCaCuO TlBaCaCuO (5.26) where a b, and c are the lattice constants and the La, Bi, and Tl compounds have assigned to them two formula units per unit cell, as explained in Chapter 8. Porosity is a measure of the proportion of empty spaces or voids within and between the solid material or grains of a sample. Prob lem 4 shows how Vs Vh , and Vc can be deter mined from measurements of zfc and fc . The x-ray density calculated from the unit cell dimensions of YBa2 Cu3 O7 is 6383 g/cm3 . Typical densities of granu lar samples vary from 4.3 to 56 g/cm3 , cor responding to porosities between 33% and 12%, respectively (Blendell et al., 1987; Mathias et al., 1987). Porosity can be reduced by applying pressure to the material. For example, a sam ple of YBa2 Cu3 O7 with a 5:1 ratio between flux exclusion and flux expulsion was com pressed at 20–30 kbar to a claimed 100% of theoretical density, = x-ray , bringing the measure flux expulsion to within about 11% of the theoretical value (Venturini et al., 1987). Researchers have also found 100% flux shielding and 95% flux expulsion in YBa2 Cu3 O7 at 4.2 K (Larbalestier et al., 1987a). Good single crystals, of course, have a porosity of zero. VII. MAGNETIZATION ANISOTROPY The magnetic properties of hightemperature superconductors are highly anisotropic, with magnetization and suscep tibility depending on the angle which the applied field makes with the c-axis. We will see in Chapter 12, Section IV, that anisotropy here is a result of the difference in the values of the coherence length, penetration depth, and effective mass measured along the c direction as opposed to values obtained from measurements in the a b-plane. Particles of anisotropic superconductors in a magnetic field experience a torque which tends to align them with the field (Kogan, 1988). Anisotropy effects can be determined by employing single crystals, epitaxial films, or grain-aligned powders. Epitaxial films are generally single-crystal films with the c-axis perpendicular to the plane. It is, of course, preferable to work with untwinned single crystals or epitaxial films. However, these are not always available, and much good research has been carried out with aligned granular samples. Grain alignment is a technique that con verts a collection of randomly oriented grains into a set of grains with their c-axes preferen tially pointing in a particular direction. This 122 5 MAGNETIC PROPERTIES alignment can be brought about by uniaxial compression, by application of a strong mag netic field to grains embedded in, for exam ple, epoxy, or by melting a random powder sample and reforming it in the presence of a temperature gradient (Farrell et al., 1987). It is much easier to fabricate grain-aligned samples than single crystals. Grain-aligned samples, however, cannot compete with sin gle crystals in terms of degree of alignment. Untwinned monocrystals are needed for per fect alignment. Another technique for preparing sam ples with monocrystal characteristics is melttextured growth (L. Gao et al., 1991; Jin et al., 1988; Murakami et al., 1991). In melt-textured growth a granular material is melted and then slowly cooled in a ther mal gradient to produce a high degree of texturing. The effect is to reduce weaklink grain boundaries and increase critical currents. Figure 5.11a shows that both the ZFC and FC susceptibilities of YBa2 Cu3 O7 are greater in magnitude (i.e., more negative) for the applied field aligned parallel to the c-axis than they are for Bapp aligned perpendicular to c (i.e., along the copper-oxide planes); these measurements were made with grainaligned samples. The figure shows that the susceptibility data for a nonaligned power are between the results for Bapp c and Bapp⊥c . Figure 5.11c shows that the susceptibility is much less for field cooling in the field Bfc = 03 T, again with the data for Bappc lying below the data for Bapp⊥c . For a small sample the overall vol ume VT can be estimated by viewing it under a microscope. This is sometimes called the volume susceptibility, although in actuality the parameter is dimension less. Many investigators determine sample size by weighting and report what is some times called the mass susceptibility mass , defined by mass = = Experimentally, susceptibility, a dimen sionless quantity, is determined from the measured magnetic moment of the sample with the aid of Eq. (5.10), = 0 VT Bapp (5.27) (5.28) where VT is the mass of the sample. This quantity has the dimensions m3 /kg in the SI system and cm3 /g in the cgs system. Many susceptibility and magnetism measurements are carried out with a SQUID, a dc measuring instrument (see Section III). In this device, which is sketched in Fig. 5.12, a magnetized sample that has been moved into a sensor coil causes the flux through the coil to change. The current produced by this flux change is passed to the multiturn coil on the left side of the figure where it is amplified by the increase in the number of turns. The SQUID ring with its weak links detects this flux change in a manner that will be discussed in Chapter 15, Section VIII.1. The change in flux provides the magnetic moment by the expression 0 = (5.29) and from Eq. (5.27) we have for the suscep tibility, = VIII. MEASUREMENT TECHNIQUES 0 VT Bapp /VBapp (5.30) The data presented in Figs. 5.10 and 5.11 were obtained with a SQUID magnetome ter. More classical techniques, such as the vibrating sample magnetometer or perhaps the Gouy or Faraday balance, are less fre quently employed. One can make ac suscep tibility measurements using a low-frequency mutual inductance bridge operating at, for example, 200 Hz. VIII MEASUREMENT TECHNIQUES 123 Figure 5.11 (a) Zero-field-cooled (closed symbols) and field-cooled (open symbols) susceptibility versus temperature for nonaligned powder (circles) and grain-aligned samples of YBa2 Cu3 O7 in a field of 5 mT with Bappc (triangles) and Bapp⊥c (squares), (b) normalized susceptibilities for the zero-field-cooled samples of (a), (c) field-cooled measurements in 0.3 T, plotted with the same symbol convention (Lee and Johnston, 1990). Figure 5.12 The change of magnetic flux in a sensor coil loop that has been produced by raising or lowering a sample induces a current which is transferred to a multiloop coil where it is measured by a Superconducting Quantum Interference Device (SQUID). 124 5 MAGNETIC PROPERTIES IX. COMPARISON OF SUSCEPTIBILITY AND RESISTIVITY RESULTS We saw in Section V that the suscep tibility of a composite sample is a linear combination of the contributions from its component parts. Thus, susceptibility mea surements determine the magnetic state of an entire sample, and also give a better indication of the degree to which the sam ple has transformed to the super-conducting state. Resistivity measurements, on the other hand, merely show whether or not continu ous superconducting paths are in place. In addition, while a dc susceptibility measure ment provides a better experimental indicator of the overall superconducting state, a resis tivity measurement is a better practical guide for application purposes. We should also note that magnetization is a thermodynamic state variable (cf. Chapter 4, Section VI), whereas resistivity is not. The properties of zero resistance and perfect diamagnetism are the two classic ways of defining supercon ductivity. In an ideal homogeneous material both measurements should provide the same transition temperature. The transition temperatures determined by magnetic susceptibility and resistivity measurements sometimes differ somewhat. When the transition is sharp, resistivity can drop sharply to zero at a temperature slightly above the onset of the susceptibility or mag netization transition, as shown in Fig. 2.21. When the transition is broad, the -versus-T and -versus-T curves often overlap consid erably. Many articles provide susceptibility and resistivity curves for the same sample. Figure III-5 from our previous work (Poole et al., 1988) compares the resistivity, Meiss ner magnetization, ac susceptibility, and spe cific heat transitions for the same X. ELLIPSOIDS IN MAGNETIC FIELDS In Section III we treated the case of a cylindrically shaped sample in a paral lel magnetic field, noting that this geom etry was chosen to avoid demagnetization effects that could complicate the calculation of the internal magnetic field and magnetiza tion. Some commonly used superconductor arrangements in magnetic fields, such as thin films in perpendicular fields, have very pro nounced demagnetization effects. In practice, these arrangements constitute limiting cases of ellipsoids, so that in the present section we will analyze the case of an ellipsoid in an applied field. Then we will show how some common geometries are good approxi mations to elongated and flattened ellipsoids. Many of the results of this and the following few sections are applicable to both Type I and Type II superconductors. When an ellipsoid with permeability is placed in a uniform externally applied mag netic field Bapp oriented along one of its prin cipal directions, its internal fields Bin and Hin will be parallel to the applied field, and hence all of the fields can be treated as scalars. Their values will be determined by applying Eqs. (5.1) and (5.2) to the internal fields Bin = Hin = 0 Hin + M = 1 + 0 Hin (5.31) and the applied fields Bapp = 0 Happ Mapp = 0 (5.32) and utilizing the demagnetization expression NBin 1 − NHin + = 1 Bapp Happ (5.33) YBa2 Cu3 O7 sample (Junod et al., 1988). where N is the demagnetization factor, to relate the internal and applied fields. The 125 XI DEMAGNETIZATION FACTORS demagnetization factors along the three prin cipal directions of the ellipsoid are geomet rical coefficients that obey the normalization condition Nx + Ny + Nz = 1 (5.34) Bapp < 1 − NBc , as will be explained in Chapter 11, Section IV. They apply to Type II superconductors when Bapp < 1 − NBc1 , but for higher applied fields Eqs. (5.35)–(5.37) must be used since −1 < < 0. Sometimes the transition from the Meissner to the vortex state is not sharply defined and a precise value of Bc1 cannot be determined. with the largest value along the shortest prin cipal axis and the smallest value along the longest principal axis. We will confine our attention to situations in which the exter nal field is oriented along a principal direc tion since all the other orientations are much more complicated to analyze. In the follow ing section we will give explicit expressions for the demagnetization factors associated with a sphere, a disk, and a rod. Solving for Bin , Hin , and M in Eqs. (5.31) and (5.33) gives It will be helpful to write down formulae for the demagnetization factors for sample shapes that are often encountered in practice. For a sphere all three factors are the same, a = b = c and Nx = Ny = Nz , so that from the normalization condition (5.34) we obtain 1+ Bin = Bapp 1 + N Bapp /0 Hin = 1 + N Bapp M= · 0 1 + N 1 sphere (5.41) 3 For an ellipsoid of revolution with the z direction selected as the symmetry axis, the semi-major axes a = b = c along the x-, y-, and z-axes, and the demagnetization factors are N = Nz and N⊥ = Nx = Ny , subject to the normalization condition (5.35) (5.36) (5.37) for the internal fields and magnetization expressed in terms of the applied fields. We should bear in mind that the susceptibil ity is negative for a superconductor, so that the denominators in these expressions become small when approaches −1 and N approaches 1. For an ideal superconducting mate rial = −1. Equations (5.35)–(5.37) now assume a simpler form: Bin = 0 Bapp /0 1−N Bapp /0 M =− 1−N Hin = (5.38) (5.39) (5.40) These expressions are applicable to Type I superconductors subject to the condition XI. DEMAGNETIZATION FACTORS N= N + 2N⊥ = 1 (5.42) of Eq. (5.34). An oblate ellipsoid, i.e., one flattened in the x, y-plane, has c < a with N > N⊥ , and von Hippel (1954) gives (cf. Osborn, 1945; Stone, 1945; Stratton, 1941), N = 1 1 − 2 − 2 3 1/2 sin−1 c < a (5.43) where the oblate eccentricity is = 1 − c2 /a2 1/2 c < a (5.44) For a prolate ellipsoid, i.e., one elongated along its symmetry axis so that c > a and N < N⊥ , we have again from von Hippel (1954) � � � � 1 − 2 1 1+ N = ln −1 c > a 2 2 1− (5.45) 126 5 MAGNETIC PROPERTIES where the prolate eccentricity is = 1 − a2 /c2 1/2 c > a (5.46) Of especial interest are samples in the shape of a disk, which may be considered the limiting case of a very flattened oblate ellipsoid, c a, with the demagnetization factors N ≈ 1 N⊥ ≈ 0 flat disk (5.47) or in the shape of a rod, which is the limit of an elongated prolate ellipsoid, c a, with the values N ≈ 0 N⊥ ≈ 1 2 long cylinder (5.48) Correction factors i to the limiting val ues of Ni given in Eqs. (5.47) and (5.48) are shown in Figs. 5.13 and 5.14, respec tively, and listed in Table 5.1. Problems 6 and 7 give explicit expressions for these fac tors. Figure 5.15 shows how the parallel and perpendicular components of N depend on Figure 5.14 Demagnetization factors Nx = Ny = 1 1 − 4 and Nz = 4 1 of a prolate ellipsoid with 2 a = b c, using the notation of Fig. 5.13. Table 5.1 Demagnetization Factors for Ellipsoids of Revolution with Semi-axes a = b and c for the Case of a Disk (oblate, c < a), Sphere (c = a), or Rod prolate c > aa Shape Condition N⊥ N disk limit flat disk c→0 ca 0 1 1 − 1 oblate c≈a sphere c=a prolate c≈a long rod ca rod limit c→ a Figure 5.13 Demagnetization factors Nx = Ny = 1 1 and Nz = 1 − 1 of an oblate ellipsoid with 2 1 semi-major axes a = b c along the x, y, and z direc tions, respectively. 1 2 1 1 − 3 1 3 1 + 3 1 − 2 1 2 1 2 2 1 2 3 1 2 4 1 3 1 3 1 3 + 2 − 3 4 0 Values of the correction factors i are given in Problems 6 and 7. the length-to-diameter ratio of the ellipsoid. D.-X. Chen et al. (1991) reviewed demagne tization factors for cylinders; other pertinent articles are Bhagwat and Chaddah (1992), Kunchur and Poon (1991), and Trofimov et al. (1991). The electric case of depolar ization factors is mathematically equivalent (Stratton, 1941). 127 XII MEASURED SUSCEPTIBILITIES Figure 5.15 Dependence on the ratio c/a of the demagnetization factors N⊥ = Nx = Ny perpendicular to the c and N = Nz along the axis. The solid lines were calculated axis of an ellipsoid with semi-major axes a = b = using the exact expressions (5.42) to (5.46), and the dashed lines from the approximation formulae of Table 5.1 and Problems 6 and 7. XII. MEASURED SUSCEPTIBILITIES From the theoretical viewpoint the mag netic susceptibility is a fundamental prop erty of a material. It can be anisotropic, but for the present we will treat the isotropic case. It is defined by Eq. (5.3) as the ratio between the two quantities M and Hin in the interior of a superconductor, = M/Hin (5.49) In practice, research workers often report an experimentally determined susceptibility exp that has been calculated from measured val ues of the magnetization and the applied field Bapp , as follows: exp = 0 M/Bapp (5.50) This is the definition of susceptibility that often appears in solid state physics books. Equations (5.49) and (5.50) are only equiv alent for the case of “parallel geometry,” in which the applied field is along the axis of a cylinder and the demagnetization factor N is zero: Hin = Bapp /0 . When N is not zero, Eq. (5.49) is still valid because is a property of the mate rial independent of its shape. Substituting Eq. (5.37) in Eq. (5.50) gives the expression exp = /1 + N (5.51) which may be solved for the intrinsic suscep tibility in terms of the experimentally mea sured value = exp /1 − Nexp (5.52) 128 5 MAGNETIC PROPERTIES The susceptibility must be in dimension less units (SI units) to apply this expression. Equation (10.52) shows that ≤ exp , where both and exp are negative. Some authors set N = −N in Eq. (5.52) so as to write the approximate expression ≈ exp 1 − N (5.53) which, however, underestimates the magni tude of , especially when N is appreciable and is small. XIII. SPHERE IN A MAGNETIC FIELD In this section we will examine a case that is commonly treated in electromagnetic theory and solid-state physics texts—that of a sphere in a magnetic field. This will pro vide us with closed-form expressions for the fields and the magnetization, both inside and outside the sphere as well as on its surface. We mentioned in the previous section that for a sphere N = 1/3, so that using Eqs. (5.35)–(5.37) and (5.52) we have, respectively, for the two internal fields, mag netization, and susceptibility, 31 + Bin = Bapp 3+ 3Bapp /0 Hin = 3+ Bapp 3 M= · 0 3 + 3exp = 3 − exp electrodynamics texts (e.g., Jackson, 1975, p. 150), � = − r− out � a3 · 2 Bapp cos +3 r (5.58) where is the angle of the position vector r relative to the applied field direction. This is the solution to Laplace’s equation 2 = 0 (5.59) which for the case of axial symmetry in spherical coordinates has the form � � 1 d 2d r r 2 dr dr � � 1 d d + 2 · sin = 0 r sin d d (5.60) where the potential out r depends on the polar angle , but not on the azimuthal angle . This solution is subject to two boundary conditions, first, that Br and H are contin uous across the surface at r = a, and sec ond, that B = Bapp far from the sphere where r a. The first term of Eq. (10.58), rBapp cos = zBapp (5.54) (5.55) (5.56) (5.57) The B field immediately outside a super conducting sphere of radius a placed in a uniform external magnetic field Bapp may be calculated from the standard formula for the magnetic scalar potential out given in corresponds to the potential of the uniform applied field. The second term is known to be the magnetic field produced by a magnetic dipole of moment = a3 Happ / + 3. The radial component Br of the field outside, Br = − out r � � 2 a3 = 1+ Bapp cos · + 3 r3 has a value at the surface r = a of � � 3 + 1 Bapp cos Br = +3 (5.61) (5.62) (5.63) 129 XIV CYLINDER IN A MAGNETIC FIELD Setting = −1 shows that this radial field vanishes at the surface for a perfect diamag net. The polar angle component B outside, 1 B = − · out r � � a3 = 1− · Bapp sin + 3 r3 has a value at the surface of � � 3 B = B sin + 3 app (5.64) (5.65) (5.66) This field reaches a maximum along the equator, i.e., when = /2. The magnetic field lines around the sphere, which are sketched in Fig. 2.23, are closest together at this maximum field position along the equator. Equations (5.63) and (5.66) show that for the case = −1 of perfect diamagnetism, the external field is parallel to the surface with no radial component. This field may be looked upon as inducing a current density in the surface of the sphere that circulates along circles of longitude that are oriented perpendicular to the z-axis, as illustrated in Fig. 2.30. These currents serve to cancel the B field that would otherwise be present inside the sphere. The presence of the factor sin in Eq. (5.66) means that the current density along a particular longitude circle at the latitude is proportional to the radius of the circle on which it flows, where = r sin , as indicated in Fig. 5.16. This causes each such current element to produce the same magnitude of magnetic field within the sphere, as expected. We will see in Chapter 11, Section XI, that the results of this section apply directly to a sphere in the mixed state of a Type II superconductor for applied fields in the range 23 Bc1 < Bapp < Bc2 . For applied fields below 23 Bc1 the Meissner state exists with = −1. For a Type I superconductor in the applied field range 23 Bc < Bapp < Bc , the formalism applies with chosen so that Figure 5.16 Coordinates for describing current flow along the surface of a sphere in a magnetic field applied along the z direction. Hin = Bc /0 . For the condition Bapp < 23 Bc we have = −1, as will be clear from the discussion in Chapter 11, Section IV. XIV. CYLINDER IN A MAGNETIC FIELD On several occasions we have discussed the case of a long diamagnetic cylinder in an axially applied magnetic field, as shown in Fig. 12.1. In this “parallel geometry” the demagnetization factor N is zero. Inserting N = 0 in Eqs. (5.35)–(5.37) gives Eqs. (5.7)– (5.9), which we have already obtained for this case. These reduce to Eqs. (5.11)–(5.13), respectively, for the ideal Type I supercon ductor with = −1. Since N = 0, the bound ary condition—i.e., that H is continuous Hin = Happ across the interface—leaves the H field undisturbed by the presence of the 130 5 MAGNETIC PROPERTIES problem in which Laplace’s equation is solved in cylindrical coordinates with the 2 /z2 term omitted, � � 1 2 1 d · + 2 · 2 = 0 (5.72) d Figure 5.17 Magnetization M (a) and shielding cur rent flow J (c) of a superconducting rod located in an applied magnetic field with the perpendicular geometry arrangement (b). superconductor. The fields outside the cylinder are then Bout = Bapp (5.67) Hout = Bapp /0 (5.68) independent of position. An alternate arrangement that some times occurs in practice is the perpendicu lar geometry sketched in Fig. 5.17, whereby the cylinder axis remains in the z direction but the magnetic field is applied along x. For this case we see from Table 5.1 that N = 21 so that the fields inside are, from Eqs. (5.35)–(5.37), Bin = Bapp 21 + 2+ Bapp 2 0 2 + Bapp 2 M= 0 2 + Hin = = (5.69) (5.70) (5.71) 20 10 2 − exp The calculation of the fields outside for this geometry is more complicated. There is no z dependence, so this is a two-dimensional subject to two boundary conditions—first that H parallel to the surface and B per pendicular to the surface are both continu ous; second, that far from the sample B is in the x direction with the magnitude Bapp . The solution for the magnetic scalar potential is � � a2 · Bapp cos = − − out +2 (5.73) which is similar to the case of the sphere given in Eq. (5.58). The differences arise from the particular forms of the differential operators in Eqs. (5.60) and (5.72). The first term in this potential, Bapp cos = xBapp corresponds to the potential of the uniform applied field, where x = cos . The radial component B of the field outside, B =− out � = 1+ (5.74) � a2 · B cos + 2 2 app has a value at the surface of � � 2 + 1 Bapp cos B = +2 (5.75) (5.76) which vanishes for the perfect superconduc tor case of = −1. The azimuthal compo nent B outside, 1 B = − · � out � a2 = 1− B sin · + 2 2 app (5.77) (5.78) 131 XV ac SUSCEPTIBILITY becomes at the surface � � 2 B = B sin + 2 app (5.79) This surface field is zero along x and reaches a maximum value along the y direc tion, where = /2 and B /0 = Hin (cf. Eq. (5.70)). A sketch of the magnetic field lines around the cylinder would resemble that of Fig. 2.23. This case is equivalent to a two-dimensional problem with all of the field lines lying in the x y-plane. For perfect diamagnetism, = −1, we see from Eqs. (5.76) and (5.79) that immedi ately outside the cylinder the external mag netic field is parallel to the surface with no radial component. Longitudinal surface cur rents Jz flow along the surface in the +z direction on one side and in the −z direc tion on the other, forming closed loops at the ends that sustain the magnetization inside, as indicated in Fig. 5.17. These currents serve to cancel the B field that would otherwise be present inside the cylinder. The factor sin in Eq. (5.78) causes the surface-current den sity to produce the uniform magnetic field of Eq. (5.69) inside the cylinder. XV. ac SUSCEPTIBILITY Earlier in the chapter we discussed sus ceptibilities determined in constant magnetic fields. Now let us consider what happens when the external field varies harmonically in time (D.-X. Chen et al., 1990c; vide Q. Y. Chen, 1992; Hein et al., 1992; Khode and Couach, 1992). An ac field B0 cos t applied to the sample causes the magnetiza tion Mt to trace out a magnetic hystere sis loop in the course of every cycle of the applied field. The initial loop for the first cycle will be different from all the other cycles, as suggested by the initial curves starting from the middle of the loops of Figs. 5.6 and 5.7, but after several cycles a state of dynamic equilibrium is attained in which the magnetization Mt repeatedly traces out the same curve, perhaps of the types shown in Figs. 5.5 or 5.6, during every period of oscillation. If the magnetization were to change lin early with the applied field, the response would be Mt = M0 cos t in phase with the applied field, with M0 = B0 /0 . The shape of the loop causes Mt to become distorted in shape and shift in phase relative to the applied field, causing it to acquire an out-of phase component that varies as sin t. We can define the inphase dispersion and the out-of-phase (quadrature) absorption sus ceptibilities (Matsumoto et al., 1991): 0 � Mt cos t d t B0 � = 0 Mt sin t d t B0 = (5.80a) (5.80b) Higher harmonic responses n and n at the frequencies nt have also been studied (Ghatak et al., 1992; Ishida and Gold farb, 1990; Ishida et al., 1991; Jeffries et al., 1989; Ji et al., 1989; Johnson et al., 1991; Yamamoto et al., 1992). Note that the absorption susceptibility is proportional to the energy dissipation. Unfortunately, in practice it is not practical to measure Mt, so that a different approach must be followed. The usual mutual inductance method for determining and involves placing the sample in the coil of an LC tuned circuit to establish an alternating magnetic field B0 cos t in the superconductor and to detect the voltage induced in a detector pickup coil coupled to the coil of the LC circuit. The presence of the sample changes the effec tive inductance and resistance of the LC circuit, and this change is reflected in the form of the current induced in the detec tor coil. The component of the induced sig nal which is in phase with the applied field is proportional to the dispersion , while the out-of-phase component is proportional 132 5 MAGNETIC PROPERTIES to the absorption . These two responses can be separated instrumentally by a lock-in detector that compares the phase of the out put signal with that of the reference signal B0 cos t. Figures 5.18 and 5.19 present the tem perature dependence of the dispersion and absorption components of the ac suscep tibility determined for applied fields of the form Bapp = Bdc + B0 cos t (5.81) at the frequency /2 = 73 Hz. Figure 5.18 shows the results for three alternating field amplitudes B0 with Bdc = 0, and Fig. 5.19 illustrates the effect of simultaneously apply ing a dc field. We see from the figures that for a particular applied field, decreases continuously as the temperature is lowered, also that the drop in is sharper and occurs closer to Tc for lower values of B0 and Bdc . The peak in the -versus temperature curve is near the center of the sharp diamagnetic change in , as expected, inasmuch as magnetic susceptibilities, like dielectric constants, obey Kramers–Kronig relations (cf. Chapter 15, Section II.E; Poole and Farach, 1971, Chapter 20). Recent data on HgBa2 CuO4+ at high pressure exhibit this behavior (Klehe et al., 1992). These K–K relations permit to be cal culated from knowledge of the frequency dependence of , and vice versa. Increasing the applied field shifts the peak to lower temperatures and broadens it (D.-X. Chen et al., 1988; Goldfarb et al., 1987a, b; Ishida and Goldfarb, 1990; Puig et al., 1990; K. V. Rao et al., 1987). These ac response curves depend only slightly on frequency below 1 kHz so that the magnetization is able to follow the variation in the applied field. Figure 5.18 Real ( ) and imaginary ( ) components of the susceptibility of YBa2 Cu3 O7− measured in the applied ac magnetic fields with 0 Hac = 00424, 0.424, and 2.12 mT as a function of the temperature below Tc for a frequency of 73 Hz. For this experiment 0 Hdc = 0; the data were not corrected for the demagnetization factor (Ishida and Goldfarb, 1990). 133 XV ac SUSCEPTIBILITY Figure 5.19 Real ( ) and imaginary ( ) components of the susceptibility of YBa2 Cu3 O7− measured in superimposed ac and dc magnetic fields as a function of the temperature below Tc for a frequency of 73 Hz. The conditions were 0 Hac = 0424 mT, 0 Hdc = 0, 0.424, 0.993, 2.98, and 8.48 mT; the data were not cor rected for the demagnetization factor (Ishida and Goldfarb, 1990). The ac susceptibility results can be thought of in terms of the temperature depen dence of the lower-critical field Bc1 T (cf. Figs. 12.36 and 5.28). A low applied field at low temperature will be far below Bc1 T, thus in Fig. 5.18 the curve for B0 = 00424 approaches total dia-magnetic shielding. A high applied field near but still below Tc will exceed Bc1 T so that , will be smaller in magnitude and closer to its normal state value, as shown in Fig. 5.19. It is more customary to interpret ac susceptibility data in terms of one of the critical-state models that will be introduced in Chapter 13 (Chen and Sanchez, 1991) with a temperature-dependent critical current (Ishida and Goldfarb, 1990; Johnson et al., 1991; LeBlanc and LeBlanc, 1992). Ji et al. (1989) assumed the two-fluid model temper ature dependence of Eq. (2.56). Here mag netic flux in the form of vortices alternately enters and leaves the sample as the mag netization cycles around the hysteresis loop. The maximum of can be interpreted as occurring near the applied field Bapp = B∗ , where the critical current and internal field just reach the center of the sample. Sample geometry (Forsthuber and Hilscher, 1992) and size effects (Skumryev et al., 1991) have also been reported. Clem (1992) suggested that there are three main mechanisms responsible for ac susceptibility losses: (a) flux flow losses, which can also be called eddy current losses or viscous losses, arising in the absence of pinning centers, when time-varying currents arising from the oscillating applied magnetic field induce fluxons to move, (b) hystere sis losses occuring near pinning centers that impede the flux motion, as well as wherever vortices of opposite sense annihilate each other, and (c) surface pinning losses aris ing from a surface barrier to vortex entry and exit (Hocquet et al., 1992; Mathieu and Simon, 1988). An additional complication in granular superconductors is the presence of 134 5 MAGNETIC PROPERTIES both intergranular and intragranular shield ing currents. In a granular superconductor the ac sus ceptibility is expected to receive contribu tions from intergranular current flow in loops through Josephson junctions at the bound aries between grains as well as from intragranular shielding current flow within the individual grains (J. H. Chen, 1990a, b; Lam et al., 1990; Lera et al., 1992; Müller and Pauza, 1989). The -versus-T curves can exhibit both intergranular and intragranular peaks. Coreless Josephson vortices at the junctions and the more common Abrikosov vortices inside the grains alternately sweep in and out of the sample during each cycle around the hysteresis loop. XVI. TEMPERATURE-DEPENDENT MAGNETIZATION Diamagnetism is an intrinsic character istic of a superconductor. Superconductors exhibit other types of magnetic behavior as well, due to, for example, the presence of paramagnetic rare earth and transition ions in their structure. Susceptibility above Tc can have a temperature-independent contribution 0 arising from the conduction electrons along with a temperature-dependent Curie–Weiss term due to the presence of para-magnetic ions, = 0 + = 0 + K2 3kB T − (5.82) C T − (5.83) where is the magnetic moment of the para magnetic ions, K is a parameter that incor porates the concentration of para-magnetic ions and the conversion factor (1.86) for volume susceptibility, and C is the Curie constant. The Curie–Weiss temperature is negative for ferromagnetic coupling between the magnetic ions and positive for antiferro magnetic coupling. Below Tc the large dia magnetism generally overwhelms the much smaller terms of Eq. (5.82), and they become difficult to detect. A. Pauli Paramagnetism The constant term 0 in Eq. (5.82) is often Pauli-like, arising from the conduc tion electrons (cf. Eq. (1.84)). We see from Eq. (1.83) that Pauli provides an estimate of the density of states DEF at the Fermi level. B. Paramagnetism Most superconductors are paramagnetic above Tc . For example, it has been found (Tarascon et al., 1987b) that the susceptibil ity of YBa2 Cu3 O7− above Tc has a tempera ture dependence that obeys the Curie–Weiss law 1.79, with ≈ 03 B /mole of Cu and ≈ −20 to −30 K for oxygen contents in the range 0–0.6. Removing more oxygen increases and decreases , but the sam ples no longer superconduct. These measured moments are less than the Cu2+ spin-only value of 19B given by Eq. (1.82), = g SS + 1 1/2 B = 19B (5.84) where S = 21 and g ≈ 22. Oxide materials in which magnetic rare earths replace lanthanum or yttrium pro vide linear plots of 1/ versus T above Tc as shown by the solid curves in Fig. 5.20, indicating paramagnetic behav ior. For some compounds the temperatureindependent term 0 of Eq. (5.82) is zero. Vacuum annealing of the samples destroyed the superconductivity and gave linear Curie– Weiss plots below Tc , shown by the dashed curves in the figure, which provide from the extrapolated intercept at T = 0. The mag netic moments were very close to the val ues gJJ + 11/2 expected from Eq. (1.80) 135 XVI TEMPERATURE-DEPENDENT MAGNETIZATION Figure 5.20 Temperature dependence of the reciprocal susceptibility 1/ for a series of rare earth R substituted RBa2 Cu3 O7− superconductors over the temperature range 100–300 K in a field of 1 T (solid lines). Data for the corresponding nonsuperconducting vacuumannealed compounds (dashed lines) are shown for comparison. The linear behavior is indicative of paramagnetism (Tarascon et al., 1987b). for rare earth ions. The positive sign for indicates that these ions interact antiferro magnetically, with the susceptibility behav ior above Tc corresponding to Fig. 1.15. The results suggest nearly complete decoupling of the Cu–O planes responsible for the super conducting properties from the planes con taining the rare earth ions responsible for the magnetic properties. Such decoupling of the magnetic and superconducting properties was observed in Chapter 3, Section X, for the Chevrel phases; it also occurs with the heavy fermions (Jee et al., 1990; Konno and Veda, 1989). The paramagnetic contribution to aris ing from the Curie–Weiss law below Tc should appear as a rise in or M near T = . Such a rise is indeed noticeable at tem peratures low enough for the diamagnetic contribution to have already come close to the asymptotic value 0 expected experi mentally at absolute zero. In practice, this paramagnetism is often too weak to observe. However, we see from that data shown in Fig. 5.21 that it is enhanced at high applied fields. In fact, the highest fields used, Bapp > 15 T, are strong enough to overwhelm the diamagnetic contribution and drive the mag netization positive. This rise in M is also partly due to the decrease in the diamag netism as Bapp is increased. The inset to this figure shows how the Meissner frac tion, which is the value of fc expressed as a percentage of its value (−1) for per fect diamagnetism, depends on the applied field. The susceptibility above Tc of the series of compounds YBa2 Cu09 A01 3 O7− , where A is a first transition series element, is an average of the contributions from the A and Cu ions. It has been found to obey Eq. (5.82) with an effective magnetic moment given by (Xiao et al., 1987a, b), 2eff = 012A + 092Cu (5.85) where A and Cu are the moments of the A and Cu atoms, respectively. We see from Fig. 5.22 that the depression of Tc correlates 136 5 MAGNETIC PROPERTIES Figure 5.21 Appearance of a paramagnetic contribution at the low-temperature end of a field-cooled magnetization determination. The contribution becomes dominant as the field Bfc was increased from 0.5 to 4 T (i.e., from 5 to 40 kG), as shown. The inset gives the Meissner fraction (MF) as a function of the applied field from 0 to 0.5 T (Wolfus et al., 1989). moment, the lower the Tc value. Others have reported similar results (e.g., Maeno et al., 1987; Oseroff et al., 1987). C. Antiferromagnetism Figure 5.22 Dependence of the transition temperature Tc (—) and magnetic susceptibility at 100 K (– – –) on the number of valence electrons for the series of compounds YBa2 Cu09 A01 3 O7− , where A is a 3d transition element, as shown (Xiao et al., 1987a). with the size of the magnetic moment of the substituted transition ion—the larger the Cuprate superconductors generally have a negative Curie–Weiss temperature indicative of antiferromagnetic coupling (Chapter 1, Section XV). The undoped com pound La2 CuO4 is an antiferromagnet below the Néel temperature TN ≈ 245 K, which is considerably lower than the tetragonalto-orthorhombic transition temperature Tt−o = 525 K. The copper spins are ordered in the CuO2 planes in the manner shown in Fig. VIII-18 of our earlier book (1988; cf. also Freltoft et al., 1988; Kaplan et al., 1989; Thio et al., 1988; Yamada et al., 1989). Antiferromagnetic spin fluctuations in these CuO2 planes, called antiparamagnons, have also been discussed (Statt and Griffin, 1993). Compounds formed by replacing the yttrium in YBa2 Cu3 O7− by a rare-earth ion tend to align antiferromagnetically at low 137 XVII PAULI LIMIT AND UPPER CRITICAL FIELD temperature (Lynn, 1992). For example, the Er moments = 48B in ErBa2 Cu3 O7− order in the a, b-plane with antiferromag netic coupling along a and ferromagnetic coupling along b and c, in the manner shown in Fig. 5.23. The neutron-magnetic reflection intensity plotted in Fig. 5.24 versus temper ature provided the Néel temperature TN ≈ 05 K (Chattopadhyay et al., 1989; Lynn et al., 1989; Paul et al., 1989). Below TN ≈ 22 K, the Gd moments in GdBa2 Cu3 O7− align along the c-axis with antiferromagnetic coupling to all Gd nearest neighbors, as illus trated in Fig. VIII-19 of our earlier work (1988; cf. also Dunlap et al., 1988; Mook et al., 1988; Niedermayer et al., 1993; Paul et al., 1988; Watson et al., 1989). Other mag netic ions, such as Dy, Ho, Nd, Pr, and Sm, when substituted for Y, also produce anti ferromagnetic ordering (Dy: Fischer et al., 1988; Zhang et al., 1992; Ho: Fischer et al., 1988; Nd: Yang et al., 1989; Pr: Kebede et al., 1989; Sm: Yang et al., 1989). For x < 64 the undoped compound YBa2 Cu3 Ox is an antiferromagnetic non-superconductor with aligned Cu ions, and TN ≈ 500 K for x ≈ 6 (Miceli et al., 1988; Rossat-Mignod et al., 1988; Tranquada, 1990; Tranquada et al., 1992). XVII. PAULI LIMIT AND UPPER CRITICAL FIELD An electron spin in a magnetic field has the Zeeman energy Figure 5.23 Magnetic spin structure of ordered Er ions in antiferromagnetic ErBa2 Cu3 O7− determined by neutron diffraction (Chattopadhyay et al., 1989) E = gB Bapp · S 1 E± = ± g B Bapp (5.87) 2 shown in Fig. 5.25, where = gB S is the spin magnetic moment, g = 20023 for a free electron, and B is the Bohr magneton. We will approximate the g-factor by 2, and, of course, S = 21 . If the Zeeman energy level splitting (Poole and Farach, 1987) indicated in the figure, E+ − E− = 2B Bapp Figure 5.24 Temperature dependence of the inten sity of reflected neutrons from the ErBa2 Cu3 O7− sam ple of Fig. 5.23 showing the Néel temperature TN ≈ 05 K far below Tc = 88 K (Chattopadhyay et al., 1989). (5.86) (5.88) becomes comparable with the energy gap Eg , the field will be strong enough to break up the Cooper pairs and destroy the super conductivity. The magnetic field BPauli that brings this about is called the Pauli limiting field. It has the value Eg BPauli = √ (5.89) 2 2B 138 5 MAGNETIC PROPERTIES Figure 5.25 Zeeman energy level splitting E+ − E− of electrons resulting in the breakup of Cooper pairs by becoming comparable to the energy gap 2 when Bapp reaches the value Bc2 . √ where the factor 2 comes from a more detailed calculation. Inserting the BCS gap ratio Eg = 353kB Tc , this becomes BPauli = 183Tc (5.90) The data in Table 5.2 demonstrate that this provides an approximation to experimentally determined upper-critical fields Bc2 . This limiting field has also been called the param agnetic limit or the Clogston–Chandrasekhar limit (Chandrasekhar, 1962; Clogston, 1962; Pérez-González and Carbotte, 1992). For many Type II superconductors both the ratio Bc2 0/Tc and the slope dBc2 /dT at Tc are close to the Pauli value 1.83 T/K, as shown by the data listed on Table 5.2 and plotted in Fig. 5.26. The zerotemperature upper-critical fields Bc2 0 of high-temperature superconductors are gener ally too high to measure directly, but they can be estimated from the Pauli limit or from the empirical expression Bc2 ≈ 2Tc /3dBc2 /dT , which can be deduced from the data in Table 5.2. Upper critical fields Bc2 T and their temperature derivatives dBc2 /dT often depend on the orientation of the applied mag netic field. This is especially true for the high-temperature superconductors because of their planar structures. These types of critical fields and their temperature deriva tives at Tc are larger when the external field is applied perpendicular to the c-axis (i.e., parallel to the Cu–O planes) than when it is applied parallel to this axis, as shown in Fig. 5.27. This order is reversed for the lower critical field, as shown in Fig. 5.28; in other words, Bc1⊥c < Bc1c Bc2c < Bc2⊥c . This reversal is associated with the reversal in the order of sizes of the penetra tion depths and coherence lengths given by Eq. (12.46), c < ab ab < c . Therefore, we have, from Eqs. (12.51) and (12.52), the lower critical field ratio ln ab Bc1⊥c = ab = <1 Bc1c c ln c (5.91) Table 5.2 Comparison of Upper-Crititcal Feild Bc2 0, Slope dBc2 /dT at Tc and Pauli Limiting Fields BPauli = 183Tc of Selected Type II Superconductors � Material Tc K Bc2 T Bc2 /Tc T/K −dBc2 /dT T/K BPauli T 2 T 3 c CeCu2 Si2 (heavy fermion) UBe13 (heavy fermion) Nb(44%)–Ti (alloy) Gd02 PbMo6 S8 (Chevrel) Nb3 Sn A15 Nb3 Al075 Ge025 A15 Nb3 Ge A15 YBa2 Cu3 O7 (HTSC) 0.5 0.9 9.3 14 18 20.7 23.1 92 2.4 6 15 61 28 43.5 38 120–200 4.8 6.7 1.6 4.4 1.6 2.1 1.7 1.3–2.2 23 44 2.4 6.8 2.5 3.0 2.3 0.7–4.6 0.9 1.7 17 26 33 38 42 168 7.67 26.4 14.9 63.4 30.0 41.4 35.4 42.9–282 dBc2 dT � 139 XVIII IDEAL TYPE II SUPERCONDUCTOR Figure 5.26 Relation between upper-critical field Bc2 and temperature for the best classical superconductors, some of which are used for fabricating commercial magnets. In the high-temperature limit 2/3Tc < T < Tc many of the curves have a slope that is close to the value 1.83 T/K of the Pauli limit (dashed curve) (Wilson, 1983, p. 302). and its upper critical field counterpart Bc2⊥c = ab > 1 c Bc2c (5.92) where ab and c are given by Eqs. (12.48) and ab > c . These inequalities may be ver ified from the data in Tables 12.4 and 12.5. Tesanovic (1991), Tesanovic and Rasolt (1989), and Tesanovic et al. (1991) discussed the possibility of reentrant superconducting behavior in applied fields far exceeding Bc2 . XVIII. IDEAL TYPE II SUPERCONDUCTOR A Type II superconductor has sev eral characteristic parameters, such as its Ginzburg–Landau parameter , transition temperature Tc , energy gap Eg , coher ence length , penetration depth , uppercritical field Bc2 , lower critical field Bc1 , thermodynamic critical field Bc , and critical current density Jc . We have seen how these various parameters are related by simple theoretical expressions, so that if any two of them are specified, the others can be estimated. This suggests defining an ideal isotropic Type II superconductor as one whose parameters have “ideal” relationships with each other. Consider such a Type II superconductor with = 100 and Tc = 90 K. Its energy gap is obtained from the BCS relation (7.79) Eg = 3528kB Tc = 275 meV (5.93) 140 5 MAGNETIC PROPERTIES Figure 5.27 Anisotropy in the upper-critical fields of YBa2 Cu3 O7 . The initial slope dBc2c /dT at Tc (– – –) is −096 T/K, while its counterpart dBc2⊥c /dT at Tc is −4 T/K (Moodera et al., 1988). Figure 5.28 Anisotropy in the lower-critical fields of YBa2 Cu3 O7 . The initial slope dBc1c /dT at Tc is −14 mT/K, and that of dBc1⊥c /dT at Tc is −040 mT/K. The low-temperature extrapolations give 53 ± 5 mT for the applied field parallel to c and 18 ± 2 mT for Bapp perpendicular to c. Yeshuran et al. (1988) obtained the 6 K values, Bc1c = 90 ± 10 mT (not shown) and Bc1⊥c = 25 ± 5 mT (shown as × with vertical error bar). The dashed curves are BCS fits to the data (Krusin-Elbaum et al., 1989). Recall that 10G = 1 mT. 141 XIX MAGNETS The Pauli limit (5.90) provides an estimate of the upper-critical field, Bc2 = 183Tc = 165 T (5.94) Equation (12.9) gives the coherence length , � = �1/2 0 2Bc2 = 126 nm (5.95) and from the definition (12.6) of the Ginzburg–Landau parameter we obtain the penetration depth , = = 126 nm (5.96) Equations (12.10) and (12.11), respectively, give the thermodynamic and lower critical fields, B Bc = √ c2 = 116 T 2 B ln Bcl = √c = 379 mT 2 (5.97) (5.98) The critical current density Jc at 0 K is given by Eq. (2.51): Jc = Bc /0 = 695 × 108 A/cm2 (5.99) This approximates what has been called the depairing current density. Jdepair = 10Bc /40 = 553 × 108 A/cm2 (5.100) (5.101) where for YBaCuO the thermodynamic field Bc ≈ 1 T, penetration depth ≈ 02 m, and Tc ≈ 92 K. These “ideal” values are good approximations to the experimentally deter mined values for typical high-temperature superconductors. XIX. MAGNETS Superconducting magnet design requires simultaneously achieving high critical fields, high critical currents, and suitably mal leable wire. The slope dBc2 /dT ≈ −2 T/K of YBaCuO is typical, and gives a critical field of 30 T at the temperature of liquid nitro gen, as shown in Fig. 12.8, and in Table I-2 of our previous work (Poole et al., 1988). This high critical field is for the case of the externally applied field B aligned perpendi cular to the c-axis, i.e., parallel to the crys tallographic conducting planes. When Bapp is parallel to the c-axis, the critical field is four or five times lower, as already noted in Section XVII. The standard magnet materials Nb3 Sn and Nb–Ti have critical fields of about 24 T and 10 T, respectively, at 4.2 K, which are not much lower than that of YBaCuO at 77 K. Operating YBaCuO at temperatures much below 77 K will, of course, provide higher critical fields, and TlBaCaCuO, with its much higher Tc (125 K), is even better at 77 K. The problem is to obtain high-Tc superconductors that can carry large trans port currents and in addition, have the proper ductility and possess the appropriate mechan ical properties. This, however, has yet to be achieved. Vortex pinning must also be opti mized to control flux creep. A better approximation than Eq. (5.99) to the upper limit of the critical current density is given by the Ginzburg–Landau expression � � ��3/2 2 T Jcmax = 1− Jdepair (5.102) 3 Tc This gives Jc ≈ 3 × 108 A/cm2 at 0 K and Jc ≈ 12 × 107 at 77 K, respectively. Jiang et al. (1991) reported Jc ≈ 13 × 109 A/cm2 for microbridges of YBa2 Cu3 O7− films. Achievable critical currents are typi cally one-tenth the limiting values calculated from Eq. (5.102), as indicated by the data in Table I-2 of our earlier work (Poole et al., 1988). 142 5 MAGNETIC PROPERTIES PROBLEMS 1. Show that a superconductor containing a volume Vex of voids which cannot store any flux has the following ZFC and FC susceptibilities and porosity: zfc = − V s + Vh + Vc Vs + Vh + Vc + Vex fc = − Vs + Vc Vs + Vh + Vc + Vex P= Vh + Vc + Vex Vs + Vh + Vc + Vex 2. A granular, 10-mg sample of YBa2 Cu3 O7− has a density of 319 g/cm3 and the susceptibilities zfc = −08 and fc = −04. Find the porosity and the volumes of the purely superconducting, normal material, open hole-like, enclosed cavity-like and non-flux storing portions of the sample. Assume that there is no normal material present. 3. Show that the measured magnetic moment is given by Eq. (5.21), 0 fc = − Vs + Vc Bapp + Bfc − Bapp Vh when field cooling is carried out in a magnetic field Bfc that differs from the field Bapp applied for the measurement. 4. Show that the sample of Problem 1 has the following superconducting, openhole, closed-cavity, and non-flux storing volumes given by, respectively, Vs = 1 − PVT Vh = −zfc − fc VT Vc = P − 1 − fc VT Vex = 1 + zfc VT where, of course, zfc and fc are both negative. 5. Show that Eqs. (5.43) and (5.45) both have the limiting behavior N → 1/3 as → 0. 6. Show that 1 and 2 of Table 5.1 are given by 1 c 1 = 2 a 4 � c� 2 = 1− 15 a 7. Show that 3 and 4 of Table 5.1 are equal to 4 � a� 1− 15 c � � 2� � 2 1 a c 4 = ln 2 2 − 1 2 2 a c 3 = 8. Show that the expressions that were deduced in this chapter for the mag netic fields inside and outside a sphere obey the boundary conditions (1.73) and (1.74) at the surface r = a. 9. Show that the expressions that were deduced in this chapter for the magnetic fields inside and outside a cylinder in a perpendicular magnetic field obey the boundary conditions (1.73) and (1.74) at the surface. 10. Show that the Curie law, which is based on the assumption that gB Bapp /kB T 1, is still applicable for the highest-field, lowest-temperature data of Fig. 5.26. What is the value of the ratio Bapp /T for which gB Bapp /kB T = 1 for g = 20? 11. Show that for the condition = 0, a plot of versus over the frequency range 0 ≤ ≤ is a semicircle of radius 21 0 . Identify the five points at which − 0 is equal to 0, 21 , 1, 4, and on the semicircle. How would the plot change for = 41 0 ? 6 Ginzburg–Landau Theory I. INTRODUCTION In Chapter 4 we presented the thermo dynamic approach to the phenomenon of superconductivity. We used the Gibbs free energy since in the absence of a magnetic field the Gibbs free energy is continuous across the superconducting-to-normal-state transition. The situation below the transi tion temperature Tc was handled by assum ing a known magnetization and a known critical field, which were then used to cal culate the various thermodynamic functions. This approach cannot really be called a the ory because it simply incorporates known properties of superconductors into a standard treatment of thermodynamics in the presence of an applied magnetic field. To gain more understanding of the phenomenon of superconductivity let us examine some simple but powerful theories that have been developed in efforts to explain it. In the present chapter we will consider the phenomenological approach proposed by Ginzburg and Landau (GL) in 1950. This approach begins by adopting certain simple assumptions that are later justified by their successful prediction of many properties of superconducting materials. The assumptions describe superconductivity in terms of a complex order parameter the physical sig nificance of which is that ��2 is proportional to the density of super electrons. The order parameter is minimally coupled to the elec tromagnetic field, and in the presence of a magnetic field B = � × A the momentum operator −i�� becomes −i�� + e∗ A, 143 144 where e∗ is the charge associated with the “super electrons.” The free energy is a mini mum with respect to variations of both and A. The London equations, dating from 1935, follow as a natural consequence of the GL theory, as we show in Section IX (London and London, 1935). In the next chapter we will exam ine the more fundamental Bardeen–Cooper– Schrieffer (BCS) microscopic theory that first appeared in 1957. Soon after this the ory was published, its correct prediction of many observable properties of superconduc tors was recognized. The earlier GL the ory, on the other hand, was not widely accepted outside the Soviet Union until Gor’kov showed in 1959 that it is derivable from the BCS theory. This chapter will concentrate on the case of isotropic superconductors. Formula tions of the GL theory and of the London Model are also available for the anisotropic case (e.g., Coffey, 1993; Doria et al., 1990; Du et al., 1992; Klemm, 1993, 1994; Wang and Hu, 1991), and more specifically for the cuprates (Horbach et al., 1994; Schneider, et al., 1991; Wilkin and Moore, 1993). Time dependent processes have also been treated (Malomed and Weber, 1991; Stoof, 1993). II. ORDER PARAMETER Many phenomena in nature, such as the boiling of liquids and ferromagnetism, involve a transition from an ordered to a disordered phase. Each of these transitions can be characterized by an appropriate order parameter that has one value in the hightemperature disordered state and another in the low-temperature ordered state. The order parameter may be thought of as charac terizing the extent to which the system is “aligned.” In the case of boiling, the order param eter might be the density, which is high in the liquid state and low in the gaseous state. 6 GINZBURG–LANDAU THEORY The magnetic order parameter is often taken as the magnetization; it is zero in the hightemperature paramagnetic region, where the spins are randomly oriented, and nonzero at low temperatures, where the spins are ferro magnetically aligned. In the normal conduction state the elec tric current is carried by a Fermi gas of conduction electrons, as was explained in Chapter 1. The GL theory assumes that in the superconducting state the current is car ried by super electrons of mass m∗ , charge e∗ , and density n∗ which are connected by the relationships m∗ = 2m (6.1a) e∗ = ±2e (6.1b) 1 n∗s = ns 2 (6.1c) with their electron counterparts m, e, and ns , respectively. The actual “mass” here is the effective mass, and it need not be twice the mass of a free electron. The charge is neg ative for electron-type charge carriers, as is the case with many classical superconduc tors, and positive for hole conduction, as with most of the high-temperature superconduc tors. The super electrons begin to form at the transition temperature and become more numerous as the temperature falls. Therefore, their density n∗s is a measure of the order that exists in the superconducting state. This order disappears above Tc , where n∗s = 0, although fluctuations in n∗s can occur above Tc . More generally n∗s ≤ 21 ns , and Eq. (6.1c) gives us the limiting value of n∗s for T = 0. The Ginzburg–Landau theory, to be described in the following section, is formu lated in terms of the complex order parameter r, which may be written in the form of a product involving a phase factor and a modulus �r�, r = �r�ei (6.2) 145 III GINZBURG–LANDAU EQUATIONS temperature below Tc , the Gibbs free energy per unit volume Gs may be expanded as a local functional of the order parameter, 1 3 1 Gs = Gn + dr V 2m∗ × −i�� + e∗ A∗ · i�� + e∗ A 1 + B2 r 2 0 − + Figure 6.1 Temperature dependence of the order parameter ��2 showing its value �0 �2 at T = 0, and the linear behavior (---) near Tc , which extrapolates to the ordinate value a0 /b0 . This figure is drawn under the assumption �0 �2 = 41 a0 /b0 to agree with Fig. 2.44. whose square, ��2 , is the super electron density, n∗s = ��2 (6.3) The parameter is zero above Tc and increases continuously as the temperature falls below Tc , as shown in Fig. 6.1. III. GINZBURG–LANDAU EQUATIONS We saw in the previous chapter that the thermodynamic properties of the supercon ducting state can be described in terms of the Gibbs free energy density G. Ginzburg and Landau assumed that, close to the transition 0 Hr · Mr + a 1 b∗ ∗ + · · · 2 ∗ (6.4) where Gn is the free-energy density of the normal state, A is the magnetic vector poten tial, and a and b are functions of the tem perature only. If the material is normal, B = 0 H M = 0, and the magnetic contribu tion is 21 0 H 2 . In regions of perfect super conductivity B = 0 and M = −H, and the magnetic contribution is 0 H 2 . In equilib rium the superconductor distributes currents in such a way as to minimize the total free energy. The assumption is made that over a small range of temperatures near Tc the parameters a and b have the approximate values T aT ≈ a0 −1 (6.5a) Tc bT ≈ b0 (6.5b) where a0 and b0 are both defined as positive, so that aT vanishes at Tc and is negative below Tc . To determine r we require that the free energy be a minimum with respect to variations in the order parameter. Tak ing the variational derivative (Arfken, 1985, Chapter 17) of the integrand in (6.4) with respect to ∗ with held constant gives the first GL equation: 1 i�� + e∗ A2 + a + b��2 = 0 2m∗ (6.6) 146 6 GINZBURG–LANDAU THEORY In the London-Landau gauge (sometimes called the Coulomb or radiation gauge) � · A = 0 (6.7) the first GL equation can be expanded into the form 1 � 2 � 2 − 2i�e∗ A · � − e∗2 A2 2m∗ − a − b��2 = 0 (6.8) The free energy is also a minimum with respect to variations in the vector potential A, where B = � ×A (6.9) Taking the variational derivative of G with respect to A we obtain the second GL equa tion: i�e∗ ∗ � − �∗ 2m∗ e∗2 + ∗ A��2 = 0 (6.10) m � × � × A + In Cartesian coordinates this equation, expressed in terms of the London-Landau gauge (6.7), can be simplified by writing −� 2 A in place of � × � × A (see Prob lem 7). If we substitute the expression for B from Eq. (6.9) into the Maxwell expression (Ampère’s law), � ×B = 0 J (6.11) and compare the result with Eq. (6.10), we find the following proper gauge-invariant expression for the current density: 0J =− and vector potential, which can be solved to determine the properties of the superconduct ing state. For most applications the equations must be solved numerically. However, there are some simple cases in which exact closedform solutions can be found, and others in which useful approximate solutions can be obtained. We will examine some of these cases, and then transform the GL equations to a normalized form and discuss the solu tion for more complex cases. When these equations are written in a normalized form, the coherence length, penetration depth, and quantum of magnetic flux, called the fluxoid, appear as natural parameters in the theory. i�e∗ ∗ e∗2 � − �∗ − ∗ A��2 ∗ 2m m (6.12) Thus the Ginzburg-Landau theory gives us two coupled differential equations, (6.8) and (6.10), involving the order parameter IV. ZERO-FIELD CASE DEEP INSIDE SUPERCONDUCTOR To get a feeling for the behavior of , let us first consider the zero-field case A = 0 with homogeneous boundary conditions (zero gradients, � 2 = 0). The absence of gradients corresponds to a region deep inside a superconductor where the super electron density does not vary with position. Integra tion of Eq. (6.4) can be carried out directly for this zero field–zero gradient case, to give for the Gibbs free energy density Gs of the superconductor 1 Gs = Gn + a��2 + b��4 2 (6.13) where from Eqs. (6.5) b is positive and a negative below Tc . The GL equation (6.8) provides the minimum for this free energy, a + b��2 = 0 (6.14) and all of the terms of the second GL equation (6.10) vanish. The phase of is arbitrary, so we can take to be real. Equa tion (6.14) has one solution, = 0, corre sponding to the normal state and one solution for a < 0 at T < Tc , with lower free energy: ��2 = − a �a� = b b (6.15) 147 IV ZERO-FIELD CASE DEEP INSIDE SUPERCONDUCTOR Using the approximations (6.5a) and (6.5b) for a and b, respectively, we have ��2 = a0 T 1− b0 Tc (6.16) and this linear temperature dependence is shown in Fig. 6.1 for the region near T ≈ Tc . For lower temperatures ��2 is expected to deviate from linearity on its approach to its 0 K value, �0 �2 < a0 /b0 , as shown in the figure. From Eq. (6.3) we have for the super electron density n∗s = a0 T 1− b0 Tc Eq. (6.13), we obtain for the minimum Gibbs free energy density 1 a2 Gs = Gn − 2 b 1 a20 T 2 = Gn − 1− (6.18) 2 b0 Tc where 21 a2 /b, called the condensation energy per unit volume of the super electrons, is the energy released by trans formation of normal electrons to the super electron state. The condensation energy can be expressed in terms of the thermodynamic critical field Bc as follows: (6.17) which agrees with Eq. (2.69) in the super conducting region near Tc . When the expressions for from Eqs. (6.15) and (6.16) are substituted into 1 2 a2 b = Bc2 2 0 (6.19) Figure 6.2 presents a plot of Gs − Gn from Eq. (6.13) versus for the three ratios of temperatures T/Tc = 1, 0.9, and 0.8. Figure 6.2 Dependence of the difference Gs − Gn between the Gibbs free energy in the normal and super conducting states on the order parameter . (a) Normalized plots for T/Tc = 1, 0.9, and 0.8, and (b) Plot for T/Tc = 0 85 showing the minimum free-energy difference Gs − Gn = a2 /2b, which occurs for = �a�/b1/2 , and the zero, Gs − Gn = 0, at = 2�a�/b1/2 . 148 6 GINZBURG–LANDAU THEORY The minimum for each curve occurs at = �a�/b1/2 given by Eq. (6.15), and Gs −Gn = 0 at = 2�a�/b1/2 . These coordinates for the minimum and crossover points of the T/Tc = 0 8 curve are indicated in the figure. The equilibrium superconducting state exists at the minimum of each curve. The minimum gets deeper, and the order parameter for the minimum increases, as the temperature is lowered, as shown. The magnitude of the free-energy minimum at 0 K cannot be writ ten down because the temperature depen dence of Eq. (6.16) can only be a good approximation near Tc . Since the phase of the order parameter is constant we select to be real. We assume that the right half-space, x > 0, is filled with a superconductor and that the left half-space, x < 0, is a vacuum or normal material, as shown in Fig. 6.3. There fore, is a function of x, the gradient oper ator � only has an x component, and we can write Eq. (6.21) in one-dimensional form: V. ZERO-FIELD CASE NEAR SUPERCONDUCTOR BOUNDARY the normalized order parameter f satisfies the “nonlinear Schrödinger equation” Next we consider the case of zero field with inhomogeneous boundary conditions, which means that gradients can exist. Setting A = 0 in the second GL equation (6.10) gives ∗ � = �∗ �2 2 � + a + b��2 = 0 2m∗ �2 d2 f · 2 + f1 − f 2 = 0 ∗ 2m �a� dx (6.24) If we define the dimensionless variable as x = (6.25) (6.20) where which means, from Eq. (6.2), that the phase of the order parameter is independent of position. The first GL equation, Eq. (6.8), with A set equal to zero, provides us with a differential equation for the order parameter: − � 2 d2 + a + b��2 = 0 (6.22) 2m∗ dx2 When we change variables by letting 1/2 �a� = f (6.23) b − (6.21) 2 = �2 2m∗ �a� (6.26) Eq. (6.24) assumes the simplified dimension less form d2 f + f1 − f 2 = 0 d 2 Figure 6.3 Interface between a normal material on the left x < 0 and a superconductor on the right x > 0. (6.27) 149 VI FLUXOID QUANTIZATION It may be easily verified by direct substitu tion that Eq. (6.27) has the solution f = tanh √ (6.28) 2 This can be written in terms of the original variable , x = � tanh √ 2 P (6.29) where � = �a� b 1/2 vanishes. This is to be expected since from the Maxwell expression (6.11) we know that electric currents cannot exist if there are no associated magnetic fields present. The BCS theory presented in the next chapter gives an alternate expression (6.30) with → 0 as x → 0 and → � as x → �. Therefore, is the characteristic length over which can vary appreciably. The param eter , called the coherence length, is one of the two fundamental length scales associ ated with superconductivity. Its significance is shown graphically in Fig. 6.4, in which we see that is close to � far inside the super conductor, is zero at the interface with the normal material, and has intermediate values in a transition layer near the interface with a width on the order of . Substituting Eq. (6.20) in Eq. (6.12) shows that for A = 0 the current density J �VF 0 1804�VF = k B TC = For what is called the BCS or Pippard coher ence length, where 2 = Eg is the super conducting energy gap, and VF is the Fermi, velocity. The second equation comes from the BCS dimensionless ratio. 2 = 3 528 kB T C VI. FLUXOID QUANTIZATION Now that we have determined the order parameter for the case B = 0, we will pro ceed to investigate the situation when there is an applied magnetic field. In the presence of such a field an interesting result follows from Eq. (6.12). If we write r as the product of a modulus and a phase factor, as in Eq. (6.2), the gradient of will have the form � = i� + ei ��r� (6.31) and the total current from Eq. (6.12) will be given by 0J Figure 6.4 Dependence of the order parameter x on distance x inside a superconductor. The order param eter is large for x > , where is the coherence length. = �e∗ 2 e∗2 �� � − ∗ ��2 A ∗ m m (6.32) Dividing Eq. (6.32) by �e∗ ��2 /m∗ and tak ing the line integral around a closed con tour gives m∗ 0 J · d1 e∗2 ��2 � = ∗ � · d1 − A · d1 (6.33) e 150 6 GINZBURG–LANDAU THEORY For the order parameter to be single valued the line integral over the phase around a closed path must be a multiple of 2 , � · d1 = 2 n (6.34) where n is an integer. Equation (6.33) can now be written m∗ 0 J · d1 + A · d1 = n0 (6.35) e∗2 ��2 where the quantum of flux 0 has the value 0 = h e∗ (6.36) in agreement with experiment (e.g., Cabrera et al., 1989; Gough et al., 1987; S. Hasegawa et al., 1992). It is convenient to express the line inte gral of A in Eq. (6.35) in terms of the mag netic flux through the closed contour. Applying Stokes’ theorem we find A · d1 = B · dS = (6.37) (6.38) Figure 6.5 Integration paths for Eq. (6.35) encir cling no cores n = 0, encircling one core n = 1, and encircling two cores n = 2. in a region of space that contains vortices, the integer n in Eq. (6.39) corresponds to the number of cores included within the path of integration. Figure 6.5 shows contours enclosing n = 0 1, and 2 core regions. Here we are assuming that all the vortices have the same polarity, i.e., the magnetic field points in the same direction in all the vor tices. Equation (6.39) is easily generalized to include the presence of positively and nega tively directed vortices. The Little–Parks (1962, 1964) experi ment demonstrated this flux quantization by measuring the magnetic field dependence of the shift in Tc of a thin-walled superconduct ing cylinder in an axial applied field. and Eq. (6.35) becomes m∗ 0 J · d1 + = n0 e∗2 ��2 (6.39) This expression is valid for all superconduc tors, and can be applied to the intermediate and mixed states described in Chapter 11. Equation (6.39) expresses the condition whereby the sum of the enclosed flux and the line integral involving the current density J is quantized. We will see later that for Type II super conductors quantized flux occurs in vortices, which have a core region of very high field, and a field outside which decreases with dis tance in an approximately exponential man ner far from the core. Figure 6.5 sketches two such vortices. When a contour is taken VII. PENETRATION DEPTH In Section V we found how the order parameter changes with distance in the neighborhood of the boundary of a super conductor, and this provided us with the first fundamental length scale—the coher ence length . In this section we will inves tigate the behavior of the internal magnetic field in the neighborhood of a boundary when there is an applied field outside. This will give us the penetration depth L , the second of the two fundamental length scales of superconductivity. We begin by returning to the semiinfinite geometry of Fig. 6.3 with a uniform magnetic field oriented in the z direction. 151 VII PENETRATION DEPTH In the London-Landau gauge (6.7) the vec tor potential for a constant magnetic field B0 outside the superconductor x < 0 is A = Ay xĵ (6.40) with Ay x = xB0 + A0 x < 0 (6.41) where the constant A0 is selected for con tinuity with the solution Ay x inside the superconductor, as shown in Fig. 6.6. This constant does not affect the field Bx. In order to determine how the phase of the order parameter varies throughout the interior of the superconductor, let us evalu ate the line integrals of Eq. (6.35) along a rectangular contour in the x,y- plane that is closed at x = x0 and x1 → �, as indicated in Fig. 6.7. This is done for a contour of arbitrary width L, as shown. Since A is a vector in the y direction, it is perpendicular to the upper and lower horizontal parts of the contour, which are along x, so that the integral of A · dl vanishes along these paths. We also observe that no current flows into the superconductor, so that Jx = 0 and the line integrals of J · dl along these same upper and lower horizontal paths vanish. When we take the limit x1 → � the two line integrals along this vertical x1 path vanish because A and J are zero far inside the supercon ductor. As a result only the line integrals along the x0 vertical path contribute, and they may be written down immediately because there is no y dependence for the fields and currents: m∗ Jy x0 + Ay x0 = n0 L · ∗2 e �x0 �2 (6.42) Since the width L is arbitrary and n is quan tized, it follows that n = 0. Then, from the Figure 6.6 Dependence of the vector potential A(x) on distance x for the case of Fig. 6.3. A(x) depends linearly on x outside the superconductor (left), where there is a constant applied magnetic field, and decays exponentially inside the superconductor (right), becoming very small for x � L , where L is the London penetration depth. 152 6 GINZBURG–LANDAU THEORY which has a simple exponential solution inside the superconductor, Ay x = A0 exp−x/L Figure 6.7 Integration path inside a superconductor for determining the phase of the order parameter . quantization condition (6.34) and the arbitrari ness of the path, we conclude that the phase of the order parameter (6.2) is constant everywhere throughout the superconductor, and we set it equal to 0. Furthermore, since x0 in Eq. (6.42) is arbitrary, it follows that Jy x = e∗2 �x�2 Ay x m∗ (6.43) which tells us how J is related to A. To determine the x dependence of Ay , note that Eq. (6.20) is valid for a constant phase and that the second GL equation (6.10) reduces to the expression d2 A x = dx2 y 0e ∗2 �x�2 Ay x m∗ (6.44) We seek to solve this equation far enough inside the superconductor, x � , so that the order parameter attains its asymptotic value, → � , independent of x. It is convenient to define the London penetration depth L , the second of the two fundamental length scales of a superconductor: 2L = m∗ ∗2 2 0 e �� � (6.45) This permits us to write Eq. (6.44) in the form Ay x d2 Ay x = 2 dx 2L (6.46) x > 0 (6.47) for the case � L which is plotted in Fig. 6.6. The preexponential factor A0 makes Ay x from Eqs. (6.41) and (6.47) match con tinuously across the boundary at x = 0. In writing Eq. (6.46) we implicitly assumed that the London penetration depth L is greater than the coherence length . For distances from the surface x in the range 0 < x � we know from Eq. (6.29) √and the power series expansion of tanhx/ 2 for small values of the argument that x x ≈ � √ 2 0�x� (6.48) so that x is much less than � . In this range the effective penetration depth exceeds the London value (6.45), so Ay x decays more gradually there, as indicated in Fig. 6.6. To obtain the fields from the potentials we apply the curl operation B = � × A. Only the z component exists, as assumed initially, Bz x = B0 Bz x = x < 0 −A0 exp−x/L L = B0 exp−x/L (6.49) < x < � (6.50) where A0 = −L B0 from the boundary con dition at the surface x = 0. The dis tance dependences of Eqs. (6.48) and (6.49), together with the more gradual decay in the range 0 < x < , are shown in Fig. 6.8. We conclude that for this case the applied field has the constant value B0 outside the super conductor, decays exponentially with dis tance inside, and becomes negligibly small beyond several penetration depths within, as shown. From Eq. (6.43) we find that far inside the superconductor 2 0 L Jy x = −Ay x � x < � (6.51) 153 VII PENETRATION DEPTH Figure 6.8 Exponential decay of a constant applied magnetic field Bz x inside a superconductor for the case L > . Note the small devi of the ation from exponential behavior within a coherence length surface. as x → � , and hence that Jy x also satisfies Eq. (6.46) with the distance dependence A0 Jy x = exp−x/L 2 0 L = J0 exp−x/L < x < � (6.52) which is the same as Ay x of Eq. (6.47). In the range 0 < x < , which is near the surface, we see from Eq. (6.43) that Jy x is less than this value, as indicated in Fig. 6.9. Thus, we see that Bz x decays less and that the current density Jy x has a magnitude less than its value beyond the coherence length. Figure 6.9 Dependence of the current density Jy x on distance x inside a superconductor for the case L > . 154 6 GINZBURG–LANDAU THEORY In the remainder of the chapter we will ignore these surface effects for x < and only take into account the exponential decay in terms of the penetration-depth distance parameter. The factor � − 2 /0 A can be elimi nated between Eqs. (6.55) and (6.57) to give for the current density Js = VIII. CRITICAL CURRENT DENSITY An electric current is accompanied by a magnetic field. To obtain an expression for the current density independent of the magnetic field, the vector potential can be eliminated between the current density equa tion and the second GL equation. We will do this deep inside the superconductor where the order parameter r depends on posi tion only through the phase r. For this situation the order parameter, written in the form r = 0 eir (6.53) has the gradient �r = i�r and the current density (6.12) is � e∗ 2 J = ∗ 20 � − A m 0 (6.54) 2 0 f 2 1 − f 2 1/2 2 0 L (6.58) where f is given by Eq. (6.23) (we have used Eqs. (6.26) and (6.45) here). Figure 6.10 shows how Js depends on f . The largest possible current density shown in the figure, called the critical current density Jc , is obtained by maximizing Eq. (6.58) through differentiation with respect to f 2 . This gives f 2 = 23 , and we obtain what is sometimes called the Ginzburg–Landau critical current density, Jc = √ 3 3 0 2 0 L (6.59) This can also be written in terms of the ther modynamic critical field (12.10). √ 2 2Bc (6.60) Jc = √ 3 3 0 L (6.55) where 0 is given by Eq. (6.36). Substituting the expression for the order parameter from (6.53) in Eq. (6.8) and multiplying on the left by e−i gives 2 �2 2 −i i� + e A ei 2m∗ �a� 0 0 b + 0 − 30 = 0 �a� (6.56) If the Laplacian � 2 is negligible, this becomes 2 �2 2 � − A 2m∗ �a� 0 +1− 20 =0 �a�/b Figure 6.10 Dependence of the super current density (6.57) Js on the normalized order parameter f . Js f reaches a maximum at f = 2/31/2 . 155 X EXPONENTIAL PENETRATION From Eq. (2.61) this has the following tem perature dependence near Tc : √ 8 2Bc 0 T 3/2 1− Jc = √ Tc 3 3 0 L 0 (6.61) � ×B = Thus Jc becomes zero at the critical temper ature, and we know from Eq. (2.58) that it is a maximum at T = 0. IX. LONDON EQUATIONS In 1935 the London brothers, Fritz and Heinz, proposed a simple theory to explain the Meissner effect, which had been discov ered two years earlier. They assumed that the penetration depth L is a constant inde pendent of position. The equations which they derived, now called the first London equation, E= 2 0 L d J dt (6.62) and the second London equation, B=− 2 0 L � × J (6.63) were used to explain the properties of super conductors. These two equations are easily obtained from the GL theory with the aid of Eq. (6.51) expressed in vector form: 2 0 L J = −A A from Eq. (6.64) in Eq. (6.9). It should be compared with Eq. (1.72), which, in the absence of magnetization and displacement currents, becomes Ampère’s law: (6.64) If the vector potential expression (6.9) is substituted in Maxwell’s equation (1.66), we obtain dA � × E+ = 0 (6.65) dt and with the aid of Eq. (6.51) we can then write down the first London equation (6.62). The second London equation (6.63) is obtained by substituting the expression for 0J (6.66) Thus we see that Maxwell’s and London’s equations link the magnetic field B and the current density J in such a way that if one is present in the surface layer so is the other. If the expression for the current density J from Eq. (6.66) is substituted in Eq. (6.63) we obtain � 2B = B 2L (6.67) and eliminating B between these same two expressions gives � 2J = J 2L (6.68) Thus, recalling (6.46), we see that A, B, and J all obey the same differential equation. In Cartesian coordinates, Eqs. (6.67) and (6.68) correspond to the Helmholtz equation well known from mathematical physics (Arfken, 1985). In the following section we will pro vide applications of these equations to the phenomena of magnetic field penetration and surface current flow. X. EXPONENTIAL PENETRATION In Section VII we deduced the expo nential decay of the magnetic field B and the current density J, Eqs. (6.50) and (6.52), respectively, inside a superconductor in the presence of an external magnetic field B0 , and in the previous section we wrote down the Helmholtz equations (6.67) and (6.68), respectively, for these same two cases. In the present section we will apply these equa tions to several practical situations involving magnetic field penetration and surface cur rent flow in superconductors with rectangular 156 6 GINZBURG–LANDAU THEORY Figure 6.11 Flat superconducting slab with thickness 2a much less than the two broad dimensions L. The applied magnetic field B0 and super current flow J0 have the indicated directions. The thickness parameter a should not be confused with the GL parameter a of Eq. 6.4. and cylindrical shapes. Both shielding and transport currents will be discussed. Consider a flat superconducting slab oriented in the y z-plane in the presence of an applied magnetic field B0 in the z direction, as illustrated in Fig. 6.11. The slab is of length L, width L, and thickness 2a, as indicated in the figure; we assume that a � L. The solution to Helmholtz equation (6.67) which satisfies the boundary conditions Bz −a = Bz a = B0 at the edges is x B0 cosh L Bz x = a cosh −a < x < a L (6.69) This is sketched in Fig. 6.12 for L � a and in Fig. 6.13 for L � a. For the former case we have −a − �x� Bz x ≈ B0 exp L � a L (6.70) Figure 6.12 Exponential decay of a magnetic field inside a superconductor for the case L � a. Both this figure and Fig. 6.13 are symmetric about the midpoint x = 0. 157 X EXPONENTIAL PENETRATION Figure 6.13 Decrease of the magnitude of a magnetic field inside a super conductor for the case L � a. The field in the center is 1 − 21 a/L 2 times the field B0 outside. We show in Problem 5 that in the latter case the penetration is linear near each boundary, aa − x Bz x ≈ B0 1 − 2L L � a 0 � x < a (6.71a) and aa + x Bz x ≈ B0 1 − 2L L � a −a < x � 0 (6.71b) as indicated in Fig. 6.13. To derive the corresponding expres sions for the current density we find from Eq. (6.11) that for this case J and B are related through the expression = dBz dx B0 a tanh L 0 L J0 = with the value in the center a2 Bz 0 ≈ B0 1 − 2 x = 0 (6.72) 2L 0 Jy Thus the magnetic field B and the cur rent density J are mutually perpendicular, as indicated in Fig. 6.11. The current density flows around the slab in the manner shown in Fig. 6.14, and is positive on one side and negative on the other. It has the maxi mum magnitude Jy 0 = J0 on the surface, x = ±a, where (6.75) and this gives for Jy x x sinh L Jy x = J0 a sinh L −a < x < a (6.76) This expression for the current density satis fies Helmholtz equation (6.68), as expected. (6.73) and differentiating Bz x in Eq. (6.69) gives x B0 L · 0 Jy x = L cosh a L sinh −a < x < a (6.74) Figure 6.14 Cross section in the x y-plane of the slab of Fig. 6.11 showing the shielding super current flow for an applied magnetic field B0 in the z direction. 158 6 GINZBURG–LANDAU THEORY For a � L the current density flows in a surface layer of thickness L , while for the opposite limit, a � L , it flows through the entire cross section, in accordance with Figs. 6.15 and 6.16, respectively. In the latter case the distance dependence is linear such that Jx ≈ J0 x a − a < x < a as shown in Fig. 6.16. Figure 6.15 Current density Jy x inside the superconducting slab for the case a � L . This figure and Fig. 6.16 are antisymmetric about the origin x = 0. Figure 6.16 Current density Jy x inside the superconducting slab for the case a � L . Note that the magnitude of Jx decreases linearly with distance x. (6.77) 159 X EXPONENTIAL PENETRATION currents are called shielding currents in that they shield the interior from the applied field. The case of the long superconducting cylinder shown in Fig. 6.17 in an external axial magnetic field B0 is best treated in cylindrical coordinates, and, as we show in Chapter 12; Section III.B, the solutions are modified Bessel functions. In the limit L � R, the surface layer approximates a planar layer, and the penetration is approximately exponential, −R − r Bz r ≈ B0 exp L L � R Figure 6.17 Sketch of a Type I superconducting cylinder in an external magnetic field Bapp = B0 directed along its axis, an arrangement referred to as parallel geometry. The penetration of the magnetic field B into the superconductor and the current flow Jsh near the surface are shown. The London penetration depth L is also indicated. The super current which flows in the sur face layer may be looked upon as generating a magnetic field in the interior that cancels the applied field there. Thus the encircling 0 < r < R (6.78) as illustrated in Fig. 6.18, and expected on intuitive grounds. Figure 6.17 presents threedimensional sketches of the fields and cur rents. Another example to consider is a flow of transport current moving in a surface layer in the axial direction, as shown in Fig. 6.19. Note the magnetic field lines encircling the wire outside and decaying into the surface layer. Figures 6.17 and 6.19 compare these shielding and transport current cases. The figures are drawn for the limit a � L and apply to Type I superconductors that exclude the B field and current flow from the interior. They also apply to Type II superconductors in low applied fields below but near the tran sition temperature, T < Tc , since in this case Figure 6.18 Magnetic field Br inside the Type I superconducting cylinder of Fig. 6.17 for the case � R. 160 6 GINZBURG–LANDAU THEORY by the coherence length . Thus we have, for example, / z/ in cylindrical coor dinates, and use the differential operator symbols � and � 2 , � → � � → 2 2 (6.79) 2 � (6.80) to designate differentiation with respect to these normalized coordinates. The order parameter is normalized as in Eq. (6.23), = �a� b 1/2 f (6.81) the vector potential A is normalized in terms of the flux quantum 0 , 0 A= � (6.82) 2 Figure 6.19 Sketch of the current density Jtr and magnetic field B near the surface of a Type I supercon ducting cylinder carrying a transport current. the internal field Bin is small and the behav ior approximates Type I. XI. NORMALIZED GINZBURG– LANDAU EQUATIONS In Section IV we wrote down the onedimensional zero field GL equation normal ized in terms of a dimensionless coordinate (6.25) and a dimensionless order parame ter (6.23), and this simplified the process of finding a solution. Before proceeding to more complex cases it will be helpful to write down the general GL equations (Eqs. (6.6) and (6.10)) in fully normalized form in terms of the coherence length (6.26), London pene tration depth (6.45), and flux quantum (6.36). To accomplish this we express the coor dinates as dimensionless variables divided and we make use of the Ginzburg–Landau parameter , which is defined as the ratio of the penetration depth to the coherence length, = L (6.83) Using this notation the GL equations (6.6) and (6.10), respectively, expressed in the London–Landau gauge (6.7), � · � = 0, assume the normalized forms −i� − �2 f + f1 − f 2 = 0 (6.84a) 2 � × � × � + 21 if ∗ �f − f �f ∗ +�f 2 = 0 (6.84b) We can also define a dimensionless current density j from J= 0 2 2L j (6.85) 0 which gives us j = 2 � × � × � (6.86) XII TYPE I AND TYPE II SUPERCONDUCTIVITY Equation (6.84a) can be expanded and Eq. (6.84b) written as follows: � 2 f − 2i� · �f − �2 f + f1 − f 2 = 0 j = − 21 if ∗ �f − f �f ∗ − �f 2 (6.87a) (6.87b) Thus the coherence length, penetration depth, and flux quantum are the natural normal ization parameters for transforming the GL equations into dimensionless form. In the fol lowing section we will use these normalized equations to elucidate various properties of superconductors. XII. TYPE I AND TYPE II SUPERCONDUCTIVITY In Chapter 11 we will discuss how bulk normal and superconducting phases coex ist in equilibrium in an external magnetic field Bapp . We now wish to investigate this “mixed state” by considering a plane inter face between a normal phase filling the left half-space z < 0 and a superconducting phase in the right half-space z > 0, as indicated in Fig. 6.3. We expect the superconducting order parameter to vanish at the interface and, as we have seen, begin approaching its bulk equilibrium value within a characteris tic length . On the other hand, surface cur rents flow in a surface layer of width ≈ L , and full exclusion of magnetic flux occurs only deep inside the superconductor. Here we are interested in calculating the effect of the interface on the free energy of the state. This, in turn, leads naturally to the idea of a “surface tension” between the superconduct ing and normal phases. Deep within either of the homogeneous phases the free-energy density at the critical field Bapp = 0 Hc is equal to Gn0 + 21 0 Hc2 . 161 The free-energy density of the associated mixed state, including the interface, is ⎧ 1 2 ⎪ z<0 ⎪Gn0 + 2 0 Hc ⎪ ⎨ 1 Gz = Gn0 − 1 b��4 + 2 ⎪ 2 ⎪ 0 ⎪ ⎩ ×B2 − 2 20 Hc · M z > 0 (6.88) where we have used Eq. (6.4) subject to the minimization restriction (6.6) for the half-space z > 0. The surface tension ns is defined as the difference in free energy per unit area between a homogeneous phase (either all normal or all superconducting) and a mixed phase. Therefore, we can write 1 ns = dz − 21 b��4 + 2 0 2 2 ×B − 2 0 Hc · M − 21 0 Hc2 (6.89) since the integrand vanishes for z < 0. With the aid of the expression B = 0 H + M this becomes (6.90) ns = dz − 21 b��4 + 21 0 M 2 Note that as z → � M → −Hc , and by Eq. (6.15), ��2 → �a�/b, so from Eq. (6.19) the integrand vanishes far inside the super conductor where z > L , and the principal contribution to the surface tension comes from the region near the boundary. If ns > 0, the homogeneous phase has a lower free energy than the mixed phase, and therefore the system will remain super conducting until the external field exceeds Bc , at which point it will turn completely normal. Superconductors of this variety are called Type I. However, if ns < 0, the super conductor can lower its free energy by spon taneously developing normal regions that include some magnetic flux. Since the great est saving in free energy is achieved by max imizing the surface area: flux ratio, these normal regions will be as small as possible 162 6 GINZBURG–LANDAU THEORY consistent with the quantization of fluxoid. Thus the flux enters in discrete flux quanta. Returning to Eq. (6.90), the first term represents the free energy gained by conden sation into the superconducting state, while the second is the cost of excluding flux from the boundary layer. Roughly speaking, the order parameter attains its bulk value over a characteristic length , while the super cur rents and magnetic flux are confined to a distance on the order of L from the surface. If we define the dimensionless magnetization m by M2 = a2 m2 b 0 (6.91) and make use of the dimensionless order parameter (6.81), Eq. (6.90) becomes ns = a2 dz−f 4 + m2 2b (6.92) which can be written a ns = dz1 − f 4 − 1 − m2 (6.93) 2b √ Equation (6.28) gives f = tanhz/ 2 (see Problem 10 for an expression for the dis tance dependence of m). We can estimate ns by observing that f 4 = m2 = 1 in the bulk, that f 4 is small only over a distance on the order of , and that m2 is small only over a distance on the order of L . This gives the approximate result 2 ns ≈ Bc2 − L 2 0 of a normal–superconducting interface, i.e., vortices form and Type II behavior appears. We could also argue that L is basi cally the width of an included vortex, i.e., the radius within which most of the flux is con fined, and is the distance over which the super electron density rises from ns = 0 at the center of the vortex to its full bulk value, i.e., the distance needed to “heal the wound.” A long coherence length prevents the super conductor’s ns from rising quickly enough to provide the shielding current required to contain the flux, so no vortex can form. Ginzburg and Landau (1950) showed √ that ns vanishes for = L / = 1/ 2, so as a convention we adopt the following criterion: 1 < √ 2 Type I 1 > √ 2 Type II (6.95) For Type II superconductors in very weak applied fields, Bapp � Bc , the Meissner effect will be complete, but as Bapp is increased above the lower critical field Bc1 , where Bc1 < Bc , vortices will begin to penetrate the sample. The magnetization of the sample then increases until the upper critical field Bc2 is reached, at which point the vortex cores almost overlap and the bulk supercon ductivity is extinguished. Superconductivity may persist in a thin sheath up to an even higher critical field Bc3 , where the sample goes completely normal. (6.94) where we have used Eq. (6.19). The value of the integral is the difference between the area under the two terms of the integrand, as shown plotted in Fig. 6.20. If > L , the surface tension is positive and we have Type I behavior. On the other hand, for < L ns is negative, and the superconduc tor is unstable with respect to the formation XIII. UPPER CRITICAL FIELD BC2 To calculate the upper critical field Bc2 of a Type II superconductor we will exam ine the behavior of the normalized GL equa tion (6.87a) in the neighborhood of this field. For this case the order parameter is small and we can assume Bin ≈ Bapp . This sug gests neglecting the nonlinear term f 3 in 163 XIII UPPER CRITICAL FIELD BC2 Figure 6.20 Order parameter �� and magnetization M inside a superconductor which is Type I < 1 a and inside a superconductor which is Type II > 1 b, where = L / . The surface energy ns is positive for the Type I case and negative for Type II. Eq. (6.87a) and following Eq. (6.41), taking for the normalized vector potential The linearized GL equation now has the form � = b0 u � 2 f − �2 f + f = 0 (6.96) where u is a dimensionless Cartesian coordi nate perpendicular to the directions of both the applied field and the vector potential. From Eq. (6.82) we have for the magnitude of b0 , 2 2 Bapp (6.97) b0 = 0 Deep inside the superconductor the normal ized order parameter f is independent of position so that the term � · �f in the GL equation (6.87a) is zero. (6.98) This equation has bounded solutions only for special values of b0 . By analogy with the harmonic-oscillator Schrödinger equation from quantum mechanics, we can take f ≈ eu/2 , which on substitution in (6.98) gives = 2 = b0 . Solutions can be found for larger values of b0 , but these are not of physical interest. Identifying the upper critical field with the applied field of Eq. (6.97) for this solution, we have Bc2 = 0 2 (6.99) 164 6 GINZBURG–LANDAU THEORY This expression has an appealing physical explanation. If we assume that in the upper critical field the cores of the vortices are nearly touching and that the flux contained in each core is ≈ 0 , the average magnetic field is Bc2 ≈ 0 / 2 . Obviously, the existence of an upper critical field requires that Bc2 > Bc , the ther modynamic critical field. By Eq. (12.12) the ratio of Bc2 to Bc is the energy scales as n2 , so single-flux quanta are energetically favored. This is because, according to Eq. (6.15), the parameter a scales as n, from Eq. (6.12) J scales as n, and from Eq. (6.11) B scales as n. Therefore n noninteracting vortices have n times the energy of a single vortex, but one multiquan tum vortex has a magnetic energy nB2 , which scales as n2 . Bc2 √ = 2 (6.100) Bc √ Therefore, for < 1/ 2 Bc2 < Bc and no vortex state exists. In this way we can see that the condition√ for a superconductor to be Type II is > 1/ 2. A. Differential Equations XIV. STRUCTURE OF A VORTEX For the case of a semi-infinite super conductor in a magnetic field it was found, by the arguments of Section VII, that the phase of the order parameter remains fixed throughout the superconductor. Here we will consider a different geometry in which the phase of the order parameter is nontrivial. In Type II superconductors it is observed that magnetic flux is completely excluded only for external fields B < Bc1 . Above the lower-critical field, Bc1 , flux penetrates in discrete flux quanta in the form of flux tubes, or vortices. In this section we will obtain approximate expressions for the fields associated with such a vortex, both in the core region and far outside the core. We assume that the external magnetic field Bapp is applied along the z direction, parallel to the surface, and that currents flow at the surface, canceling the field inside. We are concerned with a vortex that is far enough inside the superconductor so that exponential decay of the external fields, as given by Eq. (6.50), drops essentially to zero. States with more than one quantum of flux are also possible (Sachdev, 1992), but To treat this case we assume that there is no flux far inside the superconductor. If the applied field Bapp ≈ Bc1 a single quantum of flux 0 enters in the form of a vortex with axis parallel to the applied field. The simplest assumption we could make about the shape of the vortex is to assume that it is cylindrically symmetric, so that in its vicinity the order parameter (6.81) has the form of Eq. (6.2), corresponding to fx = fxei (6.101) where x = / are normalized polar coordinates. The vector potential has ˆ , so that we can write the form A = Ax for its normalized counterpart (6.82) ˆ �x = �x (6.102) This is a two-dimensional problem since nei ther fx nor �x have a z dependence. It is easy to show that � × � has only a z com ponent (this we do by working out the curl operation in cylindrical coordinates), which is to be expected, since the magnetic field B = � × A is known to be parallel to z. If we substitute these functions in the two GL equations (6.84) and perform the Laplacian and double curl operations in cylindrical coordinates, we obtain df f 2� 1 d x − 2+ x dx dx x x f − �2 f + f1 − f 2 = 0 (6.103) 165 XIV STRUCTURE OF A VORTEX d 1 d · x� dx x dx 1 1 + 2 f2 − � = 0 x recalling Eq. 6.82, and from Eq. (6.97), (6.104) where x = / and the current density equa tion (6.87b) becomes j = f2 1 −� = 0 x (6.105) In constructing a solution to Eqs. (6.103) and (6.104) we must be guided by two requirements, first that the magnetic field and current density must be finite everywhere and, second, that the solution must have a finite free energy per unit length along the z-axis. If the free energy per unit length were infinite, the total free energy would diverge and render the solution unphysical. Further, we anticipate from the Meissner effect and Eqs. (6.50) and (6.52), that the magnetic field and the current density will decay exponen tially far from the axis of the vortex. B. Solutions for Short Distances We seek to solve Eqs. (6.103) and (6.105) for the short-distance limit, namely in the core where x < 1. Since the first term in Eq. (6.105) has the factor 1/x, it is necessary for the order parameter f to van ish as x → 0 in order for the current density to remain finite in the core. By symmetry and continuity, the current density must vanish on the axis of the vortex, and it is expected to be small everywhere in the core. Maxwell’s equation, Eq. (6.11), tells us that in this sit uation the magnetic field B is approximately constant in the core and we can write ˆ A = 21 B0 2 2 B 0 0 (6.108) If we now use this approximate solu tion (6.107) for the vector potential in Eq. (6.103) and neglect the f 3 term because we expect f � 1 in the core, we will have df 1 d x x dx dx 1 + b0 + 1 − 41 b02 x2 − 2 f = 0 x (6.109) This equation has exactly the form of Schrödinger’s equation for the twodimensional harmonic oscillator. We know from quantum mechanics texts (e.g., Pauling and Wilson, 1935, p. 105) that the constant term in the square brackets b0 + 1 is the eigenvalue, the coefficient of the x−2 term is the z component of the angular momentum, i.e., m = 1, and, for the lowest eigenvalue, the coefficient of the x2 term is related to the other two terms by the expression b0 + 1 = 2m + 1 41 b02 1/2 (6.110) Solving this for b0 gives b0 = 1 (6.111) Substituting Eq. (6.111) in Eq. (6.108) gives the magnetic field on the axis of the vortex: B0 = 0 2 2 (6.112) The solution to the ‘Schrödinger’ equa tion, Eq. (6.109), is (6.106) f = Cxe−x /4 2 or, in dimensionless units, with x = / ˆ � = 21 xb0 b0 = (6.107) (6.113) where C is a constant. √ This function reaches its maximum at x = 2, which is outside the 166 6 GINZBURG–LANDAU THEORY core, so, to a first approximation, f continu ously increases in magnitude with increasing radial distance throughout the core region. This behavior is shown by the dashed curve in and near the core region of Fig. 6.21. We can use the results of Problem 8 to obtain a better approximation to the vec tor potential and magnetic field in the core region, 3 1 ˆ A = 2 B0 − 2 (6.114) B = B0 1 − 3 2 k̂ (6.115) where � 1. These expressions are plot ted as dashed curves in the core regions of Figs. 6.22 and 6.23, respectively. C. Solution for Large Distances To obtain a solution far from the vor tex core, x � 1, it is convenient to simplify Eqs. (6.103) to (6.105) by means of a change of variable, 1 �� = � − x (6.116) which gives d2 f 1 df + · − ��2 f dx2 x dx + f1 − f 2 = 0 d2 �� 1 d�� + · dx2 x dx � � f 2 �� − 2 − 2 = 0 x j = −f 2 �� (6.117) (6.118) (6.119) where the derivatives have been multiplied out. It should be pointed out that the curl of ˆ vanishes in the region under consid 1/x eration, so that � × �� = � × �, and hence Figure 6.21 Dependence of the order parameter �� on distance from the core of a vortex. The asymptotic behaviors near the core and far from the core are indicated by dashed lines. 167 XIV STRUCTURE OF A VORTEX Figure 6.22 Distance dependence of the vector potential A associated with a vortex in the notation of Fig. 6.21. Figure 6.23 Distance dependence of the magnetic field B encircling a vortex in the notation of Fig. 6.21. the 1/x term of Eq. (6.116) does not contribute to the magnetic field (see, however, Problem 9). For the approximation f ≈ 1, the change of variable x = y puts Eq. (6.118) into the form of a first-order n = 1 modified Bessel equation: y2 d 2 �� d�� +y 2 dy dy − y2 + 1�� = 0 (6.120) The solution to this equation which satisfies the boundary conditions �� y → 0 as y → � is �� y = A�� K1 y (6.121) where K1 y is a modified first-order Bessel function. For large distances, x � , it has the asymptotic form e−x/ �� x = A� √ x (6.122) 168 6 GINZBURG–LANDAU THEORY Figure 6.24 Distance dependence of the function 2 B in the notation of Fig. 5.21. This function is proportional to the amount of magnetic flux at a distance from the origin, and the integrated area under the curve is one fluxoid, h/2e. where A�� = 2/ 1/2 A� . Figure 6.22 shows the asymptotic long-distance behavior of A. Taking the curl B = � × A in cylindri cal coordinates (cf. Eq. (6.86)) provides the corresponding magnetic field for x � , Bz ≈ e−/L / 1/2 � L (6.123) where we have restored the original coordi nate = x = yL . Figure 6.23 shows a plot of Bz versus for large and indicates the = 0 value of Eq. (6.115). To find the radial dependence of the order parameter far from the core, where the material is in the superconducting state, we have f ≈ 1, so we can write fx = 1 − gx (6.124) where gx � 1, and hence f1 − f 2 ≈ 2g As a result Eq. (6.117) assumes the form d2 1 d gx + · gx + �� 2 dx x dx − 2gx = 0 (6.125) Far from the core, x � , the behavior of gx for � 1 is determined by that of �� x, and we have gx ≈ g� e−2x/ x (6.126) where g� is positive. Comparing Figs. 6.22 and 6.23 we see that A increases in the core region, reaches a maximum near the inflection point of the B curve, and decreases outside the core. The quantity 2 B is proportional to the amount of magnetic flux at a particular dis tance from the vortex axis; it is shown plotted against in Fig. 6.24. The integrated area under this curve equals one fluxoid, h/2e. FURTHER READING The GL theory was first proposed by Ginzburg and Landau in 1950. Its value became more apparent after Gor’kov (1959) showed that it is a limiting case of the BCS theory. The theory was extended to the limit of high by Abrikosov (1957) in the same year that the BCS theory was proposed. The London and Lon don (1935), London (1950), and related Pippard (1953) equations follow from the GL theory. 169 PROBLEMS The first edition of this book mentions some articles that apply GL theory to the cuprate super conductors. PROBLEMS 1. Derive the first GL equation, Eq. (6.6), from the Gibbs free energy integral (6.4). 2. Show that minimizing the term B2 /2 0 with respect to the vector potential A in Eq. (6.4) gives the expression � 2 A/ 0 that is found in Eq. (6.10). Hint: write ijk ilm j Ak yl Am yd2 y An x 3. 4. 5. 6. 7. 8. bring the partial differentiation inside the integral, and integrate by parts. √ Show that f = coth / 2 is also a solution to Eq. (6.27), and explain why it is not used. Show that Eq. (6.17) is consistent with Eq. (2.69) in the superconducting region near Tc , and express the ratio a0 /b0 in terms of the density n of conduction electrons. Derive Eqs. (6.71a) and (6.71b). Justify Eq. (6.97): b0 = 2 2 /0 Bapp . Show that � × � × A = −� 2 A in Cartesian coordinates, assuming the London-Landau gauge. Why is this not true when the coordinate system is nonCartesian? Assume the following power series solu tions to Eqs. (6.103) and (6.104) in the region of the core: fx ≈ an xn x � 1 fx ≈ fn x x�1 n (a) Show that the lowest-order terms that exist are f1 and a1 , that the even order terms vanish, and that f12 82 f3 = − 41 a1 + 21 f1 a3 = − (b) Show that the distance depen dence of the order parame ter, vector potential, magnetic field, and current density in the neighborhood of the origin are given by �a� 1/2 �� ≈ b 3 × f1 − �f3 � � 0 A ≈ 2 3 × a1 − �a3 � Bz ≈ � 0 2 × a1 − 2�a3 � 2 � (c) Show that the expression for �� agrees with Eq. (6.113). 9. Show that �� · dl = 0, whereas � · dl = 2 for contours at infinity. What is the significance of the 1/x term in Eq. (6.116)? 10. Show that the dimensionless magnetiza tion m defined by Eq. (6.125) can be written m= M Hc and has the distance dependence m = −1 − e−z/L in Eq. (6.93) (assume zero demagnetiza tion factor). 11. Derive Eq. (6.123) for the magnetic field far from a vortex. Find the first higherorder term that is neglected in writing out this expression. This page intentionally left blank 7 BCS Theory I. INTRODUCTION Chapter 6 presents the Ginzburg– Landau (GL) theory, which originated in 1950. Despite the fact that it is a phenomeno logical theory, it has had surprising success in explaining many of the principal proper ties of superconductors. Nevertheless, it has limitations because it does not explain the microscopic origins of super-conductivity. In 1957 Bardeen, Cooper, and Schrieffer (BCS) proposed a microscopic theory of supercon ductivity that predicts quantitatively many of the properties of elemental superconductors. In addition, the Landau–Ginzburg theory can be derived from the BCS theory, with the added bonus that the charge and mass of the “particle” involved in the superconduct ing state emerge naturally as 2e and 2me , respectively. With the discovery of the heavy fermion and copper-oxide superconductors it is no longer clear whether the BCS theory is sat isfactory for all classes of superconductors. The question remains open, although there is no doubt that many of the properties of hightemperature superconductors are consistent with the BCS formalism. To derive the BCS theory it is necessary to use mathematics that is more advanced than that which is employed elsewhere in this book, and the reader is referred to standard quantum mechanics texts for the details of the associated derivations. If the chapter is given a cursory initial reading without work ing out the intermediate steps in the devel opment, an overall picture of BCS can be obtained. For didactic purposes we will end the chapter by describing the simplified case of a square well electron–electron interaction 171 172 7 BCS THEORY potential, which is also the case treated in the original formulation of the theory. As with any two-body problem, we begin by defining the center of mass coordinate, R = 21 r1 + r2 II. COOPER PAIRS One year before publication of the BCS theory, Cooper (1956) demonstrated that the normal ground state of an electron gas is unstable with respect to the formation of “bound” electron pairs. We have used quota tion marks here because these electron pairs are not bound in the ordinary sense, and the presence of the filled Fermi sea is essential for this state to exist. Therefore this is prop erly a many-electron state. In the normal ground state all oneelectron orbitals with momenta k < kF are occupied, and all the rest are empty. Now, following Cooper, let us suppose that a weak attractive interaction exists between the elec trons. The effect of the interaction will be to scatter electrons from states with initial momenta k1 k2 to states with momenta k1� k2� . Since all states below the Fermi sur face are occupied, the final momenta k1� k2� must be above kF . Clearly, these scattering processes tend to increase the kinetic energy of the system. However, as we shall now see, the increase in kinetic energy is more than compensated by a decrease in the poten tial energy if we allow states above kF to be occupied in the many-electron ground state. We begin by considering the Schrödinger equation for two electrons interacting via the potential V , �2 2 2 − + 2 + Vr1 − r2 r1 r2 2m 1 = E + 2EF r1 r2 (7.1) In (7.1) the spin part of the wavefunction has been factored out and the energy. eigenvalue E is defined relative to the Fermi level 2EF . Most superconductors are spin-singlet so the orbital part to the wavefunction, r1 r2 , must be symmetric. (7.2) and the relative coordinate, r = r 1 − r2 (7.3) In terms of these coordinates (7.1) becomes �2 2 �2 2 − −2 R r 4m R 2m r + VrR r = E + 2EF R r (7.4) The center of mass and relative coordinates now separate and we can write R r = Rr (7.5) R is simply a plane wave, R = eiK·R (7.6) while for the relative coordinate wavefunc tion r we have −2 �2 2 r + Vr r 2m �2K2 = E + 2EF − r 4m (7.7) Since we are interested in the ground state, we can set K = 0. There are solutions for � 0 that lie close to the K = 0 states and K= are needed to describe states in which a per sistent current flows. We now express r as a sum over states with momenta p > kF , 1 � r = √ apeip·r V p (7.8) In (7.8) �p denotes a summation over all �p� > kF . Substitution of the expression for 173 II COOPER PAIRS r from (7.8) in (7.7) then gives the Schrödinger equation in momentum space, 2�p − EF − E ap + Vp p� ap� = 0 K = V0 K × � (7.10) 1 = V0 � p In order to simplify the solution of (7.9) we assume that Vp p� ⎧ ⎪−V0 ⎨ = ⎪ ⎩ 0 0 ≤ � p − EF ≤ � D and 0 ≤ �p� − EF ≤ � otherwise D (7.11) In (7.11), � D is a typical phonon energy, which reflects the idea that attraction between electrons arises via exchange of vir tual phonons. With the potential (7.11) the interaction term in (7.9) becomes � p� where D − EF − �p (7.12) x is the ordinary step function and K= � ap (7.13) p is a constant. Solving (7.9) for ap, we have ap = V0 K 2�p − EF − E × � × � D − EF − �p D − EF − �p (7.15) (7.14) Note that our Cooper pair involves momenta only in the narrow region �p –EF ≤ � D just above the Fermi surface. 1 2�p − EF − E D − EF − �p (7.16) The sum over the momenta can be expressed as an integral over the energies in terms of the density of states D�. Since typically � D � EF D� is well approx imated inside the integral by its value at the Fermi surface, DEF . Thus we have EF +� p 1 d� 1 = V0 DEF 2� − EF − E EF E − 2� D = 21 V0 DEF ln E (7.17) Solving for E we have E=− Vp p� ap� = −V0 K � 1 2�p − EF − E If we assume that K �= 0, this leads to an implicit equation for the eigenvalue E, where 1 3 −ip−p� ·r Vr d re V � p (7.9) p� Vp p� = We can now self-consistently evaluate the constant K in (7.13), 2� D exp 2/V0 DEF − 1 (7.18) In the weak-coupling limit V0 DEF � 1 and the exponential dominates the denominator in (7.18) so that 2 (7.19) E ≈ −2� D exp − V0 DEF This result is remarkable in several ways. First, it tells us that the pair state we have constructed will always have a lower energy than the normal ground state no matter how small the interaction V0 . This is why we say the normal ground state is unstable with respect to the formation of Cooper pairs. Sec ond, we see in (7.18) a hierarchy of very different energy scales, EF � � D � �E� (7.20) 174 7 BCS THEORY which, if we assume that kB Tc � �E�, explains why the superconducting transition temper ature is so small compared with the Debye temperature, D = � D kB If one Cooper pair lowers the ground state by −�E�, then, clearly many pairs will lower the energy even further, and one might be tempted to conclude that all the electrons should pair up in this fashion. Such a state would then resemble a Bose–Einstein con densate of Cooper pairs. However, we must keep in mind that if we do away entirely with the normal Fermi sea the state we have con structed collapses. We can use these intuitive ideas to guide our thinking, but to arrive at the true BCS ground state we must go beyond simple one- and even two-electron pictures and realize that the superconducting state is a highly correlated many-electron state. As in any theory of a phase transition the first task is to identify the “order parame ter”, which vanishes in the high temperature, disordered phase and is non-zero in the low temperature, ordered phase. We have seen that the normal ground state is unstable with respect to the formation of “Cooper pairs” if there is an attractive interaction between electrons at the Fermi surface. This leads us to consider the BCS order parameter k1 k2 = �a k1 a k2 � (7.22a) The BCS order parameter is in general a two-by two complex matrix. We will find it useful to define the Hermitian conjugate of the order parameter, k1 k2 ∗ = �a† k2 a† k1 � (7.22b) It is easy to see that the order parameter vanishes in the normal state. The average in (7.22a) is �a k1 a k2 � = Z−1 Tr e−H a k1 k2 III. THE BCS ORDER PARAMETER (7.23) In this section and those that follow we will present the formal details of the BCS theory. The most natural mathematical lan guage to use in this case is “second quanti zation”, where all observables are expressed in terms of the electron operators an k, and their Hermitian conjugates. The opera tor an k annihilates an electron with band index n, z-component of the spin and Bloch wavevector k. The electron operators have the anticommutation relations, an k a†m k� = nm k k� � an k am k = 0 (7.21) In order to reduce the complexity of the equa tions we will encounter, the band index, n, and the spin index, , will be combined into a single discrete index, n → . where = 1/kB T H is the Hamiltonian for the normal state, and Z is the partition func tion. This Hamiltonian is invariant under the (unitary) global gauge transformation, U † a kU = e−i a k (7.24a) U † HU = H (7.24b) If we apply this transformation inside the trace in (7.23), we have �a k1 a k2 � = Z−1 Tr UU † e−H a k1 a k2 = Z−1 Tr U † e−H UU † a k1 × UU † a k2 U = e−2i �a k1 a k2 � (7.25) 175 III THE BCS ORDER PARAMETER In the first and second lines of (7.25) we have used the fact that UU † = 1, and in the second line we have also used the cyclic property of the trace, Tr ABC = Tr BCA . Since is an arbitrary phase angle, solution to (7.25) is the only possible that a k1 a k2 = 0, as expected in the normal state. If the order parameter is to be differ ent from zero, it is clear from the above argument that the statistical operator can not be invariant under a global gauge trans formation. In the general theory of phase transitions this is called spontaneous sym metry breaking: the statistical operator has a lower symmetry in the ordered state than in the normal, or disordered, state. In the case of a ferromagnet, the normal state is rotationally invariant and the thermal aver age of the magnetization, which is a vec tor, vanishes. Below the Curie temperature, however, there is a spontaneous magnetiza tion that clearly breaks the rotational sym metry of the high temperature phase. The phenomenon of superconductivity is char acterized by the breaking of global gauge symmetry. The normal state may exhibit other sym metries that are characteristic of the crystal structure of the solid. If the superconduct ing state breaks one of the symmetries of the normal state in addition to global gauge symmetry then we say the superconductor is “unconventional”. For example, in “p-wave” superconductors, the order parameter has a vector character much like the magnetization in a ferromagnet. We will assume that the translational symmetry of the superconduct ing phase is the same as that of the normal state. Under a translation by a lattice vector R the electron operator transforms as T † Ra kTR = eik·R a k (7.26) Assuming the statistical operator for the superconducting state is invariant under translations, it follows, (by an argument very much like the preceding one) that k1 k2 = eik1 +k2 R k1 k2 (7.27) From this we conclude that the order param eter vanishes unless k1 = −k2 . We can use this fact to simplify things somewhat and define an order parameter that is a function of only one wavevector, k ≡ k −k (7.28) Finally, the anticommutation relations, (7.21), imply that the order parameter is antisymmetric under exchange of all its arguments, k1 k2 = − k2 k1 (7.29a) or, in the case of translational invariance, k ≡ − −k (7.29b) If the electron spin commutes with the nor mal state statistical operator (no spin-orbit interaction), then the order parameter must transform either as a spin singlet or a spin triplet. In the singlet case, which is the most common, we can write k = k (7.30) where = − and k = −k. In the triplet case we have k √ 3 k − 1 k + i2 k / 2 √ = 1 k − i2 k / 2 3 k (7.31) where the three spatial components of the order parameter, 1 k 2 k 3 k are odd functions of the wavevector, i k = −i −k (7.32) The three components of the triplet order parameter defined by (7.31) transform under 176 7 BCS THEORY rotations in spin-space as a vector, and clearly break the invariance of the normal state under such rotations. Therefore, the triplet order parameter is unconventional, and the singlet is conventional. only terms first order in the fluctuations, we have a† k1 a† k2 V k1 k2 k3 k4 a k3 k1 k2 k3 k4 × a k4 = IV. THE BCS HAMILTONIAN We have argued that in order for the order parameter to differ from zero the statis tical operator must break global gauge sym metry. The simplest way to construct such a statistical operator is to assume the order parameter is not zero and that the fluctua tions about the order parameter are small. Thus we write a k1 a k2 = �a k1 a k2 � + a k1 a k2 − �a k1 a k2 � a† k1 a† k2 k1 k2 k3 k4 + a k1 a k2 − a† k1 a† k2 × V k1 k2 k3 k4 a k3 a k4 + a k3 a k4 − a k3 a k4 † a k1 a† k2 V k1 k2 k3 k4 ≈− k1 k2 k3 k4 † a k1 a† k2 × a k3 a k4 + k1 k2 k3 k4 × V k1 k2 k3 k4 a k3 a k4 † a k1 a† k2 V k1 k2 k3 k4 + k1 k2 k3 k4 (7.33) × a k3 a k4 (7.36) in the Hamiltonian, and expand in powers of We now use the definition of the order param eter, (7.25) and (7.35) to get the fluctuation. We begin with a Hamiltonian that includes the one-electron band structure and HBCS = 1 ∗ kV k k� k� 2 kk� a two-body interaction between electrons, + E ka† ka k + H = E ka† ka k k k † 1 + a k a† k 2 k k k k 1 2 1 2 3 4 × V k1 k2 k3 k4 k3 a k4 (7.34) Under translation by a lattice vector the inter action transforms as − + 1 ∗ kV k k� a k� a −k� 2 kk� 1 † a ka† −kV k k� k� 2 kk� (7.37) where we’ve introduced the shorthand V k k� ≡ V k −k k� −k� . The leading term in (7.37) is just a com V k1 k2 k3 k4 = e−ik1 +k2 −k3 −k4 ·R plex number, the next term is the normal state × V k1 k2 k3 k4 one-electron band structure, and the final two (7.35) terms are new. The BCS Hamiltonian can be simplified which requires k1 + k2 − k3 − k4 = G, where even further if we define the gap function, G is a reciprocal lattice vector. If we now insert the expansion, (7.33), k = V k k� k� (7.38) into the interaction term in (7.34) and keep k� 177 V THE BOGOLIUBOV TRANSFORMATION so that (7.37) now becomes HBCS = 1 ∗ kV k k� k� 2 kk� + E ka† ka k The action of the Bogoliubov transformation on the electron operators is eB a ke−B = U ka k − V ka† −k ≡ b k k 1 † a k ka† −k 2 k − a k∗ k a −k (7.39) + Note that the gap function has the same sym metries as the order parameter itself. In par ticular it is antisymmetric under exchange of labels, −k = V −k k� k� k� = � � V −k −k k k� = (7.43) which defines the quasiparticle operators b k. The coefficients U k and V k are given by U k = + 1 2! k −k∗ 1 k −k∗ 4! ∗ k −k + · · · + V k = + (7.44a) k 1 3! k ∗ −k k + · · · (7.44b) V −k −k� −k� k� = − k (7.40) V k = V −k V. THE BOGOLIUBOV TRANSFORMATION + † † ka ka −k ∗ ka k a −k (7.41) Since the electron operators anticommute, the coefficients k must be antisymmet ric under exchange of spin and band indices and k → −k, k =− −k (7.45a) whereas for the U ’s we have The BCS Hamiltonian, (7.39), is bilin ear in the electron operators, and so it can be diagonalized by a unitary transforma tion, called the Bogoliubov transformation, that mixes electron creation and annihilation operators. The generator for the Bogoliubov trans formation is the anti-hermitian operator 1 B= 2 k The V k have the same symmetry as k itself, (7.42) U ∗ k = U k (7.45b) The Bogoliubov transformation preserves the canonical commutation relations for the elec tron operators, (7.21), which lead to the fol lowing relations: ∗ U kV k − V kU −k = 0 (7.46a) ∗ ∗ U kU k − V kV −k = (7.46b) The coefficients k, or equivalently the Bogoliubov amplitudes, are chosen so that the “off-diagonal” terms, i.e. the terms that involve the product of two creation or two annihilation operators, vanish. In order 178 7 BCS THEORY to facilitate the calculation of the Bogoli ubov amplitudes it is useful to define a twocomponent operator a k (7.47) A k = † a −k The BCS Hamiltonian can then be written in the compact form 1 † A k · H k · A k + E0� 2 k (7.48) where the 2 × 2 matrix H k is E k k H k = (7.49) −∗ −k −E −k HBCS = The constant E0� arises from reordering the electron operators, E0� = 1 E k 2 k (7.50) and E k is the diagonal matrix E k = E k . The action of the Bogoliubov trans formation, (7.43), on the BCS Hamiltonian (7.48) is eB A† k · H k · A ke−B U k V k † = A k H k ∗ ∗ V −k U −k U k −V k × A k (7.51) −V∗ −k U∗ −k We see from this that the Bogoliubov trans formation acting on the electron opera tors induces a unitary transformation of the matrix H k. In the usual way, the unitary matrix that diagonalizes H k can be con structed from its eigenvectors. By inspection of (7.51) we see that the BCS Hamiltonian is diagonalized if the Bogoliubov amplitudes satisfy the eigenvalue equation E k − k U k −∗ −k −E −k −V∗ −k U k = ! k (7.52a) −V∗ −k It should be noted that by introducing the two-component operator A k we have doubled the size of the vector space. As a consequence, for every eigenvector with eigenvalue ! k there is a second eigenvec tor with eigenvalue −! k given by E k k −V k −∗ −k −E −k U∗ −k −V k = −! k (7.52b) U∗ −k If we use (7.52a,b), the Hamiltonian takes the diagonal form ! k 0 HBCS = A† k A k 0 −! k (7.53) which can be expressed in terms of the elec tron operators as HBCS = ! kb† kb k + E0� − E0�� k (7.54) where E0�� = 1 ! k 2 kn n (7.55) is a constant that arises when the quasi particle operators are normal ordered. The eigenvalues ! k appearing in (7.52) are the quasiparticle energies. VI. THE SELF-CONSISTENT GAP EQUATION By treating order parameter in the meanfield approximation the BCS Hamiltonian clearly breaks global gauge symmetry, but we must complete the theory by calculating the order parameter in the ordered state, k = Z−1 Tr e−HBCS a ka −k (7.56) 179 VI THE SELF-CONSISTENT GAP EQUATION Note that the order parameter appears both on the right and on the left-hand side of this equation, so it must be solved selfconsistently. If we apply the Bogoliubov transforma tion to (7.56), we have k = Z−1 Tr e−HBCS U ka k − V ka† −k bands that are far from the Fermi energy will contribute very little to the superconducting order parameter. If we use the definition of the gap func tion, (7.38), the gap equation (7.59) can be written entirely in terms of the order parameter, k = × U −ka −k − V −ka† k (7.57) The Bogoliubov transformation diagonalizes the BCS Hamiltonian as in (7.54), so the ther mal averages in (7.57) can be done immedi ately, with the result k = U kV k 1 − n! ∗ − V k U −kn! (7.58) where nx = ex + 1−1 is the usual FermiDirac occupation function. In general this nonlinear equation is quite difficult to solve, but near the criti cal temperature, where the order parameter is small, we can treat the symmetry-breaking terms in HBCS as a perturbation and linearize the gap equation. The details of this calcula tion are somewhat involved, and so we rel egate them to Appendix A. The final result is (A.13) 1 − n E −k − n E k E k + E −k × k p B. Solution At T = 0 The gap equation also simplifies at zero temperature, where the number of quasi particles vanishes. In this case we have, by (7.46a) lim k → U kV k T →0 1 = V 2 k 2 (7.61) which tells us that V k has the same sym metry as the order parameter. A. Solution of the Gap Equation Near Tc k = 1 − n E −k − n E k E k + E −k × V k p p (7.60) (7.59) The energy dependent factor in (7.59) has a maximum near E ≈ E ≈ 0, that is for both energies near the Fermi surface. Therefore C. Nodes of the Order Parameter Most of the superconducting materials known before the discovery of the copperoxide high temperature superconductors by Bednorz and Müller (1986) are of the “s wave” type, meaning the order parameter is a spin-singlet and positive everywhere in the Brillouin zone. There is convincing evi dence that the quasi two-dimensional hightemperature superconductors are “d-wave”, with nodal lines along the directions kx = ±ky in the plane perpendicular to the c axis. Heavy-fermion superconductors like UPt 3 may be “p-wave”, or triplet, k = − −k, requiring a node at k = 0. The order parameter must transform as an irreducible representation of the point 180 7 BCS THEORY group of the crystal structure1 . If the order parameter has a single component, it must transform as a one-dimensional represen tation of the point group. Of these onedimensional representations, there is always the identity representation, which corre sponds to the case where the order parameter does not change sign under the operations of the point group. This is referred to as “extended s-wave”. It is possible that the order parameter can still have nodes in this case. For example, the order parameter k = 0 + 1 cos kx a + cos ky a, which is invariant under the point group D4h appropri ate to a copper-oxygen plane in the cuprate materials, may have nodal lines near the cor ners of the Brillouin zone if 0 < 2 1 . On the other hand, if the order param eter transforms as one of the other onedimensional representations of the point group, it must change sign under at least one element of the point group, P Pk = − k. D. Single Band Singlet Pairing !k = E 2 k + �k�2 (7.64) from which we see why k is referred to as the gap function. The Bogoliubov amplitudes can be found, Ek 1 2 1+ �uk� = !k 2 Ek 1 1− �vk�2 = (7.65) !k 2 and are shown in Fig. 7.1. The expression for the order parameter, (7.58) then takes the very simple form k = − 1 − 2n !k k 2!k (7.66) Close to the transition temperature the order parameter is given by k = − In the case of spin-singlet pairing in a single band, the order parameter is p = p The quasiparticle energies are given by 1 − 2n Ek Vk pp 2Ek p (7.67) (7.62) where = − and p = −p is a complex scalar function. The same is true of the gap function p = p and the Bogoliubov parameter k = k. If we assume the band energies are spinindependent and invariant under parity, the form of the Bogoliubov amplitudes simplify a great deal (note that = − ) and we find E. S-Wave Pairing To proceed further we need a model for the interaction potential. A simple choice (J. Bardeen, L.N. Cooper and J. R. Schrieffer 1957) that leads to tractable expressions is (7.63) Vk p = −V0 "Ek/E0 "Ep/E0 (7.68) where 1 for − 1 ≤ x ≤ 1 "x = (7.69) 0 otherwise An exception to this can occur if two order parame ters with different symmetry are degenerate. In this case the order parameter is said to be “mixed”. Note that the choice of sign in (7.68) antic ipates that we will find a solution only if the effective interaction is attractive. In the case of phonon-mediated interactions, V0 is U k = cos k V k = sin k 1 181 VI THE SELF-CONSISTENT GAP EQUATION 1 [u(E/Δ)]2 0.75 0.5 0.25 [v(E/Δ)]2 –2 –1 1 2 E/Δ Figure 7.1 Bogoliubov amplitudes in the neighborhood of the Fermi surface. a measure of the strength of the electronphonon coupling and E0 = � D is a typical phonon energy. We then have 1 − 2n Ek k = #V0 "Ek/E0 2Ek (7.70) where # = "Ep/E0 p (7.71) p If we substitute (7.70) for the order parameter in (7.71) we get 1 − 2n Ep 1 = V0 "Ep/E0 2Ep p (7.72) This equation determines the transition tem perature, which enters through the FermiDirac function on the right hand side. The summand in (7.72) is monotonically decreasing with temperature. Above the tran sition temperature the only solution to the gap equation is k = 0. For T ≤ Tc a sec ond solution exists with k = � 0. We can solve (7.72) for the transition temperature if we replace the sum by an integral and assume the density of states in the neighborhood of the Fermi surface is constant, D0. With these approximations, (7.72) becomes E0 V0 D0 1 − 2nE 1= dE 2 E −E0 E0 tanh E/2k T B c dE = V0 D0 E (7.73) 0 In most simple superconductors E0 /kB Tc >> 1. The integral in (7.73) can then be done by parts, and in the remaining integral the upper limit set to infinity, with the result kB Tc = 2e E e−1/D0V0 $ 0 (7.74) The remarkable thing about this result is that no matter how weak the interaction between electrons, there is always a superconducting state. It is also clear that any sort of series expansion in V0 will suffer from an essential singularity at V0 = 0. Figure 7.2 shows a scat ter plot of the density of states and transition 182 7 BCS THEORY Figure 7.2 Dependence of the superconducting transition temperature Tc on the density of states D0 for various superconductors (Okazaki et al., 1990) temperatures for a variety of superconduct ing materials. 0 = F. Zero-Temperature Gap At zero temperature there are no quasi particles and the gap equation becomes k = V0 "Ek/E0 2!k × "Ep/E0 p (7.75) p Once again we define #= "Ep/E0 p (7.76) p and, following the same steps that led to the expression for the transition temperature, we find 1 = V0 Dn 0sinh−1 E0 /0 In the weak-coupling limit, E0 /0 >> 1, the zero-temperature gap is (7.77) E0 −1/V0 Dn 0 e 2 (7.78) If we take the ratio of the zero-temperature gap to the critical temperature we find 20 2$ = ≈ 353 k B Tc e (7.79) The full temperature dependence of the gap is shown in Fig. 7.3 below. Table 7.1 lists the transition temper atures and zero-temperature gaps, and the dimensionless ratio 20 /kB Tc for several superconductors. Given the crude approxi mations made in order to calculate the ratio of the zero temperature gap to the transition temperature, it is remarkable that the value of this ratio for some real materials is not too far from the weak-coupling BCS value. 183 VI THE SELF-CONSISTENT GAP EQUATION Many of the physical properties of superconductors depend on the quasiparticle density of states. In particular the presence of the gap is especially important, leading for example, to an exponential behavior in the specific heat. If we assume the density of states in the normal phase is slowly varying in the neighborhood of the Fermi surface, then the density of states in the supercon ducting state, shown in Fig. 7.4 is Figure 7.3 Temperature dependence of the BCS gap ⎧ D 0! ⎪ ⎪ √n ⎪ ⎪ ⎨ !2 − 2 DS = 0 ⎪ ⎪ D 0! ⎪ ⎪ ⎩√ n !2 − 2 !> �!� < (7.80) ! < − function . Table 7.1 Comparison of Energy Gaps for Various Superconductorsa Material Hf Cd Zn Al In Hg Pb Nb V3 GeA15 V3 SiA15 Nb3 SnA15 K3 C60 Rb3 C60 Ba06 K04 BiO3 Nd0925 Ce0075 2 CuO4 La0925 Sr0075 2 CuO4 YBa2 Cu3 O7−% Bi2 Sr2 Ca2 Cu3 O10 Tl2 Ba2 CaCu2 O8 Tl2 Ba2 Ca2 Cu3 O10 HgBa2 Ca2 Cu3 O8 a Tc K 013 052 085 12 34 42 72 93 112 171 181 19 29 185 21 36 87 108 112 105 131 2�0 meV 2�0 /kB Tc 0.044 0.14 0.23 0.35 1.05 1.7 2.7 3.0 3.1 5.4 4.7 5.9 7.5 5.9 7.4 13 30 53 44 28 48 3.9 3.2 3.2 3.4 3.6 4.6 4.3 3.8 3.2 3.7 3.0 3.6 3.0 3.7 4.4 4.3 4.0 5.7 4.5 3.1 4.3 Data on elements from Meservey and Schwartz (1969); data on the A15 compounds from Vonsovsky et al. (1982); and data on high-temperature superconductors from T. Hasegawa et al. (1991). K3 C60 and Rb3 C60 values are from Degiorgi et al. (1992), and HgBa2 Ca2 Cu3 O8 data are from Schilling et al. (1994b). Many of the 20 /kB Tc ratios are averages of several determinations, sometimes with considerable scatter; the 20 values are calculated from columns 2 and 4. The BCS value of 20 /kB Tc is 3.52. Table 3.1 provides energy gap data for many additional elements. 184 7 BCS THEORY G. D-Wave Order Parameter There is a growing consensus that the order parameter in the copper-oxide super conductors is “d-wave”. These materials are fairly anisotropic, and many treatments are quasi two-dimensional, focusing on the copper-oxygen planes that form a nearly square lattice. It is also true that many of the parent materials of the cuprates are anti ferromagnetic; doping tends to destroy the long-range AF order, but strong short range AF correlations survive in the normal state of superconducting samples. In this section we present a very simple “toy model” that leads to a d-wave order parameter. This model is not intended to be a realistic representation of any material, but merely to illustrate how such a solution to the gap equation can arise. The point group for the square, D4h , has the parity-even one dimensional repre sentations listed in the following table (D.L Scalapino, 1995), The order parameter must trans form as one of these one-dimensional representations. The gap equation, (7.66), can be cast in a more symmetric form by defining a rescaled order parameter k = fk&k (7.81) and a rescaled two-body potential, Wk p ≡ fkVk p fp where fp > 0 is the energy-dependent function fp = 1 − 2n !p 2!p The gap equation now has the simple form &k = − Wk p&p (7.83) p The simple form (7.68) for the inter action potential is insufficient to describe an order parameter that changes sign within the Brillouin zone, since, as one can see from (7.76), the parameter # vanishes in this case. Therefore let us consider an interaction Wk p that is strongly peaked for a momen tum transfer q = k − p in the neighborhood of q0 = $a $a , Wk p = V0 k − p q0 Irreducible one-dimensional representation '1+ '2+ '3+ '4+ Basis Function 1 cos kx a + cos ky a sin kx a sin ky ax cos kx a − cos ky a cos kx a − cos ky a sin kx a sin ky a (7.84) The gap equation then becomes &k = −V0 &k − q0 (7.85) If we assume that V0 > 0, that is the effective potential is repulsive, it follows that the order parameter must change sign on translation by q0 , k = −k − q0 Table 7.2 Irreducible one-dimensional representations of the point group D4h . (D.L. Scalapino (1995)) (7.82) (7.86) This rules out the extended s-wave case, k = 0 + 1 cos kx a + cos ky a, unless 0 = 0, and an order parameter that trans forms as '4+ , leaving the possibility of order parameters that transform according to the representations '2+ and '3+ . Contour plots of these two cases are shown in figures 7.5a,b. Whether the order parameter is extended s-wave, d-wave, or the even more compli cated form shown in Fig. 7.5b, is ultimately decided by which one gives the lowest free energy. 185 VI THE SELF-CONSISTENT GAP EQUATION H. Multi-Band Singlet Pairing The superconducting state in MgB2 is believed to involve more than one band. In order to investigate case where several bands may lie close to the Fermi surface, we return to (7.60) and again assume singlet pairing. We will also assume that the bands are parity invariant so Ei k = Ei −k. The gap equa tion (7.60) becomes ij k = Figure 7.4 Density of states in the superconducting state near the Fermi surface. 1 − n Ei k − n Ej k Ei k + Ej k × Vijmn kpmn p (7.87) p where the Latin indices label the bands and take the values i = 1 2 ( ( ( n. We can –π – π 2 0 π 2 π π π – π π 2 2 0 0 π – 2 –π –π – π 2 0 π 2 π 2 –π π Figure 7.5a Contour plot of kx versus ky for the d-wave order parameter belonging to the representation '3+ of the point group D4h . 186 7 BCS THEORY –π – π π 0 2 π 2 π π – π π 2 2 0 0 π – 2 –π –π – π π 0 π π 2 –π 2 2 Figure 7.5b Contour plot of kx versus ky for the order parameter belonging to the representation '2+ of the point group D4h . simplify the structure of (7.87) by defining the function fij p = 1 − nEi p − nEi p Ei p + Ej p (7.88) Note that fij p > 0, which allows us to define a rescaled order parameter, &ij p, ij p ≡ fij p&ij p (7.89) and a rescaled two-body potential Wijmn k p ≡ fij kVijmn k p fmn p (7.90) The self-consistent gap equation then becomes &ij k = Wijmn k p&mn p (7.91) p mn If we regard this as an eigenvectoreigenvalue equation, we see that the scaled order parameter is an eigenvector of W with eigenvalue 1/. If the largest eigenvalue of W is 0 , then the critical temperature is the solution of the equation c 0 c =1 (7.92) Denoting the eigenvector corresponding to 0 the maximum eigenvalue by )ij k, the 187 VI THE SELF-CONSISTENT GAP EQUATION order parameter is 0 ij k ≡ fij k)ij k (7.93) If we assume that the intra-band scat tering terms in W are large compared to the inter-band terms, the well-known methods of perturbation theory can be applied to the eigenvalue problem, (7.91). In the usual way W is separated into two parts, Wijmn k p = 0 1 Wijmn k p + Wijmn k p potential without saying anything about its origin, other than noting that in the BCS theory the exchange of virtual phonons gives rise to an attractive interaction. A detailed calculation of the electron-phonon coupling is beyond the scope of this book, so we simply refer to the central result of Eliashberg, who defines the dimensionless electron-phonon coupling constant � 2 D ph !=2 d (7.96) 0 (7.94) 0 where Wijmn k p includes all intra-band interactions (and is therefore diagonal in the 1 band indices) and Wijmn k p contains all inter-band interactions. Following standard perturbation theory, (here the eigenvectors and eigenvalues are understood to be those of W 0 ) we find the first- correction to the maximum eigenvector is2 )n W 1 )0 n 0 )ij = )ij (7.95a) 0− n n�=0 and the shift in the maximum eigenvalue is, to second order (the first order term vanishes), 2 0 = 2 )n W 1 )0 n�=0 0− > 0 (7.95b) Superconductors are characterized according to the magnitude of !, ! << 1 weak coupling !∼1 intermediate coupling (7.97) ! >> 1 strong coupling In addition to the attractive electronphonon coupling there is a residual screened Coulomb repulsive interaction characterized by the dimensionless parameter ∗c . The net electron-electron interaction is the sum of these two terms, and in the expressions (7.74) and (7.78) we make the substitution Dn 0V0 → ! − ∗c (7.98) so the transition temperature is given by n We see that only processes where the num ber of electrons in each band remains fixed contribute to the change in the order param eter and eigenvalue to lowest order. It is also interesting to note that quite generally the presence of other bands increases the eigen value, and therefore the critical temperature. In the beginning of our discussion we introduced an effective electron-electron Tc = 113D e − !−1∗ c (7.99) A number of other expressions for the critical temperature have appeared in the lit erature. McMillan (1968) gives the following empirical formula 1041 + * Tc = D exp − 145 * − ∗c 1 + 062* (7.100) 2 The inner product notation used in (7.85) involves both sums over band indices and a sum over wavevectors. Values of * and ∗c reported in the litera ture for various superconductors are listed in Table 7.3. 188 7 BCS THEORY Table 7.3 Electron–Phonon Coupling Constants and Coulomb Interaction Parameters ∗a c Material Tc K � �∗c Ru Zr Os Mo Re Pb Nb NbC TaC V3 Ge V3 Si Nb3 Sn Nb3 Ge K3 C60 Rb3 C60 Cs3 C60 BaPb BiO3 La0913 Sr0087 CuO4 La0913 Sr0087 CuO4 YBa2 Cu3 O7 YBa2 Cu3 O7 YBa2 Cu3 O7 Bi2 Sr2 CuO6 Bi2 Sr2 CaCu2 O8 Tl2 Ba2 CaCu2 O8 049 061 066 092 17 72 93 111 114 61 171 181 232 163 305 474 12 047 022 044 035 037 155 085 061 062 07 112 167 180 051 061 072 13 01 20 02 03 25 02 03 03 015 017 012 009 01 a 35 90 018 01 References Table 3.1 Table 3.1 Table 3.1 Table 3.1 Table 3.1 Ginzburg and Kirzhnits (1977, p. 171) Ginzburg and Kirzhnits (1977, p. 171) Ginzburg and Kirzhnits (1977, p. 171) Ginzburg and Kirzhnits (1977, p. 171) Vonsovsky et al. (1982, p. 303) Vonsovsky et al. (1982, p. 303) Ginzburg and Kirzhnits (1977, p. 171) Vonsovsky et al. (1982, p. 303) Novikov et al. (1992) Novikov et al. (1992) Novikov et al. (1992) Schlesinger et al. (1989) Gurvitch and Fiory (1987a,b,c) Rammer (1987) Gurvitch and Fiory (1987a,b,c) Tanner and Timusk (1992, p. 416) Kirtley et al. (1987) Tanner and Timusk (1992, p. 416) Tanner and Timusk (1992, p. 416) Foster et al. (1990) High and low estimates are given for high-temperature superconductors, some of which are averages of several investigators. Skriver and Mertig (1990) give coupling constants from rare earths. VII. RESPONSE OF A SUPERCONDUCTOR TO A MAGNETIC FIELD effective mass m. The BCS Hamiltonian in this model is In this section we consider the behavior of the order parameter in the presence of a weak, slowly varying magnetic field B which is given in terms of the vector potential, A B = ×A (7.101) Our goal here is to calculate the current den sity J induced by the externally applied mag netic field, and in this way to demonstrate the Meissner effect. To simplify the discussion we will consider singlet pairing in a single free-electron like band characterized by an HBCS = �2 3 dr 2m ie ie × − A † r · + A � � × r − d3 r† r r 1 3 3 � dr dr 2 × † r† r r� + − r r� ∗ r r� (7.102) 189 VII RESPONSE OF A SUPERCONDUCTOR TO A MAGNETIC FIELD where , the chemical potential, sets the zero-point of the energy scale. Note that the order parameter (and the gap function) is now a function of the coordinates, r r� = � r r� � In the absence of the magnetic field we recover translational symmetry, and the Bogoliubov amplitudes are U r = U keik·r (7.103) V r = V keik·r Following our earlier treatment, the BCS Hamiltonian can be written up to a c-number (i.e. complex number) in the form 1 3 dr HBCS = 2 × d3 r � † r� H r� r r Substitution into (7.107) with A = 0 gives (7.104) where the two-component field operator is r r = (7.105) † r and H r r is ⎞ r� r r� r 2 �2 ie × r − A + 2m � ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎟ ⎠ (7.106) As before, the Bogoliubov amplitudes are the components of the eigenvectors of H r� r, and satisfy the coupled equations 2 �2 ie − r + A + U r 2m � − d3 r � r r� V r� = !U r 2 �2 ie r − A V r 2m � − d3 r � r r� ∗ U r� = −!V r (7.107) � 2 k2 − U k 2m − kV k = !U k � 2 k2 − V k 2m − k∗ U k = −!V k (7.109) � H r� r ⎛ − r� r 2 2 ⎜ � ie ⎜× r + A + ⎜ 2m � ⎜ ⎜ =⎜ ⎜ − r� r∗ ⎜ ⎜ ⎝ (7.108) In the presence of a weak, slowly varying magnetic field we can apply the adi abatic approximation, and assume that the amplitudes in (7.108) are slowly varying in space, U r = U k reik·r V r = V k reik·r (7.110) and we can drop the term in the kinetic energy operator that is quadratic in A, ie r + A � 2 ≈ r2 + 2ie ·A � (7.111) Keeping only the largest terms, (7.109) becomes � 2 k2 �e + k · Ar − U k r 2m m − kV k r = !U k r � 2 k2 �e − k · Ar − V k r 2m m − k∗ U k r = −!V k r (7.112a) 190 7 BCS THEORY If we move the terms involving the vector potential to the right, we have 2 2 � k − U k r − kV k r 2m �e = ! − k · Ar U k r m 2 2 � k − V k r − k∗ U k r 2m �e = − ! − k · Ar V k r (7.112b) m Comparing this with (7.109), we see that the Bogoliubov amplitudes follow the vector potential adiabatically through their depen dence on the eigenvalue �e (7.113) k · Ar m The current density is given by !k r = !k + ie� † Jr = r r 2m e2 −† r r − Ar† r r m (7.114) and its thermal average is �Jr� = ie� Un r∗ Un r 2m n where the total electron density is ne = ! − �vk�2 1 − n! (7.117) The current density induced by the applied field is �Ji r� = − e 2 ns Ar m (7.118) where the “density of super-electrons” is 2 e� 2 1 2 +n ns = n e − k − 3 m V k +! (7.119) and we have used rotational symmetry to write k ki kj +n 1 2 +n = k +! 3 ij k +! (7.120) Note that at zero temperature the second fac tor in Eq. (7.119) vanishes, and the density of super-electrons is equal to the total density of electrons. If we substitute our expression (7.118) into Ampere’s law, we have London’s equation 2 × × A = !− L A −Un r∗ Un r n! + Vn r∗ Un r − Vn r∗ Un r 2 �uk�2 n! V n (7.121) where the London penetration depth, !L , is given by e2 Ar Un r∗ Un r e 2 ns m 2 !− (7.122) L = 0 n ∗ n m × n! + V r V r1 − n! (7.115) The perfect diamagnetism that is characteristic Keeping only terms to first order in the vector of superconductors is embodied in Eq. (7.121). potential, we have 2 e� 1 APPENDIX A. DERIVATION OF THE �Ji r� = −2 m V GAP EQUATION NEAR TC +n e2 ne × ki kj Aj − Ar The order parameter is given by +! m k (7.116) k = Z−1 Tr e−H a ka −k (A.1) × 1 − n! − 191 APPENDIX A. DERIVATION OF THE GAP EQUATION NEAR Tc The BCS Hamiltonian, (7.39), is bilinear in the electron operators, which means thermal averages of the type (A.1) can be calculated by purely algebraic means. First, we introduce the Bloch operators a k = e a ke H −H Integrating (A.7) to first order gives K = 1 − d � H1 � 0 1 e E k+E −k − 1 = 1− 2 k E k + E −k (A.2) The equation for the order parameter can be written as × a† ka† −k k k = Z−1 Tr e−H a ke−H eH a −k 1 − e− E k+E −k E k + E −k × a ka −k (A.9) − ∗ k = Z−1 Tr e−H a −k a k (A.3) where we’ve used the cyclic property of the trace. Near the transition temperature the sym metry breaking terms in the BCS Hamilto nian are small and can be treated as a pertur bation, so we split the Hamiltonian into two parts, H = H0 + H1 where (A.4) H0 = E ka+ ka k k and 1 † a k ka† −k H1 = 2 k −a k∗ ka −k (A.5) (A.6) where K satisfies − dK = H1 K d a k = e−E k K −1 a kK 1 e E p+E −p − 1 = e−E k a k + 2 p E p + E −p × a† pa† −p a k p = e−E k a e E p+E −p − 1 1 × k + e−E k p 2 E p + E −p p × a† p k −p − k pa† −p = e−E k a k − e−E k In the interaction picture we write e−H = e−H0 K We then have for a k to first order × e E −k+E k − 1 p E − k + E k ka† −p (A.10) (A.7) with Inserting this into (A.3) we have k = �a −k a k� H1 = eH0 H1 e−H0 = 1 2 k = e−E −k −k − e−E −k e E k+E −k a† ka† × × −k k + − k∗ e E k+E −k − 1 p ! × e−r E k+E −k a ka −k (A.8) E k + E −k −knE (A.11) where nE = �a† pa k� = eE + 1−1 is the usual Fermi-Dirac occupation function. 192 7 BCS THEORY Using the antisymmetry of the order param eter, (A.11) can be written as k = e−E −k 1 + eE −k eE k+E −k − 1 × knE E k + E k = n E −k n E k × eE k+E −k−1 k E k + E k (A.12) With a little algebra we have 1 − n E −k − n E k k E k + E −k (A.13) If we now use the definition of the gap func tion, (A.13) becomes Eq. (7.60). k = k = 1 − n E −k − n E k E k + E −k × V k p p (A.14) p FURTHER READING Some of the classical articles on the BCS theory have already been mentioned at the beginning of the chapter. The article by Cooper (1956), predicting the formation of the “pairs” that bear his name, provided the setting for the BCS theory formulated by Bardeen, Cooper, and Schrieffer in 1957, and elaborated upon in the books by de Gennes (1966), Fetter and Walecka (1971), and Schrieffer (1964). The textbook by Tinkham (1985) provides a good introduction to the BCS theory, and Tilley and Tilley (1986) give a briefer introduction. Gorkov (1959) showed that the Ginzburg–Landau theory, which was discussed in the previous chapter, follows from the BCS theory. This provided a solid theoretical foundation for the GL theory. Chapters 4–14 of the book, Theories of High Temperature Superconductivity (Halley, 1988), discuss applications of the BCS theory. Allen (1990) reviewed the BCS approach to electron pairing. The pairing state in YBa2 Cu3 O7− is discussed by Annett et al. (1990). We will cite some representative articles. The weak and strong limits of BCS have been dis cussed (Carbotte (1990), Cohen, 1987; Cohen and Penn, 1990; Entin-Wohlman and Imry, 1989; Nasu, 1990). There is a crossover between a BCS proper regime of weakly coupled, real space-overlapping Cooper pairs and a Bose–Einstein regime involving a low density boson gas of tightly bound fermion pairs (Pistolesi and Strinati, 1994; Quick et al., 1993; Tokumitu et al., 1993). The BCS theory has been applied to high tem perature superconductors (Berlinsky et al., 1993; Ihm and Yu, 1989; Japiassu et al., 1992; Jarrell et al., 1988; Kitazawa and Tajima, 1990; Lal and Joshi, 1992; Lu et al., 1989; Marsiglio, 1991; Marsiglio and Hirsch, 1991; Penn and Cohen, 1992; Pint and Schachinger, 1991; Sachdev and Wang, 1991). The present chapter, although based in part on the electron–phonon coupling mechanism (Jiang and Carbotte, 1992b; Kirkpatrick and Belitz, 1992; Kresin et al., 1993; Marsiglio and Hirsch, 1994; Nicol and Carbotte, 1993; Zheng et al., 1994), is nevertheless much more general in its formalism. Unconventional phonon or nonphonon coupling can also occur (Annett et al. (1991), Bussmmann-Holder and Bishop, 1991; Cox and Maple, 1995; Dobroliubov and Khlebnikov, 1991; Keller, 1991; Klein and Aharony, 1992; Krüger, 1989; Spathis et al., 1992; Tsay et al., 1991; Van Der Marel, 1990), involving, for example, excitons (Bala and Olés, 1993; Gutfreund and Little, 1979; Takada, 1989), plasmons (quantized plasma oscillations; Côte and Griflin, 1993; Cui and Tsai, 1991; Ishii and Ruvalds, 1993), polaritons (Lue and Sheng, 1993), polarons (elec tron plus induced lattice polarization; Kabanov and Mashtakov, 1993; Konior, 1993; Nettel and MacCrone, 1993; Wood and Cooke, 1992) and bipolarons (de Jongh, 1992; Emin, 1994; Khalfin and Shapiro, 1992). Both s-wave and d-wave pairings have been considered (Anlage et al., 1994; Carbotte and Jiang, 1993; Côte and Griflin, 1993; Lenck and Carbotte, 1994; Li et al., 1993; Scalapino, 1995; Wengner and Östlund, 1993; Won and Maki, 1994). Kasztin and Leggett (1997) discussed the nonlocality of d-wave superconductivity, Prozovov and Giannetta (2006) examined the electrodynamics of unconventional pairing, and Hirsch feld and Golden feld (1993) commented on the effects of impurities. Some authors question the applicability of BCS to high temperature superconductors (Collins et al., 1991; Kurihara, 1989). Tesanovic and Rasolt (1989) suggested a new type of superconductivity in very high magnetic fields in which there is no upper critical field. The BCS theory has been examined in terms of the Hubbard (Falicov and Proetto, 1993; Micnas et al., 1990; Sofo et al., 1992) and Fermi liquid (Horbach et al., 1993, Ramakumar, 1993) approaches, which are discussed in Chapter 10. FURTHER READING Carbotte (1990) reviewed Eliashberg (1960a, b) the ory and its relationship with BCS. Representative arti cles concern (a) high temperature superconductors (Jin et al., 1992; Lu et al., 1989; Marsiglio, 1991; Mon thoux and Pines, 1994; Sulewski et al., 1987; Wermbter and Tewordt, 1991a; Williams and Carbotte, 1991), 193 (b) anisotropies (Combescot, 1991; Lenck et al., 1990; Radtke et al., 1993; Zhao and Callaway, 1994), (c) transport properties (Kulic and Zeyher, 1994; Ullah and Dorsey, 1991), (d) weak coupling limits (Combescot, 1990; Crisan, 1887), and (e) strong coupling limits (Bulaevskii et al., 1988; Heid, 1992 (Pb); Rammer, 1991). This page intentionally left blank 8 Cuprate Crystallographic Structures I. INTRODUCTION Chapter 3 shows that the majority of single-element crystals have highly symmet rical structures, generally fcc or bcc, in which their physical properties are the same along the three crystallographic directions x, y, and z. The NaCl-type and A15 compounds are also cubic. Some compounds do have lower symmetries, showing that supercon ductivity is compatible with many differ ent types of crystallographic structure, but higher symmetries are certainly more com mon. In this chapter we will describe the structures of the high-temperature supercon ductors, almost all which are either tetrago nal or orthorhombic, but close to tetragonal. In Chapter 3, we also gave some exam ples of the role played by structure in determining the properties of superconduc tors. The highest transition temperatures in alloys of transition metals are at the bound aries of instability between the bcc and hcp forms. The NaCl-type compounds have ordered vacancies on one or another lat tice site. The magnetic and superconducting properties of the Chevrel phases depend on whether the large magnetic cations (i.e., pos itive ions) occupy eightfold sites surrounded by chalcogenide ions, or whether the small magnetic ions occupy octahedral sites sur rounded by Mo ions. The structures described here are held together by electrons that form ionic or cova lent bonds between the atoms. No account 195 196 is taken of the conduction electrons, which are delocalized over the copper oxide planes and form the Cooper pairs responsible for the superconducting properties below Tc . The later Chapter 10 will be devoted to explain ing the role of these conduction electrons within the frameworks of the Hubbard model and band theory. Whereas the present chapter describes atom positions in coordinate space, the Hubbard Model/Band Structure chapter relies on a reciprocal lattice elucidation of these same materials. We begin with a description of the per ovskite structure and explain some reasons that perovskite undergoes various types of distortions. This prototype exhibits a num ber of characteristics that are common to the high-temperature superconducting cuprates (see Section V). We will emphasize the structural commonalities of these materi als and make frequent comparisons between them. Our earlier work (Poole et al., 1988) and the comprehensive review by Yvon and François (1989) may be consulted for more structural detail on the atom posi tions, interatomic spacings, site symmetries, etc., of these compounds. There have been reports of superconductivity in certain other cuprate structures (e.g., Murphy et al., 1987), but these will not be reported on in this chapter. There is a related series of layered compounds Bi2 O2 Mm−1 Rm O3m+1 called Aurivillius (1950, 1951, 1952) phases, with the 12-coordinated M = Ca, Sr, Ba, Bi, Pb, Cd, La, Sm, Sc, etc., and the 6-coordinated transition metal R = Nb, Ti, Ta, W, Fe, etc. The m = 1 compound Bi2 NbO6 belongs to the same tetragonal space group I4/mmm D417h as the lanthanum, bismuth, and thallium high temperature superconduc tors (Medvedeva et al., 1993). We assume that all samples are well made and safely stored. Humidity can affect composition, and Garland (1988) found that storage of YBa2 Cu3 O7− in 98% humidity exponentially decreased the diamagnetic sus ceptibility with a time constant of 22 days. 8 CUPRATE CRYSTALLOGRAPHIC STRUCTURES II. PEROVSKITES Much has been written about the high-temperature superconductors being per ovskite types. The prototype compound barium titanate, BaTiO3 , exists in three crystallographic forms with the following lattice constants and unit cell volumes (Wyckoff, 1964): cubic: tetragonal: ortho rhombic: a=b=c= 40118 Å a = b = 39947 c = 40336 √ a = 4009√2 Å b = 4018 2 Å c = 3990 Å 3 V = 6457 Å V = 6437 Å 3 V = 26426 Å (8.1) 3 A. Cubic Form Above 201 C barium titanate is cubic and the unit cell contains one formula unit BaTiO3 with a titanium atom on each apex, a barium atom in the body center, and an oxygen atom on the center of each edge of the cube, as illustrated in Fig. 8.1. This corresponds to the barium atom, titanium atom, and three oxygen atoms being placed Figure 8.1 Barium titanate BaTiO3 perovskite cubic unit cell showing titanium (small black circles) at the vertices and oxygen (large white circles) at the edge-centered positions. Ba, not shown, is at the body center position (Poole et al., 1988, p. 73). 197 II PEROVSKITES in positions with the following x, y, and z coordinates: E site: Ti F site: O C site: Ba 0 0 0 0 0 21 0 21 0 21 0 0 21 21 21 Ti on apex three oxygens centered on edges Ba in center. Table 8.1 Ionic Radii for Selected Elementsa Small Cu2+ Bi5+ 0.72Å 0.74 Å Y3+ 0.89 Å Small-Medium Cu+ Ca2+ Nd3+ 0.96 Å 0.99 Å 0.995 Å Tl3+ Bi3+ 0.95 Å 0.96 Å Medium-Large La3+ Hg2+ 1.06 Å 1.10 Å Sr 2+ 1.12 Å Large Pb2+ K+ Ba2+ 1.20 Å 1.33 Å 1.34 Å Ag+ O2− F− 1.26 Å 1.32 Å 1.33 Å (8.2) The barium in the center has 12 nearestneighbor oxygens, so we say that it is 12-fold coordinated, while the titanium on each apex has 6-fold (octahedral) coordination with the oxygens, as may be seen from the figure. (The notation E for edge, F for face, and C for center is adopted for reasons that will become clear in the discussion which follows.) Throughout this chapter we will assume that the z-axis is oriented vertically, so that the x and y axes lie in the horizon tal plane. Ordinarily, solid-state physics texts place the origin (0, 0, 0) of the perovskite unit cell at the barium site, with titanium in the center and the oxygens at the centers of the cube faces. Our choice of origin facili tates comparison with the structures of the oxide superconductors. This structure is best understood in terms of the sizes of the atoms involved. The ionic radii of O2− (1.32 Å) and Ba2+ (1.34 Å) are almost the same, as indicated in Table 8.1, and together they form a per fect fcc lattice with the smaller Ti4+ ions (0.68 Å) located in octahedral holes sur rounded entirely by oxygens. The octahe dral holes of a close-packed oxygen lattice have a radius of 0.545 Å; if these holes were empty the lattice constant would be a = 373 Å, as noted in Fig. 8.2a. Each tita nium pushes the surrounding oxygens out ward, as shown in Fig. 8.2b, thereby increas ing the lattice constant. When the titanium is replaced by a larger atom, the lattice constant expands further, as indicated by the data in the last column of Table 8.2. When Ba is a See Table VI-2 of Poole et al. (1988) for a more extensive list. Figure 8.2 Cross section of the perovskite unit cell in the z = 0 plane showing (a) the size of the octahedral hole (shaded) between oxygens (large circles), and (b) oxygens pushed apart by the transition ions (small cir cles) in the hole sites. For each case the lattice constant is indicated on the right and the oxygen and hole sizes on the left (Poole et al., 1988, p. 77). 198 8 CUPRATE CRYSTALLOGRAPHIC STRUCTURES Table 8.2 Dependence of the Lattice Constants a of Selected Perovskites AMO3 on the Alkaline Earth A (right) and the Ionic Radius of Transition Metal Ion M (left); the Alkaline Earth Ionic Radii are 0.99 Å (Ca), 1.12 Å (Sr), and 1.34 Å Baa Lattice constant a, Å Transition metal Transition metal radius, Å Ca Sr Ba Ti Fe Mo Sn Zr Pb Ce Th 0.68 — 0.70 0.71 0.79 0.84 0.94 1.02 384 — — 392 402 — 385 437 391 387 398 403 410 — 427 442 401 401 404 412 419 427 440 480 a Data from Wyckoff (Vol. 2, 1964, pp. 391ff). replaced by the smaller Ca (0.99 Å) and Sr (1.12 Å) ions, by contrast, there is a corre sponding decrease in the lattice constant, as indicated by the data in columns 3 and 4, respectively, of Table 8.2. All three alkaline earths, Ca, Sr, and Ba, appear prominently in the structures of the high-temperature superconductors. B. Tetragonal Form At room temperature barium titanate is tetragonal and the deviation from cubic, c − a/ 21 c + a, is about 1%. All of the atoms have the same x, y coordinates as in the cubic case, but are shifted along the z-axis relative to each other by ≈ 01 Å, pro ducing the puckered arrangement shown in Fig. 8.3. The distortions from the ideal struc ture are exaggerated in this sketch. The puck ering bends the Ti–O–Ti group so that the Ti–O distance increases while the Ti–Ti dis tance remains almost the same. This has the effect of providing more room for the tita nium atoms to fit in their lattice sites. We will see later that a similar puckering distortion occurs in the high-temperature superconduc tors as a way of providing space for the Cu atoms in the planes. Figure 8.3 Perovskite tetragonal unit cell showing puckered Ti–O layers that are perfectly flat in the cubic cell of Fig. 8.1. The notation of Fig. 8.1 is used (Poole et al., 1988, p. 75). C. Orthorhombic Form There are two principal ways in which a tetragonal structure distorts to form an orthorhombic phase. The first, shown at the top of Fig. 8.4, is for the b-axis to stretch relative to the a-axis, resulting in the for mation of a rectangle. The second, shown at the bottom of the figure, is for one diago nal of the ab square to stretch and the other diagonal to compress, resulting in the for mation of a rhombus. The two diagonals are perpendicular, rotated by 45 relative to the 199 II PEROVSKITES √ stants are ≈ 2 times longer than the original constants, so that the volume of the unit cell roughly doubles; thus, it contains √ exactly twice as many atoms. (The same 2 factor appears in Eq. 8.1 in our discussion of the lattice constants for the orthorhombic form of barium titanate.) When barium titanate is cooled below 5 C it undergoes a diagonal- or rhombal type distortion. The atoms have the same z coordinates (z = 0 or 21 ) as in the cubic phase, so the distortion occurs entirely in the x y-plane, with no puckering of the atoms. The deviation from tetragonality, as given by the percentage of anisotropy, Figure 8.4 Rectangular- (top) and rhombal- (bottom) type distortions of a two-dimensional square unit cell of width a (Poole et al., 1989). % ANIS = 100b − a = 022% 1 b + a 2 (8.3) is less than that of most orthorhombic copper oxide superconductors. We see from Fig. 8.5 that in the cubic phase the oxygen atoms in the z = 0 plane are separated by 0.19 Å. The rhombal distortion increases this O–O sepa ration in one direction and decreases it in the other, in the manner indicated in Fig. 8.6a, to produce the Ti nearest-neighbor configu ration shown in Fig. 8.6b. This arrangement helps to fit the titanium into its lattice site. The transformation from tetragonal to orthorhombic is generally of the rhombal type for La1−x Sr x 2 CuO4 and of the recti linear type for YBa2 Cu3 O7− . D. Planar Representation Figure 8.5 Rhombal expansion of monomolecular tetragonal unit cell (small squares, lower right) to bimolecular orthorhombic unit cell (large squares) with new axes 45 relative to the old axes. The atom posi tions are shown for the z = 0 and z = 21 layers (Poole et al., 1988, p. 76). original axes, and become the a b dimen sions of the new orthorhombic unit cell, as shown in Fig. 8.5. These a b lattice con Another way of picturing the structure of perovskite is to think of the atoms as forming horizontal planes. If we adopt the notation [E F C] to designate the occupation of the E, F, and C sites, the sketches of per ovskite presented in Figs. 8.1 and 8.3 follow the scheme z=1 z = 21 z=0 TiO2 – O–Ba TiO2 – Ti at E, O at two F sites O at E, Ba at C Ti at E, O at two F sites (8.4) 200 8 CUPRATE CRYSTALLOGRAPHIC STRUCTURES III. PEROVSKITE-TYPE SUPERCON DUCTING STRUCTURES Figure 8.6 Shift of the oxygens (large circles) in the a, b-plane around the titanium atom (small circle) of perovskite from the room-temperature tetragonal (and cubic) configuration (a) to the rhombal configuration (b) of its low-temperature orthorhombic structure. The planes at the heights z = 0 21 , and 1 can be labeled using this notation. The usefulness of this labeling scheme will be clarified in Section V. This completes our treatment of the structure of perovskite. We encountered many features that we will meet again in the analogous superconductor cases, and we established notation that will be useful in describing the structure of the cuprates. In Section V of Chapter 9 we will discuss several cubic and close-to-cubic perovskite superconducting compounds. In their first report on high-temperature superconductors Bednorz and Müller (1986) referred to their samples as “metallic, perovskite-like mixedoxygen-deficient valence copper compounds.” Subse quent work has confirmed that the new superconductors do indeed possess these characteristics. In the oxide superconductors Cu2+ replaces the Ti4+ of perovskite, and in most cases the TiO2 -perovskite layering is retained as CuO2 layers, which is common to all of the high-temperature superconductors; such superconductors exhibit a uniform lattice size in the a b-plane, as the data in Table 8.3 demonstrate. The compound BaCuO3 does not occur because the Cu4+ ion does not form, but this valence constraint is overcome by replace ment of Ba2+ by a trivalent ion, such as La3+ or Y3+ , by a reduction in the oxygen content, or by both. The result is a set of “layers” con taining only one oxygen per cation located between each pair of CuO2 layers, or none at all. Each high-temperature superconductor has a unique sequence of layers. We saw from Eq. (8.2) that each atom in perovskite is located in one of three types of sites. In like manner, each atom at the height z in a high-temperature superconduc tor occupies either an Edge (E) site on the edge (0, 0, z), a Face (F) site on the mid line of a face (0 21 z or 21 0 z or both), or a Centered (C) site centered within the unit cell on the z-axis 21 21 z. The site occupancy notation [E F C] is used because many cuprates contain a succession of Cu O2 – and – O2 Cu layers in which the Cu atom switches between edge and cen tered sites, with the oxygens remaining at their face positions. Similar alternations in position take place with Ba, O, and Ca layers, as illustrated in Fig. 8.7. Hauck et al. (1991) proposed a classi fication of superconducting oxide structures Table 8.3 Crystallographic Characteristics of Oxide Superconducting and Related Compoundsa Compound Code Symm Type Enlarg. Form. Units Å a0 Å Å c0 Å c0 /Cu % Anis Tc K Comments BaTiO3 BaTiO3 BaTiO3 BaPbO3 BaPb07 Bi03 O3 BaBiO3 Ba06 K04 BiO3 La2 CuO4 La2 CuO4 YBa2 Cu3 O6 YBa2 Cu3 O8 Bi2 Sr2 CaCu2 O8 Bi2 Sr2 Ca2 Cu3 O10 Tl2 Ba2 CuO6 Tl2 Ba2 CaCu2 O8 Tl2 Ba2 Ca2 Cu3 O10 TlBa2 CuO5 TlBa2 CaCu2 O7 TlBa2 Ca2 Cu3 O9 TlBa2 Ca3 Cu4 O11 TlBa2 Ca4 Cu5 O13 HgBa2 CuO4 HgBa2 CaCu2 O6 HgBa2 Ca2 Cu3 O8 — — — — — — — 0201 0201 0212 0212 2212 2223 2201 2212 2223 1201b 1212 1223c 1234 1245 1201 1212 1223 C T O C T M C T O T O O O T T T T T T T T T T T A A A A S A A S S A A S S S S S A A A A A A A A 1 1√ 2 1√ √2 2 1 1√ 2 1 1√ 5√2 5 2 1 1 1 1 1 1 1 1 1 1 1 1 1 2 1 4 2 1 2 4 1 1 20 20 2 2 2 1 1 1 1 1 1 1 1 4.012 3.995√ 4013 2 4.273√ 4286√2 4355 2 4.293 3.81 √ 3960 2 3.902 3.855√ 381√2 383 2 3.83 3.85 3.85 3.85 3.85 3.81 3.85 3.85 3.86 3.86 3.86 4012 403 3990 4273 4304 4335 4293 1318 1318 1194 1168 306 37 2324 294 3588 909 127 152 190 223 95 126 177 — — — — — — — 659 659 398 389 765 617 116 735 598 909 635 51 475 442 95 63 52 0 0 0.23 0 0 0.13 0 0 6.85 0 1.43 0 0.57 0 0 0 0 0 0 — — — 04 12 — 30 35 35 — 92 84 110 90 110 125 52 80 120 114 101 95 122 133 T > 200 C 20 C T < 5 C a b 201 c 0 0 0 = 9017 Sr, doped Sr, doped Code symmetry (cubic C, tetragonal T, orthorhombic O, monclinic M); type (aligned A, staggered S); enlargement in a, b-plane (diagona √ distortion 2, superlattice 5); formula units per unit cell; lattice parameters (a0 c0 , the single layer compound, and c0 per Cu ion); % anisotropy; and transition temperature Tc . For the orthorhombic compounds tabulated values of a0 are averages of a0 and b0 . The single layer compound Bi2 Sr2 CuO6 does not superconduct. 40% of Ba replaced by La; 50% of Tl replaced by Pb. 202 8 CUPRATE CRYSTALLOGRAPHIC STRUCTURES Figure 8.8 Unit cell of YBa2 Cu3 O7 showing the molecular groupings, reflection plane, and layer types. Figure 8.7 Types of atom positions in the layers of a high-temperature superconductor structure, using the edge, face, center notation [E F C]. Typical site occu pancies are given in the upper right (Poole et al., 1989). in terms of the sequence (a) superconducting layers Cu O2 – and – O2 Cu , (b) insulating layers, such as [Y – –] or [– – Ca], and (c) holedonating layers, such as Cu Ob – or [Bi – O]. The high-temperature superconductor compounds have a horizontal reflection plane (⊥ to z) called h at the center of the unit cell and another h reflection plane at the top (and bottom). This means that every plane of atoms in the lower half of the cell at the height z is duplicated in the upper half at the height 1 − z. Such atoms, of course, appear twice in the unit cell, while atoms right on the symmetry planes only occur once since they cannot be reflected. Figure 8.8 shows a Cu O2 – plane at a height z reflected to the height 1 − z. Note how the puckering preserves the reflection symme try operation. Superconductors that have this reflection plane, but lack end-centering and body-centering operations (see Section VII), are called aligned because all of their cop per atoms are of one type; either all on the edge (0, 0, z) in E positions or all centered 21 21 z at C sites. In other words, they all lie one above the other on the same vertical lines, as do the Cu ions in Fig. 8.8. IV. ALIGNED YBa2 Cu3 O7 The compound YBa2 Cu3 O7 , sometimes called YBaCuO or the 123 compound, in its orthorhombic form is a superconduc tor below the transition temperature Tc ≈ 92 K. Figure 8.8 sketches the locations of the atoms, Fig. 8.9 shows the arrangement of the copper oxide planes, Fig. 8.10 provides more details on the unit cell, and Table 8.4 lists the atom positions and unit cell dimensions (Beno et al., 1987; Capponi et al., 1987; Hazen et al., 1987; Jorgensen et al., 1987; Le Page et al., 1987; Siegrist et al., 1987; Yan and Blanchin, 1991; see also Schuller et al., 1987). Considered as a per ovskite derivative, it can be looked upon as a stacking of three perovskite units BaCuO3 YCuO2 , and BaCuO2 , two of them with a missing oxygen, and this explains why IV ALIGNED YBa2 Cu3 O7 Figure 8.9 Layering scheme of orthorhombic YBa2 Cu3 O7 with the puckering indicated. The layers are perpendicular to the c-axis (Poole et al., 1988, p. 101). Figure 8.10 Sketches of the superconducting orthorhombic (left) and nonsuperconducting tetragonal (right) YBaCuO unit cells. Thermal vibra tion ellipsoids are shown for the atoms. In the tetragonal form the oxygen atoms are randomly dispersed over the basal plane sites (Jorgensen et al., 1987a, b; also see Schuller et al., 1987). 203 204 8 CUPRATE CRYSTALLOGRAPHIC STRUCTURES Table 8.4 Normalized Atom Positions in the YBa2 Cu3 O7 Orthorhombic Unit Cell (dimensions a = 383 Å, b = 388 Å, and c = 1168 Å) Layer Atom x y z Cu O – Cu(1) O(1) 0 0 0 1 1 O – Ba O(4) Ba 0 0 1 2 1 2 Cu(2) O(3) O(2) 0 0 0 Cu O2 – 0 – – Y Y 1 2 1 2 0 Cu O2 – O(2) O(3) Cu(2) 1 2 1 2 1 2 0.6445 0.6219 0.6210 0.3790 0.3781 0.3555 0 0 1 2 1 2 1 2 0 1 2 1 2 O – Ba Ba O(4) 0 0 Cu O – O(1) Cu(1) 0 0 0 1 2 0.8432 0.8146 B. Copper Coordination Now that we have described the planar structure of YBaCuO it will be instructive to examine the local environment of each copper ion. The chain copper ion Cu(1) is square planar-coordinated and the two cop pers Cu(2) and Cu(3) in the plane exhibit fivefold pyramidal coordination, as indicated in Fig. 8.11. The ellipsoids at the atom posi tions of Fig. 8.10 provide a measure of 0.1854 0.1568 0 0 c ≈ 3a. It is, however, more useful to dis cuss the compound from the viewpoint of its planar structure. A. Copper Oxide Planes We see from Fig. 8.9 that three planes con taining Cu and O are sandwiched between two planes containing Ba and O and one plane con taining Y. The layering scheme is given on the right side of Fig. 8.8, where the superscript b on O indicates that the oxygen lies along the b-axis, as shown. The atoms are puck ered in the two Cu O2 – planes that have the [– – Y] plane between them. The third cop per oxide plane Cu Ob – , often referred to as “the chains,” consists of –Cu–O–Cu–O– chains along the b axis in lines that are per fectly straight because they are in a horizon tal reflection plane h ; where no puckering can occur. Note that, according to the figures, the copper atoms are all stacked one above the other on edge (E) sites, as expected for an aligned-type superconductor. Both the copper oxide planes and the chains contribute to the superconducting properties. Figure 8.11 Stacking of pyramid, square-planar, and inverted pyramid groups along the c-axis of orthorhom bic YBa2 Cu3 O7 (adapted from Poole et al., 1988, p. 100). Minor adjustments to make more room can be brought about by puckering or by distorting from tetragonal to orthorhombic. 205 IV ALIGNED YBa2 Cu3 O7 the thermal vibrational motion which the atoms experience, since the amplitudes of the atomic vibrations are indicated by the rela tive size of each of the ellipsoids. C. Stacking Rules The atoms arrange themselves in the various planes in such a way as to enable them to stack one above the other in an effi cient manner, with very little interference from neighboring atoms. Steric effects pre vent large atoms such as Ba (1.34 Å) and O (1.32 Å) from overcrowding a layer or from aligning directly on top of each other in adjacent layers. In many cuprates stacking occurs in accordance with the following two empirical rules: 1. Metal ions occupy either edge or cen tered sites, and in adjacent layers alternate between E and C sites. 2. Oxygens are found in any type of site, but they occupy only one type in a particular layer, and in adjacent layers they are on different types of sites. occupying the vacant sites along a. Superlat tice ordering of the chains is responsible for the phase that goes superconducting at 60 K. YBaCuO is prepared by heating in the 750–900 C range in the presence of various concentrations of oxygen. The compound is tetragonal at the highest temperatures, increases its oxygen content through oxy gen uptake and diffusion (Rothman et al., 1991) as the temperature is lowered, and undergoes a second-order phase transition of the order-disorder type at about 700 C to the low-temperature orthorhombic phase, as indicated in Fig. 8.12 (Jorgensen et al., 1987, 1990; Schuller et al., 1987; cf. Beyers and Ahn, 1991; Metzger et al., 1993; Fig. 8). Quenching by rapid cooling from a high temperature can produce at room temper ature the tetragonal phase sketched on the right side of Fig. 8.10, and slow anneal ing favors the orthorhombic phase on the Minor adjustments to make more room can be brought about by puckering or by distort ing from tetragonal to orthorhombic. D. Crystallographic Phases The YBa2 Cu3 O7− compound comes in tetragonal and orthorhombic varieties, as shown in Fig. 8.10, and it is the latter phase which is ordinarily superconducting. In the tetragonal phase the oxygen sites in the chain layer are about half occupied in a random or disordered manner, and in the orthorhombic phase they are ordered into –Cu–O– chains along the b direction. The oxygen vacancy along the a direction causes the unit cell to compress slightly so that a < b, and the resulting distortion is of the rectangular type shown in Fig. 8.4a. Increasing the oxygen content so that < 0 causes oxygens to begin � 0 0 (bottom) and 0 (top) sites (scale on left), and the oxygen content parameter (center, curve scale on right) for quench temperatures of YBaCuO in the range 0–1000 C. The parameter curve is the average of the two site-occupancy curves (adapted from Jorgensen et al., 1987a; also see Schuller et al., 1987; see also Poole et al., 1988). Figure 8.12 � Fractional occupancies of the � 1 0 2 �1 2 206 8 CUPRATE CRYSTALLOGRAPHIC STRUCTURES left. Figure 8.12 shows the fractional site occupancy of the oxygens in the chain site 0 21 0 as a function of the temperature in an oxygen atmosphere. A sample stored under sealed conditions exhibited no degra dation in structure or change in Tc four years later (Sequeira et al., 1992). Ultra-thin films tend to be tetragonal (Streiffer et al., 1991). E. Charge Distribution Information on the charge distribution around atoms in conductors can be obtained from a knowledge of their energy bands (see description in Chapter 10). This is most eas ily accomplished by carrying out a Fouriertype mathematical transformation between the reciprocal ks ky kz -space (Chapter 8, Section II of the first edition) in which the energy bands are plotted and the coordi nate x y z-space, where the charge is dis tributed. We will present the results obtained for YBa2 Cu3 O7 in the three vertical symme try planes (x z, and y z, and diagonal), all containing the z-axis through the origin, shown shaded in the unit cell of Fig. 8.13. Contour plots of the charge density of the valence electrons in these planes are sketched in Fig. 8.14. The high density at the Y3+ and Ba2+ sites and the lack of contours around these sites together indicate that these atoms are almost completely ionized, with charges of +3 and +2, respectively. It also shows that these ions are decoupled from the planes above and below. This accounts for the magnetic isolation for the Y site whereby magnetic ions substituted for yttrium do not interfere with the superconducting proper ties. In contrast, the contours surrounding the Cu and O ions are not characteristic of an ordinary ionic compound. The short Cu–O bonds in the planes and chains (1.93–1.96 Å) increase the charge overlap. The least overlap appears in the Cu(2)–O(4) vertical bridging bond, which is also fairly long (2.29 Å). The Cu, O charge contours can be represented by a model that assigns charges of +162 Figure 8.13 Three vertical crystallographic planes (x, z-, and y, z-, and diagonal) of a tetragonal unit cell of YBa2 Cu3 O7 , and standard notation for the four crys tallographic directions. Figure 8.14 Charge density in the three symmetry planes of YBaCuO shown shaded in Fig. 8.13. The x, z, diagonal and the y, z planes are shown from left to right, labeled 100 110 , and 010 , respectively. These results are obtained from bandstructure calculations, as will be explained in the following chapter (Krakauer and Pickett, 1988). IV ALIGNED YBa2 Cu3 O7 207 and −169 to Cu and O, respectively, rather than the values of +233 and −200 expected for a standard ionic model, where the charge +233 is an average of +2 +2, and +3 for the three copper ions. Thus the Cu–O bonds are not completely ionic, but partly covalent. F. YBaCuO Formula In early work the formula YBa2 Cu3 O9− was used for YBaCuO because the proto type triple pervoskite YCuO3 BaCuO3 2 has nine oxygens. Then crystallographers showed that there are eight oxygen sites in the 14-atom YBaCuO unit cell, and the for mula YBa2 Cu3 O8− came into widespread use. Finally, structure refinements demon strated that one of the oxygen sites is sys tematically vacant in the chain layers, so the more appropriate expression YBa2 Cu3 O7− was introduced. It would be preferable to make one more change and use the formula Ba2 YCu3 O7− to emphasize that Y is analo gous to Ca in the bismuth and thallium com pounds, but very few workers in the field do this, so we reluctantly adopt the usual “final” notation. In the Bi–Tl compound notation of Section VIII, B, Ba2 YCu3 O7− would be called a 0213 compound. We will follow the usual practice of referring to YBa2 Cu3 O7− as the 123 compound. G. YBa2 Cu4 O8 and Y2 Ba4 Cu7 O15 These two superconductors are some times referred to as the 124 compound and the 247 compound, respectively. They have the property that for each atom at position x y z there is another identical atom at position x y + 21 z + 21 . In other words, the structure is side centered. This property prevents the stacking rules of Section C from applying. Figure 8.15 Crystal structure of YBa2 Cu4 O8 show ing how, as a result of the side-centering symmetry oper ation, the atoms in adjacent Cu–O chains are staggered along the y direction, with Cu above O and O above Cu (Heyen et al., 1991; modified from Campuzano et al., 1990). The chain layer of YBa2 Cu3 O7 becomes two adjacent chain layers in YBa2 Cu4 O8 , with the Cu atoms of one chain located directly above or below the O atoms of the other, as shown in Fig. 8.15 (Campuzano et al., 1990; Heyen et al., 1990a, 1991; Iqbal, 1992; Kaldis et al., 1989; Marsh et al., 1988; Morris et al., 1989a). The transition temper ature remains in the range from 40 K to 80 K when Y is replaced by various rare earths (Morris et al., 1989). The double chains do not exhibit the variable oxygen stoichiometry of the single ones. The other side-centered compound, Y2 Ba4 Cu7 O15 , may be considered according to Torardi, “as an ordered 1:1 inter-growth of the 123 and 124 compounds YBa2 Cu3 O7 +YBa2 Cu4 O8 = Y2 Ba4 Cu7 O15 ” (Bordel et al., 1988, Gupta and Gupta, 1993). The 123 single chains can vary in their oxygen content, and superconductiv ity onsets up to 90 K have been observed. 208 8 CUPRATE CRYSTALLOGRAPHIC STRUCTURES This compound has been synthesized with several rare earths substituted for Y (Morris et al., 1989b). V. ALIGNED HgBaCaCuO The series of compounds HgBa2 Can Cun+1 O2n+4 where n is an integer, are prototypes for the Hg family of superconductors. The first three members of the family, with n = 0 1 2, are often referred to as Hg– 1201, Hg–1212, and Hg–1223, respectively. They have the structures sketched in Fig. 8.16 (Tokiwa-Yamamoto et al., 1993; see also Martin et al., 1994; Putilin et al., 1991). The lattice constants are a = 386 Å for all of them, and c = 95, 12.6, and 15.7 Å for n = 0 1 2, respectively. The atom positions of the n = 1 compound are listed in Table 8.5 (Hur et al., 1994). The figure is drawn with mercury located in the middle layer of the unit cell, while the table puts Hg at the origin (000) and Ca in the middle 21 21 21 . Figure 8.17 presents the unit cell for the n = 1 compound HgBa2 CaCu2 O6+ drawn with Ca in the mid dle (Meng et al., 1993a). The symbol rep resents a small excess of oxygen located in the center of the top and bottom layers, at positions 21 21 0 and 21 21 1 which are labeled “partial occupancy” in the figure. If this oxy gen were included the level symbol would be [Hg – O] instead of [Hg – –]. These Hg com pound structures are similar to those of the series TlBa2 Can Cun+1 O2n+4 mentioned above in Section VIII.F. We see from Fig. 8.16 that the cop per atom of Hg–1201 is in the center of a stretched octahedron with the planar oxygens O(1) at a distance of 1.94 Å, and the apical oxygens O(2) of the [O – Ba] layer much further away (2.78 Å). For n = 1 each copper atom is in the center of the base of a tetragonal pyramid, and for n = 2 the additional CuO2 layer has Cu atoms which Figure 8.16 Structural models for the series HgBa2 Can Cun+1 O2n+4 . The first three members with n = 0 1 2 are shown (parts a, b, and c, respectively) (Tokiwa-Yamamoto et al., 1993). 209 V ALIGNED HgBaCaCuO Table 8.5 Normalized Atom Positions in the Tetragonal Unit Cell of HgBa2 Ca086 Sr014 Cu2 O6 + a Layer Atom x y z Hg – – Hg O(3) 0 0 1 1 O – Ba O(2) Ba 0 0 0.843 0.778 Cu O(1) O(1) 0 0 0 Cu O2 – 0 – – Ca Ca, Sr 1 2 1 2 0 Cu O2 – O(1) O(1) Cu 1 2 1 2 1 2 0.621 0.627 0.627 0.373 0.373 0.379 O – Ba Ba O(2) 1 2 1 2 0 0 Hg – – O(3) Hg 1 2 1 2 0 0 a 1 2 1 2 0 0 1 2 1 2 1 2 1 2 0 0.222 0.157 0 0 Unit cell dimensions a = 38584 Å and c = 126646 Å, space group is P4/mmm, D41 h . The Hg site is 91% occupied and the O(3) site is 11% occupied = 011. The data are from Hur et al. (1994). Figure 8.17 Schematic structure of the HgBa2 CaCu2 O6+ compound which is also called Hg–1212 (Meng et al., 1993a). are square planar coordinated. The layer ing scheme stacking rules of Section IV.C are obeyed by the Hg series of compounds, with metal ions in adjacent layers alternat ing between edge (E) and centered (C) sites, and oxygen in adjacent layers always at dif ferent sites. We see from Table 8.5 that the [O – Ba] layer is strongly puckered and the Cu O2 – layer is only slightly puckered. The relationships between the layering scheme of the HgBa2 Can Cun+1 O2n+4 series of compounds and those of the other cuprates may be seen by comparing the sketch of Fig. 8.18 with that of Fig. 8.29. We see that the n = 1 compound HgBa2 CaCu2 O6 is quite similar in structure to YBa2 Cu3 O7 with Ca replacing the chains [Cu O –]. More surpris ing is the similarity between the arrangement of the atoms in the unit cell of each compound and the arrangement of the atoms in the semi-unit cell of the corresponding HgBa2 Can Cun+1 O2n+4 Tl2 Ba2 Can Cun+1 O2n+6 Figure 8.18 Layering schemes of three HgBa2 Can Cun+1 O2n+4 compounds, using the notation of Fig. 8.29. 210 8 CUPRATE CRYSTALLOGRAPHIC STRUCTURES compound. They are the same except for the replacement of the [Tl – O] layer by [Hg – –], and the fact that the thallium compounds are body centered and the Hg ones are aligned. Supercells involving polytypes with ordered stacking sequences of different phases, such as Hg–1212 and Hg–1223, along the c direction have been reported. The stoichiometry is often Hg2 Ba4 Ca3 Cu5 Ox corresponding to equal numbers of the Hg– 1212 and Hg–1223 phases (Phillips, 1993; Schilling et al., 1993, 1994). Detailed structural data have already been reported on various Hg family com pounds such as HgBa2 CuO4+ (Putlin et al., 1993) and the n = 1 compound with partial Eu substitution for Ca (Putlin et al., 1991). The compound Pb07 Hg03 Sr2 Nd03 Ca07 Cu3 O7 has Hg in the position (0.065, 0, 0), slightly displaced from the origin of the unit cell (Martin et al., 1994). Several researchers have reported synthesis and pre treatment procedures (Adachi et al., 1993; Itoh et al., 1993; Isawa 1994a; Meng, 1993b; Paranthaman, 1994; Paranthaman et al., 1993). Lead doping for Hg has been used to improve the superconducting properties (Iqbal et al., 1994; Isawa et al., 1993; Martin et al., 1994). VI. BODY CENTERING In Section V we discussed alignedtype superconductor structures that possess a horizontal plane of symmetry. Most hightemperature superconductor structures have, besides this h plane, an additional symme try operation called body centering whereby for every atom with coordinates x y z there is an identical atom with coordinates as determined from the following operation: 1 x → x± 2 1 y→± 2 z → z± 1 2 (8.5) Starting with a plane at the height z this oper ation forms what is called an image plane at the height z ± 21 in which the edge atoms become centered, the centered atoms become edge types, and each face atom moves to another face site. In other words, the bodycentering operation acting on a plane at the height z forms a body centered plane, also called an image plane, at the height z ± 21 . The signs in these operations are selected so that the generated points and planes remain within the unit cell. Thus if the initial value of z is greater than 21 , the minus sign must be selected, viz., z → z − 21 . Body centering causes half of the Cu–O planes to be Cu O2 – , with the copper atoms at edge sites, and the other half to be – O2 Cu , with the copper atoms at centered sites. Let us illustrate the symmetry features of a body-centered superconductor by consid ering the example of Tl2 Ba2 CaCu2 O8 . This compound has an initial plane Cu O2 – with the copper and oxygen atoms at the verti cal positions z = 00540 and 0.0531, respec tively, as shown in Fig. 8.19. For illustrative purposes the figure is drawn for values of z closer to 0.1. We see from the figure that there is a reflected plane Cu O2 – at the height 1 − z, an image (i.e., body centered) plane – O2 Cu of the original plane at the height 21 + z, and an image plane – O2 Cu of the reflected plane (i.e., a reflected and body centered plane) at the height 21 − z. Figure 8.19 illustrates this situation and indi cates how the atoms of the initial plane can be transformed into particular atoms in other planes (see Problem 5). Figure 8.20 shows how the configurations of the atoms in onequarter of the unit cell, called the basic subcell, or subcell I, determine their config uratinon in the other three subcells II, III, 211 VII BODY-CENTERED La2 CuO4 Nd2 CuO4 AND Sr2 RuO4 Figure 8.20 Body-centered unit cell divided into four regions by the reflection and body centering operations. Figure 8.19 Body-centered tetragonal unit cell con taining four puckered CuO2 groups showing how the initial group (bottom) is replicated � � by reflection in the horizontal reflection plane z = 21 , by the body center ing operation, and by both. and IV throught the symmetry operations of reflection and body centering. VII. BODY-CENTERED La2 CuO4 Nd2 CuO4 AND Sr2 RuO4 The body-centered compound M2 CuO4 has three structural variations in the same crystallographic space group, namely the M = La and M = Nd types, and a third mixed variety (Xiao et al., 1989). Table 8.5 lists the atom positions of the first two types, and Fig. 8.21 presents sketches of the structures of all three. The compound Sr2 RuO4 is iso morphic with La2 CuO4 . Each of these cases will be discussed in turn. A. Unit Cell of La2 CuO4 Compound (T Phase) The structure of the more common La2 CuO4 variety, often called the T phase, can be pictured as a stacking of CuO4 La2 groups alternately with image (i.e., body cen tered) La2 O4 Cu groups along the c direction, as indicated on the left side of Fig. 8.21. (Cavaet et al., 1987; Kinoshita et al., 1992; Longo and Raccah, 1973; Ohbayashi et al., 1987; Onoda et al., 1987; Zolliker et al., 1990). Another way of visualizing the struc ture is by generating it from the group Cu05 O2 La, comprising the layers [O–La] and 1 Cu O2 – in subcell I shown on the right 2 side of Fig. 8.22 and also on the left side of 212 8 CUPRATE CRYSTALLOGRAPHIC STRUCTURES Figure 8.21 (a) Regular unit cell (T phase) associated with hole=type La1−x Sr x 2 CuO4 superconductors, (b) hybrid unit cell (T∗ phase) of the hole-type La2−x−y Ry Sr x CuO4 superconductors, and (c) alternate unit cell (T phase) associated with electron-type Nd1−x Cex 2 CuO4 superconductors. The La atoms in the left structure become Nd atoms in the right structure. The upper part of the hybrid cell is T type, and the bottom is T . The crystallographic space group I4/mmm is the same for all three unit cells (Xiao et al., 1989; see also Oguchi, 1987; Ohbayashi et al., 1987; Poole et al., 1988, p. 83; Tan et al., 1990). Fig. 8.23. (The factor 21 appears here because the Cu O2 – layer is shared by two subcells.) Subcell II is formed by reflection from subcell I, and subcells III and IV are formed from I and II via the body-centering oper ation in the manner of Figs. 8.19 and 8.20. Therefore, subcells I and II together con tain the group CuO4 La2 , and subcells III and IV together contain its image (body cen tered) counterpart group La2 O4 Cu. The BiSrCaCuO and TlBaCaCuO structures to be dis cussed in Section VIII can be generated in the same manner, but with much larger repeat units along the c direction. B. Layering Scheme The La2 CuO4 layering scheme consists of equally-spaced, flat CuO2 layers with their oxygens stacked one above the other, the copper ions alternating between the (0, 0, � � 0) and 21 21 21 sites in adjacent layers, as shown in Fig. 8.24. These planes are body-centered images of each other, and are perfectly flat because they are reflection planes. Half of the oxygens, O(1), are in the planes, and the other half, O(2), between the planes. The copper is octahedrally coordi nated with oxygen, but the distance 1.9 Å from Cu to O(1) in the CuO2 planes is much leess than the vertical distance of 2.4 Å from Cu to the apical oxygen O(2), as indicated in Fig. 8.25. The La is ninefold coordinated to� � four O(1) oxygens, to four O(2) at 21 21 z sites, and to one O(2) at a (0, 0, z) site. C. Charge Distribution Figure 8.26 shows contours of constantvalence charge density on a logarithmic scale drawn on the back x, z-plane and on the diagonal plane of the unit cell sketched in Fig. 8.13. These contour plots are obtained from the band structure calcula tions described in Chapter 10, Section XIV of the first edition. The high-charge density at the lanthanum site and the low charge den sity around this site indicate an ionic state La3+ . The charge density changes in a fairly 213 VII BODY-CENTERED La2 CuO4 Nd2 CuO4 AND Sr2 RuO4 Figure 8.22 Structure of La2 CuO4 (center), showing the formula units (left) and the level labels and subcell types (right). Two choices of unit cell are indicated, the left-side type unit cell based on formula units, and the more common right-side type unit cell based on copper-oxide layers. regular manner around the copper and oxy gen atoms, both within the CuO2 planes and perpendicular to these planes, suggestive of covalency in the Cu–O bonding, as is the case with the YBa2 Cu3 O7 compound. D. Superconducting Structures The compound La2 CuO4 is itself an anti ferromagnetic insulator and must be doped, generally with an alkaline earth, to exhibit pronounced superconducting properties. The compound La1−x Mx 2 CuO4 , with 3% to 15% of M = Sr or Ba replacing La, are orthorhombic at low temperatures and low M contents and are tetragonal otherwise; super conductivity has been found on both sides of this transition. The orthorhombic distortion can be of the rectangular or of the rhombal type, both of which are sketched in Fig. 8.4. The phase diagram of Fig. 8.27 shows the tetragonal, orthorhombic, superconducting, and antiferromagnetically ordered regions for the lanthanum compound (Weber et al., 1989; cf. Goodenough et al., 1993). We see that the orthorhombic phase is insulating at high temperatures, metallic at low tem peratures, and superconducting at very low temperatures. Spin-density waves, to be dis cussed in Chapter 10, Section IX, occur in the antiferromagnetic region. E. Nd2 CuO4 Compound (T Phase) The rarer Nd2 CuO4 structure (Skantakumar et al., 1989; Sulewski et al., 214 8 CUPRATE CRYSTALLOGRAPHIC STRUCTURES Figure 8.23 Layering schemes of the La2 CuO4 (T, left) and Nd2 CuO4 (T , right) structures. The locations of the four subcells of the unit cell are indicated in the center column. 1990; Tan et al., 1990) given on the right side of Fig. 8.21 and Table 8.6 has all of its atoms in the same positions as the standard Figure 8.24 La2 CuO4 structure, except for the apical O(2) oxygens in the [O–La] and [La–O] layers, which move to form a – O2 – layer between [– – La] and [La – –]. These oxygens, now called O(3), have the same x y coordinate positions as the O(1) oxygens, and are located exactly between the CuO2 planes with z = 41 or 43 . We see from Fig. 8.21 that the CuO6 octahedra have now lost their apical oxygens, causing Cu to become square planar-coordinated CuO4 groups. The Nd is eightfold coordinated to four O(1) and four O(3) atoms, but with slightly different Nd–O distances. The CuO2 planes, however, are identical in the two structures. Superconductors with this Nd2 CuO4 structure are of the electron type, in contrast to other hightemperature superconductors, in which the current carriers are holes. In particular, the electron superconductor Nd185 Ce015 CuO4− with Tc = 24 K has been widely studied (Fontcuberta and Fàbrega, 1995, a review CuO2 layers of the La2 CuO4 structure showing horizontal displacement of Cu atoms (black dots) in alternate layers. The layers are perpendicular to the c-axis (Poole et al., 1988, p. 87). 215 VII BODY-CENTERED La2 CuO4 Nd2 CuO4 AND Sr2 RuO4 Figure 8.27 Phase diagram for hole-type La2−x Srx CuO4−y indicating insulating (INS), antifer romagnetic (AF), and superconducting (SC) regions. Figure VI-6 of Poole et al. (1988) shows experimental data along the orthorhombic-to-tetragonal transition line. Spin-density waves (SDW) are found in the AF region (Weber et al., 1989). Figure 8.25 Ordering of axially distorted CuO6 octa hedra in La2 CuO4 (Poole et al., 1988, p. 88). Figure 8.26 Contour plots of the charge density of La2 CuO4 obtained from band structure calculations. The x z-crystallographic plane labeled 100 is shown on the left, and the diagonal plane labeled 110 appears on the right. The contour spacing is on a logarithmic scale (Pickett, 1989). chapter; Allen 1990; Alp et al., 1989b; Barlingay et al., 1990; Ekino and Akimitsu, 1989a, b; Lederman et al., 1991; Luke et al., 1990; Lynn et al., 1990; Sugiyama et al., 1991: Tarason et al., 1989a). Other rare earths, such as Pr (Lee et al., 1990) and Sm (Almasan et al., 1992) have replaced Nd. The difference of structures associated with different signs attached to the current carriers may be understood in terms of the doping process that converts undoped mate rial into a superconductor. Lanthanum and neodymium are both trivalent, and in the undoped compounds they each contribute three electrons to the nearby oxygens, La → La3+ + 3e− Nd → Nd3+ + 3e− (8.6) 216 8 CUPRATE CRYSTALLOGRAPHIC STRUCTURES Table 8.6 Atom Positions in the La2 CuO4 and Nd2 CuO4 Structures La2 CuO4 structure Layer Cu O2 – La – O La – O Atom x O(1) Cu O(1) 1 2 0 0 La 1 2 1 2 1 2 O(2) 0 0 La – O O – La Cu O2 – y 0 0 z Layer Atom x y z 1 2 0 0 1 1 1 1 1 1 Cu O2 – O(1) Cu O(1) 0 0 0.862 [– – Nd] Nd 1 2 – O2 – O(3) O(3) 0 1 2 0 3 4 3 4 [Nd – –] Nd 0 0 0.638 O(1) 0 Cu 1 2 1 2 O(1) 0 1 2 1 2 1 2 1 2 1 2 [Nd – –] Nd 0 0 0.362 1 2 0 1 4 1 4 0.818 1 2 1 2 0 0 0 Cu 1 2 1 2 O(1) 0 1 2 1 2 La O(2) 0 0 1 2 1 2 0.362 0.318 O(2) 0 0 0.182 – O2 – O(3) O(3) 0 La 1 2 0.138 – – Nd Nd 1 2 O(1) Cu O(1) 0 0 1 2 1 2 0 0 0 Cu O2 – O(1) Cu O(1) 0 0 O(2) La O(1) – O2 Cu Nd2 CuO4 structure 1 2 0 0 0.682 0.638 1 2 1 2 1 2 – O2 Cu to produce O2− . To form the superconductors a small amount of La in La2 CuO4 can be replaced with divalent Sr, and some Nd in Nd2 CuO4 can be replaced with tetravalent Ce, corresponding to Sr → Sr 2+ + 2e− in La2 CuO4 Ce → Ce4+ + 4e− in Nd2 CuO4 (8.7) Thus, Sr doping decreases the number of electrons and hence produces hole-type car riers, while Ce doping increases the electron concentration and the conductivity is elec tron type. There are also copper-oxide electron superconductors with different structures, such as Sr 1−x Ndx CuO2 (Smith et al., 1991) and TlCa1−x Rx Sr2 Cu2 O7− , where R is a rare earth (Vijayaraghavan et al., 1989). Electron- and hole-type superconductivity in the cuprates has been compared (Katti and Risbud, 1992; Medina and Regueiro, 1990). 1 2 1 2 1 2 1 2 1 2 1 2 1 2 0 0 0.862 0.138 0 0 0 F. La2−x−y Rx Sry CuO4 Compounds (T∗ Phase) We have described the T structure of La2 CuO4 and the T structure of Nd2 CuO4 . The former has O(2) oxygens and the latter O(3) oxygens, which changes the coordina tions of the Cu atoms and that of the La and Nd atoms as well. There is a hybrid structure of hole-type superconducting lan thanum cuprates called the T∗ structure, illus trated in Fig. 8.21b, in which the upper half of the unit cell is the T type with O(2) oxygens and lower half the T type with O(3) oxygens. These two varieties of halfcells are stacked alternately along the tetrag onal c-axis (Akimitsu et al., 1988; Cheong et al., 1989b; Kwei et al., 1990; Tan et al., 1990). Copper, located in the base of an oxy gen pyramid, is fivefold-coordinated CuO5 . There are two inequivalent rare earth sites; the ninefold-coordinated site in the T-type VII BODY-CENTERED La2 CuO4 Nd2 CuO4 AND Sr2 RuO4 halfcell is preferentially occupied by the larger La and Sr ions, witle the smaller rare earths R (i.e., Sm, Eu, Gd, or Tb) prefer the eightfold-coordinated site in the T halfcell. Tan et al. (1991) give a phase diagram for the concentration ranges over which the T and T∗ phases are predominant. G. Sr2 RuO4 Compound (T Phase) Superconductivity was found in the lan thanum and neodymium cuprates during the initial years of the high temperature super conductivity era, but the phenomenon was not found in strontium ruthenate until 1994 (Maeno et al.), and did not attract widespread attention until several years later at the arrival of the new millennium. The unit cell dimensions of the three compounds are quite close to each other La2 CuO4 Nd2 CuO4 Sr2 RuO4 a0 = 379 Å a0 = 394 Å a0 = 387 Å c0 = 1323 Å c0 = 1215 Å c0 = 1274 Å (8.8) and the ionic radius of tetravalent ruthe nium Ru4+ (0.67 Å) is close to that of diva lent copper Cu2+ (0.72 Å). The two cuprates are insulators, which become conductors and superconductors at 24 K and 35 K, respec tively, when they are appropriately doped. Sr2 RuO4 , on the other hand, is a Fermi liq uid metal (Wysokinsky et al., 2003) without doping, and has a much lower transition temperature Tc = 15 K. The c-axis resis tivity, however, becomes nonmetallic above TM = 130 K, with the in-plane resistivity remaining always metallic (Maeno et al., 1996). The lanthanum and neodymium com pounds are similar to other cuprates in their type of superconductivity, whereas strontium ruthenate is believed to be a more exotic type of superconductor, hence the recent inter est in it. Some of the significant properties of Sr2 RuO4 are: the Sommerfeld specific 217 heat constant 0 = 375 mJ/mole K2 , the specific heat jump at Tc given by C = 27 mJ/mole (Annett et al., 2002), the resis tivity anisotropy c /ab = 500 (Wysokinsky et al., 2003), the presence of incommensu rate spin fluctuations (Sidis et al., 1999), and the Pauli limiting field BPauli 2T (Maki et al., 2001). The Cooper pairs in Sr2 RuO4 are believed to be odd parity spin triplets (Litak et al., 2004), and the compound is said to exhibit time reversal symmetry break ing (Luke et al., 1998). Won and Maki (2001) pointed out that the only other spin triplet superconductors found in met als are the heavy Fermion compound UPt3 , and the Bechgaard salt organic conductors TMTSF2 X with the structure sketched in Fig. 9.39, where the monovalent counter − ion X− can be, for example, ClO− 4 or PF 6 (Won and Maaki, 2001). Analogies have been pointed out to the triplet superfluid ity found in 3 He (Rice and Sigrist, 1995, Wysokinsky et al., 2003). The Fermi surface of Sr2 RuO4 has the three quasi-two dimen sional sheets shown in Fig. 8.28, and these lead to anisotropic resistivity, susceptibil ity, and other properties. Several researchers have suggested that the superconductivity is of the odd parity p wave or f wave type (e.g. Won and Maki, 2000). The presence of some Ru in the Sr2 RuO4 -Ru eutectic system raises the transition temperature to Tc 3K. Figure 8.28 Fermi surface of Sr2 RuO4 calculated by the tight binding method. The three quasi twodimensional sheets , and are indicated. (Wysokin ski et al., 2003, Fig. 1). 218 8 CUPRATE CRYSTALLOGRAPHIC STRUCTURES VIII. BODY-CENTERED BiSrCaCuO AND TlBaCaCuO Early in 1988 two new superconduct ing systems with transition temperatures considerably above those attainable with YBaCuO, namely the bismuth- and thalliumbased materials, were discovered. These compounds have about the same a and b lat tice constants as the yttrium and lanthanum compounds, but with much larger unit cell dimensions along c. We will describe their body-centered structures in terms of their layering schemes. In the late 1940s some related compounds were synthesized by the Swedish chemist Bengt Aurivillius (1950, 1951, 1952). A. Layering Scheme The Bi2 Sr2 Can Cun+1 O6+2n and Tl2 Ba2 Can Cun+1 O6+2n compounds, where n is an integer, have essentially the same structure and the same layering arrangement (Barry et al., 1989; Siegrist et al., 1988; Torardi et al., 1988a; Yvon and François, 1989), although there are some differences in the detailed atom positions. Here there are groupings of CuO2 layers, each separated from the next by Ca layers with no oxygen. The CuO2 groupings are bound together by intervening layers of BiO and SrO for the bismuth compound, and by intervening layers of TIO and BaO for the thallium compound. Figure 8.29 compares the layering scheme of Figure 8.29 Layering schemes of various high-temperature superconductors. The CuO2 plane layers are enclosed in small inner boxes, and the layers that make up a formula unit are enclosed in larger boxes. The Bi-Sr compounds Bi2 Sr2 Can Cun+1 O6+2n have the same layering schemes as their Tl-Ba counterparts shown in this figure. 219 VIII BODY-CENTERED BiSrCaCuO AND TlBaCaCuO the Tl2 Ba2 Can Cun+1 O6+2n compounds with n = 0, 1, 2 with those of the lanthanum and yttrium compounds. We also see from the figure that the groupings of Cu O2 − planes and − O2 Cu image (i.e., body centered) planes repeat along the c-axis. It is these copper-oxide layers that are responsible for the superconducting properties. A close examination of this figure shows that the general stacking rules mentioned in Section VI.C for the layering scheme are sat isfied, namely metal ions in adjacent layers alternate between edge (E) and centered (C) sites, and adjacent layers never have oxygens on the same types of sites. The horizon tal reflection symmetry at the central point of the cell is evident. It is also clear that YBa2 Cu3 O7 is aligned and that the other four compounds are staggered. Figure 8.30 (Torardi et al., 1988a) presents a more graphical representation of the information in Fig. 8.29 by show ing the positions of the atoms in their layers. The symmetry and body centering rules are also evident on this figure. Rao (1991) provided sketches for the six com pounds Tlm Ba2 Can Cun+1 Ox similar to those in Fig. 8.30 with the compound containing one m = 1 or two thallium layers m = 2, where n = 0, 1, 2, as in the Torardi et al. figure. B. Nomenclature There are always two thalliums and two bariums in the basic formula for Tl2 Ba2 Can Cun+1 O6+2n , together with n calciums and n + 1 coppers. The first three members of this series for n = 0 1, and 2 Figure 8.30 Crystal structures of Tl2 Ba2 Can Cun+1 O6+2n superconducting compounds with n = 0 1 2 arranged to display the layering schemes. The Bi2 Sr2 Can Cun+1 O6+2n compounds have the same respective structures (Torardi et al., 1988a). 220 are called the 2201, 2212, and 2223 com pounds, respectively, and similarly for their BiSr analogues Bi2 Sr2 Can Cun+1 O6+2n . Since Y in YBa2 Cu3 O7 is structurally analogous to Ca in the Tl and Bi compounds, it would be more consistent to write Ba2 YCu3 O7 for its formula, as noted in Section IV.F. In this spirit Ba2 YCu3 O7− might be called the 1212 compound, and La1−x Mx 2 CuO4− could be called 0201. 8 CUPRATE CRYSTALLOGRAPHIC STRUCTURES Charge-density plots of Bi2 Sr2 CaCu2 O8 indicate the same type of covalency in the Cu − O bonding as with the YBa2 Cu3 O7 and La2 CuO4 compounds. They also indi cate very little bonding between the adjacent [Bi – O] and [O – Bi] layers. D. Tl-Ba Compounds C. Bi-Sr Compounds Now that the overall structures and interrelationships of the BiSr and TlBa high-temperature superconductors have been made clear in Figs. 8.29 and 8.30 we will comment briefly about each compound. Table 8.3 summarizes the characteristics of these and related compounds. The first member of the BiSr series, the 2201 compound with n = 0, has octa hedrally coordinated Cu and Tc ≈ 9 K (Torardi et al., 1988b). The second mem ber, Bi2 Sr Ca3 Cu2 O8+ , is a superconduc tor with Tc ≈ 90 K (Subramanian et al., 1988a; Tarascon et al., 1988b). There are two Cu O2 – layers separated from each other by the [– – Ca] layer. The spacing from [Cu O –] to [– – Ca] is 1.66 Å, which is less than the corresponding spacing of 1.99 Å between the levels Cu O2 – and [– – Y] of YBaCuO. In both cases the copper ions have a pyramidal oxygen coordination of the type shown in Fig. 8.11. Superlat tice structures have been reported along a and b, which means that minor modifica tions of the unit cells repeat approximately every five lattice spacings, as explained in Sect. VIII.E. The third member of the series, Bi2 Sr2 Ca2 Cu3 O10 , has three CuO2 lay ers separated from each other by [– – Ca] planes and a higher transition tempera ture, 100 K, when doped with Pb. The two Cu ions have pyramidal coordination, while the third is square planar. The TlBa compounds Tl2 Ba2 Can Cun+1 O6+2n have higher transition temperatures than their bismuth counterparts (Iqbal et al., 1988b; Torardi et al., 1988a). The first member of the series, namely Tl2 Ba2 CuO6 with n = 0, has no [– – Ca] layer and a relatively low transition temperature of ≈ 85 K. The second member n = 1, Tl2 Ba2 CaCu2 O8 , called the 2212 compound, with Tc = 110 K has the same layering scheme as its Bi counterpart, detailed in Figs. 8.29 and 8.30. The Cu O2 – layers are thicker and closer together than the correspond ing layers of the bismuth compound (Toby et al., 1990). The third member of the series, Tl2 Ba2 Ca2 Cu3 O10 , has three Cu O2 – lay ers separated from each other by [– – Ca] planes, and the highest transition tempera ture, 125 K, of this series of thallium com pounds. It has the same copper coordina tion as its BiSr counterpart. The 2212 and 2223 compounds are tetragonal and belong to the same crystallographic space group as La2 CuO4 . We see from the charge-density plot of Tl2 Ba2 CuO6 shown in Fig. 8.31 that Ba2+ is ionic, Cu exhibits strong covalency, espe cially in the Cu-O plane, and Tl also appears to have a pronounced covalency. The bond ing between the [Tl – O] and [O – Tl] planes is stronger than that between the [Bi – O] and [O – Bi] planes of Bi − Sr. 221 VIII BODY-CENTERED BiSrCaCuO AND TlBaCaCuO Figure 8.31 Contours of constant charge density on a logarithmic scale in two high-symmetry crystallographic planes of Tl2 Ba2 CuO6 . Oxygen atoms O(1), O(2), and O(3) are denoted 1, 2, and 3, respectively. The planar Cu-O(1) binding is strongest (Hamann and Mattheiss, 1988; see Pickett, 1989). E. Modulated Structures The x-ray and neutron-diffraction pat terns obtained during crystal structure determinations of the bismuth cuprates Bi2 Sr2 Can Cun+1 O6+2n exhibit weak satel lite lines with spacings that do not arise from an integral multiple of the unit cell dimensions. These satellites have modulation periods of 21 Å, 19.6 Å, and 20.8 Å, respec tively, for the n = 0 1, and 2 compounds (Li et al., 1989). Since the lattice constant a = 541 Å b = 543 Å for all three compounds, this corresponds to a superlattice with unit cell of dimensions ≈ 38a b c, with the repeat unit along the a direction equal to ≈ 38a for all three compounds. A modulation of 47b has also been reported (Kulik et al., 1990). This structural modulation is called incommensurate because the repeat unit is not an integral multiple of a. Substitutions dramatically change this modulation. The compound Bi2 Sr2 Ca1−x Yx Cu2 Oy has a period that decreases from about 48b for x = 0 to the commensurate value 40b for x = 1 (Inoue et al., 1989; Tamegai et al., 1989). Replacing Cu by a transition metal (Fe, Mn, or Co) pro duces nonsuperconducting compounds with a structural modulation that is commensu rate with the lattice spacing (Tarascon et al., 1989b). A modulation-free bismuth-lead cuprate superconductor has been prepared (Manivannan et al., 1991). Kistenmacher (1989) examined substitution-induced super structures in YBa2 Cu1−x Mx 3 O7 . Superlattices with modulation wavelengths as short as 24 Å have been prepared by employing ultra-thin deposition techniques to interpose insulating planes of PrBa2 Cu3 O7 (Jakob et al., 1991; Lowndes et al., 1990; Pennycook et al., 1991; Rajagopal and Mahanti, 1991; Triscone et al., 1990). Tanaka and Tsukada (1991) used the Kronig-Penney model (Tanaka and Tsukada, 1989a, b) to calculate the quasiparticle spec trum of superlattices. 222 8 CUPRATE CRYSTALLOGRAPHIC STRUCTURES F. Aligned TI-Ba Compounds A series of aligned thallium-based superconducting compounds that have the general formula TIBa2 Can Cun+1 O5+2n with n varying from 0 to 5 has been reported (Ihara et al., 1988; Rona, 1990). These con stitute a series from 1201 to 1245. They have superconducting transition temperatures almost as high as the Tl2 Ba2 Can Cun+1 O6+2n compounds. Data on these compounds are listed in Table 8.3. G. Lead Doping Over the years a great deal of effort has been expended in synthesizing lead-doped superconducting cuprate structures (Itoh and Uchikawa, 1989). Examples involve sub stituting Pb for Bi (Dou et al., 1989; Zhengping et al., 1990), for Tl (Barry et al., 1989; Mingzhu et al., 1990), or for both Bi and Tl (Iqbal et al., 1990). Differ ent kinds of Pb, Y-containing superconduc tors have also been prepared (cf. Mattheiss and Hamann, 1989; Ohta and Maekawa, 1990; Tang et al., 1991; Tokiwa et al., 1990, 1991). IX. SYMMETRIES Earlier in this chapter we mentioned the significance of the horizontal reflection plane h characteristic of the high-temperature superconductors, and noted that many of these superconductors are body centered. In this section we will point out additional sym metries that are present. Table VI-14 of our earlier work (Poole et al., 1988) lists the point symmetries at the sites of the atoms in a number of these compounds. In the notation of group theory the tetragonal structure belongs to the point group 4/mmm (this is the newer inter national notation for what in the older Schönflies notation was written D4h ). The unit cell possesses the inversion operation at the center, so when there is an atom at posi tion x y z, there will be another identical atom at position −x −y −z. The inter national symbol 4/mmm indicates the pres ence of a fourfold axis of symmetry C4 and three mutually perpendicular mirror planes m. The Schönflies notation D4h also specifies the fourfold axis, h signifying a horizontal mirror plane h and D indicating a dihedral group with vertical mirror planes. We see from Fig. 8.32 that the z-axis is a fourfold 90 symmetry axis called C4 , and Figure 8.32 Symmetry operations of the tetragonal unit cell showing a fourfold rotation axis C4 , three twofold axes C2 , and reflection planes of the vertical zx = v , horizontal xy = h ; and diagonal d types. 223 X LAYERED STRUCTURE OF THE CUPRATES that perpendicular to it are twofold 180 symmetry axes along the x and y direc tions, called C2 , and also along the diago nal directions C2 in the midplane. There are two vertical mirror planes d which are also vertical, and a horizontal mirror plane h . Additional symmetry operations that are not shown are a 180 rotation C2z around the z axis, Cz2 = Cz4 Cz4 (8.9) and the improper fourfold rotation S4z around that corresponds to C4z followed by, or pre ceded by, h , Sz4 = Cz4 h = h Cz4 (8.10) C4z where and h commute. The orthorhombic structure has mmm D2h symmetry. We see from Fig. 8.33 that both the rectangular and rhombal unit cells, which correspond to Figs. 8.4a and 8.4b, respectively, have three mutually perpendicular twofold axes, and that they also have three mutually perpendicular mirror planes , which are not shown. The two cases differ in having their horizontal axes and vertical planes oriented at 45 to each other. Figure 8.33 Rotational symmetry operations of an orthorhombic unit cell (a) with rectangular distortion, and (b) with rhombal distortion from an originally tetragonal cell. Cubic structures, being much higher in symmetry, have additional symmetry oper ations, such as fourfold axes C4x C4y , and C4z along each coordinate direction, three fold axes C3 along each body diagonal, and numerous other mirror planes. These can be easily seen from an examination of Fig. 8.1. Buckyballs C60 belong to the icoso hedral group, which has twofold C2 , five fold C5 , and sixfold C6 rotation axes, horizontal reflection planes, inversion sym metry, and sixfold S6 and tenfold S10 improper rotations, for a total of 120 indi vidual symmetry operations in all (Cotton, 1963). X. LAYERED STRUCTURE OF THE CUPRATES All cuprate superconductors have the layered structure shown in Fig. 8.34. The flow of supercurrent takes place in conduc tion layers, and binding layers support and hold together the conduction layers. Con duction layers contain copper-oxide CuO2 planes of the type shown in Fig. 8.24 with each copper ion Cu2+ is surrounded by four oxygen ions O2− . These planes are held together in the structure by calcium Ca2+ ions located between them, as indicated in Fig. 8.35. An exception to this is the yttrium compound in which the intervening ions are the element yttrium Y3+ instead of cal cium. These CuO2 planes are very close to being flat. In the normal state above Tc , con duction electrons released by copper atoms move about on these CuO2 planes carry ing electric current. In the superconducting state below Tc , these same electrons form the Cooper pairs that carry the supercurrent in the planes. Each particular cuprate compound has its own specific binding layer consisting mainly of sublayers of metal oxides MO, where M is a metal atom; Fig. 8.36 gives the sequences of these sublayers for the 224 8 CUPRATE CRYSTALLOGRAPHIC STRUCTURES BINDING LAYERS CONDUCTION LAYERS WITH CuO2 BINDING LAYERS CONDUCTION LAYERS WITH CuO2 BINDING LAYERS CONCUCTION LAYERS WITH CuO2 BINDING LAYERS Figure 8.34 Layering scheme of a cuprate superconductor. Figure 8.35 shows details of the conduction layers for different sequences of copper oxide planes, and Fig. 8.36 presents details of the binding layers for several cuprates. (Owens and Poole, 1996, Fig. 8.1). principal cuprate compounds. These bind ing layers are sometimes called charge reservois layers because they provide the charge for the Cooper pairs that form in the copper-oxide planes. Figure 8.30 presents a three-dimensional perspective of how con duction and binding layers are arranged in the thallium compounds containing one, two, and three copper oxide planes, i.e., having n = 1 2, and 3 in the formula Tl2 Ba2 Can−1 Cun O2n+4 . The fact that all of the cuprates have structures with alternating conduction lay ers and binding layers stacked along the z direction led to the adoption of a four digit code for designating their com position and structure. The general for mula for a cuprate superconductor with a binding layer Aj Bk Oj+k , and a conducting layer Sn−1 Cun O2n , is Aj Bk Sn−1 Cun Oj+k+2n+2 , and most high temperature superconduc tors have the more specific formula Aj B2 Sn−1 Cun Oj+2n+2 . A sublayer BO of the binding layer is always adjacent to a CuO2 sublayer of the conduction layer, with AO sublayers between BO sublayers. The sepa ration atoms S always lie between CuO2 sublayers of the conduction layer. This means that a CuO2 sublayers can only have BO or S sublayers adjacent to it. A four digit code jkmn is often employed to designate the structure type Aj Bk Sm Cun . In typical cases the binding layer con sists of oxides of A atoms which are Bi, Tl or Hg, and oxides of B atoms which are Sr or Ba. The separation atoms S of the conduction band are usually Ca, but in the yttrium super conductor they are Y. Using the notation jkmn we have the following examples of four digit codes: 0201 La1−x Srx 2 CuO4 1212 HgBa2 CaCu2 O6 1212 CuBa2 YCu2 O7 Usually written YBa2 Cu3 O7 1223 TlBa2 Ca2 Cu3 O9 2201 Bi2 Sr2 CuO6 2234 Tl2 Ba2 Ca3 Cu4 O12 225 XI INFINITE-LAYER PHASES CuO2 Conduction layer with one copper oxide plane CuO2 Ca CuO2 Conduction layer with two copper oxide planes CuO2 Y CuO2 Conduction layer of yttrium compound with two copper oxide planes CuO2 Ca CuO2 Ca CuO2 Conduction layer with three copper oxide planes Figure 8.35 Conduction layers of the various cuprate superconductors showing sequences of CuO2 and Ca (or Y) planes in the conduction layers of Fig. 8.34. (Owens and Poole, 1996, Fig. 8.3). Sometimes the A atom symbol is used as a prefix to the code, and in this notation five of the above six codes would be writ ten: La-0201, Hg-1212, Tl-1223, Bi-2201, and Tl-2234 to designate the corresponding compounds. XI. INFINITE-LAYER PHASES In 1993 superconductivity was dis covered in the series of compounds with the general formula Sr n+1 Cun O2n+1+ ; these compounds represent perhaps the simplest of the copper oxide superconductors contain ing only two metallic elements, strontium and copper. Like the cuprates these are lay ered compounds, and the parameter n des ignates the number of copper oxide layers. The layering scheme is very simple, and it can be visualized from Fig. 8.37. The bind ing layer Sr2 O for all of these compounds consists of successive Sr, O, and Sr planes, as indicated at the top of Fig. 8.37. This binding layer is much thinner than those of the cuprates; conduction layers are similar to the cuprate ones shown in Fig. 8.35 but with strontium atoms between the CuO2 planes instead of calcium or yttrium. Thus these compounds may properly be considered as cuprate types. The n = 1 compound has a structure similar to that of La2 CuO4 , discussed ear lier and shown in Fig. 8.21. This n = 1 226 8 CUPRATE CRYSTALLOGRAPHIC STRUCTURES LaO LaO Lanthanum Superconductor La2CuO4 BaO CuO BaO Yttrium Superconductor YBa2Cu3O7 SrO BiO BiO SrO Bismuth Superconductor Bi2Sr2Can–1CunO2n+4 BaO TlO TlO BaO Thallium Superconductor Tl2Ba2Can–1CunO2n+4 BaO Hg(O) BaO Mercury Superconductor HgBa2Can–1CunO2n+2 Figure 8.36 Sequences of MO sublayers in the binding layers of Fig. 8.34 where M stands for various metal ions. The parentheses around the oxygen atom O in the lowest panel indicates partial occupancy. (Owens and Poole, 1996, Fig. 8.4). compound with the formula Sr2 CuO31 has a large number of vacancies in the binding layers and a transition temperature of 70 K. These vacancies provide the doping mecha nism for holes in the CuO planes. The n = 2 compound Sr3 Cu2 O5+ has a Tc of 100 K. The limit of the series for very large n is SrCuO2 ; it has the infinite layer struc ture shown in Fig. 8.38. This material can be made into an electron-doped superconduc tor with Tc = 43 K by replacing some of the divalent Sr 2+ with trivalent La3+ ; this has the effect of putting electron carriers in the cop per oxide planes. The large n material doped with holes occurs only in a small fraction of the samples, and it has a transition tempera ture of 110 K. It is not clear what causes hole doping, but it is believed to involve some kind of defect structure. One idea is that an oxygen atom may be trapped between two Sr 227 FURTHER READING Sr O Sr Binding layer of infinite layer phases Srn + 1CunO2n + 1 + δ CuO2 Conduction layer of Sr2CuO3 + δ CuO2 Sr CuO2 Conduction layer of Sr3Cu2O5 + δ CuO2 Sr CuO2 Sr CuO2 Conduction layer of Sr4Cu3O7 + δ Figure 8.37 Binding layer (top) followed by, in succession, conduction layers of the first three infinite layer phase compounds, namely Sr2 CuO3+ Sr3 Cu2 O5+ and Sr4 Cu3 O7+ . The figures are drawn assuming = 0. (Owens and Poole, 1996, Fig. 8.17). atoms, forming an Sr–O–Sr defect. Another proposal is that a corrugated Sr–O layer is substituted for one of the copper oxide layers. XII. CONCLUSIONS Almost all the high-temperature oxide superconductors have point symmetry D4h a = b or symmetry close to D4h a ∼ b. These superconductors consist of horizontal layers, each of which contains one positive ion and either zero, one, or two oxygens. The copper ions may be coordinated square planar, pyramidal, or octahedral, with some additional distortion. Copper oxide layers are never adjacent to each other, and equivalent layers are never adjacent. The cations alter nate sites vertically, as do the oxygens. The copper oxide layers are either flat or slightly puckered, in contrast to the other metal oxide layers, which are generally far from planar. The highest Tc compounds have metal layers (e.g., Ca) with no oxygens between the copper oxide planes. FURTHER READING Chapter 8 by R. Gladyshevskii and P. Galez in the Handbook of Superconductivity edited by C. P. Poole, Jr., provides the structures of most of the cuprates. The Inter national Tables for X-Ray Crystallography (Henry and Lonsdale, 1965, Vol. 1) provide the atom positions and symmetries for all of the crystallographic space groups. 228 Figure 8.38 Crystal structure of the infinite layer phase SrCuO2 . (Owens and Poole, 1996, Fig. 8.18). PROBLEMS 1. Show that the radius of the octahedral hole lattice of atoms in an fcc close-packed √ of radius r0 is equal to 2 − 1 r0 . What is the radius of the hole if the lattice is formed from oxygen ions? 2. Show that the radius of the tetrahedral hole in an fcc close-packed � lattice of�atoms of radius r0 is equal to 3/21/2 − 1 r0 . What is the radius of the hole if the lattice is formed from oxygen ions? 3. The “image perovskite” unit cell is generated from the unit cell of Fig. 8.1 by shifting the origin from the point (0, 0, 0) to the point 21 21 21 . Sketch this “image” cell. Show that the planes of atoms in this cell are the image planes related by the body centering operation to those of the original perovskite. This image cell is the one that usually appears as a figure to represent perovskite in solidstate physics texts. 8 CUPRATE CRYSTALLOGRAPHIC STRUCTURES 4. Calculate the distance between the yttrium atom and its nearest-neighbor Ba, Cu, and O atoms in the superconductor YBa2 Cu3 O7 . 5. Write down the x y z coordinates for the five numbered atoms in the initial plane of Fig. 8.19. Give the explicit symmetry operations, with the proper choice of sign in Eq. (8.5) for each case, that transform these five atoms to their indicated new positions on the other three planes. 6. Explain how the international and Schön flies symbols, mmm and D2h respec tively, are appropriate for designating the point group for the orthorhombic superconductors. 7. What are the symmetry operations of the A15 unit cell of Fig. 3.19? 8. The D2h point group consists of eight symmetry operations that leave an orthorhombic cell unchanged, namely an identity operation E that produces no change, three twofold rotations C2i along I = x y z, three mirror reflection planes ij , and an inversion i. Examples of these symmetry operations are E x→x y→y z→z C2x x→x y → −y z → −z xy x→x y→y z → −z i x → −x y → −y z → −z A group has the property that the suc cessive application of two symmetry operations produces a third. Thus, we have, for example, C2x xy = zx C2y C2x = C2z = iC2y zx yz zx = C2x These four results have been entered into the following multiplication table 229 PROBLEMS E E Cx2 y C2 Cz2 i xy yz zx Cx2 y C2 Cz2 i xy yz zx zx Cz2 zx for the D2h group. Fill in the remain der of the table. Hint: each element of a group appears in each row and each column of the multiplication table once and only once. 9. Construct the multiplication table for the D4h point group which contains the 16 symmetry elements that leave a tetragonal unit cell unchanged. Which pairs of symmetry elements A and B do not commute, i.e., such that AB = BA? Hint: follow the procedures used in Problem 8. Cz2 10. Draw diagrams analogous to those in Fig. 8.29 for the first two members of the aligned series TlBa2 Can Cun+1 O5+2n , where n = 0 1. 11. Draw the analogue of Fig. 8.22 for the Nd2 CuO4 compound, showing the loca tion of all of the Cu and O atoms. How do Figs. 8.24 and 8.25 differ for Nd2 CuO4 ? 12. Select one of the compounds Tl2 Ba2 CuO6 Bi2 Sr2 CaCu2 O8 , Bi2 Sr2 Ca2 Cu3 O10 , Tl2 Ba2 Ca2 Cu3 O6 and construct a table for it patterned after Tables 8.5 or 8.6. This page intentionally left blank 9 Unconventional Superconductors I. INTRODUCTION The classical superconductors which are discussed in Chap. 3 consist of elements, alloys, intermetallic compounds, and ionic compounds. They are all s-wave types with properties that are explained well by the stan dard isotropic BCS theory. The cuprate high temperature superconductors discussed in Chap. 8 exhibit Cooper pairing of a d-wave type, and are anisotropic in their proper ties. Their symmetries are either tetrago nal or orthorhombic, but close to tetragonal. The nonclassical or unconventional nature of their properties arises from their layered structures, as described in Chap. 8. This chapter will cover materials which exhibit other types of unconventional superconduc tivity. Some of these unconventional super conductors were discussed in the previous edition, such as heavy electron types, charge transfer organics and borocarbides toward the end of Chap. 3, and perovskites and buckministerfuller4enes in both Chap. 3 and Chap. 7 of that edition, while others were discovered in more recent years. The present chapter will cover the properties of all these superconducting materials. II. HEAVY ELECTRON SYSTEMS For several years prior to 1987 there was a great deal of interest in the study of heavyelectron superconductors, i.e., superconduc tors whose effective conduction-electron mass m∗ is typically more than 100 electron 231 232 9 UNCONVENTIONAL SUPERCONDUCTORS masses. Physicists have given these mate rials a somewhat more pretentious name “heavy fermion superconductors.” The first such superconductor, CeCu2 Si2 , was discov ered in 1979 (Steglich et al., 1979), and some time passed before the phenomenon was con firmed by the discovery of other examples, such as UBe13 (Ott et al., 1983) and UPt3 (Stewart et al., 1984). Since then many addi tional cases have been found. Many of the investigators who became active in the field of cuprate superconductivity obtained their experience with the heavy-electron types. Work on heavy-electron superconductors has been reviewed in a number of studies (Coles, 1987; Ott, 1987; Stewart, 1984). The Cooper pairing in the heavy elec tron systems is of the = 1 or p-wave type. Since the superconducting charge carriers are Cooper pairs formed from heavy electrons and since these pairs are bosons, it would be more appropriate to call these compounds “heavy boson superconductors.” This, how ever, is never done, so we will conform to the conventional usage. Ordinary supercon ductors are not usually called boson super conductors either. The large effective mass has a pro nounced effect on several properties of superconducting materials since it enters into the expression (Eq. (1.41)) for the electron density of states at the Fermi level: 1 DEF = 2 2 � 2m∗ �2 �3/2 EF1/2 Heavy-electron compounds have densities of states that correspond to values of m∗ ≈ 200me in Eq. 9.1, as shown by the data in Table 9.1. The rare-earth element Ce has two 4f electrons and the actinide element U has three 5f electrons. In compounds each of these elements has f electron configura tions that can mix as linear combinations or hybridize with the conduction electrons and together produce sharp energy bands near the Fermi level. The narrow width of such a band gives it a high density of states, and hence, by Eq. 9.1, a large effective mass. A situation of this type is sketched in Fig. 9.1 in which a narrow hybridization band super imposed on the usual √ conduction electron expression DE E from Fig. 6.5 of the Table 9.1 Properties of Several Heavy-Electron Superconductorsa Compound CeAl3 CeCu6 NpBe13 UBe13 UCd11 UPt 3 U2 Zn17 CeCu2 Si2 UNi2 Al3 UPd2 Al3 URu2 Si2 a Tc (K) 0 85 0 43 06 10 ≈20 13 TN (K) 34 88 50 50 97 07 46 14 0 17 5 (9.1) (K) �eff /�B −43 −88 −42 −70 −23 −200 −250 −140 2 62 2 68 2 76 31 3 45 29 45 26 m∗ /mc 192 187 220 Tc is the superconducting transition temperature; TN is the Néel temperature; is the Curie-Weiss temperature; eff is the effective magnetic moment and m∗ /mc is the ratio of the effective mass to the free electron mass. Some of the data are borrowed from Stewart (1984). Additional data are from Geibel et al. (1991a) on UNi2 Al3 , from Geibel et al. (1991b and 1991c) on UPd2 Al2 , and Issacs et al. (1990) on URh2 Si2 . 233 II HEAVY ELECTRON SYSTEMS between a conduction electron and an f elec tron wave function (Hofmann and Keller, 1989). We see that the sharpness of the peak in DEF depends on the strength of this interaction. The electrons in these f shells of Ce and U are also responsible for the forma tion of the superconducting state. Other rare earths and actinides do not form these types of hybridization bands at the Fermi level. Much of the evidence for the high effec tive mass comes from experimental observa tions in the normal state. For example, the conduction-electron contribution to the spe cific heat from Eq. (1.52) Figure 9.1 Density of states of a heavy fermion com pound showing a peaked, narrow, half-occupied band at the Fermi level. (first edition, Fig. 3.26) Figure 9.2 Density of states of a narrow hybridiza tion band calculated for three values of the hybridization between a conduction electron and an f electron wave function (Hofmann and Keller, 1989). first edition. The figure is drawn for the situ ation where the Fermi level is at the center of the hybridization band. Figure 9.2 shows the density of states at the Fermi level calculated for three values of the effective hybridization 1 = 2 DEF kB2 3 (9.2) is proportional to the density of states (9.1) and hence is unusually large for heavy-electron compounds. The electronic specific-heat coefficients for heavyelectron superconductors are, on average, more that 10 times larger than those of other superconducting compounds, as may be seen by consulting Table 4.1. The dis continuity Cc − Tc in the specific heat at the transition temperature is also corre spondingly large for heavy-electron com pounds, so the ratio Cs − Tc / Tc is close to the usual BCS value of 1.43, as may be seen from the same table. Figure 9.3 shows a measurement of this discontinuity in the compound UPt3 . Heavy-electron systems often exhibit two ordering transitions, a superconducting transition at Tc and an antiferromagnetic ordering transition at the Néel temperature TN , with typical values given in Table 9.1. The superconducting transition is illustrated by the drop in magnetic susceptibility at Tc (shown in Fig. 9.4 for URu2 Si2 ). When the magnetic moments of the ions couple anti ferromagnetically, the magnetic susceptiblil ity often exhibits Curie-Weiss behavior (cf. Eq. (1.79)). Many of these compounds have effective magnetic moments exceeding the 234 9 UNCONVENTIONAL SUPERCONDUCTORS Figure 9.3 Specific heat of the heavy fermion compound UPt3 in the neighborhood of the transition temperature. The solid lines correspond to a single ideally sharp transition while the dashed lines are fits to the data with two adjacent sharp transitions (Fisher et al., 1989). Figure 9.4 Dependence of magnetic susceptibility on tempera ture for the heavy fermion compounds URu2−x Rhx Si2 , with in the range 0 ≤ ≤ 0 02 (Dalichaouch et al., 1990). 235 II HEAVY ELECTRON SYSTEMS Figure 9.5 Peak near 16K in the resistivity-versus-temperature plot of the heavy fermion compound URu2 Si. The inset shows the supercon ducting transition below 1K in an expanded scale (Mydosh, 1987; see also Palst et al., 1987). Bohr magneton, as shown in Table 9.1. The table lists several other properties of these materials. The heavy-electron superconductors have anisotropic properties that become apparent in such measurements as those for the critical fields, electrical resistivity, ultra sonic attenuation, thermal conductivity, and NMR relaxation. Figures 9.5 and 9.6, respec tively, show typical anisotropies in the resis tivity (Coles, 1987; Mydosh, 1987; Palst et al., 1987) and upper-critical field (Assmus et al., 1984; Stewart, 1984). The presence of a peak in the resistivity shown in Fig. 9.5 is characteristic of the heavy fermions. The lower-critical fields Bc1 are several mT at 0 K, while the upper-critical fields Bc2 at 0 K approach 1 or 2 tesla as shown by the example in Fig. 9.6. The critical field derivatives dBc2 /dT are high in absolute magnitude, such as −10 T/K for CeCu2 Si2 and −44 T/K for UBe13 . The London penetration depth L is several thousand angstroms, consistent with the large effective mass m∗ , which enters as a Figure 9.6 Upper critical-field anisotropy in tetrago nal heavy fermion superconductor CeCu2 Si2 parallel to, respectively perpendicular to, the Ce planes. Note the lack of anisotropy at Tc where both orientations have the same slope, −23T/K, as given by the dashed line. The inset shows the temperature dependence of the resistivity under various applied fields (Assmus et al., 1984). square root factor in the classical expression in (2.28) � L = m∗ 0 ns e 2 �1/2 (9.3) In ordinary superconductors magnetic impurities suppress the superconducting state 236 due to the pair-breaking effect of the mag netic moments. In anisotropic superconduc tors, on the other hand, any kind of impurity is pair breaking. In particular, small amounts of nonmagnetic impurities replacing, for example, uranium, beryllium, or platinum, bring about a pronounced lowering of Tc . Some researchers have suggested that the heavy-electron materials exhibit an uncon ventional type of superconductivity that does not involve the ordinary electron-phonon interaction (Bishop et al., 1984; Coles, 1987; Gumhalter and Zlatic, 1990; D. W. Hess et al., 1989; Ott, 1987; Ozaki and Machida, 1989; Rodriguez, 1987; Stewart, 1984). There have also been reports of high effective masses in the oxide supercon ductors, with, for example, m∗ /m ≈ 12 (Matsura and Miyake, 1987) in LaSrCuO, and m∗ /m ≈ 5 (Gottwick et al., 1987), m∗ /m = 9 (Salamon and Bardeen, 1987), and m∗ /m ≈ 102 in YBaCuO (Kresin and Wolf, 1987). Some more recently dis covered heavy-electron superconductors are Ce3 Bi4 Pt3 (Riseborough, 1992), UNi2 Al3 (Geibel et al., 1991a; Krimmel et al., 1992), UPd2 Al3 (Geibel et al., 1991b, c; Krimmel et al., 1992; Sato et al., 1992), and YBiPt (Fisk et al., 1991). 9 UNCONVENTIONAL SUPERCONDUCTORS why such a simple compound could be such a good superconductor. Two years later the journal Physica C devoted a special issue to the topic (Vol. 385, Nos. 1–2, March 2003), which we will denote by PhC. A. Structure Magnesium diboride has the AlB2 hexagonal structure sketched in Fig. 9.7, with a0 = 0 3084 nm and c0 = 0 3262 nm, cor responding to crystallographic space group P3mlD3d 3 . Mg is in the special position 000, and B is in the two special posi tions 1 /3 2 /3 1 /2 and 2 /3 1 /3 1 /2 in the unit cell. There are alternating layers of magnesium and boron atoms perpendicular to the c axis, with the Mg adopting a close packed pla nar hexagonal arrangement, and the B atoms in a graphite- type hexagonal arrangement. Each boron atom has a triangular array of magnesiums above and below it, and each magnesium has an array of six borons above and six below, as is clear from the figure. The nearest neighbor distances are III. MAGNESIUM DIBORIDE Superconductivity in magnesium diboride was discovered by Nagamatsu et al. in 2001. MgB2 is a simple intermetallic compound with a hexagonal unimolecular unit cell. It was a surprise to find that its transition temperature Tc � 39K is so far above that of all other intermetallic compounds. Its superconductivity is the simple BCS phonon mediated s-wave type, but complicated by the presence of two energy gaps. During the year after its discovery the superconducting community of scientists embarked on a worldwide concentrated effort to unravel the reasons Figure 9.7 Arrangement of magnesium atoms (large open circles) in planes z = 0 and z = c, with a planar hexagonal arrangement of boron atoms (solid dots) at the height z = 1 /2 c between these planes. (Thanks are due to Michael A. Poole for preparing this figure). 237 III MAGNESIUM DIBORIDE dB-B = 0 177 nm dMg-B = 0 250 nm (9.4) dmg-Mg = 0 308 nm Since boron has the valence electron config uration 2s2 p and magnesium has 3s2 , only s and p electrons are involved in the electronic structure and the Cooper pairing. Within the boron layers the bonding is strongly covalent, and between the boron and mag nesium layers the bonding is more metalliclike, involving some electron delocalization [Mazin and Antropov, 2003]. Boron has two naturally occur 10 ring isotopes: B19 78% and 12 B80 22%, and magnesiusm has three: 24 25 Mg78 99% Mg10 00%, and 26 Mg11 01%. When Tc was measured with isotopically enriched samples it was found that the isotope effect exponent = 0 32 for boron, somewhat below the theoretical BCS value of = 0 5. Figure 9.8 shows the isotopic shift determined by magnetization and resistivity measurements. The shift for magnesium enrichment was negligible. This indicates that the phonons involved in the Cooper-pairing were mainly from vibrations of the lighter boron atoms, with phonons arising from Mg vibrations making very little contribution. B. Physical Properties In the special issue of the journal Phys ica C mentioned above Canfield et al., (2003) wrote an introductory article which summa rized the basic physical properties of MgB2 , and a number of these properties are listed in Table 9.2. Some of these data are averages, and do not take into account the presence of two gaps in the energy bands. Figure 9.9 shows the temperature dependence of the resistivity in zero field and in applied mag netic fields between 2.5T and 18T. We see that the transition temperature is lowered and the transition is broadened for increasing fields, as expected. Figure 9.10 presents the temperature dependence of the magnetiza tion of aligned single crystals in a magnetic field of 0.5mT applied along the c crystal lographic direction. We see that the mag netization below Tc is much more negative for zero field cooling (ZFC) than it is for field cooling (FC). The hysteresis loop in the inset obtained at a temperature of 10K corresponds to a critical current density Jc < 105 A/cm2 . C. Anisotropies Figure 9.8 Isotope shift determined by magnetiza tion (upper panel) and resistivity (lower panel) measure ments. (Canfield et al., 2003, Fig. 1). Magnesium diboride has the layered crystal structure illustrated in Fig. 9.7 and this causes some of its physical properties to be anisotropic, with values that differ for measurements made in the a, b plane and along the c direction. The temperature depen dence of the penetration depth factor 238 9 UNCONVENTIONAL SUPERCONDUCTORS Table 9.2 Basic physical properties of the superconductor MgB2 . Some parameters are anisotropic, with only average values listed here. Superconducting transition temperature Tc Coherence length 0 Penetration depth Ginzburg-Landau parameter electron mean free path Residual resistivity ratio RRR = 300K/42K Debye temperature D Fermi surface electron velocity VF Isotope effect constant Upper critical field Bc2 , clean sample � 0 dirty sample � 0 Irreversibility field Birr , clean sample dirty sample Thermodynamic critical field Bc Lower critical field Bcl Critical current density Jc ∗ 39K∗ 5 nm∗ 140 nm∗ � 25 � 60 nm∗ � 20 340K 4 8 × 105 m/sec∗ 0.32 16T∗ 30T∗ 7T∗ 15T∗ 0.43T 30mT � 4 × 105 A/cm2∗ Values obtained from Canfield et al. (2003) article cited above. Figure 9.9 Temperature dependence of the resistivity of MgB2 crystals in zero field and in an 18T applied magnetic field. The inset presents low field data for applied fields, from bottom to top, of 0, 2.5, 5, 7.5, 10, 12.5, 15, 16, 17, and 18T. (Canfield et al., 2003, Fig. 2). = T − 0 (9.5) presented in Fig. 9.11, shows that is larger for a magnetic field applied along the c direction than it is for the field applied in the a, b plane. These measurements were made using a sensitive radio frequency tech- nique, and the inset to the figure gives the ratio of the observed frequency shifts for the applied field perpendicular to and parallel to the c axis. The second critical field Bc2 is also anisotropic, being about six times larger for fields applied in the a, b plane than for fields along the c axis, as shown in Fig. 9.12a. 239 III MAGNESIUM DIBORIDE Figure 9.10 Temperature dependence of the magnetization for field cooled (FC) and zero field cooled (ZFC) measurements in an applied field along the crystallographic c direction with Bapp = 0 5 mT. The inset shows a hysteresis loop of a MgB2 single crystal at 10K with Bapp � c. (Lee, 2003, Fig. 3). from Eq. (12.56b) that B c2 i = 0 /2j k it follows that H = ab /c . Equation (12.43) shows that the product i i for all three direc tions i, j, k = a, b, c is expected to be constant for each superconductor, which means that the critical field anisotropy factor can also be written in the form H = c /ab . The selfconsistency of these three expressions for H can be checked experimentally. D. Fermi Surfaces Figure 9.11 Temperature dependence of the pen etration depth factor = T − 0 for measure ments made in the ab plane a and in the axial direction c . The insert shows the ratio of changes in the circuit resonant frequency F for the magnetic field applied in the a, b plane and parallel to the c axis. (Fletcher et al., 2005, Fig. 1). The temperature dependence of the criti cal field anisotropy factor H = B c2 ab /B c2 c is indicated in Fig. 9.12b. Since we know A sketch of the configuration of the Fermi surface of MgB2 published in the above mentioned special issue of Physica C by Kogan and Bud’ko (2003) is presented in Fig. 9.13, and Cooper et al. (2003) pro vide a similar sketch in the same issue. The three energy bands (#3,4 and 5) that cross the Fermi level give rise to four Fermi sur face sheets, two axial quasi two-dimensional -band sheets, and two contorted threedimensional -band sheets, as shown in the figure. The -bands originate from the boron 240 9 UNCONVENTIONAL SUPERCONDUCTORS Figure 9.12 (a) Temperature dependence of the upper critical field for measurements made in the a, b plane (lower data set) and parallel to the c axis (upper data). Squares and triangles represent measurements made using two different samples and two different measurement techniques. (b) Temperature dependence of the upper critical field anisotropy given by the factor H = Bc2 ab /Bc2 c in the notation used in the text. The full lines are theoretical curves calculated by the method of Miranvoic et al. (Angst. et al., 200, Fig. 3). valence electron in-plane sp2 hybridization involving bonding px and py orbitals that are somewhat weakly coupled [see Samuely et al., 2003], and form two concentric nearly cylindrical sheets along the –A– axis in the kz direction of the Brillouin zone, as shown in the figure. Because of their cylindrical shape these sheets have a two dimensional character. Conduction electrons can move in the kz direction on these -band surfaces from one Brillouin zone to the next since eight adjacent zones join together at the special point , and the cylindrical surfaces are continuous across the boundary. It is clear from the figure that the -bands, which arise from aromatically hybridized (covalent) bonding and antibond ing pz orbitals of boron that are more strongly coupled, form very convoluted surfaces that are three dimensional in character. The sheet from band 3 involves electron-type antibond ing, and that from band 4 is hole-type bond ing. We see from Fig. 9.13 that the surface of -band No.5 crosses into the next Brillouin zone along the kx and ky directions at the special points L, and the surface of -band No. 4 crosses the zone boundaries at special points M. All of these -band crossings cor respond to electron flow in the kx ky , plane. As a result of these geometric characteris tics of the Fermi surface electrical properties such as the resistivity, and other properties of magnesium diboride are anisotropic, and hence depend on the direction of an applied magnetic field. Lee et al. (2001) provide sketches of extremal orbits of electrons encircling spe 241 III MAGNESIUM DIBORIDE Figure 9.13 Fermi surface of MgB2 calculated by Choi et al., 2002. Four sheets formed from three energy bands, and points of special symmetry in the tetragonal Brillouin zone, are indicated. (Kogan and Bud’ko, 2003, Fig. 4). Cooper et al. (2003) identify the bands. cial points , A, K, L, and M on the Fermi surface. De Haas-van Alphen experiments can be carried out with preferentially ori ented applied magnetic fields to determine the areas enclosed by these orbits in kspace, and thereby confirm the configuration of these various energy surfaces in k-space (Cooper et al., 2003). E. Energy Gaps The superconducting energy gap dif fers for the two -bands and for the two bands, and the spread in the correspond ing gap values is sketched in Fig. 9.14. The pi gap has the approximate value � 2 8meV, and for the larger sigma gap � 6 8meV. The temperature dependencies of these gaps are of the conventional type, decreasing to zero as the transition temper ature is approached from below, as indi cated in Fig. 9.15. It is this multigap feature that makes magnesium diboride so interest ing as a superconductor, and endows it with some unique properties. The transition tem perature Tc is the same for both gaps, and they have the respective reduced gap values /kB Tc � 1 7 and /kB Tc � 4, one being less than and one greater than the BCS value of 3.528. 242 9 UNCONVENTIONAL SUPERCONDUCTORS Figure 9.14 Distribution in energy of the lower -band gap near 2meV and the upper -band gap near 7 mV. (Kogan and Bud’ko, 2003, Fig. 5). Figure 9.15 Temperature dependence of the pi-band gap and the sigma-band gap . The data points determined from experimental conductance measure ments are compared to BCS theoretical curves. (Daghero et al., 2003, Fig. 5). Data from many experiments are easier to explain using a two gap model, such as those involving crystal field, Hall effect, pho toemission, Raman scattering, specific heat, thermoelectric power, and tunneling mea surements. Electron-phonon coupling calcu lations have been carried out individually for the - and for the -bands. Many of these results are found in the PhC arti cles. For example, Daghero et al. [2003] found different values for the upper critical field Bc2 for the two bands, and scanning tunneling spectroscopy for c-plane orien tation reveals only the single narrow gap, while ab-plane tunneling resolves two gaps with the larger gap dominant, as shown in Fig. 9.16 [Iavarone et al., 2003, Martinez-Samper et al., 2003, Gonnelli et al., 2004]. Figure 9.16 Simulated tunneling conductance spectra of MgB2 for tunneling along the c-axis, in an inter mediate case, and in the a, b plane. (Iavarone et al., 2003, Fig. 2). 243 IV BOROCARBIDES AND BORONITRIDES IV. BOROCARBIDES AND BORONITRIDES During the preparation of the first edition of this book superconductivity was discovered in a series of quaternary borocar bide compounds, ordinarily referred to sim ply as borocarbides, with the general for mula RCn M2 B2 where R is a transition metal and M is ordinarily Ni. The isostruc tural boronitride series has the general for mula RNn M2 B2 where nitrogen replaces carbon. The subject has been reviewed by Canfield (2000), by Hilscher and Michor (1999), and by Müller and Narozhnyi (2001). The latter review emphasizes the inter action between magnetism and supercon ductivity in these compounds. Table 9.3 Table 9.3 Superconducting transition temperatures of various borocarbide compounds (see Hilscher and Michor (1999), and Müller and Narozhuyi (2001).) Compound Tc K CeNi2 B2 C DyNi2 B2 C ErNi2 B2 C HoNi2 B2 C LuNi2 B2 C ScNi2 B2 C ThNi2 B2 C TmNi2 B2 C YNi2 B2 C LaPd2 B2 C ThPd2 B2 C YPd2 B2 C LaPt2 B2 C PrPt2 B2 C ThPt2 B2 C YPt2 B2 C YRu2 B2 C LaPt1 5 Au0 5 B2 C PrPt1 5 Au0 5 B2 C YPt1 5 Au0 5 B2 C La0 5 Lu0 5 Ni2 B2 C Sc0 5 Lu0 5 Ni2 B2 C La0 5 Th0 5 Ni2 B2 C La3 Ni2 B2 N3 01 63 10 5 78 16 5 15 8 11 12 5 18 14 5 97 10 6 65 10 97 11 65 11 14 8 15 6 39 12 lists the superconducting transition temper atures of a number of borocarbides, and Table 9.4 provides various properties of the two borocarbide superconductors YNi2 B2 C and LuNi2 B2 C. A. Crystal Structure The RNi2 B2 C compound has the tetrag onal structure sketched in Fig. 9.17 in which staggered Ni2 B2 layers alternate with flat RC planes. Schematic presentations of struc tures for n = 1, 2, 3, and 4 are sketched in Fig. 9.18. They all have the same Ni2 B2 layres and RC or RN planes. The Ni atoms are in the center of distorted B4 tetrahedra which share edges to form slabs held in place by short linear B-C-B bridges, as indicted in Figs. 9.17 and 9.18. The bonding is partly ionic and partly covalent. The distance between nearby nickel atoms in the Ni2 B2 layers is slightly less than the nearest neigh bor distances in atomic nickel, and the Ni-B bonding has a strong admixture of a covalent character. The boron to carbon interatomic distance of 1.47Å suggests that these are dou ble bonds. The resulting rigid three dimen sional framework can accommodate various sizes of transition metal atoms R. Larger transition atoms increase the R-C separation in the plane, and compress the B4 tetrahe dra, thereby decreasing the thickness of the R2 B2 layer, and decreasing the c-parameter. Higher members of the RCn M2 B2 series, with n > 1, stack RC layers one above the other in an NaCl type arrangement, as indi cated in Fig. 9.18. The right hand side of Fig. 9.17 provides a more realistic view of the atom packing in the n = 1 structure. The borocarbides with odd-n have the body-centered tetragonal crystallographic space group I4/mmm, and those with even-n are in the primitive tetragonal space group P4/nmm which has a horizontal reflection plane at the center of the unit cell. The primi tive structures have one formula unit per unit cell, while the body centered structures have 244 9 UNCONVENTIONAL SUPERCONDUCTORS Table 9.4 Tc —superconducting transition temperature, Bc2 —upper critical ﬁeld at T = 0 Bcl —lower critical ﬁeld at T = 0 Bc —thermodynamical critical ﬁeld at T = 0 0—coherence length at T = 0 0—penetration depth at T = 0 0 Ginzburg-Landau parameter at T = 0 C—speciﬁc heat jump at Tc —normal state Sommerfeld constant, NEF —density of state at the Fermi level in states per eV and unit cell, F —Fermi velocity, ph —electron-phonon coupling constant, ∗ —Coulomb pseudopotential, D —Debye temperature, 0—quasiparticle energy gap at T = 0 l—mean free path, RRR—residual resistance ratio 300K/ T ≈ Tc TD —Dingle temperature. (compiled by Müller and Marozhuyi, 2001) Property YNi2 B2 C LuNi2 B2 C Property YNi2 B2 C LuNi2 B2 C Tc K Bc2 T Bc1 mT Bc T 0nm 0nm 0 CmJ mol−1 K−1 mJ mol−1 K −2 C/ Tc 15.5 11 30 0.23 8 10, 5.5 120, 350 15, 35 460 18.5 1.77 16.5 7.5,9 30, 80 0.31, 0.54 6 130, 71 22, 12 695 19.5, 35 2.21 NEF 1/eV F 105 ms−1 ph 4.31 0.85, 3.8, 4.2 0.9, 1.20 ≈ 0 1 0 13 490 2.2 2.1, 1.7 33 43 2.8 4.05 0.96 3.7, 4.2 0.75, 1.22 ≈ 0 1 0 13 360 2.2 2.2, 1.7 70, 29 27, 44 4 two formula units per unit cell, as is clear from Fig. 9.18. I4/mmm is also the space group of the thallium Tl2 Ba2 Can Cun+1 O2n+6 and bismuth Bi2 Sr2 Can Cun+1 O2n+6 series of cuprate high temperature superconductors, whereas cuprates with aligned CuO2 lay ers such as HgBa2 Can Cun+1 O2n+4 belong to primitive tetragonal space group P4/nmm which differs from P4/nmm adapted by evenn borocarbides. B. Correlations of Superconducting Properties with Structure Parameters A number of lanthanide nickel boro carbides superconduct when the diameter of the R atom is not too large, and their tran sition temperatures are listed in Table 9.5 together with the density of states at the Fermi level DEF , and the magnetic order ing temperature for ferromagnetic (F) and antiferromagnetic (A) compounds. To obtain correlations with the structure the parameter ∗ D K 0meV 0/KB Tc lnm RRR TD K c’ was defined by Baggio-Saitovitch (2001) as the length of the basic six atom RM2 B2 C group along the axial direction for every n in the general chemical formula RCn M2 B2 , which means not taking into account extra RC layers in compounds for n > 1. We see from Fig. 9.18 that c’ is always less than the lattice parameter c, and it has the special value c� = c/2 for n = 1. Figure 9.19 shows how the lattice parameters a and c defined in Figs 9.17 and 9.18 depend on the ionic radius of the transition ion R. We see from the figure that a increases approximately linearly with the radius for both n = 1 and n = 2 com pounds. In contrast to this the axial param eter c remains fairly constant for the n = 2 series, and decreases with an increase in the radius for the n = 1 series. The C-B and NiB distances remain approximately the same for different transition ion substitutions, and the decrease in c with an increase in a results from the distortion of the NB4 tetrahedra, and 245 IV BOROCARBIDES AND BORONITRIDES Figure 9.17 Unit cell (left) of the tetragonal structure (space group 14/mmm, D4h ”) of RNi2 B2 C, and the atom packing arrangement (right). The vertical z axis is a fourfold rotation axis 4 C4 , and the centrally located RC planes are horizonotal reflection planes m h . The unit cell also has vertical reflection planes v , horizontal two-fold axes 2 C2 , and inversion symmetry (i). (Godart et al., 1995; Nagarajan, 2001, Fig. 4; Drechsler et al., 2001, Fig. 1, with kind permission from Springer Science). the consequent reduction of the thickness of the Ni2 B2 layer. C. Density of States According to Eq. (7–119) of the BCS theory chapter a high value of the super conducting transition temperature Tc is asso ciated with a large density of states DEF at the Fermi level. The LDA band struc ture calculations carried out by Rosner et al. (2001) on YNi2 B2 C show a flat band at the Fermi level near the point X (110) and pro ceeding from X toward the origin (000) in the Brillouin zone (Winzer et al., 2001). The flatness of the band puts many k-values at the Fermi level so the density of states is high there. Fig. 9.20 plots the total den sity of states, and the partial densities of states for the electrons associated with the different atoms of YNi2 B2 C. The Ni-3d and Y-4d electrons make the main contribution to DEF at the Fermi level. Divis et al. (2001) determined the total density of states for the five compounds RNi2 B2 C with R = Er, Tm, Pr, Nd and Sm, and they found that the first two compounds (Er, Tm) which supercon duct have sharp peaks of D(E) at E = EF which resemble those shown in Fig. 9.20 for YNi2 B2 C. These peaks are missing for the three nonsuperconducting compounds. The 246 9 UNCONVENTIONAL SUPERCONDUCTORS Figure 9.18 Schematic drawings of the members of the structure series RCn Ni2 B2 and RNn Ni2 B2 for n = 1 2 3 and 4 formed by borocarbides and boroonitrides, respectively, with Pearson codes designated. Shading indicates relative height above the plane of the paper. Thick lines connect non-metal atoms and thin lines Ni and B atoms. Compounds with even-n contain one formula unit per vertical distance c, and those with odd-n have two formula units per vertical distance c. (Gladyshevskii in Poole, 2000, Fig. 6.21). Figure 9.19 Values of lattice constants a, c at room temperature for RNiBC and RNi2 B2 C compounds as a function of the ionic radius of the rare earth. (Baggio-Saitovitch et al., 2001, Fig. 2, with kind permission from Springer Science). density of states at the Fermi level for several borocarbides is listed in Table 9.5. We see from the data plotted in Fig. 9.21a that the density of states DEF and the superconducting transition temperature Tc fol low a similar dependence on the rare earth transition ion type R over the entire series of borocarbides RNi2 B2 C. The Hoppfield parameter = D EF �I2 �, where �I2 � is the average electron-phonon matrix element for atom , varies with R and across the borocarbide series in the manner shown in Fig. 9.21b. The dependence of !Ni for the nickel atoms shown at the top of Fig. 9.21b is similar to the dependences of DEF and Tc shown in Fig. 9.21a. We see from these two figures that the highest values of DEF Tc and !Ni occur for the higher atomic number 247 IV BOROCARBIDES AND BORONITRIDES values calculated by the scalar full potential local orbital method (Drechsler et al. 1999) with experimentally measured values. D. Thermodynamic and Electronic Properties The specific heat of the compound YNi2 B2 C is a sum of the Sommerfeld elec tronic term N T and the low temperature Debye term "D T3 , as was explained in Sect. VII of Chapter 4. C p = N T + #D T 3 Figure 9.20 Total and partial densities of states for YNi2 B2 C. The Fermi level is at the zero of energy. (Rosner et al., 2001, Fig. 2, with kind permission from Springer Science). range of the borocarbide series. Figure 9.22 shows how the transition temperature Tc varies with the total density of states at the Fermi level for various borocarbides, using the notation RCNiB2 for RNi2 B2 C. The figure compares The plot of experimentally measured val ues of Cp /T versus T2 shown in Fig. 9.23 exhibits the usual jump in value at the tran sition to the superconducting state, with the transition from the superconducting to the normal state occurring at lower temperatures for increasing applied magnetic fields, as shown on the figure. It is clear that the mag nitude of the jump in Cp also decrease with the temperature in the manner discussed in Sect. X. of Chapter 4. The intercept of the extrapolated normal state curve for T =⇒ 0 provides an evaluation of the Sommerfeld Table 9.5 Type of the ground state of RNi2 B2 C compounds: SC—superconducting, AFM—commensurate antiferromagnet structure, SDW—incommensurate antiferromagnet order (spin density wave), WFM—weak ferromagnetism; TN —magnetic order temperature, Tc —superconducting transition temperature and NEF —density of states at the Fermi level. (compiled by Müller and Narozhnyi, 2001) Compound Ground state TN K Tc K NEF CeNi2 B2 C PrNi2 B2 C NdNi2 B2 C SmNi2 B2 C GdNi2 B2 C TbNi2 B2 C DyNi2 B2 C HoNi2 B2 C ErNi2 B2 C TmNi2 B2 C YbNi2 B2 C Mixed valence (SC) AFM AFM AFM SDW SDW WFM AFM/SC AFM/SC SDW (WFM) SC SDW/SC Heavy fermion — 4.0 4.8 9.8 19.4 15.0 11.0 5 8 6 6.8 1.5 — (0.1) — — — — — 6.2, 6.4 8, 7.5 10.5 11 — 24 2 00 2 10 2 97 3 57 4 11 4 16 4 04 4 32 4 02 248 9 UNCONVENTIONAL SUPERCONDUCTORS Figure 9.21 Calculated density of states NEF and superconducting transition temperatures Tc on the atom type R in the borocarbide RNi2 B2 C (left panel), and Hoppfield parameters ! for the four atoms (right panel). (Hilscher et al., 2001, Fig. 1, with kind permission from Springer Science). Figure 9.22 Dependence of experimentally deter mined Sommerfeld constants (upper panel) and super conducting transition temperatures Tc (lower panel) on the density of states (DOS) at the Fermi level. Values from the literature (Dreschler et al., 1999) are denoted by open circles. (Dreschler et al., 2001, Fig. 2, with kind permission from Springer Science). constant N = 20 2 mJ/moleK 2 . Figure 9.24 shows how the transition temperature and the Sommerfeld constant vary with the con centration x in the mixed crystal system Yx Lu1−x Ni2 B2 C. The figure also presents the variation of the upper and lower limits of the upper critical field Bc2 versus the concentra tion x. This mixed crystal system was con venient for study because neither YNi2 B2 C nor LuNi2 B2 C exhibit any ordered magnetic behavior. Iavarone et al. (2001) used scanning tun neling microscopy and microwave surface impedance measurements to study LuNi2 B2 C thin films grown on several substrates. The STM data provided conductance G = dI/dV versus voltage V plots, and an I versus V plot obtained by integration is shown in the inset to Fig. 9.25. The conductance min ima provided the energy gap values plot ted in Fig. 9.25, and extrapolation to T = 0 gives the gap 20 = 4 0mV. Since the transi tion temperature Tc = 15 1K this corresponds to the dimensionless ratio 20 /kB Tc = 3 0, which is slightly less than the BCS value 3.5. 249 IV BOROCARBIDES AND BORONITRIDES Figure 9.23 Dependence of the specific heat cp /T of YNi2 B2 C on the temperature squared T2 for various applied magnetic fields. (Lipp et al., 2001, Fig. 2, with kind permission from Springer Science). very well. The figure lists the two parame ters used for making the BCS fit, namely the low temperature mean free path = 2 nm, and Tc = 14 5K. Hall effect measurements were carried out with the two compounds YNi2 B2 C and LuNi2 B2 C, and for each compound the Hall resistivity $xy was negative in both the nor mal and the superconducting states. Thus the sign reversal at Tc that is typical for the cuprates was not observed with these two borocarbides. Figure 9.24 Concentration dependence x of the Superconducting transition temperature Tc (upper panel), the Sommerfeld constant (middle panel), and the upper and lower bounds of the upper critical field Bc2 (lower panel) of Yx Lu1−x Ni2 B2 C. (Lipp et al., 2001, Fig. 4, with kind permission from Springer Science). In order to carry out microwave surface impedance measurements superconducting films of LuNi2 B2 C where made end plates of a sapphire Al2 O3 cylindrical resonator. Microwave frequency shift measurements f provided the values of the penetration depth T which are plotted in Fig. 9.26. It is clear that the data fit the theoretical BCS curve E. Magnetic Interactions The borocarbides are a class of com pounds in which magnetism and supercon ductivity can coexist. The magnetism arises from the magnetic moments of the transition ions R, which are proportional to the magne 1 ton numbers g %JJ + 1& /2 which are plotted in Fig. 9.27 for the rare earth series of atoms. These ions provide local magnetic moments in the lattice at sites between the Ni2 B2 layers (see Fig. 9.17), and are responsible for the weak ferromagnetism, antiferromagnetism or spin density waves that exist in some of the borocarbides. The magnetic transition 250 9 UNCONVENTIONAL SUPERCONDUCTORS Figure 9.25 Temperature dependence of the superconducting energy gap /0 for two different LuNi2 B2 C junctions. The inset gives a typical I-V curve with the gap positions indicated by arrows. (Iavarone et al., 2001, Fig. 2, with kind permission from Springer Science). Figure 9.26 Temperature dependence of the penetration depth shift from its value at 4.5K, T − 4 5K, for LuNi2 B2 C films grown on copper. The fit parameters to the BCS curve are indicated in the upper left. (Iavarone et al., 2001, Fig. 3, with kind permission from Springer Science). temperatures TM to these ordered magnetic states, as well as the nature of the type of magnetic order that is present in particular borocarbide compounds, are listed in Table 9.5. A measure of the effectiveness of local moments on the superconducting properties is given by the de Gennes factor gJ − 12 JJ + 1 (see Freudenberger et al., 251 IV BOROCARBIDES AND BORONITRIDES Figure 9.27 Dependence of the magneton number gJJ + 11/2 and the de Gennes factor gJ −12 JJ+1 on the individ ual atoms of the rare earth series. (Thanks are due to Michael A. Poole for preparing this figure). 2001, and Hilscher et al., 2001) plotted in Fig. 9.27 for the second half of the lanthanide series, where gJ , is the Landé gfactor, and J is the total angular momentum quantum number. For example gadolinium has a 6 S7/2 ground state so J = 7/2 gJ = 2, and gJ − 12 JJ + 1 = 15 75. The magnetic transition temperature TM correlates with the de Gennes factor in the manner shown in Fig. 9.28 which suggests that the coupling Figure 9.28 Dependence of the magnetic transition temperature TM on the de Gennes factor gJ − 12 JJ + 1 for three series of borocarbide compounds. (Baggio-Saitovitch et al., 2001, Fig. 7, with kind permission from Springer Science). 252 9 UNCONVENTIONAL SUPERCONDUCTORS between the 4f electrons of the R atoms involves the RKKY interaction whereby the magnetic interchange between these 4f elec trons takes place through the intermediary of magnetization induced in the conduction electrons. We see from the figure that the values of TM increase linearly with the de Gennes factor for n = 1 RNi2 B2 C, whereas the n = 2 (RNiBC) data exhibit a peak for dysprosium, as do the data for the RRh4 B4 compounds. The superconducting transition temper ature Tc also exhibits a regular variation with the de Gennes factor across the lan thanide series for the n = 1 compounds as shown in Fig. 9.29, and has linear correla tions with the crystallographic c’/a ratio, as indicated in Fig. 9.30. The latter correlations exist for the usual borocarbide compounds RCn M2 B2 , as well as for mixed borocar bides Rx� R1��−x Cn M2 B2 which contain two types of rare earth ions R� and R�� . The vari ation of TC and TM with concentration x of dysprosium in the series from nonmagnetic YNi2 B2 C to magnetic DyNi2 B2 C is shown in Fig. 9.31. Figure 4 of Müller and Narozh nyi (2001) highlights the linear variations of TC and TM on the de Gennes factor with opposite slopes. Hall probe measurements were carried out to determine how magnetic flux lines from an applied magnetic field penetrate into an ErNi2 B2 C superconducting crystal using the Hall sensor arrangement sketched at the top of Fig. 9.32. It is clear from the figure that at the temperature of 7.2K, which is between the magnetic ordering temperature TM � 6K and the superconducting transi tion temperature Tc = 10 8K, more magnetic flux penetrates into the sample in the center than at its edges. There is a large gradient of flux between the two sensors 2 and 11 immediately outside the sample and sensors 3 and 10, respectively, located just inside the edge of the crystal due to the shield ing currents of density J flowing near the edge, arising from the Maxwell curl expres sion o J = ' × B. In the absence of appre- Figure 9.29 Dependence of the magnetic transition temperature TM on the de Gennes factor gJ − 12 JJ + 1 for RNi2 B2 C compounds. (Baggio-Saitovitch et al., 2001, Fig. 8, with kind permission from Springer Science) IV BOROCARBIDES AND BORONITRIDES Figure 9.30 Dependence of the superconducting transition temperature Tc on the c’/a ratio for several series of borocarbide compounds. (Baggio-Saitovitch et al., 2001, Fig. 9, with kind permission from Springer Science). Figure 9.31 Dependence of the superconducting and the mag netic transition temperatures Tc and TM , respectively, on the concen tration x in the Y1−x Dyx Ni2 B2 C series of borocarbide compounds. (Hossain et al., 1999). 253 254 9 UNCONVENTIONAL SUPERCONDUCTORS Figure 9.32 Magnetic flux line profiles measured for increasing (open symbols) and decreasing (closed symbols) applied magnetic fields in an ErNi2 B2 C sin gle crystal. The Hall probe sensor positions 0 and 12 represent the applied magnetic field Bapp . (Dewhurst et al., 2001, Fig. 1, with kind permission from Springer Science). ciable pinning the flux lines that enter at the surface migrate toward the center and accu mulate there, as shown in the figure. Increas ing the applied field strength increases the accumulation toward the center, as shown. For a decreasing external field the density of flux lines is fairly uniform across the sample, as shown. When the measurements were repeated at the much lower tempera ture T = 2 75K < TM , where bulk pinning is appreciable, most of the flux entered at one side of the sample near the edge. For higher applied fields there was a second accumula tion of flux on the other side of the sample with an almost flux fee region between the two accumulations. When the external field was gradually decreased under these condi tions the flux remained more uniform across the sample, as was the case with the 7.2K measurements. F. Magnetism of HoNi2 B2 C Some borocarbides exhibit a complicated magnetic behavior, and HoNi2 B2 C is an exam ple. The temperature dependence of the resis tivity presented in Fig. 9.33 shows a sharp Figure 9.33 Temperature dependence of the resis tivity of HoNi2 B2 C (upper panel) in the presence of applied magnetic fields in the range from 0 to 0.3 T, showing the reentrant superconductivity near 6K. The neutron diffraction intensity results (lower panel) iden tify the presence of the commensurate, the spiral c∗ incommensurate, and the postulated a∗ incommensurate structures, sketched in Fig. 35, in the neighborhood of the near reentrant behavior. (Müller et al., 201, Fig. 8, with kind permission from Springer Science). drop to zero at the transition temperature of 7.8K in zero magnetic field. The applica tion of a magnetic field of 0.14T induces a near-reentrant behavior, namely a finite onset of resistivity below TC in a magnetic field near the magnetic ordering temperature of TM = 5 2K, and the application of higher fields increases further, as shown. The behavior is called near-reentrant because its onset requires the presence of an applied field. The specific heat plot of Fig. 9.34 con firms that there are additional phases in the sample. Müller et al. (2001) interpret these 255 IV BOROCARBIDES AND BORONITRIDES Figure 9.34 Temperature dependence of the spe cific heat Cp of a 2 mm × 3 mm × 0 1 mm HoNi2 B2 C monocrystal measured in zero magnetic field. The con tributions from the three phases that are present are indicated by arrows. (Müller et al., 2001, Fig. 2, with kind permission from Springer Science). reentrant data in terms of the magnetic struc tures sketched in Fig. 9.35. Structure (a) is commensurate with ferromagnetically aligned planes antiferromagnetically coupled to each other, and it occurs below 6–7K, as shown by the vertical dashed line in Fig. 9.33b. Figure 9.35b illustrates an incommensurate c∗ structure with a spiral arrangement of the spins along the c direction, called a spin wave state, which is present in the neighborhood of the reentrant state at 5.2K. The postulated incom mensurate structure a∗ sketched in Fig. 9.35c appears to be more closely related to the reen trant behavior than structure c∗ . If the Ho atoms are replaced by a small percentage of Y or Lu atoms the spiral c∗ structure dominates over the commensurate one of Fig. 9.35a, but there is very little change in structure a∗ at the onset of the near-reentrant behavior. Müller et al. (2001) suggest that the a∗ structure is associated with the Fermi surface nesting, and is closely related to enhanced pair-breaking induced by the magnetic field applied at the reentrant temperature TN . The compound HoNi2 B2 C also has metamagnetic phases with spin orderings ↑ ↑ ↓ and ↑ ↑ → which are intermediate between the ferromagnetic ↑ ↑ ↑ ↑ and anti ferromagnetic ↑ ↓ ↑ ↓ types, as well as a paramagnetic phase. Figure 9.36a presents a magnetic phase diagram in the applied mag netic field versus temperature plane when the Figure 9.35 Magnetic structures of HoNi2 B2 C determined by neutron diffraction: (a) com mensurate, (b) spiral incommensurate c∗ type, and (c) postulated incommensurate a∗ type. (Müller et al., 2001, Fig. 4, with kind permission from Springer Science). 256 9 UNCONVENTIONAL SUPERCONDUCTORS Figure 9.36 Magnetic phase diagrams of HoNi2 B2 C: (a) in the applied magnetic field versus temperature plane with the field applied along the tetragonal a axis, and (b) in the applied field versus the angle plane, where is the angle in the plane perpendicular to the c axis that the applied magnetic field makes with the magnetically easy [001] direction. The regions where the ferromagnetic ↑↑↑↑, antiferromagnetic ↑↓↑↓, metamagnetic ↑↑↓ and ↑↑→) and paramagnetic (para) phases are present are indicated (see Müller and Narozhnyi, 2001). (Canfield et al., 1996). field is applied along the tetragonal a axis. Figure 9.36b presents a magnetic phase dia gram in the applied magnetic field versus angle plane when the field is applied per pendicular to the tetragonal c axis, making an angle with respect to the magnetically easy [110] direction. Metamagnetic phases are also found in the borocarbide supercon ductors TbNi2 B2 C and DyNi2 B2 C. V. PEROVSKITES The main perovskites that superconduct are the two cubic compounds Ba1−x Kx BiO3−y and MgCNi3 and a series of lower symmetry perovskites BaPb1−x Bix O3 that exhibit superconductivity over part of their ranges of structural stability. In the first two sections we discuss the two cubic exam ples which differ markedly in their types of superconductivity, and then in the follow ing section we examine the lower symme try cases which have some affinities to the cuprates. A. Barium-Potassium-Bismuth Cubic Perovskite The compound Ba1−x Kx BiO3−y which forms for x > 0 25, crystallizes in the cubic pervoskite structure with a = 4 29Å (Cava et al., 1988; Jin et al., 1992; Mattheiss et al., 1988). K + ions replace some of the Ba2+ ions in the C site, and Bi ions occupy the E sites of Eq. (7.2) (Hinks et al., 1988b; Kwei et al., 1989; Pei et al., 1990; SalemSugui et al., 1991; Schneemeyer et al., 1988). Some oxygen sites are vacant, as indicated by y. Hinks et al. (1989) and Pei et al. (1990) determined the structural phase diagram (cf. Kuentzler et al., 1991; Zubkus et al., 1991). We should note from Table 8.1 that the potassium (1.33Å) and barium (1.32Å) ions are almost the same size, and that Bi5+ (0.74Å) is close to Ti4+ (0.68Å). Bismuth represents a mixture of the valence states Bi3+ and Bi5+ which share the Ti4+ site in a proportion that depends on x and y. The larger size (0.96Å) of the Bi3+ ion causes the lattice constant a to expand 7% beyond its cubic BaTiO3 value. Oxygen vacancies help to compensate for the larger size of Bi3+ . The compound Ba1−x Kx BiO3−y was not discovered until after the advent of high-Tc V PEROVSKITES (Cava et al., 1988; Mattheiss et al., 1988), and is of particular significance for several reasons. It is the first oxide superconductor without copper that has a transition temper ature above that of all the A15 compounds (≈ 40K for x ≈ 0 4). This high Tc occurs without the presence of a twodimensional metal-oxygen lattice. Features of Ba1−x Kx BiO3−y , such as the fact that it contains a variable valence state ion and utilizes oxygen vacancies to achieve charge compensation, reappear in the hightemperature superconducting compounds. Many experimental measurements have been made on this system, such as magne tization (Huang et al., 1991b; Kwok et al., 1989), photoemission (Hamada et al., 1989; Jeon et al., 1990; Nagoshi et al., 1991), x-ray absorption (Salem-Sugui et al., 1991), energy gap (Schlesinger et al., 1989), and the irreversibility line (Shi et al., 1991); a value for the isotope effect exponent ≈ 0 38 has been reported (Hinks et al., 1988b, 1989; W. Jin et al., 1991). Uemura et al. (1991) point out that Ba1−x Kx BiO3−y shares with the cuprates, Chevrel phase compounds, heavy fermions, and organic superconductors a transition temperature Tc which is high relative to its Ns /m∗ (carrier density-to-effective mass) ratio. B. Magnesium-Carbon-Nickel Cubic Perovkskite The perovskite compound MgCNi3 , with the unit cell depicted in Fig. 9.37, has carbon atoms in octahedral Ni sites, and the lattice constant a = 3 809. Mao et al. (2003) report the following characteristic parameters: Tc = 7 63K = 46 o = 4 6nm 0 = 213nm D = 280K = 9 2 mJ/moI-NiK2 Bc1 = 13mT Bc = 0 22T Bc2 = 14 4T 2/kB Tc = 4 6 C/ Tc = 2 3. In some cases other researchers have reported values (He et al. 2001; Rosner et al. 2002); which differ from 257 Figure 9.37 Unit cell of the perovskite compound MgCNi3 showing C in the center, Ni at the face centers and Mg at the apices of the cell. (Thanks are due to Michael A. Poole for preparing this figure). these, such as D = 440K by Zhi-Feng et al. (2002). Many of these are typical values which make MgCNi3 seem like a conventional superconductor, but in reality it is an exotic type. There are several reasons for this. Most perovskites are ionic compounds, like Ba1−x Kx BiO3−y which was discussed above, characterized by a strongly electronegative ion F− or O2− at the F site of Eq. 8-2, and positively charged ions at the C and E sites. In contrast to this MgCNi3 is an intermetallic compound with the metallic ion Ni at the site that is ordinarily occupied by electronegative fluorine or oxygen. The presence of the magnetic Ni ions at the F-sites makes the compound unstable toward ferromagnetism, and hole doping with Co or Fe can bring on the ferromagnetism. Hole doping with 3% Co or Fe lowers Tc by 1K, and electron doping with only 1% Cu destroys the superconductivity altogether. In addition there is a strong singularity in the density of electronic states just below the Fermi level which is associated with a van Hove singularity. Several properties such as specific heat, nuclear magnetic resonance relaxation rates, and tunneling measurements support an swave mechanism of superconductivity. In contrast to this the dominance of non s-wave 258 Figure 9.38 Penetration depth of MgCNi3 plotted versus the square of the temperature T2 . The fits of the data to the power laws T2 44 (dotted line) and T2 (solid line) are indicated. The inset shows the residuals for these fits. The standard s-wave curve is included for comparison purposes. (Prozorov et al., 2003, Fig. 3). pairing is supported by the appearance of a zero-bias conductance peak attributed to Andreev bound states (Mao et al. 2003), and the significant suppression of superconduc tivity brought about through the introduc tion of nonmagnetic disorder by irradiation (Karkin et al., unpublished). A more defini tive test is the comparison of the temper ature dependence of the penetration depth T = T − Tmin with the standard s-wave BCS behavior shown in Fig. 9.38 (Prozorov et al. 2003). This result indi cates the presence of low energy quasipar ticles and hence unconventional non s-wave superconductivity which is consistent with d-wave pairing in the presence of strong impurity scattering, although other uncon ventional mechanisms could possibly explain the observations. C. Barium-Lead-Bismuth Lower Symmetry Perovskite In their pioneering article Bednorz and Müller (1986) called attention to the dis covery of superconductivity in the mixedvalence compound BaPb1−x Bix O3 by Sleight and other researchers. (Bansil and Kaprzyk, 9 UNCONVENTIONAL SUPERCONDUCTORS 1991; Batlogg et al., 1988; Gilbert et al., 1978; Prassides et al., 1992; Sleight et al., 1975; Sleight, 1987; Suzuki et al., 1981a, b; Thorn, 1987). It was pointed out in these studies that the stoichiometric form of this compound presumably has the composition Ba2 Bi3+ Bi5+ O6 ; structurally, it is distorted perovskite. The metallic compound BaPbO3 is a cubic perovskite with the relatively large lattice constant (Wyckoff, 1964; cf. Nitta et al., 1965; Shannon and Bierstedt, 1970) listed in Table 8.3. At room tem perature �semiconducting BaBiO3 is� mon √ oclinic a ≈ b ≈ c/ 2 # = 90 17� , but close to orthorhombic (Chaillout et al., 1985; Cox and Sleight, 1976, 1979; cf. Federici et al., 1990; Jeon et al., 1990; Shen et al., 1989). These two compounds form a solid solution series BaPb1−x Bix O3 involving cubic, tetragonal, orthorhombic, and monoclinic modifications. Superconduc tivity appears in the tetragonal phase, and the metal-to-insulator transition occurs at the tetragonal-to-orthorhombic phase boundary x ≈ 0 35 (Gilbert et al., 1978; Koyama and Ishimaru, 1992; Mattheiss, 1990; Mattheiss and Hamann, 1983; Sleight, 1987; cf. Bansil et al., 1991; Ekino and Akimitsu, 1989a, b; Papaconstantopoulous et al., 1989). The compound BaPb1−x Bix O3 supercon ducts in the composition range 0 05 ≤ x ≤ 0 3 with Tc up to 13K. Many consider this system, which disproportionates 2Bi4+ → Bi3+ + Bi5+ in going from the metallic to the semiconducting state, as a predecessor to the LaSrCuO system. The highest Tc of 13K, came with the comparatively low carrier con centration of 2 × 1021 − 4 × 1021 (Than et al., 1980). The intensity of the strong vibrational breathing mode near 100 cm−1 was found to be proportional to Tc (Bednorz and Müller, 1986; Masaki et al., 1987). These results led Bednorz and Müller to reason that, “Within the BSC system, one may find still higher Tc ’s in the perovskite type or related metal lic oxides, if the electron-phonon interactions VI CHARGE-TRANSFER ORGANICS 259 and the carrier densities at the Fermi level can be enhanced further.” It was their deter mination to prove the validity of this conjec ture that led to the biggest breakthrough in physics of the latter part of the 20th century. Their choice of materials to examine was influenced by the 1984 article of Michel and Raveau (1984) on mixed-valent Cu2+ Cu3+ lanthanum-copper oxides containing alkaline earths. VI. CHARGE-TRANSFER ORGANICS Organic compounds and polymers are ordinarily considered as electrical insula tors, but it is now known that some of them are also good electrical conductors. For example, the organic compound 7, 7, 7, 8, -tetracyano-p-quinodimethane, called TCNQ for short, forms highly conducting salts with a number of compounds, and the properties of these and other organic con ductors were widely studied in the 1970s. Several of the TMTSF2 X charge-transfer salts superconduct under pressure, where TMTSF is an electron donor and the mono valent counter ion X − is, for example, − − − − − AsF− 6 CIO4 FSO3 PF 6 ReO4 SbF 6 , or − TaF6 . Figure 9.39 gives the structural formu lae of some of the principal organic molecules that play the role of electron donors in conduct ing and superconducting organics. Figure 9.40 shows the number and range of transition tem peratures associated with each. The electrical properties of organic con ductors are often highly anisotropic. TCNQ salts behave as quasi-one-dimensional conductors, and salts of other organ ics, such as bis(ethylenedithia)tetrathiafulvalene, called BEDT-TTF for short, exhibit low-dimensional behavior (Brooks et al., 1992; Fortune et al., 1992), with Tc reported in excess of 13K (Schirber et al., 1991). In addition, the superconducting properties of the organics, such as the critical fields and the coherence length, are often Figure 9.39 Structures of the principal molecules that form organic conductors and superconductors (Ishiguro and Yamaji, 1990, p. 2). Figure 9.40 Number of known organic supercon ductors classified by their molecular type as a function of Tc (Ishiguro and Yamaji, 1990, p. 263). anisotropic. For example, the triclinic com pound #–ET2 I3 has lower-critical fields Bc1 = 5 9, and 36 T along the a b, and c crystallographic directions, respectively 260 9 UNCONVENTIONAL SUPERCONDUCTORS Figure 9.41 Increase in the transition temperature Tc with time (Ishiguro and Yamaji, 1990, p. 259). and corresponding upper-critical fields Bc2 = 1 78, 1.70, and 0.08 T (Schwenk et al., 1985; Tokumoto et al., 1985). The coherence lengths are plane = 350 Å in the conducting plane and ⊥ = 23 Å (Ishiguro and Yamaji, 1990, p. 260). Other anisotropic properties are the plasma frequency (0.89 and 0.48 eV) and the effective mass m∗ /mc = 2 0 and m∗ /mc = 7 0) parallel to and perpendicular to the −110 direction, respectively (Kuroda et al., 1988). The transition temperatures Tc of the organics are in the range of typical classi cal superconductors as shown in Fig 9.41. Some of the organics, such as BEDT TTF, exhibit interesting similarities with the cuprates because of their layered structures (Farrell et al., 1990b). of 60 carbon atoms at the vertices of the dotriacontahedron (32-sided figure) that is sketched in Fig. 9.42. The term fullerene is used here for a wider class of compounds Cn with n carbon atoms, each of whose carbon VII. BUCKMINSTERFULLERENES The compound C60 , called buckminster fullerene, or fullerene for short, consists Figure 9.42 Structure of the buckminsterfullerene molecule C60 . 261 VII BUCKMINSTERFULLERENES Figure 9.43 The three resonant structures of the (hypothetical) tetrahedral com pound C4 . atoms is bonded to three other carbons to form a closed surface, with the system con jugated such that for every resonant struc ture each carbon has two single bonds and one double bond. The smallest possible com pound of this type is tetrahedral C4 , which has the three resonant structures shown in Fig. 9.43. Cubic C8 is a fullerene, and we show in Problem 17 that it has nine res onant structures. Icosahedral C12 is also a fullerene, but octahedral C6 and dodecahe dral C20 are not because their carbons are bonded to more than three neighbors. These hypothetical smaller Cn compounds have not been synthesized, but the larger ones, such as C60 C70 C76 C78 , and C82 , have been made and characterized. Some of them have several forms, with different arrangements of twelve pentagons and numerous hexagons. Clusters of buckminsterfullerenes, such as icosahedral C60 13 , have also been studied (T. P. Martin et al., 1993). The C60 molecule might be called the world’s smallest soccer ball! Because of its resemblance to the geodesic dome of architect R. Buckminster Fuller it has been referred to as buckminsterfullerene, or fullerene for short. The dual resem blances have prompted the sobriquet buck yball. All sixty carbon atoms are equiva lent so the 13 C NMR spectrum is a narrow singlet. There are 12 regular pentagons and 20 hexagons with three carbon to carbon band lengths that are slightly longer than the other three. The outer diameter of the C60 molecule is 7.10 Å and its van der Waals separation is 2.9 Å, so that the nearest-neighbor dis tance (effective diameter) in a solid is 10.0 Å. The bonds shared by a five-membered and a six-membered ring are 1.45 Å long, while those between two adjacent six-membered rings are 1.40 Å long. Above 260K these molecules form a face centered cubic lat tice with lattice constant 14.2 Å; below 260K it is simple cubic with a = 7 10 Å (Fischer et al., 1991; Kasatani et al., 1993; Troullier and Martins, 1992). When C60 is doped with alkali metals to form a superconductor it crystallizes into a face centered cubic lattice with larger octahedral and smaller tetrahedral holes for the alkalis. The C60 ions are ori entationally disordered in the lattice (Gupta and Gupta, 1993). The compound C60 is not itself a super conductor, but when alkali metals are added it becomes superconducting. The doped compound forms a face-centered cubic lat tice with a lattice constant of 10.04 Å. The structure has two tetrahedral holes (sites) and one octahedral hole per C60 molecule. If all of these holes are occupied by alkali met als A, the resulting compound is A3 C60 . An example of such a compound is K2 RbC60 with the potassiums in the smaller tetrahedral holes and the rubidiums in the larger octa hedral holes. The transition temperatures of several of these doped fullerenes are given in Table 9.6. The compound Rb3 C60 has been 262 9 UNCONVENTIONAL SUPERCONDUCTORS Compound K3 C60 K2 RbC60 Rb2 KC60 Rb3 C60 Rb2 CsC60 Cs2 RbC60 Cs3 C60 Tc K 19 22 25 29 31 33 47 found to have an isotope effect exponent = 0 37 (Ramirez et al., 1992a). VIII. SYMMETRY OF THE ORDER PARAMETER IN UNCONVENTIONAL SUPERCONDUCTORS a. Hole-doped high-Tc cuprates To our knowledge, the first penetra tion depth measurement to claim non s-wave superconductivity was that of Gross et al. (Gross, Chandrasekhar et al. 1986; GrossAlltag, Chandrasekhar et al. 1991) on a heavy fermion material, UPt 3 . Those authors observed power-law behavior of the pene tration depth, T − 0 = ∼ T n with the exponent n = 1 2 3 depending on the mutual orientation of the vector potential to a p-wave gap vector, and originating from different nodal structures (nodal points and lines) in a 3D Fermi surface. Early penetration depth measurements in high-Tc cuprates claimed either s-wave pairing, probably due to insufficient sensi tivity, or T 2 behavior, due to poor qual ity samples. Microwave measurements on single crystals YBaCuO by Hardy et. al. (Hardy, Bonn et al. 1993) were the first to show the linear T dependence characteristic of line nodes. By now, this linear variation has been observed in several copper oxides. In Figure 9.44 we show data for a single crystal of optimally doped YBaCuO, mea sured with a tunnel diode oscillator at a fre quency of 12 MHz. The superfluid density 1.00 150 λa 0.95 λb 0.90 ρs,a 0.85 0.80 100 50 Δλ [Å] The early suggestion that high temperature superconductors might exhibit unconventional, d-wave pairing, (Annett, Goldenfeld et al. 1991; Monthoux, Balatsky et al. 1991) has lead to a wide variety of new experimental probes with sensitivity sufficient to test this hypothesis. The pioneering work of Hardy and coworkers demonstrated that high resolution measure ments of the London penetration depth could detect the presence of nodal quasiparticles characteristic of a d-wave pairing state (Hardy, Bonn et al. 1993). Since that time, a large number of new superconductors have been discovered, many of which exhibit nontrivial departures from BCS behavior. For some further reading, the reader is encouraged to explore the following articles: (Desirant and Shoenberg 1948; Carbotte 1990; Van Harlingen 1995; Annett 1997; Hardy, Kamal et al. 1998; Klemm 1998; Maki 1998; Brandow 1999; Timusk and Statt 1999; Tsuei and Kirtley 2000; Carbotte and Marsiglio 2003). A. Symmetry of the Order Parameter in Cuprates ρs,i = [λ i(0)/λ i(T)]2 Table 9.6 Transition Temperature Tc of some Alkali Metal-Doped C60 Compounds ρs,b 0 0 5 10 15 20 20 30 T [K] Figure 9.44 Linear temperature dependence of the superfluid density and penetration depth in clean YBCO crystal. 263 VIII SYMMETRY OF THE ORDER PARAMETER IN UNCONVENTIONAL SUPERCONDUCTORS $s and are shown with the ac field par allel to both the a and b crystalline axes. $s is linear over a substantially wider range than , illustrating the point made earlier that these two quantities have the same T dependence only asymptotically as T → 0. For the optimally doped sample shown here, d/dT ≈ 4 2 Å/K in close agreement with the microwave data. Remarkably, this lin ear variation indicative of nodal quasipar ticles has been found to persist, relatively unchanged, even in extremely underdoped YBaCuO samples (Hoessini, Broun et al. 2004). This result remains one of the mys teries of superconductivity in the copper oxides (Lee and Wen 1997; Sheehy, Davis et al. 2004). b. Electron-doped cuprates The situation in electron-doped cuprates has been far more controversial, probably owing to the difficulty in growing high qual ity single crystals. Early microwave data in Nd2−x Cex CuO4−y (NCCO) down to 4.2 Kelvin were interpreted within an s-wave model (Anlage, Wu et al. 1994). However, Cooper suggested that the spin paramag netism of Nd3+ ions could be masking a power law temperature dependence expected if the material were d-wave (Cooper 1996). Lower temperature measurements on single crystals of NCCO clearly showed a vary large spin paramagnetic effect on the pen etration depth below 4 K, as we describe later (Alff, Meyer et al. 1999; Prozorov, Giannetta et al. 2000; Prozorov, Giannetta et al. 2000). Additional measurements on nonmagnetic Pr 2−x Cex CuO4−y (PCCO) down to 0.4 K showed a superfluid density varying as T 2 . Our data are shown in Figure 9.45, for several crystals. Data for Nb, a fully gapped s-wave superconductor, are shown for com parison. The quadratic power law is consistent with a d-wave pairing state exhibiting unitary limit impurity scattering, as we discuss later (Hirschfeld and Goldenfeld 1993, Prozorov, Nb data 1.0 isotropic s-wave 0.9 ρs 0.8 0.7 0.0 different PCCO crystals 0.1 0.2 0.3 (T/Tc)2 Figure 9.45 Superfluid density in three PCCO crys tals plotted versus T/Tc 2 to emphasize dirty d-wave behaviour. Data for Nb obtained in the same apparatus are also shown, along with the expected behavior for an isotropic s-wave superconductor. 2000 #202; Kokales, Fournier et al. 2000; Prozorov, Giannetta et al. 2000). Coincident measurements of half-integral flux quanta in PCCO films (Tsuei and J.R. Kirtley 2000) also gave evidence for d-wave pairing in PCCO. Later mutual inductance measure ments on PCCO thin films have shown a variety of temperature dependencies rang ing from T 3 to T and, more recently, expo nential, depending upon the method of film growth and the presence of a buffer layer (Kim, Skinta et al. 2003). Our own measure ments on laser ablated thin films of PCCO continue to show a power law behavior that depends upon the oxygen doping level (Snezhko, Prozorov et al. 2004). Figure 9.46 shows data for optimally doped PCCO film and the fit to the disordered d-wave behavior, Eq.(Hirschfeld), which apparently describes the data very well. To avoid possible demagnetizing effects in the H � c orientation, we also measured the PCCO films with H � ab– plane. For films of order or less in thickness, the signal is very weak and the data is somewhat noisy, as shown in the inset. Nonetheless, to the best of our knowledge, the inset to Figure 9.46 is the first reported measurement of a thin film in such an orientation. The data are fully 264 9 UNCONVENTIONAL SUPERCONDUCTORS Pr1.85Ce0.15CuO4–y film 1.00 BCS Δ/ Tc = 0.43 Prozorov, Giannetta et al. 2000; Prozorov, Giannetta et al. 2000). 0.95 ρs B. Organic Superconductors 300 0.90 PCCO film, H || ab-plane PCCO single crystal 0.85 Δλ(Å) 200 100 0 0.0 0.80 0.0 0.1 0.2 0.3 0.4 T/Tc 0.1 0.2 BCS Δ/ Tc = 1.76 0.3 0.4 T/Tc Figure 9.46 (main frame) Superfluid density in opti mally doped PCCO film measured in with H�c axis; s-wave BCS behaviour is shown by dashed lines, while a fit to Eq. (Hirschfeld) is shown by solid line. The inset shows a comparison between single crystal (solid line) and thin film data, the latter measured in the H�ab – plane orientation. A standard BCS curve is also shown. consistent with previous measurements on single crystals. Tunneling measurements in PCCO show zero bias conductance peaks. These are now believed to arise from Andreev bound states (discussed later) and are thus direct evi dence for unconventional pairing. However, the presence of these states appears to depend upon doping so s-wave pairing for some range of parameters is not ruled out (Biswas, Fournier et al. 2002). A large number of and experimental and theoretical works cur rently support d-wave pairing in the electrondoped cuprates. Raman spectroscopy (Liu, Luo et al. 2005; Qazilbash, Koitzsch et al. 2005), ARPES (Armitage, Lu et al. 2001; Matsui, Terashima et al. 2005) specific heat (Yu, Liang et al. 2005) and Hall effect (Lin and Millis 2005) are all consistent with the dwave picture. A fuller discussion of this issue is outside the scope of this chapter. We point out that precision penetration depth measure ments were the first to call into question the s-wave picture of superconductivity in these materials (Kokales, Fournier et al. 2000; Probably the most thoroughly stud ied organic superconductors belong to the class generically referred to as -ET2 X (Ishiguro, Yamaji et al. 1998; Kondo and Moriya 1998; McKenzie 1998; Schmalian 1998; Louati, Charfi-Kaddour et al. 2000). These are highly anisotropic, nearly two dimensional layered superconductors with parameters in the extreme Type II limit. NMR measurements show evidence of a spin gap and d-wave pairing (Mayaffre, Wzietek et al. 1995; Soto, Slichter et al. 1995), some what similar to the situation in the copper oxides. We discuss two of the most widely studied compounds, -ET2 CuNCS2 with Tc = 10 4 K and -ET2 Cu%NCN2 &Br with Tc = 11 6 K. Both materials superconduct under atmospheric pressure. Early penetra tion depth measurements claimed s-wave pairing, but lower temperature and higher precision measurements by Carrington et al. down to 0.35 K provided strong evidence for nodal quasiparticles (Carrington, Bonalde et al. 1999). That data are shown in Figure 9.47. The distinction between penetration depth and superfluid density is particularly important here, since changes rapidly with temperature, and its absolute value is large. The measured quantity is = T − 0 36 K, from which the in-plane super fluid density is calculated for several choices of T ≈ 0. SR measurements typically give 0 ≈ 0 8 m (Le, Luke et al. 1992). For any plausible choice of 0 the data clearly follow a power law. Fits correspond to the dirty d-wave form discussed earlier and yield values of the impurity crossover T ∗ ≈ 0 8 K. The fact that the measurements extend down to T/TC = 0 03 rules out all but an extremely small energy gap. By now, a large number of other measurements VIII SYMMETRY OF THE ORDER PARAMETER IN UNCONVENTIONAL SUPERCONDUCTORS also indicate d-wave pairing (Behnia, Behnia et al. 1998; Arai, Ichimura et al. 2001; Izawa, Yamajuchi et al. 2002; Printeric, Tomic et al. 2002). However, there is still no consensus on the location of the purported nodes on the Fermi surface. In addition, some specific heat measurements do show evidence for an energy gap in these materials (Elsinger, Wosnitza et al. 2000). Despite this very strong evidence for nodal quasiparticles, the superfluid density T/Tc ρ = [λ(0)/λ(T)]2 1.0 0 0.05 0.1 0.15 0.2 1.8 1.3 1.0 0.8 0.9 0.8 λ (0) 1.0 0.8 0.6 0.7 0.4 0.2 0.0 0.6 0 0 2 4 6 8 10 12 0.5 1 1.5 2 2.5 T [K] Figure 9.47 In plane superfluid density for differ ent choices of (0) in -ET2 Cu%NCN2 &Br. Fits to the data use the dirty d-wave interpolation formula. The inset shows data up to Tc (Carrington, Bonalde, et al. 1999). 100 a a 10–1 Δλ [μm] 0.2 10–2 d 0.03 0.1 [T/Tc] b c 0.3 d 0.1 0 0 0.02 0.04 0.06 0.08 0.1 [T/Tc]1.5 Figure 9.48 for two samples of -ET2 Cu%NCN&2 Br (a,b) and two samples -ET2 CuNCS2 (c,d) plotted versus T 3/2 (Carrington, Bonalde et al. 1999). 265 is never purely linear, and in fact exhibits an interesting regularity. Figure 9.48 shows the penetration depth itself plotted versus T 1 5 . Over nearly a decade of tempera ture, samples of both -ET2 Cu%NCN2 &Br (a,b) and samples -ET2 CuNCS2 (c,d) fit this power law with extraordinary pre cision. Many samples that have been mea sured since that time show precisely the same behavior. Although the dirty d-wave func tional form can, with an appropriate choice of parameters, appear as a T 1 5 power law, the fact that every sample measured obeys this law would imply a remarkable regular ity in the impurity crossover temperature T ∗ . We have observed no such regularity in the copper oxides. At the time the data were reported, Kosztin et al. had proposed a Bose Einstein/BCS crossover theory for the under doped copper oxides (Kosztin, Chen et al. 1998; Chen, Kosztin et al. 2000). They pre dicted a superfluid density that would vary as T + T 1 5 , the new T 1 5 component com ing from finite momentum pairs, similar to a Bose-Einstein condensate. However, when plotted as a superfluid density, our data do not fit this power law. Interestingly, more recent measurements on the heavy fermion compound CeCoIn5 also exhibit the same ∝ T 1 5 behavior (Özcan, Broun et al. 2003). They speculate that the fractional power law behavior may come from a renor malization of parameters near to a quantum critical point. Several different experiments indicate that CeCoIn5 is also a d-wave super conductor, so the experimental situation is rather analogous to the organics. Chia et al. also observed the same power law in this material and believed it can be explained by nonlocal effects (Chia, Van Harlingen et al. 2003). However, nonlocality is unlikely to be relevant for organic superconductors, which exist in an extreme Type II limit. -ET2 Cu%NCN2 &Br and -ET2 CuNCS2 are highly anisotropic layered superconductors. By orienting the ac measurement field along the conducting planes, 266 9 UNCONVENTIONAL SUPERCONDUCTORS the magnetic response is dominated by interplane currents which penetrate in from the edges on a length scale ⊥ , the interplane penetration depth. In general, there is no sim ple formula for ⊥ involving just the gap function and the Fermi surface parameters. This is because ⊥ depends on both the pairing state and the details of the transport between conducting planes. If this transport is coherent, then $⊥ = ⊥ 0/⊥ T 2 will exhibit the same temperature dependence as $� = ⊥ 0/� T 2 . If not, $⊥ will gener ally follow a higher power law than $� in a d wave superconductor. The precise exponent can vary from n = 1 to n = 3 and in special cases, as high as n = 5 (Graf, Palumbo et al. 1995; Radtke, Kostur et al. 1996; Hirschfeld, Quinlan et al. 1997; Sheehy, Davis et al. 2004). In most copper oxides one has 1 − $⊥ ∝ T 2–2 5 , indicating incoherent transport between the conducting planes (Hoessini, Broun et al. 2004). Figure 9.49 shows both ⊥ and the superfluid density $⊥ in -ET2 CuNCS2 . ⊥ 0 � 100 m is sufficiently large that it can be determined directly from the fre quency shift of the resonator, as described earlier. We find that 1 − $⊥ ∝ T 1 3–1 5 . Fit ting the inplane superfluid density to a pure power law we obtain 1 − $� ∝ T 1 2–1 4 , which has very nearly the same exponent. (The latter depends somewhat on the choice 1.00 128 κ -(ET)2Cu(SCN)2 ρ = 1–0.025 T 0.95 124 122 λ (μm) interplane ρs 126 1.49 of � 0.) Coherent interplane transport is somewhat surprising given the extreme anisotropy of the ET-class of organic super conductors. Nevertheless, recent magnetore sistive measurements do demonstrate a small but but unequivocal three dimensional char acter to the Fermi surface. It should also be stressed that the power law variation shown in Figure 9.49 is another very clear demon stration of nodal quasiparticles in the organic superconductors. ⊥ 0 is so large relative to ⊥ that $⊥ ≈ 1 − 2⊥ T/⊥ 0 is an excellent approximation within the temper ature range over which the gap is constant. Therefore, the power law exponent is not particularly sensitive to the choice for ⊥ 0. There is no hint of an energy gap down to the lowest temperatures measured. C. Inﬂuence of Bandstructure on Superconductivity Even conventional s-wave superconduc tors can exhibit unconventional behaviour if the bandstructure has certain peculiarities. In general, in most superconductors, there is more than one sheet of the Fermi sur face. If those were completely independent, one would expect possibly different super conducting gaps with their own Tc and Hc . Usually however, significant interband scat tering smears this out resulting in a single effective gap. However, when the dimension ality of different sheets of the Fermi surface differs significantly, the interband scattering is reduced and two-band superconductivity becomes possible. Another important ingre dient is the density of states contributed by each sheet of the Fermi surface. 0.90 120 0.0 0.5 1.0 1.5 2.0 2.5 118 3.0 T (K) Figure 9.49 Interplane penetration depth and super fluid density for -ET2 Cu%SCN&2 . Fits are to pure power laws. a. MgB2 There is by now considerable evidence that MgB2 is a two-band superconductor. By this we mean that each Fermi surface sheet possesses a different gap function. Although strong interband scattering leads to a sin gle Tc , the gap magnitudes on the and VIII SYMMETRY OF THE ORDER PARAMETER IN UNCONVENTIONAL SUPERCONDUCTORS surfaces are significantly different. This was first observed in tunneling measure ments where two conductance peaks were observed, one of which was more easily suppressed in a magnetic field (Schmidt, Zasadzinski et al. 2002; Zalk, Brinkman et al. 2006). Penetration depth measure ments on MgB2 wires indicated s-wave pair ing but with a gap magnitude significantly smaller than the weak coupling BCS value (Prozorov, Giannetta et al. 2001). Subse quent penetration depth measurements on single crystals by Manzano et al. were fit to a two-band -model discussed previously (eqs. (27,28)). The data and fits are shown in Figure 9.50. The deviation from a sin gle gap picture is very clear. It was found that the larger gap on the sheet is = 75 ± 5 k and the -band gap is = 29 ± 2K (Manzano, Carrington et al. 2002). Mea surements by Fletcher et al. determined the temperature dependence of the anisotropy in the interplane versus in-plane penetration depth (Fletcher, Carrington et al. 2005). It was found that at low temperatures c /ab is approximately unity, and it increases to about 2 at Tc . This is opposite to the tem perature dependence of the coherence length anisotropy, which decreases from about 6 to about 2. This observation has provided firm quantitative evidence for a two-gap nature of superconductivity in MgB2 . Figure 9.50 provides a good example of using two components of the superfluid den sity and the full temperature range BCS treat ment to show the two-gap nature of MgB2 single crystals. So far, MgB2 remains the only superconductor with two confirmed dis tinct gaps, although both vanish at the same temperature. b. NbSe2 Structurally similar to MgB2 NbSe2 was also believed to have two distinct gaps. The recent penetration depth measure ments performed on different single crys tals (Fletcher, Carrington et al. 2006) do not support this conjecture, and lead to the conclusion that there is a single anisotropic s-wave gap, or there is some possibility of two slightly different gaps on 2D Nb sheets of the Fermi surface, but not on the Se 3D sheet (which appears to be fully gapped). Figure 9.51 plots the in-plane London penetration depth in single crystal NbSe2 A weak coupling BCS behavior with a ρ = [λ (0)/λ(T)]2 ρσ 0.8 Δ(T)/Δ(0) 1 1 0.6 ρBCS ρa 0.4 ρc 0.2 ρπ π σ BCS 0 0 T/Tc 1 0 0 5 10 15 267 20 25 T [k] 30 35 40 Figure 9.50 Two components of the superfluid density in single crystal MgB2 (from Fletcher, Carrington et al. 2005). Solid lines are fits to the -model. The inset shows the temper ature dependencies of the two gaps used for the fits. 268 9 UNCONVENTIONAL SUPERCONDUCTORS 20 λ (Å) 10 1800 0.8 5 0 1600 1400 0 ρab δ = 32.8 μm ρ = 5.4 μ Ω⋅cm λ ( μ)m 2000 0 5 10 15 T (K) ρC Δ/Δiso 1.5 0.6 1.0 0.5 0.4 isotropic s-wave c 0.0 –0.5 Δ 0 / Tc = 1.27 1 Tc = 6.2 K 1.0 Tc = 7.34 K skin depth 15 ρ = λ2(0)/λ2(T) 2200 –1.0 0.33 Tc 2 3 0.2 –1.0 –0.5 0.0 0.5 1.0 b 4 T (K) Figure 9.51 London penetration depth in 2H-NbSe2 . Inset shows full temperature range and extracted from the skin depth resistivity. slightly reduced gap is indicated. The reduced gap is due to anisotropy. A detailed analysis is given elsewhere (Fletcher, Carrington et al. 2006). Stronger interband scattering and a significantly differ ent density of states on different energy bands are probably responsible for such behaviour. Another aspect to consider is the stack ing sequence of 2H-NbSe2 , where lay ers are held together only by van der Waals forces. This makes the material closer to layered superconductors where interlayer transport makes the penetration depth appear more gapped than in-plane response (at least in the case of d-wave super conductors (Radtke, Kostur et al. 1996; Hirschfeld, Quinlan et al. 1997; Sheehy, Davis et al. 2004)). The anisotropic electro magnetic response has been analysed in Ref. (Dordevic, Basov et al. 2001). An additional feature of NbSe2 is the incommensurate charge-density wave state observed below 33 K. Currently there is no clear understand ing how it might affect the superconducting properties. c. CaAlSi A good example of an anisotropic 3D s-wave superconductor is CaAlSi, isot sructural with MgB2 but exhibiting almost ideal weak-coupling BCS behaviour with, an –1.5 0.0 0.0 0.2 –1.0 0.5 0.0 0.5 a 1.0 0.4 0.6 0.8 1.0 T/Tc Figure 9.52 Two components of the superfluid den sity measured in single crystal CaAlSi. Solid lines show the results of a full 3D BCS fit with an ellipsoidal gap shown in the inset as the fit parameter. anisotropic 3D gap. In this system both com ponents of the superfluid density were mea sured, and full temperature range BCS cal culations with anisotropic ellipsoidal gap as the fitting parameter were carried out. Figure 9.52 shows the result of simulta neous fitting two components of the super fluid density in a lower-Tc version of the CaAlSi superconductor. In higher – Tc sam ples the anisotropy is greatly reduced and most likely the highest – Tc material is an isotropic weak coupling BCS superconduc tor (Prozorov, Olheiser et al. 2006). Most probably the single gap is due to significant interband scattering and the 3D nature of the in-plane and interplane bands. D. Some Other Superconductors a. Heavy-fermion superconductors In a set of remarkable low-temperature measurements using a SQUID magnetome ter, Gross et al. obtained power law temperature dependencies of T with different exponents corresponding to dif ferent orientations of the sample in the heavy fermion superconductor UBe13 (Gross, Chandrasekhar et al. 1986; Gross-Alltag, Chandrasekhar et al. 1991). The measure ments provided strong evidence for p-wave 269 VIII SYMMETRY OF THE ORDER PARAMETER IN UNCONVENTIONAL SUPERCONDUCTORS ρ⊥(T) 2000 Δλ(T) (Å) 0.5 1500 1000 Δλ⊥ 0.0 0.0 0.5 1.0 1.5 2.0 2.5 Δλll 500 0 0.2 0.4 0.6 0.8 1.0 1.2 1.4 T (K) Figure 9.53 Magnetic penetration depth in two ori entations in heavy fermion superconductor, CeCoIn5 . Reprinted with permission from Ref. (Chia, Van Harlin gen et al. 2003). Copyright: American Physical Society. superconductivity for which the theoreti cal description is complicated by the vector nature of the superconducting gap (it depen dence on the mutual orientation of the vector potential and the crystal axes). The general consensus seems to be that these materials have p-wave symmetry of the order parame ter (Joynt and Taillefer 2002). A more recent addition to the heavy fermion superconducting family is CeCoIn5 . Figure 9.53 shows the penetration depth measured in two orientations in this mate rial taken from Ref. (Chia, Van Harlingen et al. 2003). Arguing that the effect of impu rities should be visible on both components (and, apparently it is not seen in ⊥ T ), it was concluded that a quadratic variation of the in-plane component is due to a non-local response of a superconductor with nodes. A strong-coupling correction have also been suggested. of the magnetic penetration depth and pair ing symmetry is open, and we are currently working on its resolution. In magnetic boro carbides the penetration depth has a large influence on the underlying magnetic struc ture and therefore it is useless for establish ing the pairing symmetry. However, these systems are very interesting from the point of view of the interplay between supercon ductivity and magnetism (Ghosh, Krishna et al. 1997; Chia, Bonalde et al. 2001; Chia, Cheong et al. 2005). c. Sr2 RuO4 The penetration depth in Sr2 RuO4 as shown in Fig. 9.54 does not follow a stan dard s-wave behavior. Moreover, measure ments of the NMR Knight shift across the superconducting transition had indicated a triplet pairing state. In that case, the gap is a vector and the data analysis is very dif ficult. Current debates are between various versions of p- and f- wave pairing (Annett 1999; Bonalde, Yanoff et al. 2000; Won and Maki 2000). 1.0 0.8 0.6 0.4 1.00 λ2(0)/λ2(T) 1.0 λ2(0)/λ2(T) 2500 0.96 0.2 0.92 0.00 b. Borocarbides At some point it seemed that non magnetic borocarbides are s-wave materi als, maybe with some degree of anisotropy. However, most of the single crystals had residual metallic flux, which could mask the true behaviour. Annealing in vacuum could change the behaviour as well. The question 0.0 0.0 0.2 0.02 (T/Tc)2 0.04 0.4 0.6 0.8 1.0 T/Tc Figure 9.54 Superfluid density in Sr2 RuO4 . Lines show various fits and the Authors concluded that there is a nodal gap and nonlocal quadratic corrections (see Section). Reprinted with permission from Ref. (Bonalde, Yanoff et al. 2000). Copyright: American Physical Soci ety. 1.0 6 0.8 0.6 λ Δ (Å) d. MgCNi3 The recently discovered non-oxide perovskite superconductor MgCNi3 (He, Huang et al. 2001) is viewed as a bridge between high-Tc cuprates and conventional inter metallic superconductors. This material is close to a magnetic instability on hole dop ing. It was suggested that strong magnetic fluctuations may lead to unconventional pair ing (Rosner, Weht et al. 2002). As far as pairing symmetry is concerned, the current experimental situation is controversial. On one hand, evidence for conventional s-wave behavior is found in specific heat measure ments (Lin, Ho et al. 2003), although the authors disagree on the coupling strength. The T1 nuclear spin-lattice relaxation rate of 13 C, seems to exhibit a behavior character istic of an s-wave superconductor (Singer, Imai et al. 2001). On the other hand, a zerobias conductance peak (ZBCP) attributed to Andreev bound states has been observed, and it was argued that the observed ZBCP could not be due to intergranular coupling or other spurious effects (Mao, Rosario et al. 2003). Nonmagnetic disorder intro duced by irradiation was found to signif icantly suppress superconductivity (Karkin, Goshchitskii et al. 2002). Such suppression is not expected in materials with a fully devel oped s-wave gap, and is a strong indica tion of an order parameter with nodes. The oretical calculations support this conclusion (Granada, da Silva et al. 2002). Furthermore, recent theoretical developments predict the possibility of a unique unconventional state (Voelker and Sigrist 2002), which might rec oncile apparently contradictory experimental observations. It is very difficult to experimentally identify the non-exponential contribution of low-energy quasiparticles due to the pres ence of nodes in the superconducting gap on the Fermi surface. In the case of thermal measurements, this electronic contribution is masked by a large phonon contribution. For electromagnetic measurements, sensitivity is 9 UNCONVENTIONAL SUPERCONDUCTORS Δλ (normalized) 270 0.4 MgCNi3 4 2 0 0.00 Nb 0.05 0.10 0.15 (T/Tc)2 0.2 0.0 0.0 Nb 0.2 0.4 0.6 0.8 1.0 T/Tc Figure 9.55 Penetration depth measured in MgCNi3 superconductor. The main frame compares the full tem perature range to a conventional s-wave (Nb). The inset shows the low temperature regime which clearly indicats a quadratic (non-exponential) behavior of the penetra tion depth. typically a problem. Precise measurements of the London penetration depth are therefore very important see Fig. 9.55. IX. MAGNETIC SUPERCONDUCTORS A. Coexistence of superconductivity and magnetism Coexistence of superconductivity and magnetism is one of the most interesting sub jects in the physics of correlated electrons. Many review books and articles have been published on this subject (Abrikosov, 1988, Bulaevskii, 2984, Buzdin and Bulaevskii, 2986, Fischer and Peter, 1973, Izyumov and Skryabin, 1974, Khan and Raub, 1985, Kulic, 2006, Maple, 1983, Matthias, 1979, Nakanishi, 1984, Whitehead et al., 1985, Fischer 1990). Indeed, in a simple pic ture, ferromagnetism cannot coexist with sin glet pairing, because of the antiparallel spin arrangement. Triplet pairing, on the other hand can coexist with ferromagnetism, and this has been discussed (Matthias, 1979), but there are only few superconductors where triplet pairing is realized and it is not clear if there is an example of a bulk 271 IX MAGNETIC SUPERCONDUCTORS superconductors such as layered antifer romagnetic Sm1 85 Ce0 15 CuO4−y or heavy fermion CeCoInx . Finally, the most interesting case is when TFM < Tc . In this case ferromagnetism develops on a superconducting background, and close to the ferromagnetic transition the spin structure is significantly modified either by helicoidal rotation or by split ting into domains. The exact structure of the coexisting phase is determined by many factors, including the magnetic and super conducting anisotropies. There are only a few well-established examples of ferromag netic superconductors – the best known and most studied are HoMo6 S8 and ErRh4 B4 (Abrikosov, 1988, Buzdin and Bulaevskii, 1986, Buzdin et al., 1984). An example of the AC magnetic susceptibility in the latter in various applied magnetic fields is shown in Figure 9.56. In zero applied magnetic field, both nor mal state – superconductor (SC) and super conductor – ferromagnet transitions are very sharp. However, when a magnetic field is applied the behavior in the mixed state is non-trivial, closer to the ferromagnetic tran sition. An apparent delay or suppression of a superfluid density may be related to a field – 8500 Oe ErRh4B4 single crystal 0.00 –0.25 4πχ ferromagnetic triplet superconductor. Most superconductors are singlet (including s, d and g pairing states, and thus all con ventional superconductors, borocarbides and cuprates). Therefore it is not surprising that the majority of known magnetic supercon ductors are antiferromagnetic. There are dis cussions of so called weak ferromagnetic superconductors, such as ruthenocuprates Rz−( Cex RuSr2 Cu2 Oy (R=Eu and Gd), but it is still unclear whether this is bulk super conductivity (Felner, 2003). A more estab lished example is the low-temperature phase in ErNi2 B2 C (Canfield et al., 1997, KawanoFurukawa, 2001). Ferromagnetism, however, can coexist with superconductivity if the exchange interaction is indirect. as is the case of elements with partially occupied 4f and 5f orbitals. If such RKKY – type exchange is not strong (so that the ferromagnetic transition temperature, TFM , is only few degrees), ferromagnetism can coexist with superconductivity. In all cases the resulting state is inhomogeneous. If TFM is larger than the superconducting transition temperature, Tc , superconductivity will either not appear at all or will destroy the ferromagnetism, depending on the ratio between the effective molecular magnetic field, I (in energy units) and the superconducting order parameter, √ 0 . If I < 0 / 2 superconductivity sup presses ferromagnetism, and in the opposite case it does not. The transition between two states as a function of the parameter I is a first order √ phase transition. However, even if I > 0 / 2 it is possible to have coexisting superconducting and ferromagnetic states. In this case, both magnetic and superconducting order parameters are spatially modulated. This is the so called Larkin-OvchinnikovFulde-Ferrell state (LOFF) (Ovchinnikov, 1964, Fulde and Ferrell, 1964), which has been a goal for experimentalists for the last forty years. Yet no definite experimental evidence for such a state exists, although there are many indirect results in several –0.50 –0.75 –1.00 FM 0 H=0 PM SC 2 4 6 8 10 T (K) Figure 9.56 The AC susceptibility measured by a tunnel diode superconductor (R. Prozorov and M. W. Vannette) in single crystal ErRh4 B4 (grown by the P. C. Canfield group) in different applied magnetic fields, Normal (paramagnetic, (PM)), superconducting (SC), and ferromagnetic (FM) phases are clearly evident. 272 dependent vortex core-size, and even to the development of ferromagnetism in the vor tex cores. It could also be due to a predicted domain structure or an exotic spin structure. In addition, the FM-SC-FM transition is hys teretic with a distinctly different behavior upon warming or cooling. Clearly, despite a vast literature and tremendous theoretical and experimental efforts, the topic is far from being settled, and more work is needed to understand the coexistence of bulk supercon ductivity and bulk magnetism. B. Antiferromagnetic Superconductors Borocarbides with the general formula RT2 B2 C (R=Sc, Y, La, Th, Dy, Ho, Er, Tm, Lu and T=Ni, Ru, Pd, Pt) constitute a very interesting class of materials. Whereas not all combinations of T and R result in super conductivity, many do. Many Nickel-based (T=Ni) borocarbides exhibit antifferomag netism coexisting with superconductivity. Some prominent examples are ErNi2 B2 C and HoNi2 B2 C (Canfield et al., 1997. With a transition temperature around 16 K and a Neel temperature of about 6 K, ErNi2 B2 C also shows features characteristic of ferro magnetism below 2.3 K, and therefore is believed to be a weak ferromagnetic super conductor. The compound HoNi2 B2 C, on the other hand, exhibits several antiferromag netic structures coexisting with superconduc tivity, and nearly reentrant behavior at the Néel temperature. Other examples of antiferromagnetic superconductors include RRh4 B4 (R=Nd, Tm, Sm), RMo6 S8 (R=Tb, Dy, Er, Gd, Nd), and ErMo6 Se8 . As expected, antiferromagnetic order does not prohibit superconductivity, but certainly influences it. For example, antiferromagnetic supercon ductors may exhibit gapless superconductiv ity and a nonmonotonic temperature depen dence of the upper critical field (Buzdin and Bulaevskii, 1986). More examples can be found in Fischer (1990). 9 UNCONVENTIONAL SUPERCONDUCTORS C. Magnetic Cuprate Superconductor – SmCeCuO Thus far our discussion has been limited to relatively low-Tc superconductors. Some cuprates also exhibit magnetic ordering, but due to their layered structure superconductiv ity and magnetism do not coexist in the same volume (we do not discuss weak antiferro magnetic ordering of Cu in Cu–O planes, which is well understood). We restrict our selves to one example in which a magnetic ordering transition has a profound influence on the penetration depth: The electron-doped copper oxide SCCO (Prozorov et al., 2004). In the parent compound Sm2 CuO4 , rare earth Sm3+ ions order at 5.95 Kelvin (Jiang et al., 1992). The ordering is ferromagnetic within each layer parallel to the conducting planes, and antiferromagnetic from one layer to the next (Sumarlin et al., 1993). Ce doping and subsequent oxygen reduction result in a superconductor Sm1 85 Ce0 15 CuO4–( (SCCO) with TC ≈ 23K. Figure 9.57 shows a full-temperature scale variation of the penetration depth in single crystal SCCO in two orientation. The interplane shielding is very weak, yet it exhibits a transition to a more diamagnetic state below about 4 K. The in-plane response shows this effect more clearly. It was tempt ing to associate this transition to the loss of spin – disorder scattering below the ordering temperature of the Sm3+ sublattice. How ever, the magnetic field dependence is sug gesting a different scenario. Figure 9.58 (left) shows the low temper ature penetration depth measured in SCCO for several values of a magnetic field applied along the c-axis. First, there is clear evidence for a phase transition near T ∗ H ≈ 4K that is rapidly suppressed by the magnetic field. Second, the penetration depth drops below the transition indicating stronger diamagnetic screening. This enhanced diamagnetism is quite different from the weaker screening that results from paramagnetic impurities dis cussed earlier. The two effects are consistent 273 IX MAGNETIC SUPERCONDUCTORS 0 hac(t) –10 Δf ~ Δλ(T) –20 –30 –3000 –40 T* 0 2 4 –50 6 8 10 12 –7700 hac(t) –6000 –7800 T* 0 –9000 0 5 10 2 –7900 4 6 15 8 10 20 25 T (K) Figure 9.57 Temperature variation of the penetration depth in an SCCO superoncductor at two orientations. The insets show low temperature regions where a distinct break of the diamagnetic signal is evident. 4 8 8 H (kOe) HDC hac(t) 6 3 2 2 0.0 4 0.5 1.0 T*(HDC) HDC = 0 1 2 3 4 5 T (K) 1.5 T –1 (K –1) H*[kOe]≈ 2 1 0 4 0 H* (kOe) Δ λ (μm) 7 kOe 6 6.4 −1.5 T* 0 6 1 2 3 4 T* (K) Figure 9.58 Magnetic field dependence of the penetration depth in single crystal SCCO (left), and the downturn field H∗ as a function of the temperature (right). The downturn field is linear in 1/T∗ , as shown by the data replotted in the inset (right), with a model involved a spin-freezing tran sition at T ∗ H. Work during the 1980’s on the effects on the influence of random impu rities on superconductive properties showed that while spin fluctuations can be pair break ing, the freezing out of these processes will reduce spin-flip scattering and lead to a sharpened density of quasiparticle states (Schachinger et al., 1988). The latter leads, in turn, to stronger diamagnetic screening and a shorter penetration depth. That one must consider a spin-glass type of transition is sup ported by the rapid suppression of the transi tion by a magnetic field. An ordinary antifer romagnetic transition is relatively insensitive to fields on this scale. In fact, heat capac ity measurements on the parent compound in fields up to 9 T showed only a tiny shift 274 of the ordering temperature. Therefore, the processes required to induce superconductiv ity not only reduce the magnetic ordering temperature, but apparently also result in a disordered spin system. It is well known that the transition temperature in spin-glasses is a strong function of the magnetic field. In fact, it was found that the field dependence T ∗ H shown in Figure 9.58 (right) has precisely the functional form observed in Fe92 Zr 8 , a well-known spin glass system (Ryan et al., 9 UNCONVENTIONAL SUPERCONDUCTORS 2001). At this point, it is not known whether the spins actually freezing are the Sm3+ . It is possible that the Sm spins interact with Cu2+ spins in the conducting layers, for which spin freezing near 4 K is a wellknown phenomenon in cuprate superconduc tors (Lascialfari et al., 2003). This example also serves to demonstrate the invaluable role of an external magnetic field in interpreting penetration depth measurements on complex superconductors. 10 Hubbard Models and Band Structure I. INTRODUCTION In addition to the phenomenological Ginzburg-Landau theory and the micro scopic BCS theory presented in Chapters 5 and 6 respectively, there are other less fun damental theoretical approaches which have been used to explain the presence of super conductivity of some classes of compounds, and to interpret superconducting properties of individual superconductors. This chapter will summarize two of these theoretical approaches, namely the Hubbard model and band structure calculations. Further details of these methods can be found in Chap. 8 of the first edition. Some of the basic properties of electrical conductivity are clarified very well by the independent electron approximation in which the wave functions are plane waves eik··r−t and the energy is all kinetic Ek = Eo a/2 kx 2 + Ky 2 + kz 2 (10.1) where kx = 2/x ky = 2/y kz = 2/z, and a cubic structure is assumed with lattice spacing a. Energy bands are plots of Ek ver sus the value of k along various directions of the Brillouin zone. Many of the most interesting proper ties of materials, such as magnetic ordering and superconductivity, require theories that go beyond the independent-electron approx imation. In order to understand these phe nomena it is necessary to take into account 275 276 10 HUBBARD MODELS AND BAND STRUCTURE electron correlations. The simplest model of correlated electrons is the one-state Hubbard (1963, 1964) model, and so we will empha size it. wavefunctions of these electrons is used to calculate the potential, the Schrödinger equations are solved with this potential to obtain new wavefunctions, and these new wavefunctions are then used to provide an improved potential. The process is repeated until the difference between the new poten tial and the previous potential is less than some predetermined limit. II. ELECTRON CONFIGURATIONS Free electron energy bands calculated using the independent electron approxima tion are an oversimplification of the true state of affairs. For actual compounds there are additional factors to be taken into account. The unit cell contains several atoms with each atom contributing one or more elec trons, as listed in Table 10.1. A separate Schrödinger equation is written down for each electron, and these equations are solved self-consistently. An initial guess for the A. Conﬁgurations and Orbitals Table 10.1 gives the electronic configu rations of several atoms that occur commonly in superconductors. For each atom the table gives the total number of electrons, the num ber of electrons in the core that do not directly enter the calculations, the configu ration of the outer electrons, and the con figuration of an ion that may be present if Table 10.1 Electron Conﬁgurations of Selected Atoms Commonly Used for Band Structure Calculations of Superconductorsa Atom number Symbol Coreb 8 O Be 4 2s2 2p4 14 19 20 23 29 Si K Ca V Cu Ne 10 Ar 18 Ar 18 Ar 18 Ar 18 3s2 3p2 3p6 4s 4s2 3d3 4s1 4p1 3d10 421 38 39 41 50 56 57 80 81 82 83 Sr Y Nb Sn Ba La Hg Tl Pb Bi Kr 36 Kr 36 Kr 36 – – 46 Xe 54 Xe 54 – – 78 – – 78 – – 78 – – 78 5s2 4d1 5s2 4d3 5s1 5p1 5s2 5p2 5p6 6s2 5d1 6s2 5d10 6s2 5d10 6s2 6p1 5d10 6s2 6p2 5d10 6s2 6p3 a b c c Atom configuration No. valence elctrons 4 4 1 2 5 11 2 3 5 4 2 3 2 3 4 5 Ions Ion configuration No. electrons O1− O2− Si4+ K+ Ca2+ V3+ Cu1+ Cu2+ Cu3+ Sr 2+ Y3+ Nb4+ Sn4+ Ba2+ La3+ Hg2+ Tl3+ Pb4+ Bi3+ Bi4+ Bi5+ 2p5 2p6 – – – 3d2 3d10 3d9 3d8 – – 4d1 – – – 5d10 5d10 5d10 5d10 6s2 5d10 6s1 5d10 5 6 0 0 0 2 10 9 8 0 0 1 0 0 0 0 0 0 2 1 0 Core electrons listed in square brackets are sometimes included in the basis set. The core of Sn is Kr plus the fourth transition series 4d10 closed shell. The core of Tl, Pb, and Bi is Xe plus the rare earth 4f 14 and fifth transition series 5d10 closed shells. 277 II ELECTRON CONFIGURATIONS a simple ionic picture is adopted. The nota tion used is nlN , where n is the principal quantum number corresponding to the level, the orbital quantum number l is 0 for an s state, 1 for a p state and 2 for a d state, and N is the number of electrons in each l state. A full l state contains 22l + 1 electrons, corresponding to 2,6, and 10 for s p, and d states, respectively. The wavefunctions of these outer electrons are called orbitals. The various s p, and d orbitals have the unnormalized analytical forms given in Table 10.2, and the electronic charge distri bution in space of the d orbital is sketched in Fig. 10.1. Each orbital represents the charge of one electron; the sign on each lobe is the sign of the wavefunction. For example, we see from the table that pz is given by r cos , which is positive along the positive z-axis = 0, negative along the negative z-axis � = , and zero in the x y-plane � = 21 . Linear combinations of atomic orbitals, called hybrid orbitals, are used to form covalent bonds that hold the atoms together, as illustrated in Fig. 10.2 for bondTable 10.2 Unnormalized Analytical Expressions in Cartesian and Polar Coordinates for the s p, and d Orbitalsa Orbital Cartesian form Polar form s 1 x r y r z r xy r2 yz r2 zx r2 x2 − y 2 r2 3z2 − r 2 r2 1 px py pz dxy dyz dzz dx2 −y2 dz a l = 0 1, and 2, respectively. sin cos sin sin B. Tight-Binding Approximation cos sin2 sin cos sin cos sin sin cos cos sin2 cos2 3 cos2 ing between an oxygen � �p orbital px and a copper d orbital dx2 −y2 . The figure shows, first, a bonding case in which the signs of the two orbitals that form the hybrid are the same in the region of overlap, second, and antibonding case in which the signs are oppo site where overlap occurs, and, third, a nonbonding case where there is no appreciable overlap. Figure 10.3 presents a sketch of a Cu-O2 plane of a high temperature cuprate superconductor. Each orbital can accommodate two elec trons of opposite spin. In the usual case the two electrons enter the low-lying bonding level to form a chemical bond that holds the atoms together while the anti-bonding level remains empty, as illustrated in Fig. 10.4. The “bonding overlap” case is called a sigma bond, and a Cu-O bond of this type can be called a 3dx2 −y2 − 2p bond. We will see later that the band structures of superconduc tors generally consist of many fully occupied bonding levels, called valence bands, which lie below the Fermi level, many unoccupied antibonding levels well above it, and one or more partly occupied hybrid orbitals that pass through the Fermi level. The same approach may be used to treat holes as well as electrons. For example, the copper ion 3d9 may be considered as a filled d shell 3d10 plus one 3d hole, while the oxygen mononegative ion 2p5 may be treated as a full p shell 2p6 plus one 2p hole. −1 − sin2 In Section I we talked about the nearly free electron case in which the poten tial energy is small and the eigenfunctions approximate plane waves. Here the energy bands are broad and overlapping. At the beginning of the present section we dis cussed atomic orbitals, and noted that when the atomic potential energy is dominant the eigenfunctions approximate atomic orbitals centered on individual atoms. This is the case for core electrons whose energy levels lie deep within the atom and do not depend on k. 278 10 HUBBARD MODELS AND BAND STRUCTURE Figure 10.1 Spacial distribution of electron density for the five d orbitals. The signs ± on the lobes are for the wavefunction; the sign of the electric charge is the same for each lobe of a particular orbital (Ballhausen, 1962). Figure 10.2 Examples of bonding (left), nonbonding (center), and antibonding (right) configurations involving the dx2 −y2 orbital with px and py orbitals. In this section we will discuss the intermediate case in which valence-electron orbitals centered on adjacent atoms overlap as shown in Fig. 10.5. Here the isolated atom picture is no longer valid, but the overlap is not sufficiently great to obscure the identity of the individual atomic contribution. This limit, which corresponds to narrow bands with appropriate atomic quantum numbers assigned to each band, is referred to as the tight-binding approximation. This approach is employed in the Hubbard model as well as in the full band structure calculations to be discussed in Sections III – VI. To clarify the nature of this approach we will examine the case of one atomic state—for example, an s state—which is well isolated in energy from nearby states. A possible basis set for a crystal made up of N such atoms includes states in which the electron is localized on one atom, r − R, where r is an atomic wave function and R is a direct lattice vector. These states overlap and are not orthogonal, and the overlap integral defined by � R − R� = d3 r∗ r − Rr − R� (10.2) is a measure of nonorthogonality. When the overlap integral for nearest-neighbor atoms is small, the atomic states are approximately orthogonal. 279 II ELECTRON CONFIGURATIONS Figure 10.3 Orbitals used for a model of Cu-O planes in a cuprate supercon ductor. Each copper contributes a dx2 −y2 orbital and each oxygen contributes either a px or a py orbital, as shown. The unit cell contains one of each type of ion, and hence one of each type of orbital. The figure shows four unit cells. Figure 10.5 Overlap Ri − Rj of atomic wavefunctions for nearby atoms. Figure 10.4 Hybridization of a copper dx2 −y2 orbital with an oxygen px orbital to form a low-energy bonding configuration and a high-energy antibonding configu ration. Two antiparallel electrons that form a chemical bond are shown in the bonding level. These states, however, do not behave under lattice transformations, r � → r + R, according to Bloch’s theorem k r + R = eik·R k r (10.3) We can remedy this situation by construct ing Bloch states, i.e., linear combinations of localized states of the form k r = N−1/2 � R eik·r r − R (10.4) 280 10 HUBBARD MODELS AND BAND STRUCTURE which are orthogonal but not normalized, � � d3 rk∗� rk r =e−ik−k ·R � 0 = k � k r k� ≤ k k� = k d3 rk∗� r (10.5) (10.6) We show in Problem 9 that k is the Fourier transform of the overlap integral k = � e−ik·R R where Va r-R�� is the potential due to the nucleus at the lattice position R�� and the summation in Eq. (10.11) excludes the case R = R� . We can see from Fig. 10.5 that overlap integrals fall off very rapidly with distance. The same is true of the exchange inte grals. Therefore, we are justified in retain ing in 10.7 and 10.10 only terms in which R� is either R or a nearest neighbor to R, which gives k ≈ 0 + (10.7) e−ik·R R R R Since the full Hamiltonian H is sym metric under lattice transformations and the Bloch states k r for different values of k are orthogonal, it follows that in the simple one-band approximation k r is an eigen state of H. The eigenvalue k can be eval uated calculating the expectation value � 3 by d rk∗� rHk r. We show in Problem 10 that this gives k = a + � Bk k ≈ 0 + 21 cos kx a + cos ky a (10.12) and Bk ≈ 21 cos kx a + cos ky a (10.13) so that k ≈ a + 2 cos kx a + cos ky a (10.14) 0 (10.8) where we have assumed that << 0 and 1 << 0 . The width of the band measured where the energy of an isolated atom a along the line − X, for example, is = includes a kinetic-energy part p2 /2m and a 0 0–/a 0 = 4/0 . The exchange Coulomb part uR, integral determines the degree of disper sion in the band. If is very small, as is � uR = d3 r∗ r − RVa r − Rr − R the case for well-separated atoms, the bands are nearly flat and centered about the atomic (10.9) energy level a . Since k is a slowly vary ing function of k, it is possible to form a k is given by Eq. (10.7) and Bk is the superposition of states with different k but Fourier transform of the exchange integral essentially the same energy. If we wish, we R, can construct a wave packet that is centered � on one atom, and in this way return to our (10.10) Bk = e−ik·R R original set of atomic orbitals. R � Typical band structure calculations take R − R� = d3 r∗ r − R into account several atomic orbitals n r–R for each atom, so we can define the Bloch � � � states × Va r − R�� r − R� � R�� nk r = N−1/2 eik·r n r − R (10.15) (10.11) R 281 III HUBBARD MODEL where n now labels each of the atomic states in the basis. The formalism leading to Eq. 10.8 must now be generalized some what to include a greater number of overlap integrals, nm R − R� = � d3 r∗n r − Rm r − R� (10.16) and exchange integrals, � nm R−R� = d3 rn∗ r −R � � � �� × Va r −R m r −R� R∗ (10.17) and their respective Fourier transform coun terparts nm k and Bnm k. The eigenstates are linear combinations of atomic orbitals, and the associated method is often referred to as LCAO. Having covered some background on energy bands and chemical bonding, we will proceed to describe the Hubbard model which, despite its simplicity, exhibits many properties that are characteristic of supercon ductors (Anderson 1987a; cf. Hirsch 1985a, b, 1987). This will prepare the way for understanding the more complex band struc tures of the elements, of the A15 com pounds, and finally, of the high-temperature superconductors. A. Wannier Functions and Electron Operators In the tight-binding approximation we made use of the Bloch states k r as given by Eq. (10.4), which are superposi tions of atomic functions r–R over lattice positions. These states are orthogonal, and k−1/2 from Eq. (10.7) constitutes their normalization constant. A summation of nor malized Bloch states over all of the k-states of a band, � Wr − R = N1/2 k−1/2 e−ik·R k k (10.18) provides a new wavefunction Wr–R associated with the atom at lattice position R. This wavefunction represents a Wannier state. The Wannier states are useful because the overlap of two Wannier states at different lattice sites R and R� is zero. For two differ ent bands with indices n and n� , the associ ated Wannier states Wn r–R and Wn� r–R are orthogonal, corresponding to the general orthonormality condition � d3 rWn∗ r − RWn� r − R� = nn� RR� (10.19) The Wannier states are also complete: �� ∗ Wn r − RWn r � − R = r − r � r� R (10.20) III. HUBBARD MODEL The essential principles of the Hubbard Model can be explained by using only one electron orbital, but the use of three such orbitals provides a more realistic description of a cuprate superconductor. We will start with the first and then pass on to the sec ond after saying a few words about the wave functions that are involved. If the band is narrow each Wr–R is local ized about one lattice point R. Using Wannier states as a basis, the electron operator for a single band can be written as � r = N−1/2 a RWr − R R (10.21) The operators a† R and a R are, respec tively, the electron creation operator and the 282 10 HUBBARD MODELS AND BAND STRUCTURE electron annihilation operator, and together they form the number operator n R for electrons of spin in the Wannier state Wr–R, n R = a† Ra R (10.22) where no summation is intended. These operators satisfy the anticommutation rule The Hamiltonian consists of a kinetic energy term proportional to a “hopping amplitude” t > 0 that represents the electron correlation; a term −N̂ , where is the chemical potential and N̂ is the total number of electrons; and an on-site Coulomb repul sion term (10.9), U > 0. We thus have � † a Ra R� H =−t RR� † Ra � R� + a � R� a† R = RR� (10.23) � + a† R� a R � − a† Ra R and have the properties R a− �0� = 0 +U a− �−� = �0� a† − �0� = �−� n+ Rn− R (10.25) R a− �+� = 0 a− �±� = �+� R � (10.24) a† − �−� = 0 a† − �+� = �±� a† − �±� = 0 Similar expressions can be written for the spin-up operators, a+ † and a+ . The wavefunctions �j� correspond to sites occupied by a spin-up electron �+�, by a spin-down electron �−�, or by two electrons of opposite spin �±�, while �0� denotes a vacant site. We will use these expressions and extensions of them to the two-electron case �ij� to evaluate the energy of some Hubbard Hamiltonians. B. One-State Hubbard Model In a one-state Hubbard model there is one electron orbital per unit cell. To con struct this model we begin, as in the tightbinding approximation, with electrons local ized in atomic-like states at the positions R of the atoms. We assume that there is only one valence orbital per atom and each atom can accommodate 0, 1, or 2 electrons. where = 0 for the undoped case when the orbitals are half filled with electrons. The kinetic energy is the sum of two her mitian conjugates. The “hopping amplitude” t given by t= �2 � 3 d rW ∗ r − R · Wr − R� 2m (10.26) is a measure of the contribution from an electron hopping from one site to another neighboring site. It is assumed that the over lap of Wannier functions separated by more than one lattice spacing is negligible, and that t is the same for all nearest-neighbor pairs R R� . The chemical potential term is included because we are interested in the change in the properties of the model as the number of electrons is varied. The Coulomb repulsion is assumed to be the same for all sites. The Hamiltonian takes into account only nearest-neighbor correlation and on-site Coulomb repulsion. The Hamiltonian (10.25), simple as it appears, embodies a great deal of physics. This Hamiltonian, or a generalization of it, is the starting point for a number of theories of high-Tc superconductivity, the Mott insu lator transition, and other phenomena related 283 III HUBBARD MODEL to highly correlated many-electron systems. Allen (1990) went so far as to state what he called the Hubbard hypothesis: “The funda mental physics of the oxide superconductors is contained in the Hamiltonian (10.25) on a two-dimensional square lattice for small numbers of holes.” In Sections III.D, III.E, and III.F we will discuss examples of the limiting case U >> t. Typical values have been given of t ∼ 025 − 05 eV and U ∼ 3–4 eV (Ruckenstein et al., 1988). The opposite limit, U << t, has also been discussed (e.g., see Varma et al., 1988). C. Electron-Hole Symmetry As we shall see, the Hubbard Hamiltonian exhibits an electron-hole sym metry. Such symmetry is of considerable importance, in that most high-temperature superconductors are hole types with a close to a half-full conduction band. To demon strate this symmetry it is convenient to begin by writing out the generalized Hamiltonian (10.25) in the more symmetric form � † a Ra R� H =−t RR� + a† R� a R � − a† Ra R b R = a† − R (10.28) where and − denote opposite spin direc tions. We then have for the number operator, from Eq. (10.22), n R = a† Ra R = b− Rb† − R = 1−b † − (10.29) Rb− R = 1 − ñ− R (10.30) where the anticommutation rule (10.23) is applied to obtain the number operator ñ R = b† Rb R for holes. Using these expressions, the Hamiltonian can be written in terms of hole operators, H =t � b† Rb R� RR� + b† R� b R � + Ns + b† Rb R R � �� � � 1 1 +U ñ+ R − ñ− R − 2 2 R (10.31) where Ns is the number of sites on the lattice. The thermodynamic potential is given by R +U � R � �� � 1 1 n+ R − n− R − 2 2 (10.27) This can be done because the extra terms simply shift the chemical potential and the zero point of energy. The next step is to consider a transfor mation to “hole” operators by recalling that a site in k-space that is missing an electron is occupied by a hole, so destruction of a hole is equivalent to creation of an electron. Accord ingly, we can define the “hole” operators b † R = a− R T t U = −kB T log Tre−H/kT (10.32) = −2Ns + − T −t U (10.33) If the lattice is bipartite, that is, if it can be decomposed into two sublattices, A and B, with the property that an atom of one sublat tice has atoms of the other sublattice as its nearest neighbors, the electron-hole transfor mation can be modified to � a† R R∈A (10.34) b R = −† −a− R R ∈ B 284 10 HUBBARD MODELS AND BAND STRUCTURE This has the effect t → −t, so that Eq. (10.33) becomes T t U = −2Ns + − T t U (10.35) The average number of particles N T is N T = −d/d = 2Ns − N− T (10.36) (10.37) and for = 0 we obtain N0 T = Ns Here we show that hopping removes the degeneracy, and, in addition, show by sim ple perturbation theory that the effect of the hopping term is to lower the energy of an antiferromagnetic pair relative to a ferromag netic pair of nearest-neighbor electrons. Consider a nearest-neighbor pair of electrons that occupies one of the two anti ferromagnetic states, with antiparallel spins � + −� and � − +� (10.39) or one of the two ferromagnetic states, with parallel spins (10.38) that is, one electron per site. Because of the simple relationship (10.37) we need only consider ≥ 0; the properties of the system for < 0 are then easily found by means of the electron-hole transformation (10.34). D. Half-Filling and Antiferromagnetic Correlations The high-temperature superconductors and related compounds typically have a set of full low-lying bands, an almost half-full hybrid band near the Fermi level, and a set of empty bands at higher energy. The halffull, one-state Hubbard model stimulates this hybrid band, and thereby provides a sim ple approximation to the materials. Later, we will see how a three-state Hubbard model more closely approximates the behavior of high-temperature superconductors. We take = 0 so that !�n R� = 1. Thus there is on average one electron per lattice site. If the on-site repulsion is large, U � t, states with double occupancy will be suppressed. Therefore, let us consider as a subset of all states of the half-filled band those states with exactly one electron at each site. The Coulomb repulsion term U!n+ Rn− R only exists for a site that is doubly occupied, so it vanishes in this case. Were it not for the hopping term, these states would all be degenerate with zero energy. � + +� and � − −� (10.40) where + denotes spin up, and − signifies spin down. In addition to these four states, there are two higher energy states �0±� and � ± 0� (10.41) in which both electrons are localized on the same atom. We wish to apply perturbation theory up to second order for the case U � t corre sponding to the expression 0 1 2 E i = E i + E i + Ei (10.42) for the ith-order energy, where Ei = �i �HCoul �i � + �i �Hhop �i � + � ��i �Hhop �j ��2 j�=i Ej − Ei (10.43) As noted earlier, there is no Coulomb con tribution for the four states (10.39) and (10.40), so that the zero-order term vanishes, 0 Ei = 0. The first-order energy must be eval uated from the expression 1 Ei − �i �Hhop �i � (10.44) where the hopping operator Hhopp has the explicit form + Hhop = − ta+ + 1a+ 2 + a+ 2a+ 1 + + a+ − 1a− 2 + a− 2a− 1 (10.45) 285 III HUBBARD MODEL Since each term of this operator changes the spin state, the first-order energy (10.44) also vanishes. Second-order perturbation theory entails evaluating the matrix elements �i �Hhop �j � � j. The only nonvanishing terms are for i = �+ − �Hhop �0±� = �+ − �Hhop � ± 0� = �− + �Hhop �0±� = �− + �Hhop � ± 0� = −t Although we have employed a basis in which one component of the spin, conventionally the z-component, is diagonal, the Hubbard Hamiltonian is invariant under rotations in spin space. To second order in perturbation theory, the effective Hamiltonian for the sub set of states can therefore be written in the Heisenberg form, HHeis = −J!SR · SR� where the exchange coupling term is (10.46) J = 4t2 /U The denominator Ej –Ei of the second-order term of Eq. (10.43) is −U , which gives for the energy of the two antiferromagnetic states E+− = E−+ = − 2t2 U (10.47) Since the energy of the two ferromagnetic states is zero (Problem 17), E++ = E−− = 0 (10.49) (10.48) the hopping term has the effect of lowering the energy of an antiferromagnetic pair rela tive to that of a ferromagnetic pair. E. t-J Model In one variant of the Hubbard model, called the t-J : model, the Coulomb repulsion U term in the Hamiltonian is replaced by the Heisenberg term J!Si · Sj (Anderson, 1978a, b; Rodriguez and Douçot, 1990; Zhang and Rice, 1988; Halley, 1988, Chapters 15–20). This model may be obtained as the large-U limit U � t of the Hubbard model (Harris and Lange, 1967; Marde et al., 1990). We will justify it in terms of the discussion in the previous section. If we restrict our attention to states with one electron per site, we can describe the states completely in terms of the spin- 21 oper ators for the electrons at each site, Sk R. (10.50) Typical values of the parameters, t ≈ 04 eV and U ≈ 35 eV (Ruckenstein et al., 1987), give J close to the experimentally deter mined value J ≈ 014–016 eV (Gagliano and Bacci, 1990; Singh et al., 1989). We conclude that at half filling, in the limit U/t → �, the ground state of the Hubbard model is equivalent to that of a Heisenberg antiferromagnet. The Heisenberg term used in the t-J model corresponds to the Hamiltonian + H = −t!a+ i aj + aja ai + J!Si · Sj (10.51) Undoped materials can be understood in terms of the two-dimensional Heisenberg term (Chakravarty et al., 1988; Dagotto et al., 1990), and in the presence of empty sites the hopping matrix element t can rep resent holes propagating in a fluctuating antiferromagnetic background arising from this J!Si · Sj term (Poilblanc and Dagotto, 1990; Zotos et al., 1990). Many believe that the t-J model embraces the essential fea tures of high-temperature superconductivity (Ohkawa, 1990), and there is an extensive literature on the subject. The symbol t-J is used to designate the two terms in the Hamiltonian (10.51). In the same spirit, the ordinary Hubbard model could be called the t-U model, but this notation is never employed. The t-J 286 10 HUBBARD MODELS AND BAND STRUCTURE and Hubbard models have been compared (e.g., Bhattacharya and Wang, 1992; Dagotto et al., 1992). �1 − 1� =� − −� singlet E = −4t2 /U (10.53) F. Resonant-Valence Bonds The Hubbard model is deceptively sim ple, and while some exact results for the ground state are known in the limit U/t → � and for the case of half filling, the nature of the ground states for arbitrary U and t are not known. An alternate choice of basis for elu cidating the nature of the low-lying levels of the model makes use of “resonant-valence bond” (RVB) states (Anderson, 1987a, b; Emery and Reiter, 1988; Feine, 1993; Kivelson, 1989; Wittmann and Stolze, 1993; and Zhang and Rice, 1988). Electrons at nearest-neighbor sites are paired into “bonds” and linear combinations of the basis states are used to construct eigenstates of the total electronic spin (Allen, 1990). For two electrons the total spin S can be 1 or 0, and the corresponding triplet (S = 1, M = 0 ±1 and singlet S = M = 0 wavefunctions are, respectively, �11� =� + +� 1 �10� = √ � + −� + � − +� 2 triplet E = 0 1 �VB� = √ � + −� − � − +� 2 (10.52) where we have used the notation �SM� on the left side. There are two additional ionized states �A� and �B� which are both singlets, 1 �A� = √ �0±� − � ± 0� E = U 2 (10.54a) 4t2 1 �B� = √ �0±� + � ± 0� E = Ul + U 2 (10.54b) and, of course, a state in which there are no electrons, �vacuum� = �00� The singlet state with two electrons labeled �VB� is the lowest in energy, and it con stitutes the “valence bond” state. The ener gies of these two electron states as given in (10.52)–(10.54b) are sketched in Fig. 10.6 The RVB theory starts by assuming that the ground state of insulating La2 CuO4 is a linear combination of �VBij� states for vari ous pairs of electrons i j, Figure 10.6 Energy levels of the two-site, nearest-neighbor electron-pair problem at half filling, shown for the zero-order (left), Hubbard model (center), and resonant valence-bond (right) approximations. 287 III HUBBARD MODEL �RVB� = c12 �VB12� + c34 �VB34� + c56 �VB56� + · · · (10.55a) and in the presence of a single hole with spin down h− paired with a spin-up electron e+ this becomes �RVB 1 hole� = c12 �h−��e+� + c34 �VB34� + c56 �VB56� + · · · (10.55b) where the hole can hop between sites. G. Spinons, Holons, Slave Bosons, Anyons, and Semions In the RVB formulation of the twodimensional large-U Hubbard model, the spin and charge degrees of freedom are separated. The elementary excitations are either neutral spin- 21 solitons (fermion soli tary excitations, Doda et al., 1982; Doi et al., 1992; Drazi and Johnson, 1989; Kivshar, 1991; Rokhsar, 1990; Tighe et al., 1993), called spinons, or charged boson particles, called holons (Allen, 1990; Anderson and Zou, 1988; Kivelon, 1989; Nori et al., 1990; Schmeltzer, 1994; Schofield and Wheatley, 1993; Sinha, 1992; Wang, 1989; Xing and Liu, 1991; Zou and Anderson, 1988). There is a version of the t-J model, called the slave boson representation, in which the Hamiltonian contains spinon and holon creation and annihilation operators (Schönhammer, 1990; Sheng et al., 1990). The so-called slave boson operators are intro duced to specify and keep track of empty and singly occupied sites (Arrigoni et al., 1990; Jolicoeur and LeGuillou, 1991; Rodriguez and Douçot, 1992). From a more general viewpoint, the slave boson formulation maps a purely fermionic model onto an effective bosonic one (Lilly et al., 1990), and the slave boson fields provide a larger quan tum mechanical (Fock) space that is sub ject to constraints involving the slave boson operators (Jolicoeur and LeGuillou, 1991; Rodriguez and Douçot, 1992; Zhang et al., 1993; Zou and Anderson, 1988). In addi tion, the slave bosons carry a conserved quantum number, namely charge (Zou and Anderson, 1988). In quantum mechanics we learn that the wavefunction Ur2 r1 for the exchange of two particles is given by Ur2 r1 = ei Ur2 r1 (10.56) where = 0 for bosons which are sym metric under interchange, and = for fermions which are antisymmetric. Wilczek (1982a, b) coined the word anyon for a par ticle with some other value in the range − < < , and such a particle is said to have fractional statistics. It violates the usual time reversal (T) and parity (P) conservation laws. Anyons have been used to explain the fractional quantum Hall effect in semicon ductor heterojunctions (Arovas et al., 1984; Halperin, 1984; Prange and Girvin, 1987). Kalmeyer and Laughlin (1987; Laughlin, 1988a, b) suggested that semions, anyons with = ±/2, Ur2 r1 = iUr2 r1 (10.57) might be the charge carriers responsible for high temperature superconductivity. In principle this can be tested by experiments involving T, P symmetry, but the results have not been encouraging (Shen and Lu, 1993; Zhou and Chen, 1993). Some studies of an anyon gas suggest that its ground state is superconducting, that a collective excitation is a phonon mode, and that a single particle excitation can be identified as a vortex (Choi et al., 1992; Gelfand and Halperin, 1992; Mori, 1991; Zhang et al., 1990). H. Three-State Hubbard Model The one-state Hubbard model that we discussed in Section II.B involved one orbital 288 per unit cell, with two parameters, a hop ping amplitude t and an on-site Coulomb repulsion U . We will now extend the model to a unit cell, shown outlined in Fig. 10.3, containing a Cu atom that contributes a dx2 −y2 orbital, and two oxygens one of which contributes a px orbital, the other a py orbital (Jefferson et al., 1992). This corresponds to the configuration of the CuO2 plane shown in the figure, which is believed to be respon sible for the super-conducting properties of the cuprates. In this plane each copper has four oxygen nearest neighbors and each oxy gen has two copper nearest neighbors. The figure is drawn with the signs on the orbital lobes selected so that all of the overlaps are of the bonding type. The convention chosen for assigning positive (e.g., +px ) and nega tive (e.g., −py ) signs to the orbitals is given in the figure. 10 HUBBARD MODELS AND BAND STRUCTURE I. Energy Bands The energy bands calculated by Entel and Zielinksi (1990) are plotted in Fig. 10.7a, and the density of states, together with the partial contributions from the p electrons np and d electrons nd , is plotted in Fig. 10.7b. The conditions for the calculation are clear from the labels in the energy scale of Fig. 10.7a hopping amplitudes tp = "p = 0 td = "d = 36 eV, and Coulomb repulsion terms Upp = 4 eV Udd = 105 eV. We see that a predominately p-type band rises above the Fermi level at the corner point M, and that the Fermi surface consists of the p-like pocket of holes indicated in the Brillouin zone shown as an inset to Fig. 10.7a. The low-lying, mainly p-type pair of bonding bands, and the higher, predominately dtype antibonding band, are separated from Figure 10.7 Band structure for the three-state Hubbard model for 4.5 electrons per unit cell. The model assumes one d state and two bonding p states per unit cell: (a) Energy bands with the Fermi energy below the gap, (b) density of states, Energies involving hopping amplitudes "p = 0 "d = 36 eV, and Coulomb repulsion terms Upp 40 eV, and Udd = 105 eV are indicated in the ordinate scale of (a). Total density of states #t together with the partial p and d contributions #p and #d are shown. The free-electron result #f is included for comparison. Bands are occupied indicated by cross hatching below the Fermi level EF = 62 eV, (from Entel and Zielinski (1990)). 289 III HUBBARD MODEL the three bands near the Fermi level by insu lating gaps. Since there are three orbitals in the set chosen for the calculation, and since each can contain two electrons of opposite spin, it takes six electrons to fill all of the bands. As electrons are added to the system, the Fermi level rises in the manner shown in Fig. 10.8. Note the two sharp jumps in EF where the two band gaps are located. The amount of dispersion, or range of energy, over which a band is spread is called the width of the band. The width depends on the number of electrons in the unit cell. The predominately p-type band (No. 5) that passes through the Fermi level in Fig. 10.7a for the n = 45 electron case has the greatest dispersion. We see from Figs. 10.7a and 10.7b that there are regions where the energy bands are flat, and at these energies the density of states becomes large, corresponding to what are called van Hove singularities (cf. XIII. A). Singularities of this type will be encountered later in the chapter. A DOS peak associated with a CuO2 plane van Hove singularity can Figure 10.8 Three-state Hubbard model showing the variation with band filling of the Fermi energy (chemical potential) at T = 100 K, The metal-to-insulator transi tion occurs at the discontinuity in the Fermi energy near n = 5 (Entel and Zielinski, 1990). cause a peak in the transition temperature Tc as a function of hole doping (Mahan, 1993; Markiewicz, 1991a, 1991b; Pattnaik et al., 1992; Penn and Cohen, 1992). The ability to calculate occupation num bers ni for individual electrons associated with the various bands permits us to deter mine the contribution of the electrons from each atom in the unit cell of a superconduc tor to the density of states. In the following sections we will present several such plots of individual atom density of states versus energy. J. Metal-Insulator Transition When the fifth band of Fig. 10.7a is almost full, the Fermi level lies near the top of the band. Adding more electrons fills this band and additional electrons enter the sixth band far above it. This causes the Fermi level to rise above the energy gap to the level of the top band. When this occurs the system under goes a transition from a metal to an insu lator. Evidence for this transition is seen in the discontinuity at the position of the upper energy gap where there are five electrons per cell. Figure 10.9 presents the metal-to insulator phase diagram, showing the metal lic and insulating regions as a function of the p electron Coulomb repulsion energy Upp and the energy difference between the p and d hopping integrals, = 21 td – tp , called the charge-transfer energy (Entel and Zielinski, 1990). We see from the figure that a charge-transfer insulator (CTI) arising from the presence of a charge-density wave forms for Udd � , and that a Mott insulator (MI) forms for Udd � . The present calculation is for the ratio Udd / = 58, so that it corre sponds to the metallic region above the ordi nate value Udd / > 5, which could be close to the transition to a charge-transfer insula tor. The p orbital Coulomb repulsion energy Upp has much less effect on the phase dia gram than its d orbital counterpart Udd . The phase diagram of an actual superconductor 290 Figure 10.9 Metal-to-insulator phase diagram for the three-state Hubbard model with Vdp = 0, where the charge transfer energy is given by = 21 td –tp . The regions where the charge-transfer insulator (CTI) and the Mott insulator (MI) occur are indicated. For the charge-transfer insulator, which arises from the presence of a charge-density wave, np > nd for the band beneath the gap (Entel and Zielinski, 1990). 10 HUBBARD MODELS AND BAND STRUCTURE the point of Fig. 10.7a. It causes the “new fifth band” to become more d-like so that we have nd > np for low values of Upp , as indicated in Fig. 10.10 instead of the oppo site ratio nd < np for the large Upp case of Fig. 10.7. Now that we have surveyed several vari eties of Hubbard models we will proceed to describe the band structure results obtained for several superconductors. Many of the fea tures characteristic of the three-state Hub bard model will be found duplicated in the move sophisticated band structures to be discussed. IV. BAND STRUCTURE OF YBa2 Cu3 O7 can be more complicated, Hebard (1994b) discusses the nature of the superconductor– insulator transition. The orbital character of the bands depends on Upp . This is shown in Fig. 10.10 for the fifth band when the number of elec trons in the unit cell is maintained at the value 4.9. There is a strong dependence of the ratio nd /np on Upp since decreasing Upp from its chosen value of 4 eV to below 3.6 eV raises band 3 above bands 4 and 5. This accords with the proximity of these bands at We will begin our discussion of the energy bands of the high-temperature super conductors with the compound YBa2 Cu3 O7 since its structure is of the aligned type; as explained in Chapter 8, Section IV, and hence its Brillounin zone is simpler than those of the cuprates which are body cen tered. This section will describe the band structure reported by Pickett et al. (1990) and Pickett (1989; cf. Costa-Quintana et al., 1989; Curtiss and Tam, 1990; Krakaer et al., 1988; Singh et al., 1990; Wang (1990) J. Yu et al., 1991). The bands reflect the princi pal structural features of the compound—the presence of two CuO2 planes containing the Cu(2), O(2), and O(3) atoms, and a third plane containing chains of Cu(1)–O(1) atoms along the b direction, as shown in Fig. 10.11 and described in Chapter 8, Section IV. The ortho-rhombic Brillouin zone, also shown in the figure, has a height-to-width ratio Figure 10.10 Dependence of the occupation num 2/c/2/a = a/c ≈ 033 bers np and nd in the band beneath the gap on the intra-atomic Coulomb repulsion energy Upp for n = 49 electrons per unit cell in the three-state Hubbard model (Entel and Zielinski, 1990). which is the reciprocal of the height-to-width ratio of the unit cell in coordinate space. 291 IV BAND STRUCTURE OF YBa2 Cu3 O7 Figure 10.11 Two views of the YBa2 Cu3 O7 unit cell and sketch of the corresponding Brillouin zone (Krakauer et al., 1988). A. Energy Bands and Density of States The energy bands of YBa2 Cu3 O7 near the Fermi surface are presented in Fig. 10.12 along the principal directions connecting the symmetry points X Y , and S in the cen tral kz = 0 horizontal plane of the Brillouin zone. The bands change very little at the cor responding symmetry points Z, U, T, and R of the top kz = 21 plane. The highest tran sition temperature is found in the case of a small amount of oxygen deficiency, ≈ 01, in the formula YBa2 Cu3 O7− . This slightly less than half-full condition, where = 0 for half-full, means that there are missing electrons near EF , and that the conductiv ity is of the hole type. This is confirmed by Hall effect measurements, as will be seen in Chapter 16 Section VI. The two narrow CuO plane-related bands are shown in Fig. 10.12 strongly dis persed, i.e., rising far above the Fermi sur face at the corner points S and R of the Brillouin zone of Fig. 10.11. These two bands are almost identical in shape, resem bling the Hubbard band that is shown ris ing above EF at the corner point M of the Brillouin zone in the inset of Fig. 10.7a. The much broader chain band that is shown strongly dispersed in both the S and the Y (also R and T ) or chain directions far above EF arises from the Cu–O sigma bonds along the chains formed from the oxygen py and copper dx2 −y2 orbitals, as illustrated in Fig. 10.13 There is another chain band which undergoes very little dispersion, stay ing close to the Fermi surface, but it rises slightly above EF at S and R, as shown in the figure. Oxygen deficiency depopu lates the chains, and this is reflected in the absence of chain bands in the semicon ducting compound YBa2 Cu3 O6 (Yu et al., 1987). The lack of appreciable dispersion in the bands along kz demonstrated by the similar ity of Figs. 10.12a and 10.12b means that the effective mass m∗ defined by Eq. (1.47), � � 1 1 d 2 Ek = 2 (10.58) m∗ � dkz2 E F is very large, and since the electrical con ductivity from Eq. (1.22) is inversely pro portional to the effective mass, this means 292 Figure 10.12 Energy bands of YBa2 Cu3 O7 along the principal directions in the Brillouin zone sketched in Fig. 10.11. The two plane bands rise sharply above the Fermi level at points S and R, and the broader chain band is high in energy between S and Y , and between R and T (Pickett et al., 1990). that the conductivity is low along the z direc tion. In contrast, the plane and chain bands appear parabolic in shape along kx and ky , corresponding to a much lower effective mass. This explains the observed anisotropy in the normal-state electrical conductivity, c /ab ≈ 20. The total density of states and the con tribution of each copper and oxygen to DE are presented in Fig. 10.14. There are peaks (called van Hove singularities, II, I) in the partial DOS of the planar oxygens O(2) and O(3) at energies at which the planar Cu(2) atoms also have peaks, whereas chain Cu(1) have peaks that match those of the O(1) and O(4) oxygens bonded to it. This suggests that the planes and chains are partially decoupled 10 HUBBARD MODELS AND BAND STRUCTURE Figure 10.13 Sigma bonding between Cu(1) and O(1) orbitals along chains in the crystallographic b direction of YBa2 Cu3 O7 . from each other, as we might have expected, since the bridging oxygen O(4) is 1.8 Å from Cu(1) compared to the much longer distance 2.3 Å from Cu(2). Super current can flow along both the planes and chains. B. Fermi Surface: Plane and Chain Bands The Fermi surface of YBa2 Cu3 O7 is plotted in Fig. 10.15 for the kz = 0 and kz = /a horizontal planes of the Brillouin zone, with the symmetry points S and R, respectively, selected as the origin, in accor dance with Fig. 10.16. The close similarity 293 V BAND STRUCTURE OF MERCURY CUPRATES Figure 10.14 Density of states of YBa2 Cu3 O7 . The top panel shows the total density of states, the second panel gives the partial DOS of Cu(1) [—] and Cu(2) [----], the third panel presents the same for O(1) [—] and O(4) [----], and the bottom one gives O(2) [—] and O(3) [----] (Krakauer et al., 1988). between the respective left kz = 0 and right kz = /a panels of the figure confirms that there is very little dispersion in the verti cal kz direction. The shapes of these Fermi surfaces can be deduced from where the cor responding bands cross the Fermi surface in Fig. 10.12. The two plane–band Fermi surfaces pre sented in the four center panels of Fig. 10.15 consist of large regions of holes in the cen ter, with narrow bands of electrons around the periphery. The surface of one plane band makes contact with the zone bound ary between points Y and due to the small maximum that rises above EF between these points in Fig. 10.12. When 0.2 fewer electrons are present, the Fermi surface is lowered and the contact with the zone bound ary extends over a larger range between Y and . Adding 0.2 more electron raises the Fermi surface above the small relative max imum near Y , and the zone boundary is no longer reached. Thus the oxygen content, which determines the electron concentration, influences details of the shape of the Fermi surface. As already noted in Section A, the highest Tc occurs for ≈ 01. The regions of holes around the central points R and S (not shown) resemble their counterpart around point M of the three-state Hubbard model. The two chain-band Fermi surfaces sketched in the upper and lower pairs of pan els of Fig. 10.15 differ considerably. The upper panels show the highly dispersed chain band that lies above EF everywhere except from to X, where it is below EF , as shown in Fig. 10.12. This corresponds to a narrow one-dimensional-like slab containing electrons that extends continuously from cell to cell along the direction –X– $ $ $ , and parallel to it there is a wide hole-type slab along Y –S–Y $ $ $ , as shown at the top of Fig. 10.15. The edges of this wide slab are mostly parallel, a condition needed for nest ing, but are not close enough to the boundary to create strong nesting, as will be explained in Section VIII. The other chain band lies entirely below the Fermi level except for a narrow region near point S in Fig. 10.12. Figure 10.15 shows this small hole region in the zone centers S and R of the lower two panels. V. BAND STRUCTURE OF MERCURY CUPRATES Band structure calculations have been carried out for the aligned Hg-1201 and the Hg-1221 members of the HgBa2 Can Cun+1 O2n+4+ series of compounds, and we will summarize some of the results that were obtained. The Brillouin zone is the tetragonal anologue of the orthorhombic one sketched in Fig. 10.11 with point y identical with point x, and T identical with u from symmetry. 294 10 HUBBARD MODELS AND BAND STRUCTURE Figure 10.15 Fermi surfaces of YBa2 Cu3 O7− calculated from the band structure with the electron (e) and hole (h) regions indicated. The left panels are for the midplane of the Brillouin zone kz = 0 with point S at the center and those on the right are for the top plane kz = /a with point R at the center. Points S and R are not labeled. The two top panels show a well dispersed chain band that rises far above the Fermi level. The second pair of panels shows the first plane band; it crosses the Fermi level closest to points X and Y in Fig. 10.12. The third pair of panels presents the second plane band with the crossing further from these points. The bottom panels display the chain band, which is mostly below the Fermi surface, rising above it only near point S (and point R) in Fig. 10.12. The solid lines are for the calculated Fermi surface with = 0, the short dashed curve is for = 02 containing 0.2 fewer electron, and the long-dashed curve is for = −02 with 0.2 more electron (Krakauer et al., 1988). 295 V BAND STRUCTURE OF MERCURY CUPRATES Figure 10.16 Relationship between Brillouin zone boundary in Fig. 10.11 (dashed lines) when point or Z is at the center and Fig. 10.15 (solid lines) when S or R is chosen as the center. The band structure calculations were carried out by adding to the usual orbital set the following upper core level orbitals: Cu 3s and 3p O 2s Ba5s and 5p, and Hg 5p and 5d, with = 0. Ca 3s and 3p orbitals were Figure added for Hg-1223. Figures 10.17 and 10.18 show the energy bands and density of states for the n = 0 compound (Singh, 1993), and Figs. 10.19 and 10.20 present their counter parts for the n = 2 compound (Rodriguez, 1994; Singh, 1994). In addition the articles provide Fermi surface across sections for the two compounds. The bands of HgBa2 CuO4 presented in Fig. 10.17 are highly two dimensional, with very little dispersion in the z direction shown from to Z in the figure. Only one band crosses the Fermi surface, and that is the pd ∗ band derived from the CuO2 planes, which is characteristic of all the layered cuprates. An unoccupied band arising from hybridization of Hg 6pz and O(2) 2pz orbitals lies above the Fermi level, and approaches it without ever crossing it. As a result the pd ∗ band is exactly half full, and the stoi chiometric compound = 0 is expected to be a Mott insulator. This is in contrast to the case of Ba2 Tl2 CuO6 , where the hybridization band does dip below the Fermi level. 10.17 Energy bands of stoichiometric HgBa2 CuO4 = 0 along the –S–X– directions defined by Fig. 10.11 for the kz = 0 plane, and along the corresponding Z–U–R–Z directions of the kz = 21 plane in reciprocal space. The horizontal dashed line at E = 0 denotes the Fermi level (Singh et al., 1993a). 296 10 HUBBARD MODELS AND BAND STRUCTURE Figure 10.18 Total (top panel) and local site densities of states derived from the band structure of HgBa2 CuO4 shown in Fig. 10.17, where 1 Ry = 136 eV O1 is in the CuO2 layer, and O(2) is in the [O–Ba] layer (Singh et al., 1993a). Figure 10.19 Energy bands of stoichiometric compound HgBa2 Ca2 Cu3 O8 = 0 using the notation of Fig. 10.18. The five lowest energy bands shown are the Hg 5d manifold, and because of their flatness they produce the large Hg DOS shown in Fig. 10.20 at E = 06 Ry (Singh et al., 1993b). 297 V BAND STRUCTURE OF MERCURY CUPRATES Figure 10.20 Total (top panel) and local site densities of states derived from the bands of HgBa2 Ca2 Cu3 O8 shown in Fig. 10.19 where 1 Ry = 136 eV O1 is in the central Cu(1) layer, O(2) is in the Cu(2) layer, and apical O(3) is in the [O–Ba] layer (Singh et al., 1993b). We see from Fig. 10.20 that the density of states of HgBa2 CuO4 at the Fermi level is quite small because only the pd ∗ band passes through this level, and it is quite steep there. Near but below the Fermi level the DOS arises mainly from the Cu and O(1) atoms of the CuO2 planes. The hybrid band is largely responsible for the DOS shown above EF in Fig. 10.20. The HgBa2 CuO4+ calculations were carried out for stoichiometric materials, i.e., = 0, so no account was taken of the possibility of the presence of oxygen in the Hg plane at the 21 21 0 21 21 1 site of O(3) listed 298 in Table 8.5. The table mentions 11% oxygen occupancy of this site, and this would result in the presence of Cu3+ ions as observed, corresponding to hole doping in the CuO2 planes and metallic behavior. In addition calculations were carried out of the positron charge density that is pre dicted for angular correlation of annihilation radiation (ACAR) experiments carried out with positron irradiation, and the resulting contour plots are shown in Fig. 10.21 for two planes of the crystallographic unit cell. The charge density is smallest at the atom positions because the positrons avoid the positively charged atomic cores. It is largest at the empty O(3) site along the �110� direction. Table 10.3 shows the calculated electric field gradients Vii at all of the HgBa2 CuO4 atom positions, where Vxx = dEx /dx, etc. For each site Laplace’s equation is obeyed, Vxx + Vyy + Vzz = 0, and at sites of tetrago nal symmetry Vxx = Vyy . The gradients are smallest in magnitude for Cu in the planar direction, and largest for Hg. The energy bands of the stoichiomet ric HgBa2 Ca2 Cu3 O8+ compound = 0 are shown in Fig. 10.19 and the density of states plots are in Fig. 10.20. There are some Figure 10.21 Contour plot of positron charge den sity normalized to one positron per HgBa2 CuO4 unit cell determined by ACAR. Adjacent contours are sep arated by 0.0005 e+ /a.u. The density is largest in the voids (O(3) site) of the Hg layer. A uniformly distributed positron would have a density 0.00104 e+ /a.u. (Singh et al., 1993a). 10 HUBBARD MODELS AND BAND STRUCTURE Table 10.3 Electric Field Gradients at the Atom Sites of HgBa2 CuO4 in Units of 1022 V/m2 . The x, y, z Directions Are along the Crystallographic a, b, c Directions, Respectively, but for the O(1) Site the x Direction is Toward the Neighboring Cu Atoms. Four of the Sites have Tetragonal Symmetry: Vxx = Vyy Site Vxx Vyy Vzz Cu O(1) Ba O(2) Hg 0096 131 −033 −070 385 0096 −087 −033 −070 385 −0192 −044 066 139 −770 very strong similarities with HgBa2 CuO4 , but there are also some marked differences. There are three pd ∗ well dispersed antibonding bands that cross the Fermi surface, one for each CuO2 layer, and they are almost superimposed. The hybrid band dips below the Fermi surface at the X and U points and takes electrons from the pd ∗ , band so there are less electrons in the CuO2 planes, corre sponding to the bands of these planes being less than half full. Thus this three-layer Hg compound is self-doped: the Hg layer pro duces hole doping of the CuO2 layers. This is analogous to the Tl2 Ba2 CuO6 case men tioned below. We see from Fig. 10.20 that the den sity of states near but below the Fermi level arises from the three CuO2 planes, while that slightly above EF is due to Hg and the oxy gen atom O(3) in the Hg plane. Subsequent band structure calculations carried out by Singh and Pickett (1994) showed that oxygen occupation of the 21 21 0 21 21 1 site produces additional hole doping of the CuO2 planes. They mentioned that measured values of are 0.06, 0.22, and 0.4 for the n = 0 n = 1, and n = 2 mercury compounds, correspond ing to 0.12, 0.22, and 0.27 holes per Cu atom, respectively, for these three compounds. VI BAND STRUCTURES OF LANTHANUM, BISMUTH, AND THALLIUM CUPRATES 299 VI. BAND STRUCTURES OF LANTHANUM, BISMUTH, AND THALLIUM CUPRATES The lanthanum La1−x Sr2 Cu2 O4 , bis muth Bi2 Sr2 Can Cun+1 O2+2n and thallium Tl2 Ba2 Can Cun+1 O2+2n cuprate supercon ducting compounds have body centered crystal structures, and the tetragonal ones have the Brillouin zone sketched in Fig. 10.22. The geometrical relationship between two adjacent Brillouin zones is shown in Fig. 10.23. The body centered cuprates which exhibit a small orthorhombic distortion from tetragonality have a slightly distorted version of this Brillouin zone which is depicted in Fig. 8.42 of the second edition of this text. A. Orbital States For the undoped compound La2 CuO4 , the copper contributes five d states while each of the four oxygens provides three p states for a total of 17 orbitals. These orbitals are occupied by 33 electrons, which may be counted in one of two ways. Counting by ions, there are nine 3d9 from Cu2+ and six 2p6 from each of the four O2− ions. The ionic state La3+ has no valence electrons. Figure 10.23 Geometrical relationship between adjacent La2 CuO4 Brillouin zones (Kulkarni et al., 1991). Note that the kx ky axes in this figure are rotated by 45� relative to the axes of Fig. 10.22. The description in the text is in terms of the axes of Fig. 10.22 Counting by atoms, there are three from each La, 11 from Cu, and four from each oxy gen. These numbers are listed in Table 10.1. Contour plots of the valence charge den sity around these atoms in coordinate space that were calculated from the band structure are sketched in Fig. 8.26, and discussed in Chapter 8, Section VII.C. If 10% of the La is replaced by Sr to give the superconducting compound La09 Sr 01 2 CuO4 charge neutrality can be maintained by a 3+ change in copper valence to Cu20+ 8 Cu02 , with 22+ an average of Cu . From Table 10.1 we see that Cu2+ has the configuration 3d9 and Cu3+ the configuration 3d8 , which means that Cu contributes 8.8 electrons, instead of 9, and the total number of electrons is 32.8, not 33. A deficit of oxygen can also contribute to the maintenance of charge neutrality. B. Energy Bands and Density of States Figure 10.22 Brillouin zone of body-centered La2 CuO4 with the symmetry points indicated. The sym bols and U denote general points along the [110] directions (adapted from Pickett, 1989). The energy bands of nonsuperconduct ing La2 Cu2 O4 are presented in Fig. 10.24. The superconducting doped compound 300 10 HUBBARD MODELS AND BAND STRUCTURE Figure 10.24 Energy bands of La2 CuO4 along the symmetry directions of the Brillouin zone defined in Fig. 10.22, with EF taken as the zero of energy. These bands also apply to the doped compound La09 Sr01 2 Cu4− . This compound has fewer electrons so its Fermi energy is below (adapted from Pickett et al., 1987). La09 Sr01 2 Cu2 O4 has the same band con figuration, but with the Fermi level slightly lower. In both cases there are 16 low-lying “bonding” bands below the Fermi energy fully occupied by 32 of the 33 valence elec trons, one bonding “hybrid” band near EF and 17 empty higher-energy “antibonding” bands. The hybrid band contains exactly one electron for La2 CuO4 and 0.8 electron for the doped compound La09 Sr01 2 CuO4 , as already noted. Its principal excursion above EF in the X direction is analogous to that of its counterpart at point M in the threestate Hubbard model of Fig. 10.7a. That the bands are in fact two-dimensional is seen by observing in Fig. 10.24 how flat they are along the vertical paths from to Z ((0,0,0) to (0,0,1)), from (1,0,0) to (1,0,1), and from to U ((h,h,0) to (h, h, 1), where h is arbi trary). We can again argue from Eq. (10.58) that the effective mass m∗ is large in the kz direction, and hence that the electrical conductivity is low for current flow perpen dicular to the planes. The hybrid band that crosses the Fermi surface lies below it at special points and Z so these points are electron-like regions, and at point X the same band rises far above the Fermi surface so this is a hole region, as is clear from the sketch of the Fermi surface in Fig. 10.25. Since doping with strontium lowers EF the top of the hybrid band at posi tion A, B on Fig. 10.24 rises above the Fermi level, and it transforms from being electronlike to being hole-like at its peak. The result is that the overall configuration of the Fermi surface changes from being electron-type with enclosed holes to being hole-type with enclosed electrons, as shown in Fig. 10.25. In the former case there is an interconnected region of electrons with isolated patches of holes around special point X, and in the lat ter case there is an interconnected region of holes with isolated islands of electrons at points and Z. This changeover occurs at a Van Hove singularity arising from the hybrid band being fairly flat near points N and A, B of the Fermi level. VI BAND STRUCTURES OF LANTHANUM, BISMUTH, AND THALLIUM CUPRATES 301 Figure 10.25 Fermi surfaces (a) of La2 CuO4 with enclosed holes, and (b) of La09 M01 2 CuO4 with enclosed electrons. See Figs. 10.22 and 8.38 for a clarification of the path –A–B–Z. The bold arrows on (b) approximate nesting wave vectors drawn somewhat longer than the –X distance. The changeover from enclosed holes to enclosed electrons occurs at a van Hove singularity (Pickett, 1989). Since the point Z is a distance /c above , as shown in Fig. 10.22, the electron regions of the superconductor La09 Sr01 2 CuO4− extend vertically, from to Z to , and so on, forming a cylin der of irregular cross-section (Klemm and Liu, 1991) containing electrons surrounded by holes. The shapes of this cross section around the point and around the point Z are shown in Fig. 10.25a. In like manner, the compound La2 CuO4 has vertical cylinders of holes centered at the point X and surrounded by electrons. The change from cylinders of holes to cylinders of electrons is reminiscent of the electron–hole symmetry that was dis cussed in Section III.C. The density of states at the Fermi level is highest in regions where the energy bands are fairly flat. It is clear from Fig. 10.26 that this increase of the density of states at EF when the lowering occurs is mainly associated with the copper and oxygen Oxy atoms in the CuO2 planes where the superelectrons are concentrated. Figures 10.27 and 10.28 show that the density of states at the Fermi Levels of the compounds Bi2 Sr2 CaCu2 O8 and thallium Tl2 Ba2 CuO6 is likewise highest in the CuO2 planes at the copper and oxygen (O(1)) atom positions. Figure 10.26 Total density of states (top) and partial densities of states for the individual atoms of La2 CuO4 determined from the band structure. The Oxy oxygens are in the CuO2 planes (Pickett et al., 1987). The sketch of the “Fermi surface” of La2 CuO4 in Fig. 10.25 is not in accord with experiment because La2 CuO4 is an antiferromagnetic insulator with a 2eV energy gap, and hence no Fermi surface may be defined for it. This shows the limitations of band structure calculations. 302 10 HUBBARD MODELS AND BAND STRUCTURE Figure 10.27 Total (top) and partial densities of states from the band structure of Bi2 Sr2 CaCu2 O8 . The distributions of Cu and O are similar to those from the other cuprates. Most of the Bi density lies above EF , but two Bi derived bands do drop to or below EF (Krakauer and Pickett, 1988). VII. FERMI LIQUIDS In the independent electron approxi mation we treat conduction electrons as noninteracting particles obeying Fermi– Dirac statistics, i.e., as constituting a Fermi gas. When the electrons continue to obey FD statistics and interact with each other in such a way that their properties remain close to those of a Fermi gas, they constitute what may be called a Fermi liquid. Landau (1957) developed a method of taking account of electron–electron interac tions in such a manner as to maintain a oneto-one correspondence between the states of a free-electron gas and those of the inter acting electron system. The existence of such a one-to-one correspondence constitutes the usual definition of a Fermi liquid. In such a liquid the Pauli exclusion principle permits electrons at the Fermi surface to Figure 10.28 Total (top) and partial densities of states from the band structure of Tl2 Ba2 CuO6 . The Cu– O densities are similar to those from the other cuprates. The Tl2 and O(2) spectral density extends just to EF from above (Hamann and Mattheiss, 1988). experience only momentum-changing colli sions. Elementary excitations of quasiparti cles and quasiholes correspond to those of a Fermi gas. In what are called marginal Fermi liquids, the one-to-one correspondence con dition breaks down at the Fermi surface, but many of the properties continue to resemble those of a Fermi liquid (Baym and Pethick, 1991; Levine, 1993; Williams and Carbotte, 1991; Zimanyi and Bedell, 1993). Transport properties of the cuprates, such as resistivity and the Hall effect, are often described by considering the conduc tion electrons as forming a normal Fermi liquid (Crow and Ong, 1990; Tsuei et al., 1989). Varma et al., (1989) ascribed anoma lies in these normal-state properties to marginal Fermi liquid behavior. Anderson (1987c) attributes the superconductivity of the cuprates to the breakdown of Fermi liq uid theory and suggested the applicability of IX CHARGE-DENSITY WAVES, SPIN-DENSITY WAVES, AND SPIN BAGS what are called Luttinger liquids (Anderson, 1990a, b). VIII. FERMI SURFACE NESTING The phenomenon of Fermi surface nest ing occurs when the two sheets of the Fermi surface are parallel and separated by a com mon reciprocal lattice wave vector G = knest . We see from the bottom of Fig. 10.25 that the two sheets of the Fermi surface of La1−x Sr x 2 CuO4 on either side of the hole region are roughly parallel, and that the reciprocal lattice spacing across the region is close√to the wave vector 110/a, of length 2/a, which is also the distance from to X (Crow and Ong, 1990; Emery, 1987a; Pickett, 1989; Virosztek and Ruvalds, 1991; Wang et al., 1990). Two such nesting wave vectors are shown as bold arrows in the figure. The lanthanum compound approaches near-perfect nesting with knest equal to a reciprocal lattice vector. If more electrons are added to the bands, the hole region contracts and the nesting vec tor turns out to be less than G. Decreasing the number of electrons enlarges the hole region, but this also leads to an instability in which the Fermi surface switches from the config uration of isolated hole regions shown at the right of the figure to the isolated electron regions in the left drawing. Further doping decreases the size of these electron regions until the spanning vector k is no longer a reciprocal lattice vector G, and the Fermi surface is no longer nested. More generally, nesting may lead to instabilities in the Fermi surface even in the absence of this “switchover” instability. This can be seen from the viewpoint of pertur bation theory by considering the fact that the energy denominator in the perturbation expression 1/Ek − Ek+G of Eq. (10.43) can approach zero over a wide range of k values for a nesting wave vector knest . The result 303 might be the generation of either a chargedensity wave (CDW), a spin-density wave (SDW), or both. The yttrium compound also exhibits a nesting feature, as may be seen from the parallel Fermi surfaces of Fig. 10.15. However, the spanning k-vectors are not close to the reciprocal lattice vectors, the energy denominators Ek − Ek+G do not become small as in the lanthanum case, and no instability develops. IX. CHARGE-DENSITY WAVES, SPIN-DENSITY WAVES, AND SPIN BAGS We noted in Sections V and VI.A con tour plots of the charge density around the atoms of a superconductor can be determined from a band-structure calculation. Exam ples of such plots were given in Figs. 8.14 and 8.26 for the yttrium and lanthanum com pounds, respectively. In this section we will be concerned with the charge density of an independent electron gas that is calculated self-consistently (cf. Section III) using the Hartree–Fock approximation referred to in Chapter 1, Section II. If this method is applied to an indepen dent electron gas using a potential that is periodic in space and independent of spin, self-consistency can be obtained with solu tions involving charge density which is peri odic in space. In other words, the solution is a charge-density wave. The CDW can have periodicities that are incommensurate with the lattice spacings, and as noted above in Section VIII, CDW is favored by Fermi sur face nesting. A crystal structure distortion and the opening up of a gap at the Fermi surface accompany the formation of a CDW and stabilize it by lowering the energy. The presence of the gap can cause the material to be an insulator. Sufficiently high doping of La2 CuO4 with Sr or Ba disables the nesting 304 and destabilizes the CDW, thereby convert ing the material to a metal and making it superconducting. In quasi-one-dimensional metals the CDW instability that leads to a struc tural distortion is called a Peierls instabil ity (Burns, 1985), a phenomenon which has been discussed in the superconductor litera ture (e.g., Crow and Ong, 1990; Fesser et al., 1991; Gammel et al., 1990; Nathanson et al., 1992; Ugawa et al., 1991; Wang et al., 1990). This CDW represents a nonmagnetic solu tion to the Hartree–Fock equations for an independent electron gas. Solutions with uni form charge densities that are fully mag netized can also be obtained. Overhauser (1960, 1962) assumed an exchange field that oscillates periodically in space and obtained a lower energy solution involving a nonuniform spin density whose magni tude or direction varies periodically in space. This solution corresponds to a spin density wave. Generally, the SDW is incommensu rate because its periodicities are not multiples of the crystallographic lattice parameters, and, as noted, a nesting Fermi surface is favorable for the excitation of a SDW state (Burns, 1985). The antiferromagnetic insula tor state of La2 CuO4 mentioned at the end of Section VI.B involves antiparallel nearestneighbor spins, so that it is the SDW of maximal amplitude and shortest wavelength (Phillips, 1989a). The antiferromagnetism of itinerant electrons, as in a conductor, can be described as a spin-density wave (Kampf and Schrieffer, 1990; Wang et al., 1990). One attempt to understand the mecha nism of high-temperature superconductivity has involved the use of what are called spin bags (Allen, 1990; Anisimov et al., 1992; Goodenough and Zhou, 1990; Schrieffer et al., 1988; Weng et al., 1990). Consider the case of a half-filled band and an appro priately nested Fermi surface, so that the gap SDW extends over the Fermi surface and the system is an antiferromagnetic insulator. The presence of a quasi-particle alters the nearby 10 HUBBARD MODELS AND BAND STRUCTURE sublattice magnetization and forms a region of reduced antiferromagnetic order. Such a region is called a spin bag because it is a metallic domain of depleted spin immersed in a surrounding SDW phase. This spin bag, which moves together with the quasiparticle, has a radius rbag equal to the SDW coherence length, namely rbag = �%F /SDW (Kampf and Schrieffer, 1990). Two spin bags attract each other to form a Cooper pair and, as a result, two holes tend to lower their energy by shar ing one common bag. X. MOTT-INSULATOR TRANSITION If the lattice constant of a conduc tor is continuously increased, the overlap between the orbitals on neighboring atoms will decrease, and the broad conduction bands will begin to separate into narrow atomic levels. Beyond a certain nearestneighbor distance what is called a Mott tran sition occurs, and the electrical conductivity of the metal drops abruptly to a very small value. The metal has thus been transformed into what is called a Mott insulator. One of the chronic failures of bandstructure calculations has been an inability to obtain the observed insulating gaps in oxides such as FeO and CoO. In the prototype Mott insulator NiO the calculated gap has been observed to be an order of magnitude too small (Wang et al., 1990). The Mott insulator problem involves learning how to accurately predict the electronic properties of materials of this type. For the large U case the ground state of the undoped x = 0 Hubbard model system is a Mott insulator, sometimes called a MottHubbard insulator. In the cuprates almost all of the Cu ions are in the 3d9 state, and there is one hole on each site of the system. There exists a large gap for excitations to levels where two antiparallel holes can occupy the same site. This gap of several eV, called the Mott–Hubbard gap, is too large to permit 305 PROBLEMS significant thermal excitation to occur. The system can, however, lower its energy by having individual holes make virtual hops to and from antiparallel neighbors. This virtual hopping process can be maximized by having the spin system assume an antiferromagnet ically ordered configuration. Such ordering has been found experimentally in insulating members of the yttrium and lanthanum fam ilies of compounds (Birgeneau et al., 1987; Crow and Ong, 1990). Some of the cuprate superconductors order antiferromagnetically at very low temperatures. The Mott tran sition in high-temperature superconductors has been widely discussed (Aitchison and Mavromators, 1989; Arrigoni and Strinati, 1991; Brandt and Sudbø, 1991; Cha et al., 1991; Dai et al., 1991; Hallberg et al., 1991; Hellman et al., 1991; Ioffe and Kalmeyer, 1991; Ioffe and Kotliar, 1990; Kaveh and Mott, 1992; Khurana, 1989; Mila, 1989; Millis and Coopersmith, 1991; Reedyk et al., 1992a; Schulz, 1990; Spalek and Wojcik, 1992; Torrance et al., 1992). XI. DISCUSSION In this chapter we presented the Hub bard model approach and then described band-structure calculations that have been carried out for several types of superconduc tors. The calculated bands, densities of states, and Fermi surface plots together provide a good explanation of the normal-state prop erties of the various materials. For example, they describe well the planar nature of the conductivity in the high-temperature super conducting compounds and yield plots of electron density that elucidate the chemical bonding of the atoms. The calculated density of states at the Fermi level does not corre late well with known Tc values in various compounds, however. Some results of band-structure calcula tions agree well with experiment, whereas others exhibit rather poor agreement. There are differences in the calculated results pub lished by different investigators. This would appear to indicate that these calculations are unreliable for estimating properties that have not yet been measured, and thus are more descriptive of superconductivity than predic tive of it. In particular, investigators have not been successful in anticipating whether or not new compounds will be superconductors, and if so, with how high a Tc . Neverthe less, it is our belief that band structures do provide insight into the nature of supercon ductors that could not be obtained otherwise, in addition to elucidating their normal-state properties. FURTHER READING See the first edition for more details and more references on Hubbard models and bond structure. PROBLEMS 1. Show that k is the Fourier trans form of the overlap integral R (Eq. (10.7)), where k = � e−ik·R R R 2. Calculate the expectation value � d3 rk∗ rHk r and show that the energy in the one-band case is given by Eq. (10.8): "k = "a + Bk k 3. Write down expressions similar to Eqs. (10.13) and (10.12) for a diatomic lattice of the NaCl or ZnS type. Why are equations of this type not valid for diatomic lattices in general? 306 10 HUBBARD MODELS AND BAND STRUCTURE 4. Show that the only nonvanishing oper ations involving one-electron number operators are n+ �+� = �+� n− �−� = �−� n+ �±� = �±� n− �±� = �±� 5. Why does the first-order energy shift of the hopping term: Hhop (10.52) vanish? 6. What is the total number of electrons outside the closed shells in the com pound La09 Sr015 2 CuO39 ? How many are contributed by each atom and how many/by each ion? What is the average valence of copper? 7. Show that the denominator Ej − Ei of the second-order term in Eq. (10.43) is equal to the Coulomb repulsion term U for the states �j� = �0±� and � ± 0�. 8. Prove that the only nonvanishing terms of �i �Hhop �j � for i = � j are given by Eq. (10.46). 9. Show that the energy of the ferromag netic states (10.40) is zero, as given by Eq. (10.48). 10. Prove Eq. (10.40), namely that J = 4t4 /U . 11. Show that in the Hubbard model the ionic states �0±� and � ± 0� have the energy U + 2t2 /U , as shown in Fig. 10.6. 12. Show that in the RVB model the two ionic states �00� and �ion� have the respective energies U and U + 4t2 /U , as shown in Fig. 10.6. 13. Show that in the RVB model the states �VB� and �ion� mix, and have the eigenenergies Ei = 21 U ± 41 U 2 + 4t2 1/2 . Show that these reduce to those shown in Fig. 10.6 for the limit U � t. 14. Find the length of the distances to Z (vertical), to Z (horizontal), to X to N to P, and X to P in the Brillouin zone of La2 CuO4 (Fig. 10.22). Express the answers in nm−1 . 15. Explain why S = 006, 0.22, and 0.40 for the n = 0 1 2 Hg com pounds HgBa2 Can Cun+1 O2n+4 give 0.12, 0.22, and 0.27, respectively, holes per Cu atom. 11 Type I Superconductivity and the Intermediate State I. INTRODUCTION In Chapters 5, 6, and 7 we showed that the superconducting state can only exist in a material when the external B field at the surface is less than the critical field Bc for a Type I superconductor and less than the upper critical field Bc2 for a Type II superconductor. For a rod-shaped sample in a parallel external field, the demagnetiza tion factor is zero, so the field H at the surface equals the externally applied field, Hin = Happ , and the situation is not compli cated. For other field directions and other sample shapes, the fact that the demagne tization factor does not vanish complicates matters because it raises the question whether the external field can exceed the critical field over part of the surface but not over the remainder. When this occurs with a Type I superconductor, the sample lowers its free energy by going into an intermediate state involving partial penetration of the external field into the interior. In the present chapter we will examine how this happens. We will discuss thin films, the domains that form in thin films in the intermediate state and the magnetic field configurations associated with 307 308 11 TYPE I SUPERCONDUCTIVITY AND THE INTERMEDIATE STATE thin films. We will also treat the interme diate state induced by transport current in a wire. Most of the chapter will be devoted to these discussions of the intermediate state of a Type I superconductor. A Type II superconductor exists in what is called the Meissner state of total flux exclusion, Bin = 0, for applied fields in the range Bapp < Bc1 and in the mixed state of partial flux penetration when the applied field is in the range Bc1 < Bapp < Bc2 between the lower and upper critical fields. The way in which the demagnetiza tion factor affects these Meissner and mixed states will be discussed the next chapter. For now, bear in mind that the term, interme diate state, applies to Type I superconduc tors, and the term, mixed state, to Type II superconductors. II. INTERMEDIATE STATE We learned in Chapter 1 that the mag netic fields inside any material, including a superconductor, satisfy the general expres sion (1.69) Bin = �0 �Hin + M�� (11.1) We saw in Chapter 2 that an ideal Type I superconductor has the following internal magnetic fields: ⎫ Bin = 0 ⎪ ⎪ ⎬ Type I M = −Hin Bc ⎪ ⎪ Superconducting State Hin < ⎭ �0 (11.2) In this chapter we will see that in the interme diate state of an ideal Type I superconductor, the Hin field is pinned at the value Bc /�0 . This provides us with the relationships ⎫ Bc ⎬ Hin = Type I �0 Intermediate State ⎭ �0 M = Bin − Bc (11.3) for the fields inside. Finally, above Tc the normal state exists with the field configurations M ≈0 Bin ≈ �0 Hin Normal State Above Tc (11.4) where we have written M ≈ 0 since in the normal state ��� � 1, as we showed in Chapter 1, Section XV. In Chapter 5 we were concerned with the internal fields of a superconducting ellipsoid in an applied magnetic field, and we made use of expression (10.33), NBin + �1 − N��0 Hin = Bapp � (11.5) where N is the demagnetization factor. The magnetostatic properties of the intermediate state follow from Eqs. (11.3) combined with (11.5). Since it is not obvious why the inter nal field Hin is pinned at the value Bc /�0 in the intermediate state, we will provide some justification for this in the next section before applying Eq. (11.5) to elucidate the proper ties of this state. III. SURFACE FIELDS AND INTERMEDIATE-STATE CONFIGURATIONS We saw in Chapter 5, Section XIII, that the surface field Bsurf ��� immediately out side a perfectly superconducting sphere has no radial component; it is parallel to the sur face, with the value at the angle � given by Eq. (5.66) with � = −1, 3 Bsurf ��� = Bapp sin �� 2 (11.6) If the applied field Bapp is less than 2Bc /3, the surface field will be less than Bc for all angles, and the perfectly superconduct ing state can exist. If, on the other hand, the applied field is greater than 2Bc /3, we see III SURFACE FIELDS AND INTERMEDIATE-STATE CONFIGURATIONS 309 from Eq. (11.6) that there will be a range of angles near � = �/2, �c < � < � − �c � (11.7) where �c = sin −1 2Bc � 3Bapp (11.8) for which the surface field will exceed Bc . Thus the sphere is unable to remain perfectly superconducting. In the range of applied fields 2 B < Bapp < Bc � 3 c (11.9) the surface field must decompose into super conducting and normal regions that prevent the average internal field Hin from exceed ing the critical value Hc . In other words, the sphere must enter the intermediate state. For lower applied fields it is perfectly supercon ducting, whereas for higher applied fields it is in the normal state, as indicated in Fig. 11.1. The arrows in the figure show how the intermediate state can be traversed by varying either the applied magnetic field or the temperature. One possibility for an intermediate state is for the sphere to go normal in a band around the equator delimited by �c of Eq. (11.8). This, however, would not satisfy the boundary conditions. Another possibility would be for a normal outer layer to sur round a superconducting inner region. But such states do not exist because it is ener getically more favorable for a sphere to split into small regions of normal material adja cent to regions of superconducting material. We know that below Tc the superconducting state is energetically favored. Thus, the for mation of the intermediate state is the way in which a material can continue to possess some of this favorable superconducting-state energy while still satisfying the boundary conditions on the surface field. Figure 11.1 Dependence of the critical field Bc �T� of a Type I superconductor on temperature (upper curve), where Bc = Bc �0� is the critical field at 0 K. The figure also plots the curve 23 Bc �T�, which is the lower limit of the intermediate state (I) of a superconducting sphere. The vertical arrow indicates the path S → I → N traversed by a zero-field-cooled sphere as increasing applied fields bring it from the superconducting state (SC) at Bapp = 0 through the intermediate state to the normal state (N) that exists for Bapp > Bc �T�. The hor izontal path N → I → S traversed by field cooling of the sphere is also shown. It is easier to picture how the interme diate state forms by considering the case of a Type I superconducting film in a perpen dicular magnetic field. We assume a demag netization factor N = 0�9 corresponding to the phase diagram of Fig. 11.2. When the applied field is raised to a value slightly above 0�1Bc �T�, small regions of normal material appear embedded in a superconduct ing matrix, as shown in Fig. 11.3a. This is reminiscent of the vortex lattice that forms in Type II superconductors. We see from the sequence of structures in Figs. 11.3a–11.3f that as the applied field increases along the vertical path of Fig. 11.2, normal regions grow at the expense of the superconduct ing regions. For very high applied fields, as in Fig. 11.3f, when most of the material has become normal, there is still a tendency for the extensive normal regions to be sur rounded by what appear to be filaments 310 11 TYPE I SUPERCONDUCTIVITY AND THE INTERMEDIATE STATE IV. TYPE I ELLIPSOID Now that we have clarified the nature of the intermediate state, it will be instructive to write down the equations of the internal fields in a perfectly superconducting ellip soid. For such an ellipsoid the factor 2Bc /3 in Eq. (11.9) becomes �1–N�Bc , and for the purely superconducting state we have, from Eqs. (5.35)–(5.37), Bapp < �1 − N�Bc � Figure 11.2 Magnetic phase diagram of a film with demagnetization factor N = 0�9 in a perpendicular mag netic field. This large demagnetization factor causes the intermediate state to be quite extensive. The vertical isothermal path S → I traversed by the film in pass ing through the succession of configurations depicted in Figs. 11.3a–11.3f is indicated. of superconducting material. This has been referred to as a closed topology, that is, nor mal regions surrounded by a superconducting phase (Huebener, 1979). We have just described the passage through the intermediate state for increas ing values of the applied field experienced by a sample that has been precooled in zero field (ZFC) at a particular temperature below Tc . We showed that this S → I path pro ceeded along the vertical line in Fig. 11.2. Figure 11.1 shows a vertical S → I → N path for a ZFC sphere that starts in the supercon ducting state, passes through the intermedi ate state as the field increases at constant temperature, and finally reaches the normal state for Bapp > Bc �T�. Another way of attain ing the intermediate state is by field cool ing the sphere along the N → I → S path in the same figure. As the sample gradu ally cools through the intermediate region, it expels flux by forming superconducting regions embedded in a normal matrix, corre sponding to what is called an open topology, the opposite of what happens in the case S → I → N. (11.10) Bin = 0� (11.11) Hin = Bapp /�1 − N��0 � (11.12) �0 M = −Bapp /�1 − N�� (11.13) � = −1� (11.14) This states exists over the range given by Eq. (11.10). The equations for the intermediate state obtained by combining Eqs. (11.3) and (11.5) are �1 − N�Bc < Bapp < Bc � 1 �B − �1 − N�Bc �� N app Hin = Bc /�0 � Bin = 1 �B − Bapp �� N c 1 � = − �1 − Bapp /Bc �� N �0 M = − (11.15) (11.16) (11.17) (11.18) (11.19) The last equation (11.19), will be derived in the following section. The fields given by Eqs. (11.16)–(11.18) are, of course, aver ages over the normal and superconducting regions, as depicted in Figs. 11.3a–11.3f. Setting N = 1/3 in Eqs. (11.15)–(11.19) recovers the expressions for a sphere. Figures 11.4, 11.5, 11.6, and 11.7 show how the various fields and the susceptibility of a sphere vary with the applied field in the 311 V SUSCEPTIBILITY Figure 11.3 Intermediate state domain configurations of a 9.3-�m thick super conducting Pb film in a perpendicular magnetic field at 4.2 K. The structure is shown for the following field values: (a) 9.5 mT, (b) 13.2 mT, (c) 17.8 mT, (d) 21.8 mT, (e) 34.8 mT, and (f) 40.9 mT. The critical field Bc = 80 mT for Pb. The photographs were obtained using a magneto-optical method in which normal and superconduct ing regions are displayed as bright and dark, respectively. Figure 11.2 plots this sequence of increasing fields (Huebener, 1979, p. 22). perfectly superconducting and intermediatestate ranges. The internal field Bin is zero up to 23 Bc and then increases linearly to its normal state value, as shown in Fig. 11.4. Figure 11.5 shows how Hin increases at first, and then remains pinned at Hc throughout the intermediate state. The magnitude of the magnetization, presented in Fig. 11.6, increases more rapidly than it would for a parallel cylinder, then drops linearly to zero. We see from Eqs. (11.4) and (11.19) and Fig. 11.7 that the susceptibility stays pinned at the value � = −1 until the intermediate state is reached and then drops linearly to zero. V. SUSCEPTIBILITY We have seen that a material in the intermediate state is an admixture of normal and superconducting regions that co exist at the mesoscopic level. Viewed from a macroscopic perspective, we average over this structure, considering the material to be homogeneous with uniform susceptibility � = M/Hin given by �= M � Hc (11.20) Substituting the expression from Eq. (11.18) in the latter expression gives Eq. (11.19). 312 11 TYPE I SUPERCONDUCTIVITY AND THE INTERMEDIATE STATE Figure Figure 11.4 Internal magnetic field Bin in the Meiss 11.6 Magnetization M and (11.18)) for the case of Fig. 11.4. (Eqs. (11.13) ner (S) and intermediate (I) states of a Type I supercon ducting sphere �N = 1/3� as a function of the applied field Bapp (Eqs. (11.11) and (11.16), respectively). In this and Figs. 11.5, 11.6, and 11.7, the solid lines rep resent the function that is being plotted, vertical dashed lines indicate the boundaries of the Meissner, intermedi ate, and normal regions, and the unit slope line �− · − · −� gives the behavior for zero demagnetization factor �N = 0�. Figure 11.7 Magnetic susceptibility � (Eqs. (11.14) and (11.19)) for the case of Fig. 11.4. Figure 11.5 Internal field Hin and (11.17)) for the case of Fig. 11.4. (Eqs. (11.12) Since � is an average of the value −1 in the superconducting regions and 0 in the normal regions, for the intermediate state it lies in the range −1 < � < 0� (11.21) assuming the value � = −1 for Bapp ≤ �1 − N�Bc and � = 0 for Bapp ≥ Bc . Susceptibility is an intrinsic property of a material defined by Eq. (1.77) in terms of the internal field Hin , �= M � Hin (11.22) When the magnetization of a sample is measured in an applied magnetic field Bapp = �0 Happ , the experimentally deter mined susceptibility is often deduced from the expression 313 VI GIBBS FREE ENERGY FOR THE INTERMEDIATE STATE �exp = M/Happ � (11.23) and the ratio of these gives for the interme diate state � = �exp Bapp /Bc � (11.24) We can also use a more general expression (10.52), � = �exp /�1 − N�exp �� where B is the externally applied field. The free energy density is easily calculated for the superconducting region (11.10) by substitut ing the expression for M from Eq. (11.27) in (11.26). Carrying out the integration we obtain (11.25) to obtain � from �exp . G�Bapp � = K + 2 1 Bapp � 1 − N 2�0 which is an expression that is valid for Bapp < �1 − N�Bc . For higher applied fields, the interval of integration must be split into two parts, G�Bapp � = K − �1−N�Bc 0 MdB − VI. GIBBS FREE ENERGY FOR THE INTERMEDIATE STATE B MdB� (11.26) 0 where K is a constant to be evaluated. For the pure superconducting region, we have from Eq. (11.13), M = −B/�0 �1 − N�� (11.27) For the intermediate state region M is given by Eq. (11.18), M = −�Bc − B�/N�0 � B MdB� �1−N�Bc (11.30) The intermediate state can be described in thermodynamic terms using the formalism for the Gibbs free energy that was developed in Chapter 4, Sections VII–X. In this section we sometimes simplify the notation by writ ing B for the applied field Bapp and Bc for the critical field Bc �T� at a finite temperature. Consider the case of a zero-field-cooled Type I superconductor in an applied mag netic field that is isothermally increased from Bapp = 0 to Bapp = Bc �T� along a vertical S → I → N path of the type shown in Figs. 11.1 and 11.2. To calculate the Gibbs free energy density along this path, we begin by integrat ing Eq. (4.33), G�B� = K − (11.29) (11.28) Inserting the appropriate expressions (11.27) and (11.28) for the magnetization and carry ing out the two integrations, we obtain after some cancellation of terms G�Bapp � = K − �1/2N�0 ��Bc − Bapp �2 + Bc2 /2�0 � (11.31) an expression that is valid for �1 − N�Bc < Bapp < Bc . At the onset of the normal state �Bapp = Bc �, this reduces to the expression G�Bc � = K + Bc2 /2�0 (11.32) for the free energy density of what is now the normal state. Further integration beyond Bc does not yield anything more because in the normal state � ≈ 0, and hence M ≈ 0, as we showed in Table 1.2. The constant K is selected as the nega tive of the condensation energy Bc2 /2�0 K = −Bc2 /2�0 (11.33) to make the free energy vanish at the upper critical field. This makes G�Bapp � the free energy of the superconducting state relative to that of the normal state at T = 0. The quan tity (11.33) is the condensation energy of 314 11 TYPE I SUPERCONDUCTIVITY AND THE INTERMEDIATE STATE Figure 11.8 Dependence of the Gibbs free energy G on the applied magnetic field Bapp for six values of the demagnetization factor, N (0, 0.1, 1/3, 1/2, 0.9, and ≈ 1), all at T = 0 K. Equations (11.35) were used to plot the curves. Eq. (6.19) found from the Ginzburg–Landau theory and indicated in Fig. (6.2b). If we define two normalized quantities g�b� = G�Bapp �/�Bc2 /2�0 �� b = Bapp /Bc � (11.34a) (11.34b) Eqs. (11.29) and (11.31) become, respec tively, for the superconducting and interme diate regions at T = 0, g�b� = −1 + g�b� = b2 1−N −�1 − b�2 N 0 < b < 1 − N� (11.35a) 1 − N < b < 1� (11.35b) with the special values ⎧ ⎪−1 b=0 ⎨ g�b� = −N b = 1 − N ⎪ ⎩ 0 b=1 (11.36) at the boundaries of the various regions. Equations (11.35) are plotted in Fig. 11.8 for the cases of parallel geome try �N = 0�, a cylinder in a parallel field �N = 0�1�, a sphere �N = 13 �, a long cylinder in a perpendicular field �N = 21 �, and a disk in a perpendicular field �N = 0�9� N ≈ 1�. We see from this figure that a disk or flat plate is in the intermediate state for almost all applied fields below Bc . (This will be dis cussed in Section VIII.) The transformation from the superconducting to the intermediate state occurs when G crosses the dashed line of unit slope in Fig. 11.8. For each case the superconducting state exists at lower fields (the curve for G below the dashed line in the figure), while the intermediate state exists above the line. Figure 11.8 presents plots of the Gibbs free energy from Eqs. (11.35) versus the applied field for several demagnetization fac tors at T = 0. Related figures in Chapter 4 (Figs. 4.10, 4.11, 4.15, and 4.19) present plots of the Gibbs free energy versus temper ature for several applied fields with N = 0. 315 VII BOUNDARY-WALL ENERGY AND DOMAINS Figure 11.9 Dependence of the Gibbs free energy G on the applied magnetic field Bapp for demagnetization factors N = 0� 21 , and 1 at several reduced temperatures t = T/Tc , as indicated in Fig. 11.10. The sample is in the superconducting or mixed state to the upper left of the dashed line and in the normal state to the lower right of the line. The figure is drawn for the condition �0 � Tc2 /Bc2 = 1/� = 2�8. Problem 8 shows how to combine the rel evant expressions—(11.35) for T = 0, and (4.51) for N = 0—to obtain more general expressions that are valid in the supercon ducting and intermediate states when all three quantities T� Bapp , and N have nonzero values. Using these results, the Gibbs free energy G�Bapp � for N = 0� 21 , and 1 is plot ted in Fig. 11.9 versus the applied field for the reduced temperatures t = T/Tc = 0, 0.55, 0.7, 0.8, 0.9, and 1.0, as indicated in Fig. 11.10. We see from these plots that when the temperature is increased, the range of applied fields over which the material super conducts decreases. However, the fraction of this range that is in the intermediate state remains the same since it depends only on the demagnetization factor. VII. BOUNDARY-WALL ENERGY AND DOMAINS We have been discussing the field con figurations and the Gibbs free energy in superconductors without taking into account the details of the resulting domains. In this and the following two sections we will dis cuss these domains and their significance. We begin with the case of a Type I supercon ductor placed in an applied magnetic field which is in the intermediate range (11.15), and then comment on a Type II superconduc tor in the mixed state with Bc1 < Bapp < Bc2 . 316 11 TYPE I SUPERCONDUCTIVITY AND THE INTERMEDIATE STATE Figure 11.10 Dependence of the critical field Bc �T� of a Type I supercon ductor on temperature. The points on the curve designate the values of the critical fields for the reduced temperature points indicated on the dashed line of Fig. 11.9. We adopt the model of a Type I super conductor in the intermediate state that splits into domains of normal material with � ≈ 0 embedded in pure superconducting regions with � = −1. The boundary between these regions contains a density of magnetic energy Bc2 /2�0 . The superconducting regions exclude the magnetic field Bin and are lower in energy because of the Cooper pair con densation energy. The super electron density ns extends into the normal region by a distance equal to the coherence length �. The magnetic field within the boundary, which is of thickness �, contributes a positive energy the magnitude of which is diminished by the effect of the penetration depth � associated with the decay of the magnetic energy. As a result of this effect, the boundary is effec tively shortened, and has thickness dbound ≈ �� − ��� (11.37) The overall energy density per unit area of the boundary layer has the value 2 Bc dbound (11.38) Ebound = 2�0 for a Type I superconductor in the interme diate state. For Type II superconductors, � exceeds � and the effective domain wall thickness from Eq. (11.37) is negative, so that the boundary energy is negative. In other words, the boundary wall energy is positive for small � and negative for large �, where � = �/� is the Ginzburg–Landau parameter. For large � it becomes energetically favorable for the superconducting material to split into domains of large magnetic field strength with positive energies and surrounding transition VIII THIN FILM IN APPLIED FIELD Figure 11.11 Domain core in the normal state with positive energy surrounded by a transition layer bound ary of thickness dbound with negative energy for the case √ � > 1/ 2. 317 Figure 11.12 Magnetic field penetration through a superconducting thin film whose thickness d is small compared to the penetration depth �. regions of negative boundary energy, as shown in Fig. 11.11. The crossover between the positive and negative √ wall energies actu ally occurs at � = 1/ 2, so that domain for mation√becomes energetically favorable for � > 1/ 2.√ For the mixed state, which occurs for � > 1/ 2, the “domains” are, of course, vortices with cores of normal material, as sketched in Fig. 12.7. This energy argument makes it plausible to conclude that the mixed or vortex state forms in Type √ II supercon ductors, which have � > 1/ 2, but does not form in Type I superconductors. VIII. THIN FILM IN APPLIED FIELD Many studies have been carried out with films that are thin in comparison with their length and width. When such a mate rial is placed in a magnetic field Bapp that is oriented perpendicular to its surface, the field penetrates in the intermediate state, as shown in Fig. 11.12. We illustrate the case for N = 56 , so the factor 1 − N = 16 for this film. Figures 11.13–11.16 show plots of Eqs. (11.10)–(11.19) giving the depen dences of Bin � Hin � M, and �, respec tively, on the applied field. The great extent of the intermediate state is evident from these plots. Figure 11.13 Internal magnetic field Bin in a super conducting film �N = 5/6� as a function of the applied field Bapp (Eqs. (11.11) and (11.16)) (cf. case of a sphere, Fig. 11.4). Here and in Figs. 11.14 and 11.15, the unit slope line �− · − · −� represents the behavior for zero demagnetization factor �N = 0�. Let us examine in more detail the case of a disk-shaped film of radius a and thick ness t � a. We know from Table 5.1 and Problem 6 of Chapter 5 that this film has a demagnetization factor N ≈ 1 − 21 �t/a, so that, from Eq. (11.15), the intermediate state extends over the range 318 11 TYPE I SUPERCONDUCTIVITY AND THE INTERMEDIATE STATE Figure 11.14 Internal field Hin (Eqs. (11.12) and (11.17)) in the film sketched in Fig. 11.12. Figure 11.16 Magnetic susceptibility � (Eqs. (11.14) and (11.19)) of the film sketched in Fig. 11.12. Bin = Bapp − 1 �t 2 Na �Bc − Bapp �� (11.40) is close to the applied field, Bin ≈ Bapp , over most of the intermediate state to a much greater extent than that shown in Fig. 11.13, since �t/2Na � 16 . When the film thickness becomes comparable with or less than the penetration depth, the situation is more com plicated, however. IX. DOMAINS IN THIN FILMS Figure 11.15 Magnetization M (Eqs. (11.13) and (11.18)) for the film sketched in Fig. 11.12. 1 �t 2 a < Bapp < 1� Bc (11.39) This means that a superconducting film with a thickness-to-diameter ratio t/2a = 10−3 and a lower critical field Bc1 = 50 mT is driven to the intermediate state by the Earth’s typical field of 50 �T. The internal field from Eq. (11.16), We just saw that a thin film in a perpen dicular field below Tc is in the intermediate state for almost all applied fields below Bc . We will proceed to investigate the nature of this state. From the boundary conditions, the macroscopic B fields are continuous across the boundary, as shown in Fig. 11.12. Bin = Bapp � (11.41) If we take into account the domain structure, a fraction of the material fn will be nor mal material with Bin = Bc and a fraction fs 319 IX DOMAINS IN THIN FILMS Figure 11.17 Passage of magnetic field lines B of a perpendicular applied field through normal domain regions with diameter Dn of a superconducting thin film. The distortion distance Ddist , normal regions in which Bin = Bc , and superconducting regions (SC) in which Bin = 0 are shown. The energy densities in the normal regions un , in regions far from the film uapp , and in regions near the film �u� are indicated. will be perfectly superconducting with Bin = 0, where fs + fn = 1� (11.42) The magnetic field avoids the superconducting parts and passes through the normal regions, as shown in Fig. 11.17. This means that Bin = fn Bc � so that (11.43) Bapp = fn Bc � (11.44) from Eq. (11.41). The boundaries or domain walls between the normal and superconduct ing regions also contain the field Bc , but it is assumed that the fraction of material fw in the domain walls is small and can be neglected. The figure gives the energy density u = B2 /2 �0 at three positions in the field. Figure 11.18 sketches the domain structure in a thin film of length L, width W , and thickness d that is oriented perpendicular to the direction of the applied field. The figure Figure 11.18 Thin film in a perpendicular applied magnetic field showing normal regions (n) of length Dn , superconducting regions (SC) of length Ds , and domain walls of thickness � separating these regions. The repetition length D = Dn + Ds + 2� is also shown. 320 11 TYPE I SUPERCONDUCTIVITY AND THE INTERMEDIATE STATE shows normal regions of width Dn and super conducting regions of width Ds separated by domain walls of thickness �. In drawing this figure we have assumed that the domains are all the same size and equally spaced. This simplifies the mathematics without changing the physics of the situation. We can define a repetition length D for the domain pattern Ds + Dn + 2� = D� (11.45) where each domain has two walls. If we neglect the thickness of the domain walls, as is done on Fig. 11.17, by assuming that � � Ds � Dn , we can write Ds + Dn = D� (11.46) where Ds = fs D� Dn = fn D� (11.47) The number of domains Nd is equal to the length L divided by the domain repetition length D: Nd = L/D� (11.48) The magnitude of the B field is appre ciably distorted from its far value Bapp only within a distance Ddist of the surface given by 1/Ddist = 1/Ds + 1/Dn � (11.49) and with the aid of Eq. (11.47) we obtain Ddist = fs fn D (11.50) for the field distortion distance indicated in Fig. 11.17. Let us try to justify Eq. (11.49) by a hydrodynamic analogy. Consider the B lines as the flow lines of a fluid passing through slots or holes in a barrier, where the density of flow lines represents the speed. The speed changes appreciably near the holes only if the diameter of the holes is small and near the material between the holes only when the holes take up most of the space, as shown in Fig. 11.19. Therefore Ddist ≈ Dn in the former case, when Dn � Ds , whereas Ddist ≈ Ds in the latter case, when Dn � Ds . Figure 11.19 illustrates the cases Ds = 3Dn � Ds = Dn , and Ds = 13 Dn . The distortion of the applied magnetic field brought about by the presence of the film, as sketched in Figs. 11.17 and 11.19, serves to increase the Gibbs free energy G of the system. Figure 11.17 shows the mag netic energy densities of each region. The Gibbs free energy is also increased by the magnetic energy stored in the domain walls. A long repetition length reduces the num ber of domains and decreases the domain wall energy, whereas a short repetition length lessens the distortion of the field and decreases the field distortion energy at the expense of more domain wall energy. An intermediate domain repetition length is best, and we will derive an expression for the opti mum value of D. The magnetic energy stored in each pair of domain walls 2W�d� 21 Bc2 /�0 � gives for the total domain wall contribution to the Gibbs free energy 1 2 B /� Gw = 2Nd �W�d� 2 c 0 1 2 = 2�WL�d/D� Bc /�0 � 2 (11.51) (11.52) where we have used Eq. (11.48). The change in field energy arises from the difference between energy density near the surface, 1 f B2 /�0 , and the energy density far from 2 n c 2 /�0 , where the factor fn in the film, 21 Bapp the former expression takes into account the fact that this field exists only near the normal regions, as shown in Figs. 11.17 and 11.19. This gives for the magnetic field contribution to the Gibbs free energy 321 IX DOMAINS IN THIN FILMS Figure 11.19 Illustration of the distortion distance Ddist for the cases Ds = 3Dn with Ddist ≈ Dn �a�� 21 Dn = 21 Ds ≈ Ddist �b�, and Ds = 13 Dn with Ddist ≈ Ds �c�, where the wall thickness � is negligible, i.e., � � Dn � Ds . Gf = 2WLDdist fn − 1 2 B /� 2 app 0 = 2�WLD�fs2 fn2 1 2 B /� 2 c 0 dG = 0� dD (11.53) 1 2 Bc /�0 � 2 (11.54) where we have used Eqs. (11.42), (11.44), and (11.50). The total Gibbs free energy G is the sum of these two, namely G = Gw + Gf . Per unit area of film we have 1 2 G/WL = 2 Bc /�0 ��d/D + fs2 fn2 D�� 2 (11.55) The domain repetition distance D obtained by minimizing the total free energy per unit area, (11.56) is equal to D = �d��1/2 /fs fn � (11.57) where the product fs fn is easily deduced from Eqs. (11.42) and (11.44): fs fn = Bapp �Bc − Bapp �/Bc2 � (11.58) The thinner the film, the smaller the value of D and the greater the number of domains. D is large at both ends of the range, where either fn or fs is small, corresponding to Bapp � Bc and Bapp ≈ Bc , respectively. It is smallest in the middle, where fn = fs = 21 and Bapp = 21 Bc . 322 11 TYPE I SUPERCONDUCTIVITY AND THE INTERMEDIATE STATE This derivation assumes that the domain wall thickness � is much less than the domain sizes Dn and Ds . It does not take into account how the surface energy depresses the value of the critical field. When the film thickness is much greater than the domain wall, d � �, the critical field Bc is shifted to a lower value Bc� given by (Tinkham 1996, p. 29) Bc� = �1 − 2��/d�1/2 �Bc d � �� (11.59) A similar depression of the lower critical field Bcl occurs with Type II superconductors. X. CURRENT-INDUCED INTERMEDIATE STATE The intermediate state that we have been discussing arose from the presence of a mag netic field that exceeded the critical field at the surface of the superconductor. We will now examine the intermediate state that forms when a transport current from a cur rent generator produces a magnetic field at the surface of a superconducting wire that exceeds the critical field. In this section we simplify the notation by writing I instead of IT for the transport current. We know from Eq. (2.42) that the mag netic field at the surface of a wire of radius a carrying a current I is in the � direction with magnitude H = I/2�a� (11.60) This surface field is independent of the dis tribution of current density inside the wire. When the surface field reaches a particular value, called the critical field Bc = �0 Hc , we say that the transport current has attained its critical value Ic , corresponding to Hc = Ic /2�a� (11.61) If the current exceeds the critical value, the magnetic field at the surface will exceed Hc and the wire will no longer be able to remain a perfect superconductor. This destruction of pure superconductivity by a transport current is called the Silsbee effect. If the wire were to respond by going normal at the surface, the superconducting core would constitute a wire of even smaller radius r < a carrying the same amount of current. From Eq. (11.60) it is clear that the field at the surface of the wire would then be even larger than the field that drove the surface normal. Following this line of rea soning, the entire wire would become normal. There is, however, a second solution to the problem, proposed by F. London (1937; see also F. London, 1950), whereby the wire is assumed to have a core of radius ai that is in an intermediate state and an outer layer that is normal. We will show how this could occur. When the total current I exceeds Ic , part of the current In flows in the outer normal region and the remainder Ii along a parallel path through the core, which is in the inter mediate state, I = In + Ii � (11.62) as indicated in Fig. 11.20. The current density Jn in the outer layer is constant, with a value given by Figure 11.20 Division of applied transport current flowing through a superconducting wire of radius a into a portion In flowing in the outer normal region and a portion Ii in the intermediate state flowing in the core of radius ai . 323 X CURRENT-INDUCED INTERMEDIATE STATE Jn = In ��a2 − a2i � ai < r < a� (11.63) For this normal current In to flow there must be a potential difference between the two ends of the wire, which means that there is an axial electric field E in the normal layer given by Eq. (1.21), E = J n �n � (11.64) where both Jn and E are unknown. The intermediate state has regions of superconducting material and regions of nor mal material, so there is also an elec tric field E�r� present. All the magnetic fields that are present are independent of time, so from the Maxwell curl relation � × E = −�B/�t = 0� E is also independent of the radial distance r. Therefore, E�r� has the same value E in the normal and in the intermediate state region, and we can write an analogue of Eq. (11.64) for the interme diate state, E = Ji �r��i �r� 0 < r < ai � We show in Problem 10 that the current den sity in the intermediate state is given by Ji �r� = �ai /r�Jn r ≤ ai � (11.71) as illustrated in Fig. 11.21, where Hc = Jn ai � (11.72) Combining Eqs. (11.64) and (11.72) gives for the radius of the intermediate state region ai = Hc �n /E� (11.73) which depends on the applied current in the manner shown in Fig. 11.22. The resistivity in the intermediate state is proportional to the radius r, r �n r ≤ ai � (11.74) �i �r� = ai (11.65) where Ji �r� satisfies the boundary condition for continuity of the current density at r = ai . Thus we obtain Ji �ai � = Jn � (11.66) �i �ai � = �n � (11.67) We saw in Section II that the interme diate state is characterized by the pinning of the internal field Hin at the critical value, Hin = Hc 0 < r < ai � (11.68) This permits us to write Eq. (11.61) for the intermediate state, Hc = Ii �r�/2�r r < ai � (11.69) where Ii �r� = r 0 Ji �r��2�r�dr� (11.70) Figure 11.21 Dependence of the current density J�r� on distance r from the center in a superconducting wire of radius a that is in the intermediate state. J�r� decreases with r in the intermediate-state core region of radius ai and has a constant value Jn = Hc /ai in the outer layer, where ai ≤ r ≤ a, as shown. The extrapo lation (– – –) of the core region behavior of J�r� to the value Hc /a at the surface is indicated. 324 11 TYPE I SUPERCONDUCTIVITY AND THE INTERMEDIATE STATE Figure 11.22 Dependence of the core radius ai of a superconducting wire on the applied transport current I. The intermediate state occurs for transport currents exceeding the value Ic = 2�aHc . as shown in Fig. 11.23 (see Problem 11). This means that the longitudinal path length of the current through the normal region at the radius r is proportional to r. This fits the configuration illustrated in Fig. 11.24, which had been suggested by F. London. In this configuration the core has a sequence of conical regions of superconducting mate rial arranged along the axis with interlaced regions of normal material. It is shown in Problem 16 that the total current flowing through the wire is given by I = ��a2 + a2i �Jn � (11.75) Figure 11.23 Dependence of the resistivity ��r� of By Eqs. (11.64), (11.72), and (11.73), this may be written as a quadratic equation in terms of the electric field, I�E� = �a2 E � + �Hc2 n � �n E a superconducting wire in the intermediate state on the radial distance r from the center of the wire. Note that ��r� increases linearly with r in the intermediate-state core region, where r < ai , and has the normal state value �n in the outer region, r > ai , of the wire. (11.76) which has the solution 1/2 1 � � E = I n2 1 ± 1 − �Ic /I�2 2 �a (11.77) The average resistivity ��� is E/�J � and the average current density �J � through the wire is I/�a2 , so we can write ��� = E��a2 /I�� (11.78) 325 X CURRENT-INDUCED INTERMEDIATE STATE Figure 11.24 London model for the intermediate-state structure of a wire of radius a carrying a transport current in excess of the critical value Ic = 2�aHc , where ai is the radius of the core region (F. London, 1937, 1950). and Eq. (11.77) gives us the London model expression ⎧ ⎫ 2 1/2 ⎬ ⎨ ��� 1 I � (11.79) = 1+ 1− c ⎭ �n 2⎩ I which is valid for I > Ic . The positive sign has been selected in Eq. (11.77) because it gives the proper asymptotic behavior of ��� → �n for I � Ic . The various resistivity results in the London model can be grouped together as follows: ⎧ ⎪0 ⎪ ⎪ ⎪ ⎨1 ��� 2 = 1 2 1/2 ⎪ �n 1 + 1 − �I /I� ⎪2 c ⎪ ⎪ ⎩ 1 − 41 �Ic /I�2 I < Ic I = Ic I > Ic I � Ic � (11.80) We see that at the point I = Ic the resis tivity jumps discontinuously from 0 to the value 21 �n . It then slowly approaches �n for higher applied currents in accordance with Eq. (11.80), as shown in Fig. 11.25. Exper imental data, such as those plotted in the figure, ordinarily show a larger jump of 23 or more at I = Ic instead of 21 . A refined version Figure 11.25 London model dependence of the resistance of the intermediate state of a superconducting wire on the value of the transport current I for a fixed temperature T . Experimental data on indium wires at 2.02 K (Watson and Huebener, 1974) are shown for comparison. 326 11 TYPE I SUPERCONDUCTIVITY AND THE INTERMEDIATE STATE Figure 11.26 Temperature dependence of the resistance in the intermediate state of a current-carrying wire showing Tc decreasing by the variable amount �T for resistance in the range 21 Rn < R < Rn , and by a fixed amount �T in the range R < 21 Rn . The figure is drawn for the case of a constant applied transport current. of the London model developed by Baird and Mukherjee (1968, 1971) exhibits a larger jump and fits the data better (Huebener, 1979, p. 213; Watson and Huebener, 1974). It is interesting that the intermediate state persists above Ic , and that some supercon ductivity is predicted to remain in the core region for all finite currents. Tinkham (1996, p. 34) shows that there is also a dependence of the resistivity on tem perature, �T = Tc –T , in the neighborhood of the transition temperature, and this is shown in Fig. 11.26. We have discussed the current-induced intermediate state for superconducting wire of circular cross-section. The same phe nomenon can occur with samples of other shapes, such as tapes or thin films, but the mathematical analysis can be more complex. XI. RECENT DEVELOPMENTS IN TYPE I SUPERCONDUCTIVITY A. History and General Remarks The intermediate state has a long his tory beginning with the pioneering works of Landau (1927, 1038) and continuing to the present day (Reisin and Lipson, 2000, Prozorov et al., 2005, Choksi et al., 2004, Goldstein et al., 1996, Dorsey and Gold stein, 1998, Narayan, 1998, Hernandez and Dominguez, 2002, De Luca, 2000). The topic has been intensively studied from the early 60 s for about 30 years when most of the classical results were obtained and the thermodynamic interpretation was developed. However, the literature of that period, and especially later periods, is full of observations incompatible with the Lan dau laminar model (Solomon and Harris, 1971, Livingston and DeSorbo, 1969). These results were mostly interpreted to be due to sample imperfections, particular shape, or other special (vs. general thermodynamic) experimental circumstances. The Type-I problem involves both microscopic mechanisms of superconduc tivity and the physics of highly nonlinear systems, so exact mathematical solutions do not exist, and various approximations have to be used. Early models based on free energy minimization were insensitive to the manner in which the intermediate 327 XI RECENT DEVELOPMENTS IN TYPE I SUPERCONDUCTIVITY state was prepared, and could not predict the equilibrium pattern of flux penetration. During the past decade many new ideas and methods in physics and mathematics of complex and nonlinear systems were devel oped. These advances resulted in more gen eral approaches to the intermediate state (Liu et al., 1991, Hernandez and Dominguez, 2002, Reisin and Lipson, 2000, Dorsey and Goldstein, 1998, Goldstein et al., 1996, Jeudy et al., 2004, Prozorov et al., 2005). In particular, recent contributions considered the evolution of arbitrarily-shaped domains through a current-loop approach (Dorsey and Goldstein, 1998, Goldstein et al., 1996, Reisin and Lipson, 2000), analyzed the kinet ics of the transition as an important factor determining the structure (Liu et al., 1991, Frahm et al., 1991), studied the transforma tion of a tubular to a laminar structure in thin films (Jeudy and Gourdon, 2006), and showed the existence of a topological hys teresis (Prozorov et al., 2005). 200 Applications of the developed ideas are found in many scientific disciplines such as superconductivity and superfluidity, hydrodynamics, reaction-diffusion problems, oceanography, astrophysics, meteorology, combustion, geophysical and biological dynamics, and semiconductors (Walgraef, 1997, Strogatz, 1994, Metlitski, 2005). There is an intense ongoing research effort to explain the formation and evolution of com plex patterns observed in these systems. The selection of one pattern over another is an inherently nonlinear evaluation. Amaz ing similarities between hexagonal structures observed in Type-I superconductors (see Fig 11.27). and some chemical and hydraulic systems provide further evidence of the inti mate connection of their formation. Like wise, a well-known Landau laminar structure is not unique for Type-I superconductors. Figure 11.28 shows two very similar pat terns. Figure 11.28a shows a pattern obtained as a result of a photochemical reaction after T=5 K 4πM(1 – N) (G) 100 0 –100 flux exit –200 –400 –200 0 H (Oe) 200 Figure 11.27 Magneto-optical images of the intermediate state (at magnetic field values indicated by arrows) in pure lead, shown together with DC magnetization loops measured at 5 K. The wide hysteretic loop was measured in a cold-worked sample, whereas the inner loop was obtained in a stress-free sample (Prozorov et al., 2005). 328 11 TYPE I SUPERCONDUCTIVITY AND THE INTERMEDIATE STATE Figure 11.28 Comparison of patterns observed in (a) a photochemical reaction upon irradiation of mercury dithizonate with visible light (from (Walgraef, 1997), page 28) and (b) a laminar intermediate state pattern observed in stress-free lead upon flux exit (Prozorov et al., 2005). mercury dithizonate was irradiated with vis ible light (picture reproduced from (Wal graef, 1997)), whereas Fig. 11.28b shows a laminar intermediate state pattern in a stress-free pure lead sample upon magnetic flux exit (Prozorov et al., 2005). Another example involves the transformation of a closed topology to an open topology pat terns, which occurs in one system at dif ferent external conditions. Figure 11.29a,b shows an experimental realization of the Turing instability mechanism, based on a nonlinear interaction between reaction and diffusion in a chlorite-iodide-malonic acid reaction in gels. Figure 11.29c,d shows the intermediate state patterns in pure lead upon flux entry (c) and exit (d). Further more, closed and open topologies can coexist within one sample. We present two exam ples of such coexistence: Figure 11.30a depicts the results of a numerical analy sis of Hopf bifurcation patterns, whereas Fig. 11.30b shows the transformation of a tubular phase into a laminar structure in pure lead. To summarize, as of today, the problem of the formation and evolution of the inter mediate state in samples of arbitrary shape (especially non-ellipsoidal) and for the arbi trary values of the G-L parameter (as well as other materials parameters) has not yet been settled. Clearly, it cannot be deduced solely from energy minimization arguments, Figure 11.29 (a–b) Turing instability patterns observed in a disk gel reactor (Walgraef, 1997), and (c–d) intermediate state patterns in pure lead upon flux entry (c) and exit (d), after Ref. (Prozorov et al., 2005). Figure 11.30 Coexistence of closed and open topologies within a single ample: (a) numerical solu tion of Hopf bifurcation patterns, and (b) disruption of a tubular phase by a defect. including solving the non-linear G-L equa tions, and requires methods developed in the field of nonlinear complex systems. On the other hand, the systematic experimen tal investigation of the pattern formation in Type-I superconductors can influence other, sometimes quite remote, fields of science. An example is new concepts in the physics of neutron stars (Buckley et al., 2004). Another very important subject is pattern formation in highly nonlinear systems for which a Type-I superconductor is a perfect model system XI RECENT DEVELOPMENTS IN TYPE I SUPERCONDUCTIVITY (Coullet and Huerre, 1991, Choksi et al., 2004, Walgraef, 1997). It provides a set of characteristics, such as a very small effec tive mass of the S-N boundary, and easy manipulation by the external magnetic field, unachievable in other, mostly chemical dif fusive systems. B. The Intermediate State The intermediate state is formed in Type-I superconducting samples when the actual magnetic field at the sample’s edge exceeds the critical field, Hc , which occurs for an applied magnetic field of H = Hc �1 − D�, and it disappears when the applied field reaches H = Hc (Livingston and DeSorbo, 1969, Huebener, 2001). As illustrated in Fig. 11.31, there are four ways to arrive to a particular point on the magnetic field – tem perature, H–T , phase diagram. These four ways are field cooling (FC or �NI�H �, zerofield cooling (ZFC or �SI�H ), and ascending and descending branches of the magnetiza tion loop, �SI�T and �NI�T , respectively. We utilize the notation developed in the early lit erature as it better reflects the specifics of the transition from a Meissner superconduct ing state (S), or a normal state (N), to an intermediate state (I). Normal Hc 800 H (Oe) (NI)T laminar (open topology) 600 Intermediate (SI)H 400 (NI)H (1 – D)Hc Meissner 200 flux tubes (closed topology) 0 0 1 2 3 (SI)T 4 5 6 7 8 T (K) Figure 11.31 Four ways to obtain particular field and temperature responses on an H−T phase diagram. The diagram for a rctangular crossection lead sample with demagnetization factor D = 0�5 is shown. 329 The uncertainty in understanding the formation of an intermediate state already begins at this point. The notion of the demagnetization factor is strictly applica ble only to the samples of ellipsoidal shape (Osborn, 1945, Abrikosov, 1988). Only in this case does the magnetic field inside the sample remain uniform and equal to H/�1 − N � (denoted D in Fig. 11.31). Direct visualization of the intermediate state is ordi narily carried out on samples with flat sur faces, usually slabs or disks. There is an ongoing discussion on the effects of this non-ellipsoidal geometry, with no consensus yet achieved (Huebener, 2001, Dorsey and Goldstein, 1998, Castro et al., 1999, Castro et al., 1997). The thermodynamics of the intermedi ate state has been the subject of many works (Livingston and DeSorbo, 1969, Huebener, 2001, DeSorbo and Healy, 1964, Clem et al., 1973, Choksi et al., 2004, Farrell et al., 1972). The conventional approach is to assume some geometrical pattern of the inter mediate state, and then minimize its free energy by varying the geometrical para meters. The typical and most used structure is the Landau laminar pattern of alternat ing normal and superconducting regions. The free energy is assumed to consist of the condensation energy loss inside the normal domain, the S-N surface energy, the mag netic field energy, and energy associated with the distortion of the magnetic field out side the sample. The latter has often been analyzed in terms of interactions between the lamellae. The variety of the observed structures as well as the general difficulty of expressing the free energy by taking into account all terms inside and outside of the sample motivated various refinements of these models as well as some adjustments of the geometrical patterns, such as possi ble branching near the superconductor sur face or the lamellae corrugation (Livingston and DeSorbo, 1969). The hexagonal pat tern for the intermediate state was also 330 11 TYPE I SUPERCONDUCTIVITY AND THE INTERMEDIATE STATE analyzed (Goren and Tinkham, 1971). The closed topology patterns in the form of flux tubes (typically carrying thousands of flux quanta) were also frequently observed and discussed (Huebener and Gallus, 1973, Huebener and Kampwirth, 1974, Huebener et al., 1974, Chimenti and Huebener, 1977, Buck et al., 1981, Pavlicek et al., 1981, Parisi et al., 1983, Fietz et al., 1984, Pro zorov et al., 2005, Pavlicek et al., 1982, Livingston and DeSorbo, 1969, Huebener, 2001, Goren and Tinkham, 1971). Typical explanations included the edge barrier in (mostly) thin samples. Recent works con centrate more and more on the question of pattern formation in the intermediate state by studying the dynamics of the S-N (and N-S) transition, and/or considering systems that consist of nuclei that can evolve and change geometry upon interaction with the environment (e.g., the current-loop model) (Liu et al., 1991, Doelman and Harten, 1995, Indekeu and van Leeuwen, 1995, Goldstein et al., 1996, Castro et al., 1997, Dorsey and Goldstein, 1998, Reisin and Lipson, 2000, Blossey, 2001, Abreu and Malbouis son, 2004, Jeudy et al., 2004, Choksi et al., 2004, Prozorov et al., 2005). It should be noted that we mostly dis cussed experimental works in which the intermediate state patterns were directly observed. There is also an extensive liter ature involving the use of various indirect techniques. While these works provide important contributions, especially in terms of the analysis and overall consistency of the results with theoretical models, it is dif ficult to consider particular topological fea tures without literally viewing them. C. Magneto-Optics with In-Plane Magnetization – a Tool to Study Flux Patterns The magneto-optical technique is a pow erful method for studying the distribution of the magnetic induction B on the surface of a superconductor. Appearing in the late 50 s (Alers, 1957) and greatly improved dur ing the followed decade (Castro et al., 1999, Huebener, 1970), it has become a unique tool for the experimental study of these mate rials. The idea behind the technique is to place a transparent magnetic material (an indicator) on the surface of an object under study. Linearly polarized light propagating throughout the indicator and reflected back is rotated proportionally to the magnetiza tion strength along the direction of travel (Faraday Effect). If an indicator is made of a soft magnetic material, the distribution of the magnetization inside the indicator mimics the distribution of the perpendic ular component of the magnetic induction on the surface of the sample under study. Various indicators were used. Most known results obtained on visualization of flux pat terns in Type-I superconductors in 60 s–70 s were obtained using Ce3+ salts and later EuS-EuF systems (Kirchner, 1973, Haber meier, 2004, Huebener and Clem, 1974, Huebener, 2001). Unfortunately, the former has a very low Verdet constant (how much 1 mm of thickness rotates the polarization plane per unit of magnetic field), and the latter systems have complicated magnetic transitions at low temperatures. Neverthe less, it was possible to successfully utilize these indicators for imaging the interme diate state (Alers, 1957, Kirchner, 1969, Kirchner, 1973, Huebener and Clem, 1974, Huebener, 2001). However, measurements of the actual magnetic induction were too dif ficult. Another disadvantage of these indica tors was the need to deposit them directly onto the surface of superconductors. For reviews of the magneto-optical technique and its applications, see Ref. (Jooss et al., 2002, Huebener, 2001, Habermeier, 2004, Livingston and DeSorbo, 1969). The widespread use of magneto-optics for studying high-Tc superconductors began with the introduction of ferrimagnetic in-plane indicators (Dorosinskii et al., XI RECENT DEVELOPMENTS IN TYPE I SUPERCONDUCTIVITY A P Bi – doped Y-Fe-garnet indicator LIGHT POLARIZATION H=0 Mz = 0 mirror H Mz > 0 H Mz < 0 Light intensity ~ Mz ~Bz Figure 11.32 Principle of magneto-optical visual ization using a Y-Fe-garnet indicator with in-plane spon taneous magnetization. 1993, Vlasko-Vlasov et al., 1992, Castro et al., 1999), which have a spontaneous magnetization lying in the indicator plane. Figure 11.32 illustrates the principles of operation of such magneto-optical system. A light beam passes through a linear polar izer (P), propagates through the optically transparent indicator film, reflects from a mirror deposited on the bottom surface of an indicator, and finally arrives at an ana lyzer (A) which is oriented perpendicular to a polarizer. The spontaneous magnetization of a ferrimagnetic indicator (Curie temper ature about 400 K) is aligned in the film plane. Faraday rotation only occurs if there is a magnetic moment in the direction of the light beam, therefore without an exter nal magnetic field there is no Faraday rota tion. When a perpendicular magnetic field is applied the nonzero perpendicular compo nent �Mz � of the magnetization is induced, and the intensity of the light transmitted through an analyzer increases in proportion to the applied field strength. When such an indicator is placed on a superconductor, the distribution of the out of plane compo nent of magnetization, Mz , inside the indi cator is proportional to the distribution of the perpendicular component of the magnetic induction, Bz , on a superconductor surface. Therefore, it can be visualized as a real- 331 time two-dimensional optical picture. The main advantages of this technique are the ability to perform quantitative measurements of the magnetic induction (and even of the magnetic moment), outstanding spatial res olution and magnetic field sensitivity, and the near absence of a temperature depen dence below 100 K. Figure 11.27 presents magneto-optical (MO) images of the inter mediate state in pure lead, as well as corre sponding DC magnetization loops measured at the same temperature on the same sample (Prozorov et al., 2005). The wide hysteretic loop was measured in a cold-worked sample and corresponding MO images show den dritic flux penetration and substantial flux trapping upon reduction of the external field to zero. In contrast, the stress-free sam ple (obtained by homogeneous solidification from the melt) shows two distinct topologies of the intermediate state: a closed topology in the form of flux tubes on flux entry, and an open laminar-type structure upon flux exit. Although, a similar tube phase was observed in the 60 s, it has never been accepted as a possible true equilibrium topology (of thick samples). Moreover, recent experiments on samples of different shapes confirm that in ellipsoidal samples the tubular phase is the stable pattern of the intermediate state, both for flux penetration and flux exit. Another aspect of magneto-optical imaging is a possibility of obtaining the current density distribution from the mea sured induction pattern. This is a difficult mathematical problem, because it involves two dimensional inversion of the BiotSavart integral with kernel singularities (Wijngaarden et al., 1996, Jooss et al., 2002). Figure 11.33a shows a polygonal pattern obtained in pure lead (note the interesting hexagonal structure of heptagonal inclu sions), and Fig. 11.33b shows correspond ing current density flow. This information is important since it takes into account the success of the recent current-loop model (Choksi et al., 2004, Reisin and Lipson, 332 11 TYPE I SUPERCONDUCTIVITY AND THE INTERMEDIATE STATE Figure 11.33 (a) Experimental polygonal intermedi ate state pattern at elevated fields upon flux penetration, and (b) reconstructed current density flow. 2000, Narayan, 1998, Goldstein and Dorsey, 1998, Dorsey and Goldstein, 1998, Goldstein et al., 1996). D. AC Response in the Intermediate State of Type I Superconductors At small amplitudes of the excitation fields the response of a superconductor is reversible. In a pure Meissner state the magnetic field penetrates only to the depth determined by the London penetration depth �, and the magnetic susceptibility of both Type-I and Type-II superconductors also depends only on the London penetration depth, �. For example, for an infinite slab of width 2w� 4�� = �/w tanh �w/�� − 1 (Schoenberg, 1952), and this can be general ized for a finite slab (Prozorov et al., 2000). By sweeping the external DC magnetic field it is possible to study the dynamic magnetic susceptibility, dM/dH, without affecting the overall field distribution inside a supercon ductor. In Type-II superconductors if the amplitude of the excitation field is small the Abrikosov vortices are not displaced, but rather they oscillate around their equi librium positions providing a quasi-elastic response known as the Campbell regime (Campbell and Evetts, 1972, Blatter et al., 1994, Brandt, 1995, Coffey and Clem, 1991). In this regime the effective penetration depth becomes, �2 = �2L + �2C , where �2C = �−1 Cxx is the Campbell penetration depth, Cxx is the relevant elastic modulus (either com pression or tilt) of the vortex lattice, and � is the Labusch parameter (Coffey and Clem, 1991, Dew-Huges, 1974, Campbell and Evetts, 1972, Brandt, 1995). Figure 11.34 shows measurements of the small-amplitude AC response in a stressfree lead sample during the sweeping of an external magnetic field. Also shown are MO images. The appearance of the intermediate state manifests itself by an abrupt deviation from the H 2 behavior (due to penetration from the corners (Prozorov et al., 2005)). Clearly the response is hysteretic, but this hysteresis is only related to the topologi cal differences, and to differences in the quasi-elastic response. This conclusion is supported by comparison with the DC mag netization, Figure 11.27, where flux exit cor responds to smaller magnetization values, which in Type-II superconductors would cor respond to a larger penetration depth (Pro zorov et al., 2003). In Fig. 11.34 larger values correspond to the flux entry, and indi cate a softer phase compared to the lami nar structure observed at flux exit. As the field increases the growing flux tubes seem to form a more rigid honeycomb structure, thus leading to a decrease of the penetra tion depth at elevated magnetic fields, as observed in Fig. 11.34. In the cold-worked sample, where the flux penetration is den dritic (see Fig. 11.27), such a non-monotonic behavior is not observed. Thus this dis tinct feature may serve as a useful tool for the study the intermediate state in samples where direct MO imaging is not possible. Finally, as the field continues to increase, Fig. 11.34 shows that the superconductiv ity is quenched at Hc , but the penetration depth remains significantly lower than the normal state skin-depth due to the presence of surface superconductivity. Furthermore, the hysteresis of the AC response is observed both for M�H = const� T� and M�H� T = const� measurements. Another verification of the correspondence of the AC response to 333 XII MIXED STATE IN TYPE II SUPERCONDUCTORS Meissner State 2000 Hc3 intermediate State skin effect Δλ (nm) 1500 1000 Hc λ ~ H2 500 T = 1K 0 0 500 1000 1500 H (Oe) Figure 11.34 Magnetic penetration depth measured by using a tunnel-diode resonator, and the corresponding evolution of intermediate state patterns. the particular geometry of the intermediate state is the vanishing of the non-monotonic behavior upon the application of an inclined magnetic field (Prozorov et al., 2005). This effect is related to the induced unidirectional anisotropy of the otherwise frustrated inter mediate state structure, as first demonstrated by Sharvin (Sharvin and Sedov, 1956, Liv ingston and DeSorbo, 1969). Unfortunately, no theory of the quasi-elastic small-amplitude AC magnetic response of the intermediate state of Type-I superconductors is yet available. A theoreti cal analysis along the lines of the Campbell response, but for Type-I superconductors, is needed. Once a correlation is established and understood, the unique characteristics of the AC response will be very useful in study ing ellipsoidal samples, as well as very small samples, which cannot be directly imaged by magneto-optics. Ellipsoidal samples are important because they provide the ther modynamically equilibrium response needed to conclusively answer the basic question of the ground state intermediate state pat tern. Recent magneto-optical experiments performed on hemispheres indicate that the tubular structure is the equilibrium pattern of Type-I superconductors. XII. MIXED STATE IN TYPE II SUPERCONDUCTORS In this chapter we have been explain ing how demagnetization effects in Type I materials produce the intermediate state in an effort to prevent surface fields from exceed ing the critical field Bc� and driving the mate rial normal. In a Type II super-conductor, when Bapp becomes large enough to produce surface fields equal to the lower critical field, Bc1 , vortices appear inside the material near the surface and the mixed state forms at a lower field Bc1� than it would under the con dition N = 0. Ideally, a Type II supercon ductor is in the � = −1 or Meissner state for Bapp < Bc1� and in the mixed state above Bc1� . The mathematical description of the Meissner state of a Type II superconductor is similar to that of the Type I case that was presented above in Section IV, with Bc1 replacing Bc at the upper limit of Eq. (11.10). 334 11 TYPE I SUPERCONDUCTIVITY AND THE INTERMEDIATE STATE This limit is the shifted lower critical field Bc1� mentioned above, Bc1� = �1 − N�Bc1 � (11.81) Thus we can rewrite Eqs. (11.10)–(11.14) for a Type II superconducting ellipsoid in the Meissner state as follows: Bapp < Bc1� (11.82) Bin = 0� (11.83) Hin = Bapp /�1 − N��0 � (11.84) �0 M = −Bapp /�1 − N�� (11.85) � = −1� (11.86) This state exists over the range given by Eq. (11.82). When Bapp exceeds Bc1� , vortices begin to form and the material enters the mixed state. Since this state can exist for Hin greater than Bc1� /�0 , the value of Hin does not become pinned at the critical field, as in the Type I case, but continues to increase as the applied field increases. This removes the constraint of Eq. (11.2), so the fields are given by the following more general expres sions of Eqs. (5.35)–(5.37): Bc1� < Bapp < Bc2 � 1+� � 1 + �N Bapp Hin = � �0 �1 + �N� Bapp � M= � �0 �1 + �N� Bin = Bapp Pakulis (1990) proposed a mixed state in zero field with normal regions called ther mons that contain no magnetic flux. (11.87) (11.88) PROBLEMS 1. Find the range of angles for which the magnetic field at the surface of a perfectly superconducting sphere �� = −1� is (a) greater than, (b) equal to, or (c) less than the applied field Bapp . 2. What are the smallest and the largest pos sible values of the angle �c of Eq. (11.8) and at what applied fields do they occur? 3. Deduce the equations for Bin � Hin � M, and � in the intermediate state of a Type I superconducting cylinder in a perpendic ular magnetic field. 4. Show that the magnetic fields at the sur face of a sphere in an applied magnetic field in the intermediate state have the fol lowing radial and azimuthal components: Br = Bin cos �� B� = Bc sin �� 5. Show that the magnetic fields at the sur face of a sphere in an applied magnetic field in the perfectly diamagnetic state have the following radial and azimuthal components: (11.89) Br = 0 (11.90) 3 B� = Bapp sin �� 2 These equations resemble those of the mixed state of a Type II ellipsoid, rather than those, (11.15)–(11.19), of the corresponding Type I intermediate state. The presence of the demagnetization factor N in the denomina tor of expressions (11.88)–(11.90) causes the internal fields to be larger than they would be for the case N = 0 of a cylinder in a parallel applied field. 6. Show that the expressions �exp = �/�1 + N��� � = �exp /�1 − N�exp �� 1 Bc �exp = � 1− N Bapp are valid for the intermediate state of an ellipsoid. 335 PROBLEMS 7. Show that the boundary between the superconducting and intermediate state of an ellipsoid in a magnetic field lies along the dashed line of unit slope shown in Fig. 11.8. Show that along this bound ary the Gibbs free energy is −NBc2 /2�0 . 8. Show that the normalized Gibbs free energy g�b� t� of an ellipsoid in an applied magnetic field is given by the expressions and show that �i �r� = rE/Hc r < ai � 12. Show that the radius ai of the intermediate-state region of a currentcarrying superconducting wire is given by ai = aIc � I�1 + �1 − �Ic /I��1/2 � g�b� t� = −t2 /� − �1 − t2 �2 + b2 /�1 − N� 0 < b < �1 − N��1 − t2 � g�b� t� = −t2 /� − �1 − t2 − b�2 /N �1 − N��1 − t2 � < b < �1 − t2 �� These are plotted in Fig. 11.9 for sev eral values of N and t using the BCS expression 1/� = 2�8. 9. Show that the dashed line of Fig. 11.9 corresponds to the expression Gs = Bc2 /2�0 ��Bapp /Bc � − 1�. 10. Derive Eq. (11.71), Ji �r� = Jn �ai /r� r ≤ ai � and show that Ji �r� = Hc /r r < ai � 11. Derive Eq. (11.74), �i �r� = �n �r/ai � r ≤ ai � 13. Show that the radius ai of the intermediate-state region of a currentcarrying superconducting wire has the limiting behavior ai = a for I = Ic and that ai ≈ aIc /2I for I � Ic . 14. Show that Eq. (11.77) is the solution to Eq. (11.76). 15. Show that in the intermediate state the current density averaged over the whole wire has the value H a2 �J � = c 1 + i2 � ai a Since this is greater than Jn , we see that the formation of the intermediate state causes more current to flow in the core than would have happened if the wire had become normal. 16. Show that the total current flowing through the intermediate-state region of the wire in Fig. 11.24 is 2�a2i Jn , and that the total current flowing through the wire is given by Eq. (11.75), namely I = ��a2 + a2i �Jn . This page intentionally left blank 12 Type II Superconductivity I. INTRODUCTION In Chapters 2 and 11 we discussed Type I superconductors, which are super conductors that exhibit zero resistance and perfect diamagnetism. They are also per fect diamagnets for applied magnetic fields below the critical field Bc , and become nor mal in higher applied fields. Their coherence length exceeds their penetration depth so it is not energetically favorable for boundaries to form between their normal and super conducting phases. The superconducting ele ments, with the exception of niobium, are all Type I. We showed in Chapter 6, Section XII, that when the penetration depth is larger than the coherence length , it becomes energetically favorable for domain walls to form between the superconducting and nor mal regions. When such a superconductor, called Type II, is in a magnetic field, the free energy can be lowered by causing domains of normal material containing trapped flux to form with low-energy boundaries cre ated between the normal core and the sur rounding superconducting material. When the applied magnetic field exceeds a value referred to as the lower critical field, Bc1 , magnetic flux is able to penetrate in quan tized units by forming cylindrically sym metric domains called vortices. For applied fields slightly above Bc1 , the magnetic field inside a Type II superconductor is strong in the normal cores of the vortices, decreases with distance from the cores, and becomes very small far away. For much higher applied fields the vortices overlap and the field inside 337 338 12 TYPE II SUPERCONDUCTIVITY the superconductor becomes strong every where. Eventually, when the applied field reaches a value called the upper critical field Bc2 , the material becomes normal. Alloys and compounds exhibit Type II supercon ductivity, with mixed-type magnetic behav ior and partial flux penetration above Bc1 . Type II superconductors also have zero resis tance, but their perfect diamagnetism occurs only below the lower critical field Bc1 . The superconductors used in practical applica tions, which have relatively high transition temperatures, carry large currents and often operate in large magnetic fields, are all of Type II. Their properties will be described in this chapter. In the latter part of the chapter we will examine the properties of the vor tices, discussing how they confine flux, how they interact, and how they move about. Figure 12.1 Internal fields produced inside a per fectly superconducting cylinder = −1 in an external magnetic field Bapp = 0 Happ applied parallel to its axis. This arrangement is referred to as parallel geometry. II. INTERNAL AND CRITICAL FIELDS A. Magnetic Field Penetration The general expression (1.69) B = 0 H + M (12.1) is valid both inside and outside a super conducting sample in an applied field. For simplicity we will examine the case of an elongated cylindrical superconductor with its axis in the direction of the applied mag netic field, as shown in Fig. 12.1. For this “parallel” geometry the boundary condition (1.74) requires the H fields outside Happ = Bapp /0 and inside Hin to be equal at the surface of the sample, Happ = Hin (12.2) If we apply Eq. (12.1) to the fields inside a Type I superconductivity and recall that Bin = 0, we obtain for the magnetization in the sample, with the aid of Eq. (12.2) 0 M = −Bapp (12.3) Above the critical field Bc the mate rial becomes normal, the magnetization M becomes negligibly small, and Bin ≈ Bapp . This situation is indicated in Fig. 2.27 and plotted in Fig. 12.2, with the field 0 Hin below Bc indicated by a dashed line in the latter figure. The corresponding diagram for a Type II superconductor has two critical fields, Bc1 , the field where flux begins to penetrate, and Bc2 , the field where the material becomes normal. For this case, again applying the boundary condition (12.2), the internal field and magnetization given by 0 M = −Bapp Bin = 0 0 ≤ Bapp ≤ Bc1 (12.4a) 0 M = −Bapp − Bin Bc1 ≤ Bapp ≤ Bc2 (12.4b) are shown plotted in Figs. 12.3 and 12.4, respectively. The dashed line 0 Hin in Fig. 12.3 represents asymptote of Bin as it approaches Bc2 . Also shown in these two 339 II INTERNAL AND CRITICAL FIELDS Figure 12.2 Internal fields Bin and Hin and magne tization M for an ideal Type I superconductor. Use is made of the permeability 0 of free space in this and the following two figures so that Bin 0 Hin , and 0 M have the same units, in accordance with Eq. (12.1). Figure 12.3 Internal fields Bin and Hin and magne tization M for an ideal Type II superconductor, using the notation of Fig. 12.2. Figure 12.4 Dependence of magnetization M on the applied field for an ideal Type II superconductor. The equality of the areas separated by the thermodynamic critical field Bc is indicated. 340 12 TYPE II SUPERCONDUCTIVITY figures is the thermodynamic critical field Bc defined by the expression Bc Bc1 Bapp + 0 M dBapp = 0 Bc2 Bc −M dBapp (12.5) which makes the two areas shown shaded in Fig. 12.4 equal. Figures 12.2, 12.3, and 12.4 are idealized cases; in practice, the actual magnetization and internal field curves are rounded, as indicated in Fig. 12.5. We used the parallel geometry arrange ment because it avoids the complications of demagnetization effects; these were dis cussed later in Chapter 5, Sections X and XI. For this geometry the demagnetization factor N , which is a measure of these complica tions, is zero. B. Ginzburg-Landau Parameter In Chapter 6, Sections V and VII, respectively, we introduced two characteris tic length parameters of a superconductor— the coherence length and the penetration Figure 12.5 Dependence of internal magnetic field Bin and magnetization M on an applied field Bapp for a nonidealized Type II superconductor in which the curves near the lower-critical field are rounded. This is in contrast to the idealized cases of Figs. 12.3 and 12.4 which exhibit abrupt changes in Bin and M when the applied field passes through the value Bc1 . 341 II INTERNAL AND CRITICAL FIELDS depth . Their ratio is the Ginzburg–Landau parameter of Eq. 6.83, = (12.6) The density of super electrons ns , which characterizes the superconducting state, increases from zero at the interface with a normal material to a constant value far inside, and the length scale for this to occur is the coherence length . An external mag netic field B decays exponentially to zero inside a superconductor, with length scale . Figure 12.6 plots these distance dependences of ns and B near the boundary of a super conductor with a normal material for the two cases < 1 and > 1. For a Type I superconductor the coher ence length is the larger of the two length scales, so superconducting coherence is maintained over relatively large distances within the sample. This overall coherence of the superconducting electrons is not dis turbed by the presence of external mag netic fields. When, on the other hand, the material is Type II, the penetration depth is the larger of the two length parameters, and external magnetic fields can penetrate to a distance of several or more coherence lengths into the sample, as shown in Fig. 12.6b. Thus, near the interface relatively large magnetic field strengths coexist with high concentrations of superconducting electrons. In addition, inside the superconductor we find tubular regions of confined magnetic flux (the vor tices) as already noted. These have an effec tive radius of a penetration depth beyond which the magnetic field decays approxi mately exponentially to zero, in the manner Figure 12.6 Increase in the number of superconducting electrons ns and decay of the magnetic field Bin with distance x from the surface of the superconductor. The coherence length and penetration depth associated with the change in ns and Bin , respectively, are shown. (a) Type I superconductor, with > , and (b) Type II superconductor, with > , and Bapp < Bc1 . 342 12 TYPE II SUPERCONDUCTIVITY Figure 12.7 Sketch of (a) the magnetic field around an individual vortex, and (b) the field (top) from a group of nearby overlapping vortices (bottom). The coherencelength radius of the core, penetration-depth radius of the field outside the core, and decay of B at large distances are indicated for an individual vortex. The region of fluxoid quantization is cross-hatched for the individual vortex and for one of the overlapping vortices. illustrated in Fig. 12.7. As the applied field increases, more and more vortices form and their magnetic fields overlap, as indicated in Fig. 12.7b. Type II material is said to be in a mixed state over the range Bc1 < Bapp < Bc2 of applied fields. Values of , and for a number of superconducting materials are given in Table 12.1. Superconductors are classified as Type I or Type II depending on whether the√parameter is less than or greater than 1/ 2, respectively. We see from the table that all the elements (except for Nb) are Type I and that all the compounds are Type II, with the copper-oxide superconductors hav ing the highest values, on the order of 100. Many of the data in the table are averages from several earlier compilations that do not agree very closely. The scatter in the values of and listed in Table 12.2 for five of the elements is comparable to that of the hightemperature superconductors in Table III-1 of our earlier work (Poole et al., 1988). C. Critical Fields In Chapter 4, Section VIII, and Chapter 6, Section IV, we saw that a Type I superconductor has a critical field Bc , and in Eq. (4.37) we equated the difference Gn – Gs in the Gibbs free energy between the normal and the superconducting states to the mag netic energy Bc2 /2 0 of this critical field, G n − Gs = Bc2 20 (12.7) Since this is a thermodynamic expression, Bc is called the thermodynamic critical field. Both Type I and Type II supercon ductors have thermodynamic critical fields. In addition, a Type II superconductor has lower- and upper-critical fields, Bc1 and Bc2 , respectively, given by Bc1 = Bc2 = 0 ln (12.8) 4 2 0 2 2 (12.9) 343 II INTERNAL AND CRITICAL FIELDS Table 12.1 Coherence Length , Penetration Depth , and Ginzburg–Landau Parameter of Various Superconductorsa Material Tc K � nm � nm � �/� Source Cd Ala Ina Sna Ta Pba Nba Pb–In Pb–Bi Nb–Ti Nb–N PbMo6 S8 (Chevrel) V3 Ga A15 V3 Si A15 Nb3 Sn A15 Nb3 Ge A15 K3 C60 Rb3 C60 La0925 Sr0075 2 CuO4 b YBa2 Cu3 O7 b HgBaCaCuO HgBa2 Ca2 Cu3 O8+ 056 118 341 372 44 720 925 70 83 95 16 15 15 16 18 232 19 296 37 89 126 131 760 1510 360 180 93 82 39 30 20 4 5 2 ≈25 3 3 3 26 20 20 18 23 110 40 40 42 35 39 52 150 200 300 200 200 90 60 65 90 240 247 200 170 014 003 011 023 038 048 128 50 10 75 40 100 ≈35 20 22 30 92 124 100 95 Meservey and Schwartz (1969) Table 9.2 Table 9.2 Table 9.2 Buckel (1991) Table 9.2 Table 9.2 Orlando and Delin (1991) Orlando and Delin (1991) Orlando and Delin (1991) Orlando and Delin (1991) Orlando and Delin (1991) Orlando and Delin (1991) Orlando and Delin (1991) Orlando and Delin (1991) Orlando and Delin (1991) Holczer et al. (1991) Sparn et al. (1992) Poole et al. (1988) Poole et al. (1988) Gao et al. (1993) Schilling et al. (1994b) a b 100 Figures are rounded averages from Table 12.2. Averages of the polycrystalline data from our earlier Table III-1 (1988). Table 12.2 Coherence Length and Penetration Depth of Five Superconducting Elements from Several Reportsa Parameter Coherence length nm Penetration depth nm a Al ⎧ ⎪ ⎪ ⎨ 1360 ⎪1600 ⎪ ⎩ 1600 ⎧ ⎪ ⎪ ⎨ 51 50 ⎪ ⎪ ⎩ 16 In Sn Pb Nb Reference 360 275 360 440 175 94 230 230 510 74 90 83 39 Buckel (1991) Huebener (1979) Orlando and Delin (1991) Van Duzer and Turner (1981) 24 47 65 21 31 52 50 36 32 47 40 37 40 38 32 85 39 Buckel (1991) Huebener (1979) Orlando and Delin (1991) Van Duzer and Turner (1981) Some of the data are reported averages from earlier primary sources. Table 12.1 lists rounded averages calculated from these values, with the entry = 510 nm for Pb excluded. These can be expressed in terms of the thermodynamic critical field Bc , Bc = √ 2 2 0 (12.10) as follows: B ln Bc1 = √c 2 √ Bc2 = 2 Bc (12.11) (12.12) 344 12 TYPE II SUPERCONDUCTIVITY It is also of interest to write down the ratio and the product of the two critical fields: Bc2 /Bc1 = 2 2 / ln Bc1 Bc2 1/2 = Bc ln Figure 12.3 shows the position of the lower and upper critical fields as well as the ther modynamic critical field on the magnetiza tion curve, and Table 12.3 lists the critical fields of a few Type II superconductors. (12.13a) 1/2 (12.13b) Table 12.3 Critical Fields of Selected Type II Superconductorsa Material Nb wire, RRR = 750 Nb wire, cold-drawn In095 Pb005 (alloy) Mo≈01 Nb≈09 (alloy) Mo066 Re034 (alloy) Nb099 Ta001 (alloy) Nb–Ti CTa (NaCl Structure) Nb–N (NaCl Structure) Tc K Bcl mT 93 93 37 64 118 88 95 1810 2480 318 290 381 1730 ≈100 160 220 93 Bc mT 037 375 785 0113 204 810 Bc2 T 20 Roberts (1976) ≈100 Roberts (1976) 0049 Roberts (1976) 0414 Roberts (1976) Roberts (1976) 0445 Roberts (1976) 130 Orlando and Delin (1991); Van Duzer and Turner (1981) 046 Roberts (1976) 150 Orlando and Delin (1991); Roberts (1976) 105 Roberts (1976) ≈50 Roberts (1976) 230 Orlando and Delin (1991); Van Duzer and Turner (1981) 230 Roberts (1976) 230 Roberts (1976) 370 Orlando and Delin (1991); Van Duzer and Turner (1981) 217 Vonsovsky et al. (1982, p. 376) 283 Vonsovsky et al. (1982, p. 376) 165 Vonsovsky et al. (1982, p. 376) 174 Roberts (1976) 38 Vonsovsky et al. (1982, p. 420) 54 Vonsovsky et al. (1982, p. 420) 445 Vonsovsky et al. (1982, p. 420) 340 Vonsovsky et al. (1982, p. 420) 600 Orlando and Delin (1991) Rauchschwalbe et al. (1987) Cr3 Ir A15 V3 Ge A15 V3 GaA15 075 68 150 168 V3 Si A15 Nb3 Sn A15 Nb3 Ge A15 160 182 231 550 350 6700 4400 HfV2 (Laves) Hf05 Zr05 V2 (Laves) ZrV2 (Laves) NbSe2 PbMo6 Se8 (Chevrel) LaMo6 S8 (Chevrel) LaMo6 Se8 (Chevrel) SnMo6 S8 (Chevrel) PbMo6 S8 (Chevrel) U097 Th003 Be13 (heavy fermion) UPt3 (heavy fermion) U0985 La0015 Be13 (heavy fermion) UBe13 (heavy fermion) K3 C60 (buckyball) 92 101 85 72 38 ≈65 110 118 150 035 1870 1970 2190 72 2040 09 190 130 60 320 Rb3 C60 (buckyball) 296 120 570 HgBa2 CuO4+ 99 a 40 046 057 19 38 103 Some of the data are averages from more than one source. Reference >35 Schenström et al. (1989) Dalichaouch et al. (1991) Maple et al. (1984) Boebinger et al. (1992); Foner et al. (1992); Holczer et al. (1991); C. E. Johnson et al. (1992); Z. H. Wang et al. (1993) Foner et al. (1992); C. E. Johnson et al. (1992); Sparn et al. (1992) Thompson et al. (1993) 345 III VORTICES Figure 12.8 Comparison of the temperature dependence of the upper-critical fields Bc2 of Nb–Ti, Nb3 Ge, LaSrCuO, YBaCuO, and TlBaCaO. The slopes are close to the Pauli limit 1.83 T/K (Poole et al. 1988, p. 8). Section IV gives expressions similar to Eqs. (12.8–12.12) for anisotropic cases. When the applied magnetic field is per pendicular to the surface of the superconduc tor, the upper critical field is truly Bc2 . When it is parallel to the surface, however, it turns out that the superconducting state can persist in a thin surface sheath for applied surface fields up to the higher value Bc3 = 169 Bc2 (Saint-James and de Gennes, 1963; SaintJames et al., 1969; Van Duzer and Turner, 1981, p. 319; Walton et al., 1974; Yuan and Whitehead, 1991). The temperature dependence of the ther modynamic critical field Bc is given in Chapter 2, Section XIII. The lower and upper critical fields of Type II superconductors have a similar temperature dependence. The fields Bc2 needed to extinguish Type II super conductivity are much larger than those Bc that are sufficient for extinguishing the Type I variety. These large upper-critical fields make Type II superconductors suitable for magnet applications. Quoted upper-critical fields are usually given for 4.2 K or for extrapolations to 0 K. Values of technological interest are the 4.2 K fields for the low-temperature supercon ductors and the 77 K fields for the hightemperature superconductors. For example, Bc2 for the standard magnetic material NbTi is 10 T at 4 K and can be 30 T or more at 77 K for high-temperature superconduc tors, as shown in Fig. 12.8 (Fischer, 1978; Newhouse, 1969, p. 1268; Vonsovsky et al., 1982, p. 431). Theoretical articles have appeared that discuss upper-critical fields (e.g., Brézin et al., 1990; Estrera and Arnold, 1989; Norman, 1990; Pérez-González and Carbotte, 1992; Pérez-González et al., 1992; Santhanam and Chi, 1988; Theodorakis and Tesanovic, 1989). III. VORTICES We have seen that an applied mag netic field Bapp penetrates a superconductor in the mixed-state, Bc1 < Bapp < Bc2 . Pene tration occurs in the form of tubes, called vortices (see Fig. 12.9), which serve to con fine the flux (Abrikosov 1957; Belitz 1990). 346 12 TYPE II SUPERCONDUCTIVITY be taken from r = 0 to r = , so the sur face integral is numerically equal to the flux quantum 0 , (12.15) B · dS = 0 Figure 12.9 Sketch of shielding currents circulating around a vortex core. The highest field is in the core, which has a radius . The core is surrounded by a region of larger radius within which magnetic flux and screening currents flowing around the core are present together, as is clear by com paring Figs. 12.7 and 12.9. The current den sity Js of these shielding currents decays with distance from the core in an approximately exponential manner. Analytical expressions for the distance dependence of B and J are derived in the following section for the highkappa 1 approximation. A. Magnetic Fields Equation (6.39) provides us with an expression for the magnetic flux passing through a region, B · dS + 0 m∗ J · dI =n e∗2 2 0 (12.14) where n is the number of vortex cores enclosed by the integrals. For an isolated vor tex n = 1 because it is energetically more favorable for two or more quanta to form sep arate vortices rather than to coexist together in the same vortex. Integration of B over the cross-sectional area of an isolated vortex can and the line integral vanishes because J become negligibly small at large distances. The quantum condition (12.15) fixes the total magnetic flux in an isolated vortex at one fluxoid, including flux in the core and in the surrounding region. The possibility of vortices containing two or more quanta has been discussed (Buzdin, 1993; Sachdev, 1992; Tokuyasu et al., 1990). As the applied magnetic field increases, the density of vortices increases and they begin to overlap, making the vortex–vortex nearest-neighbor distance less than the pen etration depth. The high-density case can be treated by assuming that the magnetic field at any point is a linear superposition of the fields from all of the overlapping vortices. At high densities Bin becomes very large and the variation of the field in the space between the cores becomes very small, as indicated in Fig. 12.10. Nevertheless, the quantization condition still applies and each vortex has, on average, one quantum of flux 0 associ ated with it, as indicated in Fig. 12.7b. For a regular two-dimensional lattice arrangement of vortices, Eq. (12.15) holds as long as the integration is carried out over the vortex unit cell; the line integral (9.14) of the current density vanishes when it is taken around the periphery of this cell. When is much larger than , as is the case with the high-temperature superconduc tors, there is considerable overlap of vortices throughout most of the mixed-state range, and the magnetic flux is present mainly in the surrounding region, rather than in the actual cores. There is no limit to the length of a vor tex. Along the axis, which is also the applied field direction, the magnetic field lines are continuous. Thus the flux does not begin and 347 III VORTICES Figure 12.10 Sketch showing how the magnetic field Bin inside a superconductor increases as the con centration of vortices increases and their fields increas ingly overlap. Figure 12.11 Passage of external magnetic field lines through a flat-plat superconductor in the region of a vortex. end inside the superconductor, but instead enters and leaves at the superconductor sur face, which is also where the vortices begin and end. This is illustrated in Fig. 12.11. We have seen that a vortex has a core radius equal to the coherence length and a surrounding outer region with radius equal to the penetration depth . Such an entity can only exist in a Type II superconductor, where is greater than . A vortex does not exist, and is not even a meaningful concept under Type I conditions > . Scanning tunneling microscope studies of superconducting surfaces (H. F. Hess et al., 1989, 1990, 1991; Karrai et al., 1992; Renner et al., 1991) reveal an enhancement of the differential tunneling conductance (see Chapter 15, Section V) in the vortex core. This has been attributed to the presence of bound states of quasiparticles in the core. As the magnetic field increases, additional vor tices form accompanied by the breakup of Cooper pairs, and more and more quasiparti- cles or normal electrons become localized in the vortex cores (Daemen and Overhauser, 1989; Gygi and Schlüter, 1990a, b, 1991; Klein, 1989, 1990; Overhauser and Daemen, 1989; Shore et al., 1989; Ullah et al., 1990). B. High-Kappa Approximation To obtain a description of vortices that is more quantitative in nature as opposed to the rather qualitative description presented in the previous section, it will be helpful to have a closed-form expression for the dis tance dependence of the confined magnetic fields. For the high- limit, , which is valid for the copper-oxide superconduc tors that typically have ≈ 100, we can make use of the Helmholtz equations that were derived from the London formalism in Chapter 6, Section IX. The vortex is assumed to be infinitely long and axially symmetric so that there are no z or angular dependences of its field distribution. The problem is thus 348 12 TYPE II SUPERCONDUCTIVITY equivalent to the two-dimensional problem of determining the radial dependences. The magnetic field of the vortex is in the z direction, and its radial dependence outside the vortex core is obtained from the Helmholtz Eq. (6.67). Here we will write the Helmholtz equation in cylindrical coordinates for the two-dimensional case of axial symmetry without assuming any angu lar dependence, 2 d r dr r d dr B−B = 0 (12.16) This equation has an exact solution, Br = 0 2 2 K0 r/ from the modified Bessel function recur sion relation K1 x = −dK0 x/dx (Arfken, 1985, p. 614). The current density also satisfies the Helmholtz equation, Eq. (6.68), expressed in cylindrical coordi nates (Eq. 12.16)) as 2 d r dr (12.17) K0 K0 r/ 1 ln 2 (12.18) d dr Js + Js = 0 (12.23) Figure 12.12 compares the distance depen dence of the modified Bessel functions K0 r/ and K1 r/ associated with Br and Js r, respectively. These modified Bessel functions have asymptotic behaviors at small radial dis tances, where K0 r/ is a zeroth-order modified Bessel function. With the aid of Eq. (12.8) this can be written Br = Bc1 r r 2 ≈ ln − r ≈ ln K1 r ≈ r 1123 r r (12.24) r (12.25) r (12.26) To obtain the current density we sub stitute Eq. (12.17) in the Maxwell equation for Bin , � × Bin = 0 Js (12.19) to obtain Js r = 0 2 0 3 = J0 K1 r/ K1 r/ 1 ln 2 (12.20) (12.21) where K1 r/ is a first-order modified Bessel function, and the characteristic cur rent density Jc is defined in analogy with Eq. (2.51), Jc = Bc1 /0 (12.22) The function K1 r/ results from dif ferentiation of Eq. (12.19), as expected Figure 12.12 Comparison of the distance depen dence of the zero-order K0 and first-order K1 modi fied Bessel functions associated with the magnetic field and current density, respectively, of a vortex. Asymp totic behavior at short distances · · · · · · · is indicated. Both modified Bessel functions have the same largedistance asymptotic behavior (– – – – – –), as shown (Aktas, 1993). 349 III VORTICES where = 057721566 is the Euler– Mascheroni constant (Arfken, 1985, p. 284) and the factor 2e− = 1123. These expres sions show that K1 r K0 r near the core, , as indicated in Fig. 12.12. where r At large distances the corresponding expres sions are K0 r exp−r/ ≈ 2r/ 1/2 r (12.27) K1 r exp−r/ ≈ 2r/ 1/2 r (12.28) Figure 12.12 compares the asymptotic behaviors with the actual functions K0 r/ and K1 r/. These large-distance expres sions permit us to express the magnetic field and current density far from the core in the form B = Bc1 2 1/2 exp−r/ ln r/1/2 r (12.29) Js = Jc 2 1/2 exp−r/ ln r/1/2 We see from Eqs. 12.24 and (12.26) that both B and Js are singular at r = 0. Since the core is so small in the high-kappa approxi mation, it is appropriate to remove the singu larity by assuming that the magnetic field in the core is constant with the value B(0) given by Eq. (12.17) for r = . Even if the math ematical singularity were not removed, the total flux would still remain finite as r → 0, as is proven in Problem 5. In Problem 3 we derive the following expression for the frac tion of the total flux of the vortex that is present in the core: ≈ 0 /2 2 core / 0 , present in the core of an isolated vortex as a function of the GL parameter k. r (12.30) core Figure 12.13 Fraction of the total flux quantum, 1 ln 2 + − (12.31) 2 Figure 12.13 sketches the dependence of core / 0 on k. Since the magnetic field in the sample is confined to vortices, the total flux is 0 times the number of vortices, and the average internal field Bin , given by Bin = NA 0 (12.32) is proportional to NA , the number of vor tices per unit area. For high applied fields much larger than Bc1 but, of course, less than Bc2 , the internal field is approxi mately proportional to the applied field (see Fig. 12.3), and therefore the density of vor tices becomes approximately proportional to the applied field. C. Average Internal Field and Vortex Separation Since interaction between the vortices is repulsive, as we will show in Section V.A, the vortices assume the arrangement that will keep them furthest apart—namely, the twodimensional hexagonal lattice structure illus trated in Fig. 12.14. To observe this structure 350 12 TYPE II SUPERCONDUCTIVITY Figure 12.14 Two-dimensional hexagonal lattice of vortex cores. using what is called the Bitter (1931) tech nique, the surface is decorated by expos ing it to a gas containing tiny suspended magnetic particles that adhere to the vor tex cores and show up well on a photo graphic plate (Dolan et al., 1989; Gammel et al., 1987; Grier et al., 1991; Vinnikov and Grigor’eva, 1988). The imaging can also be done with a scanning-tunneling (H. F. Hess et al., 1989) or scanning-electron micro scope, with Lorentz electron microscopy, or with electron holography (Bonevich et al., 1993). Individual vortices have been studied by magnetic force microscopy (Hug et al., 1995; Moser et al., 1995a,b). The vortices arrange themselves in a hexadic pattern when their density is so high as to make the repulsive interactions between them appreciable in magnitude.√ Each vor tex will then occupy the area 21 3d2 of the unit cell sketched in Fig. 12.15, where d is the average separation of the vortices. Such a structure has been observed on the sur faces of classical as well as high-temperature superconductors. The average field Bin inside the superconductor is given by Bin = 1 √ 2 3d2 (12.33) and the number of vortices N equals the total cross-sectional √ area AT divided by the area per vortex 21 3d2 , A N = 1√T 3d2 2 (12.34) Figure 12.15 Vortex unit cell for the hexagonal lat √ tice of Fig. 12.14. The area of the cell is 21 3d2 . The vortex lattice structure is not always the hexagonal type depicted in Fig. 12.14 for it can also depend on the magnetic field direction. In low- Type II alloys of, for example, Nb, Pb, Tc, or V, the vortices form a square lattice when the magnetic field is parallel to a fourfold crystallographic sym metry axis and a hexagonal lattice when Bapp is along a threefold axis. When Bapp is along a twofold axis direction, a distorted hexagonal lattice is observed (Huebener, 1979, pp. 75ff; Obst, 1971). For YBa2 Cu3 O7− in tilted applied fields, an SEM micrograph shows “a pinstripe array of vortex chains” lying in the Bapp , c plane (Gammel and Bishop, 1992), and for the applied field perpendicular to the c direction, chains of oval-shaped vortices are observed (Dolan et al., 1989b). D. Vortices near Lower Critical Field When the flux first penetrates the super conductor at Bapp = Bc1 the vortices are near the surface and isolated. As the applied field increases more vortices enter, and their mutual repulsion and tendency to diffuse causes them to migrate inward. Eventually they become sufficiently dense and close enough to experience each others’ mutual repulsive forces, so they begin to arrange 351 III VORTICES themselves into a more or less regular pat tern resembling that in Fig. 12.14. For this case we can find an expression for the aver age internal field Bin in terms of the aver age separation d by eliminating 0 from Eqs. (12.8) and (12.33) Bin = Bc1 √ 2 3 ln d2 8 (12.35) Therefore, the separation of vortices when the average internal field equals the lowercritical field is given by ⎛ ⎞1/2 ⎜ d = 2⎝√ ⎟ (12.36) ⎠ 1 3 · ln 2 381 =√ (12.37) Bin = Bc1 ln √ √ Since ln 10 = 152 and ln 100 = 215, the value of does not have much effect on the separation of the vortices. Figure 12.16 shows the dependence of the average internal field on their separation 21 d/. The process of vortex entry into, and exit from, a superconductor is actually more complicated than this. It can occur in a sur face sheath similar to the one that remains Figure 12.16 superconducting for applied fields in the range Bc2 < Bapp < Bc3 , as mentioned in Section II.C. Walton et al. (1974) assumed the presence of a surface layer with “nascent” vortices that turn into nucleation sites for the formation of vortices. As the applied field increases, the interface between the surface region containing the vortices and the fieldfree bulk is able to move inward by diffusion at a velocity proportional to the field gradient (Frahm et al., 1991). Since it is the applied field rather than the internal field which is known experimen tally, it is of interest to determine how the separation of vortices depends on the ratio Bapp /Bc1 between the applied field and the lower-critical field. It is assumed that the vortices distribute themselves in a regular manner to produce a uniform internal field, Bin = Bin . Figure 12.17, an enlargement of the low-field part of Fig. 12.5, shows a typical example illustrating an internal field increasing with increasing applied field in the neighborhood of the lower-critical field. From the slope of the curve of Bin versus Bapp , we conclude that the internal field will reach the value Bc1 when the applied field approaches the upper limit of the range Bc1 < Bapp < 2Bc1 , and we estimate that this might Relationship between applied and internal fields, Bapp and Bin , and half the ratio 21 d/ between the vortex separation d and the penetration depth , for two values of . For much smaller separations d Bin approaches Bapp . 352 12 TYPE II SUPERCONDUCTIVITY Figure 12.17 The Magnitude of the internal magnetic field Bin (solid line) in a Type II superconductor in the neighborhood of the lower-critical field. Bin approaches the dashed unit slope line through the origin for very high applied fields. occur for Bapp ≈ 18Bc1 . Using this figure to convert from Bin to Bapp graphs of Bapp versus 1 d/ are plotted in Fig. 12.16. 2 We see from the figure that when the applied field is slightly greater than the lowercritical field, the vortices are much further apart than just one penetration depth. At higher applied fields, the vortices move closer together until near an applied field Bapp ≈ 2Bc1 their separation is about two penetration depths. For higher applied fields appreciable overlap occurs 21 d < . Thus, relatively low fields produce a concentration of vortices high enough for the vortices to be treated as a con tinuum rather than as isolated entities. E. Vortices near Upper Critical Field When the applied magnetic field approaches the upper-critical field Bc2 given by Eq. (12.9) the vortices are very close together, with their separation d some what greater than the coherence length . Equat ing Bin and Bc2 in Eqs. (12.9) and (12.33), respectively, we obtain an expression for the vortex nearest-neighbor distance d in terms of the coherence length: √ d = 2 / 31/2 (12.38) ≈ 269 (12.39) Since d > 2, the cores do not quite touch for this highest density case. F. Contour Plots of Field and Current Density In Section III.B we wrote down the closed-form expressions (12.17) and (12.20), respectively, for the magnetic field and cur rent density of an isolated vortex, and in Fig. 12.12 we plotted the distance depen dence of these quantities for an isolated vor tex. In this section we will provide plots that were constructed from calculations of the 353 III VORTICES Figure 12.18 Geometrical relationships of a vortex unit cell showing the midpoint M between three vortices V at which the internal field Bin is a minimum and the saddle point S midway between two vortices. The triangle V–S–M is the calculational cell, which is one-twelfth the vortex unit cell sketched in Fig. 12.15 and contains all of the information on the fields and currents. Also shown are the current circulation around the vortices V and the midpoint M (Aktas et al., 1994). position dependence of the field and the current density associated with densely packed vortices (carried out by Aktas, 1993; Aktas et al., 1994). The computations involved adding the contributions of the many overlapping vortices in the neighborhood of a particular vortex, as indicated in Figs. 12.7b and 12.10. This meant taking into account hundreds of vortices, but it was sufficient to carry out the calculations in only one-twelfth of the unit cell because the smaller calculational cell defined by the triangle V–S–M– C–V of Fig. 12.18 replicates itself 12 times in the vortex unit cell of Fig. 12.15. The magnetic field is a maximum at each vortex position V, of course, and a minimum at the midpoint M between three vortices. Figure 12.19 plots this calculated field change along the path V → S → M → C → V for the case of vortices with “radius” = 1000 Å and separation d = 400 Å, which corresponds to considerable overlap. We see from the figure that the field increases along the two paths M → S and M → C. There is a saddle point S midway between the two vortices, with the magnitude of the field decreasing slightly from S to M and increas ing appreciably from S to V. Figure 12.18 portrays the current density encircling the vortex cores V in one direc tion and flowing around the minimum points M in the opposite direction. Along the path from one vortex to the next the current density passes through zero and reverses direction at the saddle point S. Along the path from the minimum point M to a vortex V there is a curvature change point C at which the current flow switches between clockwise and counterclockwise circulation. Points V, M, and S are well defined geometrically; the 354 12 TYPE II SUPERCONDUCTIVITY Figure 12.19 Magnitude of internal magnetic field along the three principal directions V → S S → M, and M → V from the origin at the vortex V in the calculational cell of Fig. 12.18 for d = 400 Å and = 1000 Å (Aktas, 1993). position of point C along the line from V to M has to be calculated. Figure 12.20 plots the current density calculated along the path V → S → M → C → V around the periph ery of the calculational cell. A comparison of Figs. 12.19 and 12.20 indicates that the cur rent density tends to be fairly constant over more of the unit cell than is the case with the magnetic field. The previous few paragraphs describe the internal magnetic field on a meso scopic scale, with resolution over distances comparable with the penetration depth. Ordi narily, we are interested in the value of the macroscopic internal field, which is an average over these mesoscopic field varia tions. Forkl et al. (1991) used a magnetooptical Faraday effect technique to determine the distribution of the macroscopic inter nal field inside a disk-shaped sample of YBa2 Cu3 O7− ; the results are given in Figs. 12.21 and 12.22. Other investigators have published similar internal-field pro files (Flippen, 1991; Glatzer et al., 1992; Mohamed et al., 1989, 1990) and surfacefield profiles (Brüll et al., 1991; H. Muller et al., 1991). G. Closed Vortices The vortices that we have been dis cussing are of the open type, in the sense that they begin and end at the surface of the superconductor. Here the flux is contin uous with flux entering and leaving from the outside, as indicated in Fig. 12.11. We recall from Figs. 2.36 and 6.19 that a trans port current flowing in a superconductor has encircling magnetic field lines, and that the portion of this encircling magnetic flux inside the superconducting material will be in the form of vortices that close in on themselves, basically vortices with loops of totally confined flux. The encircling flux in the region outside the superconductor is not quantized. When both transport and screen ing current are present, some of the vortices close in on themselves, and some do not. 355 IV VORTEX ANISOTROPIES Figure 12.20 Current density along the three principal directions V → S S → M, and M → V measured from the origin at the vortex V in the calculational cell of Fig. 12.18 for d = 400 Å and = 1000 Å. The curvature change point C along the path M → V at which the current flow direction shifts from clockwise around V to counterclockwise around M (cf. Fig. 12.18) is indicated. Comparison with Fig. 12.19 shows that the current density exhibits more abrupt changes than the fields (Aktas, 1993). IV. VORTEX ANISOTROPIES Section III.B gave expressions for the magnetic field and current densities associ ated with a vortex in a high- isotropic super conductor. Many superconductors, such as those of the high-Tc type, are not isotropic, however, and in this section we will exam ine the configurations of the resulting vor tices. These configurations depend on the coherence length and the penetration depth, which in turn depend on the anisotropies of the carrier effective mass, so we will say a few words about these parameters first. We will emphasize the case of axial symme try; for this case the a and b directions are equivalent to each other. Such a geometry is exact for tetragonal, and a good approx imation for orthorhombic high-temperature superconductors. The reader is referred to the text by Orlando and Delin (1991) for derivations of the various expressions in this section. An alternative approach to that pre sented here considers an isolated vortex as having elastic properties that are analogous to those of a string under tension (Hanaguri et al., 1994; Toner, 1991a; Widom et al., 1992). The vortex is assumed to be held in place at its end points by the coupling to the external magnetic field, and when dis torted it tends to return to a linear configu ration. The flux-line lattice in an anisotropic superconductor is more complicated, and has been treated using anisotropic elasticity the ory (Sardella, 1992). 356 12 TYPE II SUPERCONDUCTIVITY 2 = � 2 /2m∗ a 2 = Figure 12.21 Radial distribution of internal mag netic field in a superconducting rod of 1 mm radius for applied fields from 15 mT to 222 mT. The penetration depth ≈ 20 m (Forkl et al., 1991). (12.40) ∗ m 0 e∗2 2 (12.41) the coherence length is inversely pro portional, and the penetration depth is directly proportional, to the square root of m∗ , where the factors a and of the GL theory depend on the temperature. Since the anisotropy arises from the effective mass, to a first approximation we can write for the three principal directions √ √ √ (12.42a) a ma = b mb = c mc √ √ √ a / ma = b / mb = c / mc (12.42b) Multiplying these expressions together term by term gives a a = b b = c c (12.43) which is the basic characteristic length rela tionship of anisotropic superconductors. Many superconductors, such as the cuprates, are axially symmetric with in-plane ma = mb = mab and axial-direction mc effective masses. We define the ratio by = mc /mab (12.44) Figure 12.22 Radial distribution of internal mag netic field in the superconducting rod of Fig. 12.21 following application of a field of 222 mT and in the remanent state following removal of this field (Forkl et al., 1991). A. Critical Fields and Characteristic Lengths The electron or hole carriers of an anisotropic superconductor have effective masses m∗ that depend on the direction, with the principal values ma mb , and mc along the three principal directions a b, and c of the crystal. The Ginzburg–Landau theory tells us that, on the basis of Eqs. (6.26) and (6.45), respectively [cf. Eq. 7.123)]. with reported values ≥ 29 for YBa2 Cu3 O7− (Farrell et al., 1988), ≥ 3000 for Bi2 Sr2 CaCu2 O8 (Farrell et al., 1989b), and ≥ 105 for Tl2 Ba2 CaCuO8 (Farrell et al., 1990a). Using Eqs. (12.42)–(12.44) we can show that the coherence length ab and pene tration depth ab in the a b plane are related to their values c and c along the c direction through the expression (Kes et al., 1991). = ab /c 2 = c /ab 2 (12.45) where for the cuprates (Hikita et al., 1987; Worthington et al., 1987) we have c < ab ab < c (12.46) 357 IV VORTEX ANISOTROPIES Some reported values of these quantities are listed in Table 12.4. The GL parameter i for the mag netic field in the ith principal direction is (Chakravarty et al., 1990) the same eccentricity. The equation for the current flow ellipse with = 1 is j k 1/2 = i j k where x and z are the Cartesian coordinates of points on the perimeter. The correspond ing current flow equation for the applied field along the c direction is a circle, (12.47) which gives for the cuprates with the applied field in the a b-plane ab and along the c direction c , respectively, ab c 1/2 = ab ab c (12.48a) = ab /ab (12.48b) c In the next two sections we will employ these quantities to write down explicit expressions for the core perimeter, magnetic fields, and current densities of vortices in the pres ence of anisotropies. An average GL param eter a = 1 2 3 /1 2 3 1/3 has also been defined (Clem and Coffey, 1990). B. Core Region and Current Flow The vortices described in Section III.B for 1 were axially symmetric, with the shielding current flowing in circular paths around the axis, as illustrated in Fig. 12.9 Axial symmetry is also observed for the cuprates when the applied field is aligned along c. When, however, it is along the b (or a) direction, the core cross-section is an ellipse with semi-axes ab and c along the a and c directions, as indicated in Fig. 12.23. The current flows in an elliptical path with semi-axes c and ab , as shown in Fig. 12.24, where is a numerical factor that depends on the distance of the current from the core. We know from Eq. (12.43) that ab /c = c /ab , so the core and cur √ rent flow ellipses have the same ratio of semi-major to semi-minor axis, and hence z2 x2 + =1 2c 2ab x2 + y 2 =1 2ab Bapp b Bapp c (12.49a) (12.49b) Equations (12.49a) and (12.49b) also cor respond to loci of constant magnetic field around the vortex. They are plotted on the left and right sides, respectively, of Fig. 12.23 to indicate the relative size of the two vortices. Expressions analogous to Eqs. (12.49) can be written down for the perimeters of the cores. Since the current paths are ellipses, each increment of current I flows in a channel between a pair of ellipses, in the manner illustrated in Fig. 12.24. When the channel is narrow, as it is at the top and bottom of the figure, the flow is fast, so the current density is large, as indicated. Conversely, in the wider channels on the left and right, the flow is slow and J is small, as indicated. The increment of current I through each part of the channel is the same, so the product J times the width must be constant, and we can write Jx z = Jz x (12.50) This is a special case of the fluid mechanics expression J1 A1 = J2 A2 for current flow in a pipe of variable cross section A. C. Critical Fields The isotropic expressions for the critical fields given in Section III.B can be modi fied for anisotropy by using the GL param eter i (12.47) for the applied field in the i 358 Table 12.4 Coherence Lengths i and Penetration Depths i of Various Superconductors in the Symmetry Plane (called the a b-plane) and in the Axial Direction (called the c-axis), and Values of the Anisotropy Ratio Material NbSe2 UPt3 (heavy fermion) K-ET2 CuNCS2 Tc K ab nm c nm ab nm c nm mc /mab Reference 77 23 69 782 980 230 707 11 Salamon (1989) Broholm et al. (1990) Harshman et al. (1990) >4 × 104 Farrell et al. (1990b) Lang et al. (1992a, b) Kwok et al. (1990b) 046 9 K-ET2 CuNCS2 K-ET2 CuNCN2 2 Br K-ET2 CuNCN2 2 Br 10 114 116 La0925 Sr0075 2 CuO4 La091 Sr009 2 CuO4 Nd0925 Ce0075 2 CuO4 a 34 30 215 29 33 Nd09 Ce01 2 CuO4 a Sm0925 Ce0075 2 CuO4− a Sm0925 Ce0075 2 CuO4− a 114 18 79 48 15 YBa2 Cu3 O65 YBa2 Cu3 O69 YBa2 Cu3 O694 62 83 912 20 045 YBa2 Cu3 O7− YBa2 Cu3 O7− YBa2 Cu3 O7− 66 90 89 25 34 08 07 26 YBa2 Cu3 O7− 924 43 07 27 YBa2 Cu3 O7− 92 12 03 89 550 ≈27 Salamon (1989) YBa2 Cu3 O7− 90 13 02 130 450 ≈25 Krusin-Elbaum et al. (1989) 650 37 04 86 283 80 142 150 17 Hase et al. (1991) Li et al. (1993) Wu et al. (1993) 100 ≈600 O and Markert (1993) Dalichaouch et al. (1990b) S. H. Han et al. (1992) 19 Vandervoort et al. (1991) Harshman et al. (1989) Ossandon et al. (1992a) >700 260 125 10 25 Lee and Ginsberg (1991) Chaudhari et al. (1987) Worthington et al. (1987) 180 41 Gallagher (1988) YBa2 Cu3 O7− EuBa2 Cu3 O7− EuBa2 Cu3 O7− 92 95 94 16 27 35 03 06 038 20 TmBa2 Cu3 O7− Y08 Pr02 Ba2 Cu3 O7+ Bi2 Sr2 CaCu2 O8 86 73 84 74 24 11 09 078 68 9.5 Bi2 Sr2 CaCu2 O8 Bi2 Sr2 Ca2 Cu3 O10 Bi2 Sr2 Ca2 Cu3 O10 109 109 111 29 10 009 002 Bi Pb2 Sr2 CaCu2 O8 Bi09 Pb01 2 Sr2 CaCu2 O8+ Bi09 Pb01 2 Sr2 Ca2 Cu3 O10+ 91 911 103 20 204 118 0037 Pb2 Sr2 Y CaCaCu3 O8 Tl2 Ba2 CaCu2 O8− Tl2 Ba2 Ca2 Cu3 O10 76 100 123 15 03 Tl2 Ba2 Ca2 Cu3 O10 HgBa2 CuO4+ HgBa2 Ca2 Cu3 O8+ 100 93 133 258 182 173 117 130 Noel et al. (1987) Jia et al. (1992) Johnston and Cho (1990) 500 Maeda et al. (1992) Matsubara et al. (1992) Q. Li et al. (1992) 178 H. Zhang et al. (1992) W. C. Lee et al. (1991) W. C. Lee et al. (1991) 643 ≈12b 480 8 ≥105 21 13 Welp et al. (1989) Hikita et al. (1987) Y. Tajima et al. (1988) 3500 730 Note: The axial direction is along the c-axis for high temperature superconductors, and along the a-axis for typical organic materials. a This is an electron superconductor. b An estimate, since the ratios ab /c and c /ab differ. Reedyk et al. (1992b) Ning et al. (1992) Thompson et al. (1990) Farrell et al. (1990a) Thompson et al. (1993) Schilling et al. (1994b) 359 360 12 TYPE II SUPERCONDUCTIVITY Figure 12.23 Shape of the core (shaded) and the perimeter one penetration length from the center of a vortex for an applied magnetic field along the b (left) and c (right) crystallographic directions, respectively. The magnetic field is constant along each ellipse and along each circle. The figure is drawn for the condition c = 2ab = 6ab = 12c . Figure 12.24 Flow of differential current I in an elliptical path around a vortex for an applied magnetic field along the b crystallographic axis. The current densities are Jx = I/zy on the z-axis, and Jz = I/xy on the x-axis. direction, and inserting the appropriate characteristic lengths for the directions perpendicular to i. When the applied field is along the ith principal direction, expressions (12.8) and (12.9) for the critical fields Bc1 i and Bc2 i become Bc1 i = 0 ln i 4 j k (12.51a) Bc2 i = 0 2 j k (12.51b) These can be written in terms of the thermo dynamic critical field Bc , ln Bc1 i = √ i Bc 2 i √ Bc2 i = 2 i Bc (12.52a) (12.52b) 361 IV VORTEX ANISOTROPIES where Bc itself (9.10), Bc = √ 0 2 2 i i (12.53) is independent of the direction since, from Eq. (12.43), the product i i has the same value for i = a b c. The expressions for the ratio Bc2 i/Bc1 i = 2 2 i / ln (12.54) i with a vortex in an isotropic superconductor. Now we will generalize these expressions to account for the presence of anisotropy. When the applied magnetic field is in the z direction, along the c-axis, the vortex has axial symmetry and the magnetic field and current densities have the distance depen dence, B2 x y = 2 0 K 2ab 0 x2 + y2 1/2 /ab (12.59) and the product of these critical fields, Bc1 Bc2 i 1/2 = Bc ln i 1/2 (12.55) are generalizations of Eqs. (12.13). For the particular case of axial symmetry we have for the critical fields in the a, b-plane, Bc1 ab = Bc2 ab = 0 ln ab 4 ab c 0 2 ab c (12.56a) (12.56b) and along the c direction, Bc1 c = Bc2 c = 0 ln c 4 2ab 2 0 2 ab 0 2 × 0 3ab K1 x2 + y2 1/2 /ab yi − xj x2 + y2 1/2 (12.60) where K0 and K1 are zeroth- and first-order modified Bessel functions, respectively. When the applied magnetic field is in the x direction, along the a-axis, the vortex no longer has axial symmetry, and the distance dependences are more complicated: 1/2 y2 z2 0 K + Bx y z = 2 ab c 0 c2 2ab (12.57a) (12.61) (12.57b) where ab and c are defined by Eqs. (12.48). The ratio of the upper critical fields, Bc2 ab √ = Bc2 c Js x y = (12.58) is a particularly simple expression. Table 12.5 provides some experimentally determined values of these critical field anisotropies. D. High-Kappa Approximation In Section III.B we wrote down expres sions for the radial dependence of the mag netic field and current density associated Js y z = 0 2 0 ab c 1/2 y2 z2 K1 + 2c 2ab × 1/2 y2 z2 + 2c 2ab y z × 2k− 2 j (12.62) c ab Equation (12.62) is obtained from (12.61) with the aid of relation � × B = 0 Js . Analogous expressions can be written down for Bapp along y. The asymptotic equa tions (12.24)–(12.28) for the modified Bessel functions can also be applied to the anisotropic case. 362 Table 12.5 Critical Fields of Selected Anisotropic Type II Superconductors Material CeCu2 Si2 (heavy fermion) -ET2 I3 (organic) -ET2 I3 1.6 kbar